# cif

formula: Na.43 K.1 Fe1.55 Mg2.98 Al.86 Ti.21 Ca1.85 Mn.02 Si7.49 H1.958 O23.958 F.042
compound: <missing>
formula_title: <missing>
a: 9.869
b: 18.058
c: 5.320
alpha: 90
beta: 105.03
gamma: 90
cell_volume: 915.666
crystal_density: 3.184
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Temperature-dependent Al order-disorder in the
 tetrahedral double chain of C2/m amphiboles
 Sample: S(5)

atoms_sites:
["NaA", "KA", "NaAm", "KAm", "NaA2", "KA2", "FeM1", "MgM1", "AlM2", "TiM2", "FeM2", "MgM2", "AlM3", "FeM3", "MgM3", "CaM4", "NaM4", "MnM4", "FeM4", "CaM4*", "NaM4*", "MnM4*", "FeM4*", "SiT1", "AlT1", "SiT2", "AlT2", "H", "O1", "O2", "O3", "F3", "O4", "O5", "O6", "O7"]

atoms_x:
AAAAAAAAAACgNQIAoDUCAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABgIBEAYCARAKC8EQCgvBEAcJ0LAICXBgCwPgcA8K4GAPCuBgDQfRYAQFAVANDtFAAAghQA

atoms_y:
gIQeAICEHgCAhB4AgIQeAOCAHADggBwAgGsFAIBrBQCw2woAsNsKALDbCgCw2woAAAAAAAAAAAAAAAAA4BMRAOATEQDgExEA4BMRAFCCDwBQgg8AUIIPAFCCDwBAMwUAQDMFABCBCgAQgQoAAAAAAIBrBQCgmwoAAAAAAAAAAAAAPA8AoHUIABAvBwAAAAAA

atoms_z:
AAAAAAAAAABwYwQAcGMEAAAAAAAAAAAAgIQeAICEHgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgIQeAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgBwWhIAcFoSAHCBMQBwgTEAAK4uAIAiDQBwuCwA0JUrANCVKwAgQTAA8K4GAMCxJADQNxEA

atoms_occupancy:
wMIEAIA4AQDAwgQAgDgBAMDCBACAOAEAwOsSAEAdKgDAJwkAoGgGACD0DgCAhB4AQA0DAMBcFQAAnyQAkDocAECcAAAgTgAAkF8BAJA6HABAnAAAIE4AAJBfAQCw1DkAUDQDACB1OADgkwQA4MA7AAAJPQAACT0A4MA7ACBIAQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
eLwCAHi8AgCoxwMAqMcDAPB3AQDwdwEA0HAAANBwAAD4ZgAA+GYAAPhmAAD4ZgAA8GQAAPBkAADwZAAAOKQAADikAAA4pAAAOKQAAJiKAACYigAAmIoAAJiKAAAIVwAACFcAAABfAAAAXwAA4EUCAIiQAAB4jAAAaJwAAGicAAAQuAAAAL4AAPjFAACg4QAA

qdat:
AAAAAAAAAAACEAAAAAAAMAgUBAQAAABggGBEAICAJQoJgUJA4CCpIsIQwLwwEXwLAeg6Zjd4BBFLDYNACHYIzQvxDZFgPj0S6Wgp7t1lVMzGlTdv5OAxNe0rhvNQcDT1h1Zp6A9p0hA4TA7SMEnFKZtPjLnkBZAFeGg9GF==


formula: Na.45 K.1 Mg2.97 Fe1.57 Al.97 Ti.21 Ni.01 Zn.01 Ca1.84 Mn.02 Si7.4 H1.972 O23.972 F.028
compound: <missing>
formula_title: <missing>
a: 9.867
b: 18.044
c: 5.318
alpha: 90
beta: 105.06
gamma: 90
cell_volume: 914.298
crystal_density: 3.198
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Temperature-dependent Al order-disorder in the
 tetrahedral double chain of C2/m amphiboles
 Sample: S(6)
 Note: O(5) y-coordinate changed to reproduce reported bond lengths

atoms_sites:
["NaA", "KA", "NaAm", "KAm", "NaA2", "KA2", "MgM1", "FeM1", "MgM2", "AlM2", "TiM2", "FeM2", "NiM2", "ZnM2", "MgM3", "AlM3", "FeM3", "CaM4", "MnM4", "FeM4", "CaM4*", "MnM4*", "FeM4*", "AlT1", "SiT1", "AlT2", "SiT2", "H", "O1", "O2", "O3", "F3", "O4", "O5", "O6", "O7"]

atoms_x:
AAAAAAAAAADQFAIA0BQCAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABgIBEAYCARADC+EQAwvhEAEJQLAPCVBgAgPQcA0KsGANCrBgDwgBYAQFAVAEDsFADgfhQA

atoms_y:
gIQeAICEHgCAhB4AgIQeAIB3HACAdxwAEG0FABBtBQCw2woAsNsKALDbCgCw2woAsNsKALDbCgAAAAAAAAAAAAAAAABwFREAcBURAHAVEQDgag8A4GoPAOBqDwDQNAUA0DQFABCBCgAQgQoAAAAAABBtBQDAngoAAAAAAAAAAACQPQ8AoHUIAIAtBwAAAAAA

atoms_z:
AAAAAAAAAACADQQAgA0EAAAAAAAAAAAAgIQeAICEHgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AgIQeAICEHgCAhB4AgIQeAICEHgCwYBIAsGASAECJMQBAiTEA8NctALAaDQAgvSwA8JgrAPCYKwCQPzAAAL0GAJC5JACwNBEA

atoms_occupancy:
QH4FAIA4AQBAfgUAgDgBAEB+BQCAOAEAQB0qAMDrEgBA6B0AAMQJAKBoBgDgVw4AIE4AACBOAABAOyUAQA0DAIDAFACAExwAIE4AAOAiAgCAExwAIE4AAOAiAgBADQMAwPs5AIAaBgCA7jYAQC48AAAJPQAACT0AQC48AMDaAAAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
2HMEANhzBACgEQMAoBEDAFjvAwBY7wMAsHwAALB8AADYcgAA2HIAANhyAADYcgAA2HIAANhyAADobAAA6GwAAOhsAAAgsgAAILIAACCyAAB4lgAAeJYAAHiWAAAAXwAAAF8AAPhmAAD4ZgAAuPABAFiYAACIkAAAUKAAAFCgAAAIwAAA+MUAAOjLAACA7QAA

qdat:
AAAAAAAAAAACEAAAAAAAKAgUBAQAAABggGBEAICAJQYFgMEg4CCYouIIQLwwEd4GgWg6Ji80BBFJHcPACH0IZIr5jZEgFhqJ6VgZdWzlVMzmiz8r5NAZNOyeg7tYcBp8xzNl5AbtyhgsJAbzGCXjFU7HjpiiBogFbGQWlD==


formula: Na.47 K.1 Mg3.06 Fe1.45 Al.99 Ti.33 Ca1.83 Mn.02 Si7.31 H1.958 O23.958 F.042
compound: <missing>
formula_title: <missing>
a: 9.870
b: 18.046
c: 5.318
alpha: 90
beta: 105.04
gamma: 90
cell_volume: 914.764
crystal_density: 3.189
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Temperature-dependent Al order-disorder in the
 tetrahedral double chain of C2/m amphiboles
 Sample: S(7)

atoms_sites:
["NaA", "KA", "NaAm", "KAm", "NaA2", "KA2", "MgM1", "FeM1", "MgM2", "AlM2", "TiM2", "FeM2", "MgM3", "AlM3", "FeM3", "NaM4", "CaM4", "MnM4", "FeM4", "NaM4*", "CaM4*", "MnM4*", "FeM4*", "AlT1", "SiT1", "AlT2", "SiT2", "H", "O1", "O2", "O3", "F3", "O4", "O5", "O6", "O7"]

atoms_x:
AAAAAAAAAACAfQIAgH0CAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAADwIREA8CERADC+EQAwvhEAsDkMAICXBgAgPQcAYK0GAGCtBgBAfBYA0FEVAPDwFACAjhQA

atoms_y:
gIQeAICEHgCAhB4AgIQeAOD3HQDg9x0A8GkFAPBpBQAg2goAINoKACDaCgAg2goAAAAAAAAAAAAAAAAAsBsRALAbEQCwGxEAsBsRAEC/DwBAvw8AQL8PAEC/DwDQNAUA0DQFAKCCCgCgggoAAAAAAGBoBQCgmwoAAAAAAAAAAAAgPw8AUHoIAGAqBwAAAAAA

atoms_z:
AAAAAAAAAAAwVwUAMFcFAAAAAAAAAAAAgIQeAICEHgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgIQeAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgCwYBIAsGASACCGMQAghjEAsOQuAKAlDQCQuywAgJorAICaKwBwPDAA4LkGAGDBJADAKREA

atoms_occupancy:
gJ0FAIA4AQCAnQUAgDgBAICdBQCAOAEAwFUrAECzEQCg0h4AIKEHACASCgAggwwAwHMmAEANAwAAiBMAECcAAHDsGwAgTgAA4CICABAnAABw7BsAIE4AAOAiAgCg9wMAYBE5ALCPBgBQeTYA4MA7AAAJPQAACT0A4MA7ACBIAQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
sFcCALBXAgAYPwMAGD8DADAoAgAwKAIAwHYAAMB2AADgagAA4GoAAOBqAADgagAA4GoAAOBqAADgagAAaJIAAGiSAABokgAAaJIAAKh6AACoegAAqHoAAKh6AAD4XAAA+FwAAOhiAADoYgAA0C4BAICOAACAjgAAUKAAAFCgAAAYugAA+MUAAOjLAAB46wAA

qdat:
AAAAAAAAAAACEAAAAAAAKAgUBAQAAABggGBEAICAJQYFgMFA4CCZIuIQwLwwEV4GgWg6ZjdUBBFLHcNACH4I7IrxDZFgNjsR6VgppUzlVMzGizdv5OARNOyahrtQcD79Rzdl6A9t0hg8JAbSGCXlFY9PjJjiBZAFbGgWmD==


formula: Ca3 (Fe1.54 Mn.2 Al.26) Si1.65 O12 H5.4
compound: Wessels mine, Kalahari manganese field, South Africa
formula_title: <missing>
a: 12.340
b: 12.340
c: 12.340
alpha: 90
beta: 90
gamma: 90
cell_volume: 1879.081
crystal_density: 3.309
atoms_sites: ["Ca", "FeY", "MnY", "AlY", "SiZ", "O", "O-H"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAGDjFgAgVRwAIFUcAA==
atoms_y: QEIPAAAAAAAAAAAAAAAAAAAAAACg1vz/oNb8/w==
atoms_z: IKEHAAAAAAAAAAAAAAAAAEBCDwCAOgkAgDoJAA==
atoms_occupancy: AAk9AED/LgCAGgYAQO8HAMCRIQDAkSEAQHcbAA==
atoms_u_iso: 0
atoms_aniso_label: ["Ca", "FeY", "MnY", "AlY", "SiZ", "O", "O-H"]
atoms_aniso_u11: UA4BAOD2AADg9gAA4PYAAIC7AACgAwIAoAMCAA==
atoms_aniso_u22: UA4BAOD2AADg9gAA4PYAANDPAADAVwEAwFcBAA==
atoms_aniso_u33: kOIAAOD2AADg9gAA4PYAANDPAADAVwEAwFcBAA==
atoms_aniso_u12: cGIAANDV///Q1f//0NX//wAAAADgmP//4Jj//w==
atoms_aniso_u13: AAAAANDV///Q1f//0NX//wAAAACQUv//kFL//w==
atoms_aniso_u23: AAAAANDV///Q1f//0NX//wAAAAAQWQAAEFkAAA==
pub_title:
 Structure refinement of hydrous andradite,
 Ca3Fe1.54Mn0.02Al0.26(SiO4)1.65(O4H4)1.35, from the Wessels mine,
 Kalahari manganese field, South Africa
 Note: reported coordinates of Ca and Y-site made no sense, they have been changed

qdat:
AAAAAAAAAAAAAAAAAAAABAAAgAAAAAABAAgAAAgBAEAIAAEAgAAAICAgAEBAgQIEAABBAgggggAhABCCEAIQhCEIAgCIQiAQgAQiIREBCICACIiBABEAAkQIgBAACAAACAAAAAAAAJAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: U Bi4 As2 O16 H4
compound: Black Forest, Germany
pub_title: Orthowalpurgite, (UO2)Bi4O4(AsO4)2.2H2O, a new mineral from the Black Forest, Germany
formula_title: <missing>
a: 5.492
b: 13.324
c: 20.685
alpha: 90
beta: 90
gamma: 90
cell_volume: 1513.633
crystal_density: 6.511
atoms_sites: ["U", "Bi1", "Bi2", "As", "Ou1", "Ou2", "Oo1", "Oo2", "Oo3", "Oa1", "Oa2", "Oa3", "Oa4", "Wat"]
atoms_x: IM8pACA5KQDwaw0A4EoMAIASMQAALiIAYFoYAICKHQAgTgAAYHIUACA7GABgSQYA4MP8/0CCLgA=
atoms_y: oBX//6hCBgCgmBIAkDMAACAH9/+gYgcAQH0aAEBCDwBAQg8AYMYGAAAY/P+gqvv/oAMCAMADDwA=
atoms_z: QEIPANjaAQB4tQQAwOIHAEBCDwBAQg8AACYCAAAAAAAAAAAAkCgGACDWEwAAGgQAwGwKALDnCAA=
atoms_occupancy: 0
atoms_u_iso: gDgBAIC7AACAuwAAwNoAACC/AgBg5AEAYOoAAECcAABAGQEAgLsAACBIAQCAuwAAQBkBACBCAgA=
atoms_aniso_label: ["U", "Bi1", "Bi2", "As"]
atoms_aniso_u11: oPAAALBoAAAwjgAAgLsAAA==
atoms_aniso_u22: oJ8BAIC7AAAwwAAAAPoAAA==
atoms_aniso_u33: MCQBACD9AABQ3AAAwNoAAA==
atoms_aniso_u12: UOL//wAAAADQ7v//INH//w==
atoms_aniso_u13: AAAAAJDo//9gCQAAoA8AAA==
atoms_aniso_u23: AAAAAHD+//8AAAAAQAYAAA==
qdat:
AAAAAAAAAAQAAAACEACgSVAgCSCBBhKFigwpHYR9c1k3jUueZen/C0buZT++7X3/n/n/a71/5X/jr/9///f71//96/9l9U//fffrvtp/149s5/37VnbW1tf+v+uv2849G023Qv/urVr2+euyPx6Pqiq3H/v39t7P6mXti+==


formula: Cu6 Zn2.86 As2.4 Sb.42 O21 H6
compound: <missing>
pub_title: The crystal structure of sabelliite
formula_title: <missing>
a: 8.197
b: 8.197
c: 7.312
alpha: 90
beta: 90
gamma: 120
cell_volume: 425.478
crystal_density: 4.454
atoms_sites: ["Cu", "Zn1", "Zn2", "As", "As", "Sb", "O1", "O2", "O3", "O4", "O5", "H"]
atoms_x: UPUZAAAAAACgHw4Aq7AoAAAAAAAAAAAAUIoWAKA4DgDQ8g8AAAAAAKuwKADAXBUA
atoms_y: gLkRAAAAAACQMwAAVVgUAAAAAAAAAAAAQGsdAPBvBAAAcRsAAAAAAFVYFADArxwA
atoms_z: QBkBAAAAAABg8BgA8GIbAMBUDgDAVA4AcLsGAMAICgCgYRwAgIQeADCkDQCAbQ0A
atoms_occupancy: AAk9AAAQJwBAlRYAAAk9AAA1DABA0QwAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: ELgAABBZAACQ5wAAWFYBAJDdAACQ3QAAOK4AACBmAQAoxwEAyIsBAIBMAQD4jAIA
atoms_aniso_label: ["Cu", "Zn1", "Zn2", "As", "As", "Sb", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: gLsAAMhLAABg2wAA8HIBAHjDAAB4wwAAmKMAAABjAQA4jgIAKDsBAOh6AQA=
atoms_aniso_u22: oHMAAMhLAABY9wAA8HIBAHjDAAB4wwAAkKsAAGDvAAAIRwEAKDsBAOh6AQA=
atoms_aniso_u33: 6P0AAHB2AACY5AAAmBsBACgTAQAoEwEAyNcAAAjJAQDwfAEAKCYCAAjtAAA=
atoms_aniso_u12: wFMAAPAjAACYewAAcLcAAMhfAADIXwAAqGsAAKh/AABg7wAAiJ8AAIC7AAA=
atoms_aniso_u13: CCUAAAAAAAAYKQAAAAAAAAAAAAAAAAAAEAQAAICsAABAVgAAAAAAAAAAAAA=
atoms_aniso_u23: SAgAAAAAAACwGAAAAAAAAAAAAAAAAAAAqPP//wglAADo1v//AAAAAAAAAAA=
qdat:
AAAAAAAAAAAAAAJAAAAAEAAAAEAACMAARAAAAAIgAUAgIEEAIAgQSwAgAIiwKCCAMDCEIoICI1AQjMwYgFQYQIwxmSBAT0YCXBME5qRcVJ8cEsRJMVH0q47oNmBoXO5iffI5W2fX6R6Mrpozj8100LrEnv7m7g+VYw8ztS==


formula: Ca Mn Be2 Si5 O17 H6
compound: <missing>
pub_title: The crystal structure of chiavennite
formula_title: <missing>
a: 8.729
b: 31.326
c: 4.903
alpha: 90
beta: 90
gamma: 90
cell_volume: 1340.699
crystal_density: 2.633
atoms_x: QEIPAAAAAABQ+///QEIPAOChIwCQsggAAH8IAFBCCQDghgIAQEIPAEBCDwBAQg8AAOIEANAHAABQwwAAUKYJAA==
atoms_y: cF0FAAAAAADAfQMAUBQAACAsDgAQwff/EEz+/0D6AQDwlw4AIODw/1DB+P/QiPf/AN70/8Cg+f/QiwMAIP8IAA==
atoms_z: AAAAAAAAAABgxOX/gIQeAPBjBgBA3g4A4CATALDz7f+wOAgAAAAAAAAAAACAhB4AUNIKABC7EQDg1A4AoOEPAA==
atoms_occupancy: 0
atoms_u_iso: 8B0BAIDtAACgjAAAwMEAABAhAQAgLwEAMPIAABDvAAAQfwIAUL0BANC3BAAQZwYAYBYCAHBDAQBwQwEAsEMCAA==
atoms_aniso_u11: sK0BAKBtAQBgAwEAoAkBAOBaAQDQTAEAEAgBAEAyAQDQLQIAYMsBAACwBACw8wYA4CICAKCGAQCgnwEAcKECAA==
atoms_aniso_u22: oNcAAKC+AAAwdQAAQJwAAJCwAACAuwAAwMEAADDAAABwoQIA4CgBAKDqAQDgHAMAUNwAAEDOAAAg/QAAIPcBAA==
atoms_aniso_u33: oNcAALCaAABQLQAA0J0AAKBUAQCghgEAMAsBADDZAADQqgIAsEMCAECLBwAQIwkAYEIDAHB1AQAALAEA8DACAA==
atoms_aniso_u12: AAAAAODj//9g8P//AAAAAGAiAAAw+P//0O7//zARAAAwEQAAAAAAAAAAAAAAAAAAYNf//3DM//+QGgAAIJkAAA==
atoms_aniso_u13: QAYAAAAAAACAVwAAIOr///AjAABA1P//UOL//xD1//+AK///gIkAANACBQCAs/n/MI4AADBDAACw0v//AM7//w==
atoms_aniso_u23: AAAAANAHAAAg0f//AAAAABAOAABQFAAAEMP//5Do//8wF///AAAAAAAAAAAAAAAAsFX//2Cl//9w/v//0Cb//w==
atoms_sites:
["Ca", "Mn", "Be", "Si1", "Si2", "Si3", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O-H", "Wat"]

atoms_aniso_label:
["Ca", "Mn", "Be", "Si1", "Si2", "Si3", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O-H", "Wat"]

qdat:
AAAAAACAAAAAEIACAAAAkAIAjYOFAKAKJHRA4JBCAVqwtkNUm35FimY1yEMoVBIFs/uZe6EpoX7dZaaObRULtOvb//7rHy/S/t9aqnlFPv8m+//LX813fdNZ3nv2eO6+/3/32/SR//rfRHUr2kS/ba9v+/fmT8qRf/pMkA==


formula: K.789 Na.16 Ba.014 Fe.003 (Al Si3) O8
compound: <missing>
formula_title: <missing>
a: 8.531
b: 13.007
c: 7.179
alpha: 90
beta: 116.00
gamma: 90
cell_volume: 715.981
crystal_density: 2.559
atoms_sites: ["K", "Na", "Ba", "Fe", "AlT1", "SiT1", "AlT2", "SiT2", "OA1", "OA2", "OB", "OC", "OD"]
atoms_x: 8CERAPAhEQDwIREA8CERANCEAADQhAAAcN0qAHDdKgAAAAAAkP4lAGBtMgDQsAEAQEELAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAADAaCwAwGgsAkCIHAJAiBwDQuAgAAAAAAOCUCAAAwBIAQKQHAA==
atoms_z: sFEIALBRCACwUQgAsFEIADCkDQAwpA0AwPgUAMD4FAAAAAAAsGYRAGDODQCwiw8AkLYYAA==
atoms_occupancy: ICgwAADECQDA2gAA4C4AAAAXEQAA8isAgG0NAICbLwAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: sM8CALDPAgCwzwIAsM8CAFjyAABY8gAAGOwAABjsAAAonwEACKEBAHi9AQDQZQEAiIABAA==
atoms_aniso_label: ["K", "Na", "Ba", "Fe", "AlT1", "SiT1", "AlT2", "SiT2", "OA1", "OA2", "OB", "OC", "OD"]
atoms_aniso_u11: aMMBAGjDAQBowwEAaMMBACgsAQAoLAEAgBoBAIAaAQAIUAIAePkBANioAQBAbgEAiK0BAA==
atoms_aniso_u22: gL0DAIC9AwCAvQMAgL0DACARAQAgEQEASNoAAEjaAAAgkwEAAPUAANj4AQCwOgEAaIwBAA==
atoms_aniso_u33: MKUCADClAgAwpQIAMKUCAAisAAAIrAAAYMwAAGDMAACoKQEA+LABAKjOAQBQfAEAUAQBAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAFDO//9Qzv//4Pz//+D8//8AAAAAAAAAAKjB///46f//WBEAAA==
atoms_aniso_u13: YLMAAGCzAABgswAAYLMAACh4AAAoeAAAcGcAAHBnAADo7gAAwI8AAGj2AABYmAAAOFkAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAD2//8A9v//SAMAAEgDAAAAAAAAAAAAAPgbAAAI+P//SA0AAA==
pub_title:
 High-temperature crystal structure of sanidine
 Part II. The crystal structure of sanidine at 935 C
 Sample: T = 23 C, feldspar

qdat:
AAAAAAAAAAAAAAABQAAAAABAAACJAAACUAAgwIAACRUAACAmKIDoAICFCk4AQxAsNEJoGqgQdBNFFQANG8+sUgTL9wVvAFmTqKCU0FfP0WlGHRJu0avFyY4t8qycBfdSx9DxizRTDtvUMc/ZJp1lUCJx+zWqpXzHp0bxmM==


formula: K.789 Na.16 Ba.014 Fe.003 (Al Si3) O8
compound: <missing>
formula_title: <missing>
a: 8.677
b: 13.016
c: 7.184
alpha: 90
beta: 115.73
gamma: 90
cell_volume: 730.913
crystal_density: 2.507
atoms_sites: ["K", "Na", "Ba", "Fe", "AlT1", "SiT1", "AlT2", "SiT2", "OA1", "OA2", "OB", "OC", "OD"]
atoms_x: ELsRABC7EQAQuxEAELsRAICiAACAogAA0HwrANB8KwAAAAAA4AwnALCzMgDwSQIAMM8KAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAOBQCwDgUAsAcDgHAHA4BwBgBQkAAAAAADANCQDA6xIAEKwHAA==
atoms_z: AJgIAACYCAAAmAgAAJgIAECyDQBAsg0A8CIVAPAiFQAAAAAA8GwRAGAADgAABBAAgKgYAA==
atoms_occupancy: ICgwAADECQDA2gAA4C4AAAAXEQAA8isAgG0NAICbLwAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: AIYGAACGBgAAhgYAAIYGAEj3AQBI9wEA0OIBANDiAQAwbQMAuDADAOACBADILwMAEKsDAA==
atoms_aniso_label: ["K", "Na", "Ba", "Fe", "AlT1", "SiT1", "AlT2", "SiT2", "OA1", "OA2", "OB", "OC", "OD"]
atoms_aniso_u11: 6NsEAOjbBADo2wQA6NsEAKB2AgCgdgIA8DUCAPA1AgDYJwUAkHYDALDJAwDgMAMAINwDAA==
atoms_aniso_u22: EH8HABB/BwAQfwcAEH8HAMjWAQDI1gEAMEcBADBHAQDABQMAkIcBADBxBACQ9QEACKQDAA==
atoms_aniso_u33: GK8GABivBgAYrwYAGK8GANCNAQDQjQEA+PsBAPj7AQDQPAIA4PMDAIhkBACo0QMAqG4CAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAACic//8onP//oOz//6Ds//8AAAAAAAAAAEBm//+ohf//WKwAAA==
atoms_aniso_u13: iAICAIgCAgCIAgIAiAICAOjVAADo1QAAEL0AABC9AADAuwEAqAYBAHhTAgBI+AAAwF0AAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAADi//8A4v//uPz//7j8//8AAAAAAAAAAPglAAAI2v//WGsAAA==
pub_title:
 High-temperature crystal structure of sanidine
 Part II. The crystal structure of sanidine at 935 C
 Sample: T = 935 C, feldspar

qdat:
AAAAAAAAAAAAAAACQAAAAABAAAJCAAAQYABAxAAARhIAACDINAxQCEAwxBQCCCcCLAbEGyQQ4GQvCARwvi3GBMOm2ExoIm5iLhPQZT6pWY4VIskb0OZ4sF22tIUwXqe7LOOTK6jcmd4penmVluP4dStmmLJiVUuRTlqq/j==


formula: (Si14.637 Al2.346 Fe.017) O45.601 Na.316 K.022 Mg.391 Ca.605 H23.202
compound: <missing>
formula_title: <missing>
a: 13.698
b: 25.213
c: 22.660
alpha: 90
beta: 90
gamma: 90
cell_volume: 7826.031
crystal_density: 2.156
pub_title:
 The crystal structure of gottardiite, a new natural zeolite
 Note: occupancies altered to match chemical formula

atoms_sites:
["SiT1", "AlT1", "FeT1", "SiT2", "AlT2", "FeT2", "SiT3", "AlT3", "FeT3", "SiT4", "AlT4", "FeT4", "SiT5", "AlT5", "FeT5", "SiT6", "AlT6", "FeT6", "SiT7", "AlT7", "FeT7", "SiT8", "AlT8", "FeT8", "SiT9", "AlT9", "FeT9", "SiT10", "AlT10", "FeT10", "SiT11", "AlT11", "FeT11", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "O17", "O18", "O19", "O20", "O21", "O22", "NaX1", "KX1", "MgX1", "CaX1", "WatX1", "NaX2", "KX2", "MgX2", "CaX2", "WatX2", "NaX3", "KX3", "MgX3", "CaX3", "WatX3", "NaX4", "KX4", "MgX4", "CaX4", "WatX4", "NaX5", "KX5", "MgX5", "CaX5", "WatX5", "NaX6", "KX6", "MgX6", "CaX6", "WatX6", "NaX7", "KX7", "MgX7", "CaX7", "WatX7", "NaX8", "KX8", "MgX8", "CaX8", "WatX8", "NaX9", "KX9", "MgX9", "CaX9", "WatX9", "NaX10", "KX10", "MgX10", "CaX10", "WatX10", "NaX11", "KX11", "MgX11", "CaX11", "WatX11", "NaX12", "KX12", "MgX12", "CaX12", "WatX12"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

atoms_aniso_label:
["SiT1", "AlT1", "FeT1", "SiT2", "AlT2", "FeT2", "SiT3", "AlT3", "FeT3", "SiT4", "AlT4", "FeT4", "SiT5", "AlT5", "FeT5", "SiT6", "AlT6", "FeT6", "SiT7", "AlT7", "FeT7", "SiT8", "AlT8", "FeT8", "SiT9", "AlT9", "FeT9", "SiT10", "AlT10", "FeT10", "SiT11", "AlT11", "FeT11", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "O17", "O18", "O19", "O20", "O21", "O22"]

atoms_aniso_u11:

atoms_aniso_u22:

atoms_aniso_u33:

atoms_aniso_u12:

atoms_aniso_u13:

atoms_aniso_u23:

qdat:
AAAAAAAAIVAAGAAIaZkicCWlvoUaF3Gur8ne7v2fv9ef/f7+3+7/+//e3792//+/33y3N///vf9/38/2vvGvHsG1Wql4BQEIEAEAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ni5 As2 O12 H4
compound: <missing>
pub_title: Crystal structure of Ni5(AsO4)2(OH)4 and its comparison to other M5(XO4)2(OH)4 compounds
formula_title: <missing>
a: 9.291
b: 9.008
c: 5.149
alpha: 90
beta: 98.70
gamma: 90
cell_volume: 425.979
crystal_density: 4.984
atoms_sites: ["Ni1", "Ni2", "Ni3", "As", "O1", "O2", "O3", "O-H4"]
atoms_x: gIQeAICEHgAAAAAA4PApAKCFFgAAUjUAkHsmANAmGAA=
atoms_y: gIATAFh7CQAAAAAAAAAAAJBICQAAAAAAAAAAAID4EwA=
atoms_z: AAAAAICEHgCAhB4AYGADAECkBwCw8wYAwI4VAEDb6f8=
atoms_occupancy: 0
atoms_u_iso: OF4AAEBbAABYYQAAqEgAAOB5AACwaAAAYG0AAABkAAA=
atoms_aniso_label: ["Ni1", "Ni2", "Ni3", "As", "O1", "O2", "O3", "O-H4"]
atoms_aniso_u11: 8G4AAFBpAACwgQAA8EEAAJCIAABwSQAAQGoAANBrAAA=
atoms_aniso_u22: sHcAAIhtAACoYQAAsG0AAFCCAABQmwAAUIwAAABzAAA=
atoms_aniso_u33: 2EUAAKBQAABwUwAAaD0AAMBxAAD4YQAAiG0AAKhhAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAADjr//8AAAAAAAAAAMj7//8=
atoms_aniso_u13: 4AEAALAOAACABwAA4AEAAIACAACo8///2CIAANAHAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAFDd//8AAAAAAAAAAIAMAAA=
qdat:
AAAAAAAAAAAAAAAAIAAAEABIAAAEAAAgEgAASAAAIQBAgDEIBAhRBAAwIiUQACQIEVhUUjIArYIBQYgACmbYA9xWaABTKwdxnCTMwOrdAPA3aQ7WF3jNJm34x/LdZW0vnyonQn76mn6HVJMShdWfET5qWIcxZsAxiMBeW5==


formula: Si3 Al2 O12 H3
compound: <missing>
formula_title: <missing>
a: 17.912
b: 18.474
c: 6.542
alpha: 90
beta: 90
gamma: 90.00
cell_volume: 2164.789
crystal_density: 2.045
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Flexibility and distortion of the collapsible framework of NAT topology:
 the crystal structure of H3O-natrolite

atoms_sites:
["Si11", "Si13", "Si21", "Si22", "Si23", "Si24", "Al11", "Al12", "Al13", "Al14", "O11", "O12", "O13", "O14", "O21", "O22", "O23", "O24", "O31", "O32", "O33", "O34", "O41", "O42", "O43", "O44", "O51", "O52", "O53", "O54", "O1", "H11", "H12", "H13", "O2", "H21", "H22", "H23", "O3", "O4"]

atoms_x:

atoms_y:

atoms_z:

atoms_u_iso:

qdat:
AAAAABAAQAAKBgAAokkDHADOsE4BLxWIlpmVvq8669V6ra/3/vG963q9+t/f3ve7+7+v927/f9v7/P/9/3361+r/ev6//at/3v//b3t/dp9m2/VP///v+/v/X06fqrdm/f7ff7/X95+1dZ0S/35/+X1+19t3vU2R8n3/+/==


formula: Si O2
compound: Synthetic
formula_title: <missing>
a: 15.021
b: 8.6004
c: 16.4338
alpha: 90.
beta: 91.512
gamma: 90.
cell_volume: 2122.288
crystal_density: 2.257
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 29Si MAS NMR spectrum and superstructure of modulated tridymite L3-To(MX-1)
 Sample: superstructure

atoms_sites:
["Si1(1)", "Si1(2)", "Si1(3)", "Si1(4)", "Si1(5)", "Si1(6)", "Si2(1)", "Si2(2)", "Si2(3)", "Si2(4)", "Si2(5)", "Si2(6)", "Si3(1)", "Si3(2)", "Si3(3)", "Si3(4)", "Si3(5)", "Si3(6)", "Si4(1)", "Si4(2)", "Si4(3)", "Si4(4)", "Si4(5)", "Si4(6)", "O1(1)", "O1(2)", "O1(3)", "O1(4)", "O1(5)", "O1(6)", "O1(7)", "O1(8)", "O1(9)", "O1/2(1)", "O1/2(2)", "O1/2(3)", "O2(1)", "O2(2)", "O2(3)", "O2(4)", "O2(5)", "O2(6)", "O2(7)", "O2(8)", "O2(9)", "O2/3(1)", "O2/3(2)", "O2/3(3)", "O3(1)", "O3(2)", "O3(3)", "O3(4)", "O3(5)", "O3(6)", "O3(7)", "O3(8)", "O3(9)", "O3/4(1)", "O3/4(2)", "O3/4(3)", "O4(1)", "O4(2)", "O4(3)", "O4(4)", "O4(5)", "O4(6)", "O4(7)", "O4(8)", "O4(9)", "O4/1(1)", "O4/1(2)", "O4/1(3)"]

atoms_x:

atoms_y:

atoms_z:

atoms_u_iso:

qdat:
AAAAAAIgAEAARCiEACEyFAiB5cTHvIExRIT+s3e6V53S2atzv/v2d/O/9/3/7//T/m3///9//v//9+/f7/3r3///////9////rf//t3/b/1V/9//f/917/+v///3+7f79//9vj3cv1s+eqyjcE6BAxABIABAAAAAAAAAAA==


formula: Si O2
compound: Synthetic
formula_title: <missing>
a: 5.007
b: 8.6004
c: 8.2169
alpha: 90
beta: 91.512
gamma: 90
cell_volume: 353.715
crystal_density: 2.257
atoms_sites: ["Si1", "Si2", "O1", "O2", "O3", "O4"]
atoms_x: wKkEANC3BADQmxEAAMoIAECaEQAgjyMA
atoms_y: kMESAIDsFQCg9S0A8FwcAND3CgBALgoA
atoms_z: wN0MAAD6MgBgdw8AoM8SAHB/EADguR8A
atoms_occupancy: 0
atoms_u_iso: gCwDAIAsAwCArwIAIDAFAEBsCACAeQsA
atoms_aniso_label: ["Si1", "Si2", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: 4J8CAECQAgBgYQIAAO4CAAD0AQBAPBAA
atoms_aniso_u22: oAMCAEATAgBg3gIAwNQBAAD0AQAALw0A
atoms_aniso_u33: AOIEAEABBQDAzgIAAL4KAMBcFQBAfgUA
atoms_aniso_u12: gD4AAIA+AABAnAAAQCX//wB9AACgmP7/
atoms_aniso_u13: YOQBAGDkAQCgDwAAYPb+/8Dg//+ADggA
atoms_aniso_u23: wF0AAAB9AAAg0f//oIwAAAB9AABAJf//
pub_title:
 29Si MAS NMR spectrum and superstructure of modulated tridymite L3-To(MX-1)
 Sample: average crystal structure

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAYEAGAAAAAAAMAAAAABQAQKAAKEIgAAAwEoAAABIA4GFASEEQCgwYFMAAagHCQIAVaiCsFgAAxqwwKjkADp3AB4l7oxNIJZQAA2rVOGcnFdIt0yLt3fgtBgQb61Rh2BPl9Toy3rDLufAJwv==


formula: Co2.01 Fe.74 Ni.25 As2 O16 H16
compound: <missing>
formula_title: <missing>
a: 10.251
b: 13.447
c: 4.764
alpha: 90
beta: 104.98
gamma: 90
cell_volume: 634.378
crystal_density: 3.122
atoms_x: AAAAAAAAAAAAAAAAAAAAAMhMEwDQHAkAEMMYABD0FAAg+AUAMGIYAGBDBwDg8gkAAHYWAABYGwA=
atoms_y: AAAAAICBFwCAgRcAgIEXAAAAAAAAAAAAAAAAADCDBgCQ8AYAkN8NAOCNBQBgwAcAALIMAEA2EQA=
atoms_z: AAAAAAAAAAAAAAAAAAAAAPi5FgBA4BYAoBosAPC8DACwPDEAUIkrAKAZKADADTcAALcgAECUKwA=
atoms_occupancy: AAk9AKDSHgBAlRYAIKEHAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: ABJ6AAASegAAEnoAABJ6AAASegAAEnoAABJ6AAASegAAEnoAABJ6AMDzAAAg3gEAANUCAACKAgA=
atoms_aniso_label: ["CoMe1", "CoMe2", "FeMe2", "NiMe2", "As", "O1", "O2", "O3", "OW1", "OW2"]
atoms_aniso_u11: AK8AAIDUAACA1AAAgNQAAECcAACQlwAAYAMBAFD1AADA8wAA8LMBAA==
atoms_aniso_u22: oAkBAMDzAADA8wAAwPMAACDkAACwYgEAABMBAPDrAACwYgEAUFkBAA==
atoms_aniso_u33: AH0AALCaAACwmgAAsJoAAPBuAADgkgAAoFoAAMDaAAAw2QAAEAgBAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAADD4//9Q4v//0CAAAA==
atoms_aniso_u13: MPj//6APAACgDwAAoA8AAOD8///QBwAA8Nj//7A2AACgDwAA0DkAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAADAqAADQ7v//QB8AAA==
pub_title:
 Structure and crystal chemistry of vivianite-type compounds: Crystal
 structures of erythrite and annabergite with a Mossbauer study of erythrite

atoms_sites:
["CoMe1", "CoMe2", "FeMe2", "NiMe2", "As", "O1", "O2", "O3", "OW1", "OW2", "H11", "H12", "H21", "H22"]

qdat:
AAAAAAAAAAAAAQAEAAAAAQBAACIEEAAQCABAgCUIIAIAQUCCQIwIkkFUARMAAkJ0AbYgIDjMSlItMjlQCXG6kK0ZGyU0sU6NTQzZOApG0ilwWzfggRVrD85dAqjyCusFkqI+TJDQq9EJxETNqoSvZDRYCxQBZWJa4EUeiU==


formula: (Ni2.64 Mg.36) As2 O16 H16
compound: <missing>
formula_title: <missing>
a: 10.179
b: 13.309
c: 4.725
alpha: 90
beta: 105.00
gamma: 90
cell_volume: 618.296
crystal_density: 3.146
atoms_x: AAAAAAAAAAAAAAAAAAAAAKBMEwCwGQkAgNoYANDtFACQ3QUAkGsYAMAzBwCAAgoAgLQWAMA4GwA=
atoms_y: AAAAAAAAAACYjBcAmIwXAAAAAAAAAAAAAAAAAECRBgBw7QYAUMANACAwBQAA0AcAIIMMAODIEAA=
atoms_z: AAAAAAAAAAAAAAAAAAAAAHDsFgBwPBcA8HksAIDXDADgmDEAcNcrAEAjKQCAZTgAoEMhAGBlKwA=
atoms_occupancy: wGw8AECcAACgWjIAYK4KAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: ABJ6AAASegAAEnoAABJ6AAASegAAEnoAABJ6AAASegAAEnoAABJ6ANBlAQDghgIAINgCABDKAgA=
atoms_aniso_label: ["NiMe1", "MgMe1", "NiMe2", "MgMe2", "As", "O1", "O2", "O3", "OW1", "OW2"]
atoms_aniso_u11: AK8AAACvAAAAyAAAAMgAAGCfAABgnwAAMPIAABDvAAAw8gAA0H4BAA==
atoms_aniso_u22: oAkBAKAJAQDAwQAAwMEAAKC+AACgvgAAkOIAAPDSAABAMgEAQBkBAA==
atoms_aniso_u33: AH0AAAB9AAAgsgAAILIAAHCUAABwlAAAYJ8AALDlAAAQ7wAAUA4BAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAHAXAADg/P//IBwAAA==
atoms_aniso_u13: MPj//zD4//9wMAAAcDAAAPAjAADwIwAAUPv//0BRAADwPAAAAEsAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAOD8//8Q9f//gCUAAA==
pub_title:
 Structure and crystal chemistry of vivianite-type compounds: Crystal
 structures of erythrite and annabergite with a Mossbauer study of erythrite

atoms_sites:
["NiMe1", "MgMe1", "NiMe2", "MgMe2", "As", "O1", "O2", "O3", "OW1", "OW2", "H11", "H12", "H21", "H22"]

qdat:
AAAAAAAAAAAAAQACAAAAAIAgABEBBAAEBAAQIAkiBACACJAQUBKBEpAqQERgAChrABWkBAWSjKUiyyyVAE8dKQfRSXFxqZI0SuiuycByNsnPgX2rAgmX2Dd5dAmj6CloFibNOKlBoXeiMpCJq20I28R0aBskAVqiavBCn4==


formula: Na3 Fe8 Ti2 Si12 O43 H6
compound: <missing>
pub_title: Nafertisite, a layer titanosilicate member of a polysomatic series including mica
formula_title: <missing>
a: 5.353
b: 16.176
c: 21.95
alpha: 90
beta: 94.6
gamma: 90
cell_volume: 1894.531
crystal_density: 2.879
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["Na1", "Na2", "Na2*", "Fe1", "Fe2", "Fe3", "Ti", "Si1", "Si2", "Si3", "O1", "O-H2", "O3", "O4", "O-H5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13"]

atoms_x:
gIQeAAAAAAAAAAAAQMUOAKCvDwBAvw8AgM39/4AZGwBAfRoAABj8/+CeFwDAzRcA4BUZAOBY+f8AWQYA4JMEAGAfDQAgQCwAYBMPAGDFGwAA5i0AYIv7/wAAAAA=

atoms_y:
AAAAAMCZ9v+g+O7/oGAYAJDVMAAAAAAAAAAAAMCN+P8ACxMAAOcYACBfEgCAhB4AAKf5/4CoGABgARIAgIQeAEAYFgBgkfr/QAEFAMCMDQAA+RUAgIQeAAAAAAA=

atoms_z:
AAAAAAAAAAAAAAAA8NTv/zAH8f+Q2PH/wAT6/+Db+P/g4ff/ALP3/0Bt8/+gY/L/wKX0/6Bd8/9gYu3/APvr/+BY+f9gDvv/oC37/4Dl+f9gl/n/YJf5/wAAAAA=

atoms_occupancy:
AAk9AICEHgCAhB4AANQwAADUMAAA1DAAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
QA0DAIA4AQCAOAEAQJwAAAD6AACAuwAAIE4AAKB0BABAkAIAwNQBAIA4AQDA1AEAQJwAAEANAwCAOAEAgDgBAIA4AQBAnAAAgKkDAECcAABADQMAwNQBAAASegA=

qdat:
AAAABAAAAEAAAhIAQAAYCEAUgBoSKSAFREEJCFLdm4p4DiRjOduLmGU2GhkVGH2GPvcfWrNQrwPemzVnt4/ZhyqFTVh0EW0UwQ/E8TxrGI8Fs5UwphdUg5VzF+nE2jTKmaHUERJIZUzdPUahyrVMESJBFAgJBkrayzZWsZ==


formula: Mg1.131 Mn.799 Ca.07 Si2 O6
compound: manganiferous quartzite in the United Arab Emirates
formula_title: <missing>
a: 9.725
b: 8.876
c: 5.263
alpha: 90
beta: 108.53
gamma: 90
cell_volume: 430.746
crystal_density: 3.490
atoms_sites: ["MgM1", "MnM1", "CaM2", "MnM2", "MgM2", "SiA", "SiB", "O1A", "O1B", "O2A", "O2B", "O3A", "O3B"]
atoms_x: YEoPAGBKDwDoew8A6HsPAOh7DwBgiQIAgGMhAKDkNACAtBYAMDIHACAZJgBwVwYAAOokAA==
atoms_y: cO8nAHDvJwAYcwEAGHMBABhzAQAo0hQAMDMzAPiTFAAQITMAwKMeACCoPAAA6w8AYLArAA==
atoms_z: sEYOALBGDgCgLg4AoC4OAKAuDgDwixAA0JQOAEAVCgDALQgAALoTAPDqFQDA1iIAQOgdAA==
atoms_occupancy: AJI7AAB3AQDARQQAYE0vAOB1CQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: cEkAAHBJAABQkQAAUJEAAFCRAABAagAA8G4AAPCHAAAQiwAAgKIAAKC+AABwrQAA4KsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kanoite, donpeacorite and tirodite: Mn-Mg-silicates from a
 manganiferous quartzite in the United Arab Emirates
 Sample: pyroxene

qdat:
AAAAAAAAAAAIAAAAIAAAAACCgCQAAIAECAgCgYAAAUiCEEBwcQQSMCJgBmygkFCwpE0sVQFu4hNKRhOdK9JoxWJwx9TuOP64K90j5i7fDK/86n2O1ez++r1n/639/Zd33f3pW/Nu7a5mt9vhp9+e7yPt7L+u1P7WL3vx/0==


formula: Ca.333 Na.038 K.024 (Al.768 Si2.232) O8 H4
compound: Gibelsbach, Fiesch (Valais, Switzerland)
formula_title: <missing>
a: 9.083
b: 17.738
c: 10.209
alpha: 89.95
beta: 124.58
gamma: 90.00
cell_volume: 1354.233
crystal_density: 2.262
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 (010) disorder, partial Si,Al ordering, and Ca distribution
 in triclinic (C1) epistilbite
 Sample: 293 K

atoms_sites:
["Ca1", "Na1", "K1", "Ca12", "Na12", "K12", "Ca2", "Na2", "K2", "Ca22", "Na22", "K22", "AlT11", "SiT11", "AlT12", "SiT12", "AlT13", "SiT13", "AlT14", "SiT14", "AlT21", "SiT21", "AlT22", "SiT22", "AlT23", "SiT23", "AlT24", "SiT24", "AlT31", "SiT31", "AlT32", "SiT32", "AlT33", "SiT33", "AlT34", "SiT34", "O11", "O12", "O21", "O23", "O31", "O32", "O33", "O34", "O41", "O42", "O43", "O44", "O51", "O53", "O61", "O63", "O71", "O72", "O81", "O82", "O83", "O84", "O91", "O92", "Wat1", "Wat2", "Wat2p", "Wat3", "Wat3*", "Wat3p", "Wat3p*", "Wat4"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAABAAAAABEBgQASIAACEGQiSEiMMAiYJIHvawCIseQWB2ZL1cPYl6oR6z78Od+5eC3P//39z+x6/No/a+/pP1/hK/t++du/zb/1+hf7//93/s/N/b+/2/3/J6/f/P/9/13+3s/bb/////rt+9+6tf/792/vrH+u/+/7==


formula: Ca Mg.7 Al.6 Si1.7 O6
compound: <missing>
formula_title: <missing>
a: 9.680
b: 8.828
c: 5.268
alpha: 90
beta: 106.16
gamma: 90
cell_volume: 432.390
crystal_density: 3.334
atoms_sites: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAA8IURAPCFEQDw4AYAQBgWAECCFQA=
atoms_y: oIQSADBwNwAwcDcAMLsFADC7BQAQOwUAgJMPAIAfAQA=
atoms_z: QEIPAEBCDwBAQg8AIMgNACDIDQCwUQgAUGoTAACD//8=
atoms_occupancy: AAk9AIC5KgCATxIAwCcJAEDhMwAACT0AAAk9AAAJPQA=
atoms_u_iso: gI4AABhRAAAYUQAAUEEAAFBBAACgggAASJ4AAKh6AAA=
atoms_aniso_label: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_aniso_u11: gLsAAPBVAADwVQAAEEAAABBAAACAPgAAMMAAAHBiAAA=
atoms_aniso_u22: gHAAAEBRAABAUQAAMEMAADBDAACgpQAAMI4AAMCPAAA=
atoms_aniso_u33: kGUAADBDAAAwQwAAEEAAABBAAADAqAAAwI8AAOB5AAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAwEQAAEPX//wAAAAA=
atoms_aniso_u13: YAkAAPAKAADwCgAAwBIAAMASAADAKwAA4C4AALAdAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAoPb//6D2//8wEQAAIOr//xDD//8=
pub_title:
 High-temperature crystal chemistry of C2/c clinopyroxenes along
 the join CaMgSi2O6-CaAl2SiO6
 Sample: Di70CaTs30 at 25 C

qdat:
AAAAAAAAAAAAAAAAIAAAAAECAAAACAAECAABAIAAAIgAQhAOAQBBMAAABEiEIEAgBEWUQQiSIQ6kAAQXABNBUA8mdGQCATnkAUeYOxiUy0YNJVADjrvU0Fmg3kfExz1iI3LvW7oEM2qGvIzbDuao1jbpOrU2zszzcWRk4i==


formula: Ca Mg.7 Al.6 Si1.7 O6
compound: <missing>
formula_title: <missing>
a: 9.703
b: 8.863
c: 5.281
alpha: 90
beta: 106.24
gamma: 90
cell_volume: 436.032
crystal_density: 3.306
atoms_sites: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAA8IURAPCFEQBg3wYAYBsWAOB4FQA=
atoms_y: 0HwSANBmNwDQZjcAELgFABC4BQDQNAUA4IMPAFAOAQA=
atoms_z: QEIPAEBCDwBAQg8AkMYNAJDGDQCAWQgA4FITAHCa//8=
atoms_occupancy: AAk9AIC5KgCATxIAwCcJAEDhMwAACT0AAAk9AAAJPQA=
atoms_u_iso: YPkAAHiWAAB4lgAA2HIAANhyAADgyQAAYPkAANjHAAA=
atoms_aniso_label: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_aniso_u11: QEsBAICiAACAogAAYG0AAGBtAAAgZwAAACwBAACWAAA=
atoms_aniso_u22: gLsAAJCXAACQlwAAAH0AAAB9AABgHAEAsMwAAMAMAQA=
atoms_aniso_u33: YLgAAJB+AACQfgAAYG0AAGBtAACg1wAA0OgAANC2AAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAcP7//3D+//+ADAAA0NX//7BPAAA=
atoms_aniso_u13: AAAAAOAVAADgFQAAsB0AALAdAABQLQAAIDUAAJAzAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAoPb//6D2///w8f//sOv//5C2//8=
pub_title:
 High-temperature crystal chemistry of C2/c clinopyroxenes along
 the join CaMgSi2O6-CaAl2SiO6
 Sample: Di70CaTs30 at 300 C

qdat:
AAAAAAAAAAAAAAAAIAAAAAECAAAACAAICAACAQAAAJAAgiAaAgBEYAAACNEIQIBAEQckghFEQhaoAAhMAEqGoB6VcJAEAmUYCRYoulIxHxxSj0AGHt/RQzeD5Q2RC/dFjc2c7dQYjx4a9Cuca4/FUNdCqpX7VxLNLpKhiQ==


formula: Ca Mg.7 Al.6 Si1.7 O6
compound: <missing>
formula_title: <missing>
a: 9.717
b: 8.886
c: 5.288
alpha: 90
beta: 106.29
gamma: 90
cell_volume: 438.263
crystal_density: 3.289
atoms_sites: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAYIQRAGCEEQBg3wYAsBYWADB0FQA=
atoms_y: sHkSACBiNwAgYjcA8LQFAPC0BQBgNgUAgHoPABAIAQA=
atoms_z: QEIPAEBCDwBAQg8AAMUNAADFDQCQTggA8EcTAJCd//8=
atoms_occupancy: AAk9AIC5KgCATxIAwCcJAEDhMwAACT0AAAk9AAAJPQA=
atoms_u_iso: oEABAOjBAADowQAAcJQAAHCUAABg+QAAoEABAGD5AAA=
atoms_aniso_label: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_aniso_u11: UKQBAADIAAAAyAAA0IQAANCEAADAjwAA8IEBAKC+AAA=
atoms_aniso_u22: MPIAAEDOAABAzgAAgKIAAICiAAAwVgEAsP4AAHBDAQA=
atoms_aniso_u33: gO0AAKClAACgpQAAUJEAAFCRAABgAwEAYDUBALDlAAA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAUPv//1D7//8QDgAA0Lz//+D8//8=
atoms_aniso_u13: UPv//9AgAADQIAAAYCIAAGAiAABAOAAAAEsAAEA4AAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAA8PH///Dx//8A5///AOf//2Cl//8=
pub_title:
 High-temperature crystal chemistry of C2/c clinopyroxenes along
 the join CaMgSi2O6-CaAl2SiO6
 Sample: Di70CaTs30 at 500 C

qdat:
AAAAAAAAAAAAAAAAIAAAAAEEAAAACAAIEAACAQAAAJAAgiAUBACEQAAAEJIIgICAEQ4pAhKIhC1IABCcAJUNQD0VIZAIBOowEixRfFhiHjSmLYAIPfvFBlKKsyrDNtyKnV052ygrGzo35FsRlh+J0S+Fpyt6bGmerSRFER==


formula: Ca Mg.7 Al.6 Si1.7 O6
compound: <missing>
formula_title: <missing>
a: 9.733
b: 8.909
c: 5.296
alpha: 90
beta: 106.35
gamma: 90
cell_volume: 440.652
crystal_density: 3.271
atoms_sites: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAYIQRAGCEEQCg5QYAkBMWAKByFQA=
atoms_y: IHgSAHBdNwBwXTcA0LEFANCxBQDQNAUAAG4PAHD4AAA=
atoms_z: QEIPAEBCDwBAQg8AAMUNAADFDQDwVwgAwDYTADCt//8=
atoms_occupancy: AAk9AIC5KgCATxIAwCcJAEDhMwAACT0AAAk9AAAJPQA=
atoms_u_iso: 0I0BAFj3AABY9wAAELgAABC4AADQJAEAwIkBALAwAQA=
atoms_aniso_label: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_aniso_u11: 0BQCAOAPAQDgDwEAMKcAADCnAABgnwAAsN8BAKDwAAA=
atoms_aniso_u22: 4CgBAAD6AAAA+gAAQM4AAEDOAAAQhQEAYDUBAFCLAQA=
atoms_aniso_u33: QBkBAJDJAACQyQAA4KsAAOCrAADgQQEAQH0BAJAUAQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAUPv//1D7///AEgAAEKr//wAAAAA=
atoms_aniso_u13: 8PH//4AlAACAJQAAoCgAAKAoAACwNgAAIGcAAKBBAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAsOv//7Dr///g/P//8Nj//wCD//8=
pub_title:
 High-temperature crystal chemistry of C2/c clinopyroxenes along
 the join CaMgSi2O6-CaAl2SiO6
 Sample: Di70CaTs30 at 700 C

qdat:
AAAAAAAAAAAAAAAAQAAAAAEEAAAACAAIEAACAgAAASABBCA0CACIwAAAEaIRAQEAIgwqAiUJBFqQACEYASUmgHouZyAICdowKFyU5LCEfKpsOwA4UvWaDOUfajMGf7EdMvw3tjBYWlRv0LZSNjcjJVoOjF15VVU5clkKNE==


formula: Ca Mg.5 Al Si1.5 O6
compound: <missing>
formula_title: <missing>
a: 9.697
b: 8.850
c: 5.306
alpha: 90
beta: 106.39
gamma: 90
cell_volume: 436.849
crystal_density: 3.305
atoms_sites: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAgIcRAICHEQDguQYAkBMWAIBvFQA=
atoms_y: AI4SAPBpNwDwaTcAMLsFADC7BQBQKAUAgJMPAJDiAAA=
atoms_z: QEIPAEBCDwBAQg8AoIkNAKCJDQDwDAgAoDMTAIBd//8=
atoms_occupancy: AAk9AICEHgCAhB4AQEIPAMDGLQAACT0AAAk9AAAJPQA=
atoms_u_iso: kJsBAAgVAQAIFQEAiOUAAIjlAAD4eQEASLsBADBgAQA=
atoms_aniso_label: ["CaM2", "MgM1", "AlM1", "AlT", "SiT", "O1", "O2", "O3"]
atoms_aniso_u11: kPUBAJAUAQCQFAEAsLMAALCzAAAg5AAA0BQCAOAPAQA=
atoms_aniso_u22: YE4BABAhAQAQIQEAIBYBACAWAQBQ1gEA4IwBACCTAQA=
atoms_aniso_u33: MFYBAJD7AACQ+wAA4N0AAODdAAAAqQEAUKQBAHB1AQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAwPn//8D5//9wFwAAEJH//9AgAAA=
atoms_aniso_u13: oA8AAAAyAAAAMgAA8CMAAPAjAADgRwAAEKQAAABLAAA=
atoms_aniso_u23: AAAAAAAAAAAAAAAAwOD//8Dg//9wFwAAQLv//4B2//8=
pub_title:
 High-temperature crystal chemistry of C2/c clinopyroxenes along
 the join CaMgSi2O6-CaAl2SiO6
 Sample: Di50CaTs50 at 700 C
 Note: coordinates for O3 were altered by the author May, 2003

qdat:
AAAAAAAAAAAAAAAAIAAAAAECAAAACAAICAABAQAAARAAghAcAgBCYAAACNCEQICACIVEQhEkQhWIABA2ACsCoC5i0MgUARuwBI8obhpSttQ4i2AGO7+rIcNE9paUh+SHhsbk83AwRoyPTJtYZc6xmVOHJdE2NvZ02iUMsB==


formula: Pb3 Ge3 O10 H2
compound: <missing>
pub_title: Crystal structure of Pb6[Ge6O18]2H2O, a lead cyclo-germanate similar to the mineral dioptase
formula_title: Pb6[Ge6O18].2H20
a: 15.6476
b: 15.6476
c: 7.3119
alpha: 90
beta: 90
gamma: 120
cell_volume: 1550.445
crystal_density: 6.435
atoms_sites: ["Pb", "Ge", "O1", "O2", "O3", "Wat"]
atoms_x: 8CMZAHAKFwBgBxEAYHIUACCsGgAAAAAA
atoms_y: YIQRAEDPHQDgeh0A4BUZAMC1GwAAAAAA
atoms_z: cLkwAIBOJwCg7y4AoOQbAADUMACATxIA
atoms_occupancy: 0
atoms_u_iso: 4KsAACDLAAAgywAA4KsAAAB9AABAYAoA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAIAAIAAAAgAQAgBAACAIEAgYCAAAwQQoQoIAZQiCCEAigFZIBYiWDQFkTkZCkQdgFElVoNl2IKi3ImzioqjU0aMxE0Jp1KwXKxXZpCrLI7eplGZJZJGZj9ZiTjUoQ2REbEiViQtVZkBDsWAElmJYAkxJIg==


formula: Pb Sb2 O6
compound: Cetine mine, Siena, Italy
pub_title: Rosiaite, PbSb2O6, a new mineral from the Cetine mine, Siena, Italy
formula_title: <missing>
a: 5.295
b: 5.295
c: 5.372
alpha: 90
beta: 90
gamma: 120
cell_volume: 130.436
crystal_density: 6.960
atoms_sites: ["Pb", "Sb", "O"]
atoms_x: AAAAAFVYFACgAhcA
atoms_y: AAAAAKuwKAAAAAAA
atoms_z: AAAAAICEHgDQGBIA
atoms_occupancy: 0
atoms_u_iso: IAcBAPi7AAAQDQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAEAABAAAAAAAgAAAAAAAAkAAAAQSAAACAAAAAEAAEAgABEAAAAEAERAAQAAAhQAUIASAAEQAYoAEAAAEKMQkABCQFCEAAiAISFAgCRTAIEAmEyKAECIiQEEgIowQkzIAABEyRgCGSQhGQZRgFIWB==


formula: Ca U P2 O8
compound: <missing>
pub_title: Low-temperature ordered phase of CaU(PO4)2: synthesis and crystal structure
formula_title: CaU(PO4)2
a: 13.926
b: 6.958
c: 6.136
alpha: 90
beta: 90
gamma: 90
cell_volume: 594.561
crystal_density: 5.229
atoms_sites: ["Ca", "U", "P1", "P2", "O1", "O2", "O3", "O4", "O5", "O6"]
atoms_x: sCUHACCrFgDwmRYA0L4HAJCzDADQ+wEAcAAIAICCFgBAgREAQA0cAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8A0GwEAFDEBABAQg8AQEIPAA==
atoms_z: IPAXANAdJgBApAcAAJc2AEBDLAAgsS4A0MMCAGAFOwBA5REAgHQQAA==
atoms_occupancy: 0
atoms_u_iso: CFcAAGg9AAAgUwAAUEEAAJCIAADAdgAAmIoAAHiMAABYmAAA2HIAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAgAACAAIBAgAAIIAwAgCUoAKgAQoECgVQHZAFRApcMlYkpQ4mlcIkI6bpFJkC9z8noMlX0lTT34MtuYWW5fLkYK9aF3U/ju15zR/3V4/zrvtu3fd9//3n7e7zPuc7x3+vqv07b6bnP+fu5/cz/9rd7M3==


formula: Rb2.08 Mn3 O6
compound: <missing>
pub_title: RUB-7, a new synthetic manganese oxide structure type with a 2x4 tunnel
formula_title: RUB-7
a: 14.191
b: 2.851
c: 24.343
alpha: 90
beta: 91.29
gamma: 90
cell_volume: 984.633
crystal_density: 5.917
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["Rb1a", "Rb1b", "Rb2a", "Rb2b", "Mn1", "Mn2", "Mn3", "Mn4", "Mn5", "Mn6", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12"]

atoms_x:
AKYOAEBCDwDAehAAgN4PAKCS///AXQAAwOD//8Dg//8gEgoAQOMJAEABBQAgswQAgKkDAECKAwCgYgcAgNgQAKBzGQBAABoAYMsaAED6GgAgdw4AQBIXAA==

atoms_y:
gJsvAMAgHwDANzAAADUMAICEHgAAAAAAgIQeAAAAAACAhB4AAAAAAAAAAACAhB4AAAAAAICEHgAAAAAAgIQeAAAAAACAhB4AAAAAAICEHgCAhB4AAAAAAA==

atoms_z:
APkVAMDrEgCAbQ0AgIsIAMC8BQBAVAwAYH4SACC4GAAARh4A4KsAAIAmBABAYAoAwHoQAMBQFwBA9BsAYMUbAKBtGgBAJBQAACkOACChBwDAzgIAIEICAA==

atoms_occupancy:
wMYtAMAJDgCAMRcAAPIrAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==

atoms_u_iso:
ANsBAADbAQAA2wEAANsBAMB2AADAdgAAwHYAAMB2AADAdgAAwHYAAPjFAAD4xQAA+MUAAPjFAAD4xQAA+MUAAPjFAAD4xQAA+MUAAPjFAAD4xQAA+MUAAA==

qdat:
AAAAIAAACAAABABEAYABAEAgABIAAEwgEBMABHGCAJD5KrMBQSIhrBwYCQUtGRFKQohIRgCICFn1UpyeLQSk0xrCqBEQBANIkggIBAIAaRCCBAdTNdEFemMwUHlhSCBAjkiEECBAQAAAAAAAAAB3OR1Gy1kiUEOqiEIIGU==


formula: K.978 Fe1.334 Li.486 Al1.79 Si3.11 O11.09 (F.91 H1.09)
compound: Barbora mine, Krupka, Czech Republic
pub_title: Refinement of the crystal structure of zinnwaldite 2M_1
formula_title: <missing>
a: 5.292
b: 9.187
c: 19.935
alpha: 90
beta: 95.40
gamma: 90
cell_volume: 964.891
crystal_density: 3.081
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["KMi", "FeM1", "LiM1", "AlM2", "FeM2", "FeM3", "LiM3", "SiT1", "AlT1", "SiT11", "AlT11", "SiT2", "AlT2", "SiT21", "AlT21", "O1", "O11", "O2", "O21", "O3", "O31", "O4", "O41", "O5", "O51", "O-H", "F", "O-H1", "F1"]

atoms_x:
AAAAALDvDwCw7w8AELwuABC8LgCwtNL/sLTS/9BAHADQQBwAwMDj/8DA4//QuDoA0Lg6ADCrxf8wq8X/kHgaAJCp5P8ACDkAEJbI/6DGOQDQzcb/sKoOAHDV8f+AES0A8DfT/xC+HQAQvh0AwHbn/8B25/8=

atoms_y:
4HQFALADLgCwAy4AoOYjAKDmIwAAjdz/AI3c/4B+OACAfjgAYPvH/2D7x/8w9y0AMPctALDs0f+w7NH/4E85AFBRyP8QRS0AUGbR/6D/IwAAKdz/AEsyAODKzf9wJDQAgBjM/yDaIwAg2iMAkNPd/5DT3f8=

atoms_z:
QEIPAAAAAAAAAAAAkAEAAJABAAAw+P//MPj//9BUCADQVAgAUK73/1Cu9/8wXggAMF4IALC39/+wt/f/kFMDACDK/P9QTQMAQM38/7BeCgAwAvb/0P0JAID99f/ACAoAQKz1/zAYAwAwGAMAcPf8/3D3/P8=

atoms_occupancy:
QLE7AMACJADAehAAgO42AIAaBgCATicAAC8NAEBwMQDAmAsAwMYtAEBCDwDANzAAQNEMAABjLgAApg4AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AKBDIQBgxRsAoEMhAGDFGwA=

atoms_u_iso:
cKcBAEC1AABAtQAAwKgAAMCoAADQtgAA0LYAAHCUAABwlAAAQJwAAECcAABg0QAAYNEAAHBiAABwYgAAcN8AAICJAACwmgAAQLUAANAzAQCwSQEAQEsBACAvAQCQLQEAoAkBAGBOAQBgTgEAgFEBAIBRAQA=

qdat:
AAAAAAAAAAEAAAAAAAAAAQBIgQgBBAAiIABAIAAmUIQIAjHBsCQBjQKMAFCQO21UVJiEG64nDNCLAigUOYX98qPQJgpbOeYzUZKvnNnh1/22UnqHVK+dipa7Gup1YbSvq1ywyKZIhVh+xmpTXWjqoXbei7ImIYgiLytKi4==


formula: Na3 Y C3 O12 H6
compound: <missing>
pub_title: Crystal structure of shomiokite-(Y), Na3Y(CO3)3*3H2O
formula_title: <missing>
a: 17.358
b: 10.034
c: 5.946
alpha: 90
beta: 90
gamma: 90
cell_volume: 1035.616
crystal_density: 2.514
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["Na1", "Na2", "Na3", "Y", "C1", "C2", "C3", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "Ow1", "Ow2", "Ow3", "H1", "H2", "H3", "H4", "H5", "H6"]

atoms_x:
cKEbAPAcFgDA9AQAIOAJAHBoGAAgqhIAIMwEAJALDwAwzQIAIDYEAGCnBwCANAoAEB8SAGB/FgAAyBkAgLUaAFD8AwBQwA0A8MILAIA4AQCAqQMAgG0NAECzEQCA/AoAAKYOAA==

atoms_y:
wNMWAJCACACAih0A0N4KAFBTGwAguwsAsEIXAOBkEAAguRwAEGMPAMDgGACgQQAAgBQHAIAoDAAAGBUAwHEeAIBtDQCAzBIAEAgBAEBgCgCAbQ0AwOsSAMBcFQAAcQIAgMf+/w==

atoms_z:
oNI3AGDXGADwPBkAkK4qAOAVGQAAqjcAYBc4AAAVOwBAEwIAIGk6AMBDLgDgxjoAAGktAKCGAQBA3B8AoDIPAOAVGQCg9hgAwMcYAIATHACA3g8AQEIPAECVFgBA0QwAgKIZAA==

atoms_u_iso:
4IwBAEDIAQDgjAEAsMwAACAWAQAwPQEAIBYBAEBkAQCAUQEAgFEBAJB4AQCAUQEA8LMBAKCfAQBAZAEAQGQBAKCfAQAAPwIAsCoCAMBRAgDAUQIAwFECAMBRAgDAUQIAwFECAA==

qdat:
AAAAAAAAAAAAgAAAgAAAFKABQAIKgBADhEAQ2TCEYrSMhOB1bINsElW8pUxvbWr/5cwckvXf7f8fUs19Vvz/rc19HM/s7Pf/s/+3+z+4t////9/Ld78z6299/X3vZzu53t6q9n78rXrHJ98+Ndt9nqtc1Lf0/RtxujvJ7P==


formula: Cs.968 Fe3.824 Si3.124 O12 H2
compound: <missing>
pub_title: Cs-ferriannite as a possible host for waste cesium: crystal structure and synthesis
formula_title: <missing>
a: 5.487
b: 9.506
c: 10.826
alpha: 90
beta: 99.83
gamma: 90
cell_volume: 556.388
crystal_density: 3.724
atoms_sites: ["Cs", "FeM1", "FeM2", "SiT", "FeT", "O1", "O2", "O3", "O4", "H"]
atoms_x: AAAAAAAAAAAAAAAAoNgEAKDYBACwoQMAAAsTAMAtCABwGQgAoG4FAA==
atoms_y: gIQeAAAAAACgRhQAICsKACArCgAAAAAAcDoPALAsCgCAhB4AgIQeAA==
atoms_z: AAAAAICEHgCAhB4A4IkOAOCJDgAQMAsA8EULALA8GAAQeBgAQCoTAA==
atoms_occupancy: ABU7AAAPPADA7zsAIKsvAOBdDQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0
atoms_aniso_label: ["Cs", "FeM1", "FeM2", "SiT", "FeT", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: EFMBALBoAABAagAAMI4AADCOAABAkAIAIEICAKCMAABAnAAA
atoms_aniso_u22: UEABAABLAAAASwAAIIAAACCAAAAA9AEAQJACAAB9AABgbQAA
atoms_aniso_u33: ECEBAADIAACwzAAAUKoAAFCqAACAtQEAoIYBACDLAACgCQEA
atoms_aniso_u12: AAAAAAAAAAAAAAAA4Pz//+D8//8AAAAAYPD//wAAAAAAAAAA
atoms_aniso_u13: 8CMAABAnAADAEgAAQB8AAEAfAAAgAwAAwF0AAEAfAACgDwAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAEA4AABAOAAAAAAAAQKL//wAAAAAAAAAA
qdat:
AAAAAAAAABAAAAAAAAACAAoAQCAAAEABAAAABAKMIEAAkwIgwQIIEhAABwLzEEDChIxEGgIgYkQJLkslmHOwFQgOew4gDMsdMF1uHhKVKw0bqGatiL5I5q/MsZxV7s6xtzihQCX89Yn8Tc8R7lMNUaLY3BC01+EU43OmlF==


formula: Al3 Si2 O10 H3
compound: <missing>
formula_title: Al3Si2O7(OH)3
a: 6.0885
b: 7.2832
c: 7.7234
alpha: 115.71
beta: 88.85
gamma: 92.89
cell_volume: 308.186
crystal_density: 3.234
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Al3Si2O7(OH)3, phase Pi (formerly piezotite): Crystal structure
 of a synthetic high-pressure silicate rediscovered

atoms_sites:
["Al1", "Al2", "Al3", "Al4", "Al5", "Al6", "Si1", "Si2", "Si3", "Si4", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "O17", "O18", "O19", "O20", "H1", "H2", "H3", "H4", "H5", "H6"]

atoms_x:
8Kju/xBXEQCAXur/YFMVANDRCACw1vb/MCMWAFCF6f8wLvf/4EkIAABy7f/gkBEAsDkMAGB28v/QLen/YDoVAEC9BwDww/b/gDgaAFA55f+wIvv/cGkDAMCC5f+wmhkAEPYDAJA4+/+geBQA4Mvq/+AG9v8QbgkA4HodAEAq4f9wHf//AJz//8Cr8/9QHQsA

atoms_y:
cGwPAJCT8P9wYRUAMMfq/xDH9v/QNQkAIM8QAHBL7/+gMfL/QE4NAEDPHQAw5OH/sCP//+BgAADwiQgA8L33/1AC6v+gOhYAQJMOADA/8P8gEvH/gMsOAPCjDADAG/L/UIDu/1D5EAAgjBcAQADo/wAR+f+QvgYAkGAFAKCw+v9Q++b/ABkZAEDK8P/AuA4A

atoms_z:
QIn//8B2AABwHRgAgAbo/8D/FwAwp+f/0Cju/4CHEQAA7+3/wNgRACATDgDQKfL/8BoOACDB8f9wXgkAILz2/4AhCQBwnvb/EJz5/0DJBQDgIPr/8BgGAACo5P/AcBoAUGvl/+C+GgBgcxgAEO/n/1B+GACAH+j/QPYKADAI9f8gwQoA4CX1/xAa/v9A4QEA

atoms_u_iso:
IE4AACBOAACAPgAAgD4AAPA8AADwPAAAIDUAACA1AACwNgAAsDYAAFBGAABQRgAAYDsAAGA7AACAPgAAgD4AAFBGAABQRgAAIE4AACBOAACwTwAAsE8AAMArAADAKwAAMEMAADBDAABgOwAAYDsAALA2AACwNgAAABJ6AAASegAAEnoAABJ6AAASegAAEnoA

qdat:
AAAAAAAAAAAAAAAggQAAAABAgAIAAAQBgAGAAiCCBAADBRABoAACERpBRgCJYAiDEDCgLMEmgAvIQZBFReFIkLVVYDdLhTAvbddgsE4M24VviGLlVS+BQcu2d2KB7s0r7nhdhvj4Tdf/z41XZ+rL3//W3JuiU0jX7/747y==


formula: Ca4 Mn3 B3 C O15
compound: <missing>
formula_title: <missing>
a: 10.589
b: 10.589
c: 5.891
alpha: 90
beta: 90
gamma: 120
cell_volume: 572.044
crystal_density: 3.539
atoms_sites: ["Ca1", "Ca2", "Mn", "B", "C", "O1", "O2", "O3", "O4"]
atoms_x: VVgUAKgJCAAAAAAAsEwNAAAAAADgpgUAkFcTAGB+EgBgQgMA
atoms_y: q7AoAODJMgCAhB4A0OcuAAAAAADw2RwAgOg3ACDSHADgvzcA
atoms_z: QEIPAEBCDwAAAAAAwMYtADBEBABAQg8AwMYtAHAyIQCgBSMA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AICEHgAACT0AAAk9AAAJPQCAhB4A
atoms_u_iso: gHAAAJB+AADgRwAA4GAAAICJAAAQWQAAkJcAALCBAACQyQAA
atoms_aniso_label: ["Ca1", "Ca2", "Mn", "B", "C", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: gFcAAKBzAACgQQAAUEYAAKCMAADQUgAAsJoAALBoAACgCQEA
atoms_aniso_u22: gFcAAGBtAADgRwAAoFoAAKCMAABAgwAAMFwAAJDJAADA2gAA
atoms_aniso_u33: gKIAAJCXAAAQQAAAQIMAAAB9AADgRwAAILIAAABkAAAgywAA
atoms_aniso_u12: wCsAACA1AAAAGQAAMCoAAOBHAADARAAAoCgAAIBXAACQsAAA
atoms_aniso_u13: AAAAAAAAAADQ8///AAAAAAAAAAAAAAAAAAAAACADAABgIgAA
atoms_aniso_u23: AAAAAAAAAAAQBAAAAAAAAAAAAAAAAAAAAAAAAJABAABw/v//
pub_title:
 Structure refinement of (001) disordered gaudefroyite Ca4Mn3[(BO3)3(CO3)O3]:
 Jahn-Teller-distortion in edge-sharing chains of MnO6 octahedra

qdat:
AAAAAAAAAAAEAAAAAAABAQBAAACAAgQAAAQkAICECQIIBCCAApAAJQMIBRgJIYg8AAoIEURahlDAA4xTiZZgUATEo2C5qdAcwKxcmdB5KzbuHodV9j+XwOj2v76F9ll+ujqm1snhlZJ++N2qnWwr/e6k2dkyYPz//aTTN4==


formula: Si12 Al12 O60 Ca5 Cl2.9 F.1 K2.36 Na8.64 S3
compound: <missing>
formula_title: <missing>
a: 12.8013
b: 12.8013
c: 21.4119
alpha: 90
beta: 90
gamma: 120
cell_volume: 3038.743
crystal_density: 2.528
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of afghanite, the eight-layer member
 of the cancrinite-group: evidence for long-range Si,Al ordering

atoms_sites:
["Si1", "Al1", "Si2", "Al2", "Si3", "Al3", "Si4", "Al4", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "Ca1", "Ca2", "Ca3", "Ca3a", "Ca4", "Ca4a", "Cl1", "Cl2", "Cl3", "F", "K1", "Ca1", "Na1", "K1a", "Ca1a", "Na1a", "K2", "Ca2", "Na2", "K3", "Ca3", "Na3", "K4", "Ca4", "Na4", "K4a", "Ca4a", "Na4a", "S1", "S2", "S3", "OS1a", "OS1b", "OS1c", "OS1d", "OS2a", "OS2b", "OS3a", "OS3b", "OS3c"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAAAAAAFCAACAAIEBkAKAAgkRQJohCiC9kAlU4VUsOsmEVZX21vWLSXWt7/L3HktbC9ulPpT9+7+nVH7+n+1/XG3y+68fv8/z+v3f94+du5/7fbY15037KkmF3d50uZEF8/mUKChIf04xJEQiPtCYEKAgXREQQICAiiA==


formula: Mn1.193 Cr1.807 O4
compound: <missing>
formula_title: <missing>
a: 8.4466
b: 8.4466
c: 8.4466
alpha: 90
beta: 90
gamma: 90
cell_volume: 602.623
crystal_density: 4.927
atoms_sites: ["MnT", "MnM", "CrM", "O"]
atoms_x: IKEHAICEHgCAhB4AMB8QAA==
atoms_y: IKEHAICEHgCAhB4AMB8QAA==
atoms_z: IKEHAICEHgCAhB4AMB8QAA==
atoms_occupancy: AAk9ANDjBQAwJTcAAAk9AA==
atoms_u_iso: sIEAAEBqAABAagAA0IQAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and cation distribution in some
 Mn-rich natural and synthetic spinels
 Sample: SPN255

qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAQAAAAAAAEAAAAgAAAAACAAAEAAAAAQAAIAAAAIAAIAAABAAEAAABAAQAAAQAEAAAQAIAABAAgAAIAIAAEAIAAEAIAAAAgABAEAAQAgAEAQABAIABAIAAAIACAQAAB==


formula: Mg.736 Mn.284 Fe1.911 Zn.017 Al.049 O4
compound: <missing>
formula_title: <missing>
a: 8.4075
b: 8.4075
c: 8.4075
alpha: 90
beta: 90
gamma: 90
cell_volume: 594.293
crystal_density: 4.620
atoms_sites: ["MgT", "MnT", "FeT", "ZnT", "MgM", "AlM", "FeM", "MnM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgCguQ8A
atoms_y: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgCguQ8A
atoms_z: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgCguQ8A
atoms_occupancy: YFsDACCQDgCgDSoAUA4BAHDLFABAfQEAAE4lAEBkAQAACT0A
atoms_u_iso: EFkAABBZAAAQWQAAEFkAAKBaAACgWgAAoFoAAKBaAAAQiwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and cation distribution in some
 Mn-rich natural and synthetic spinels
 Sample: JBS1

qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAQAAAAAIAAAAAAABAAAAIAAAAAAgAACAAAAAEAACAAAABAACAAAAIAAgAAAQACAAACAAgAACABAAAIAEAABABAAAgAgAAgBAAAACAAEAQABAEAAIBAAEAgAEAgAAAgAEBAAA==


formula: Mg.475 Mn.446 Fe2.068 Zn.006 Ti.002 O4
compound: <missing>
formula_title: <missing>
a: 8.4454
b: 8.4454
c: 8.4454
alpha: 90
beta: 90
gamma: 90
cell_volume: 602.366
crystal_density: 4.764
atoms_sites: ["MgT", "MnT", "FeT", "ZnT", "MgM", "FeM", "MnM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgBAyQ8A
atoms_y: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgBAyQ8A
atoms_z: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgBAyQ8A
atoms_occupancy: AJABAAA4GACg0yIAMFwAAPC2DQDgsC0A8IEBAKAPAAAACT0A
atoms_u_iso: EIsAABCLAAAQiwAAEIsAAOCSAADgkgAA4JIAAOCSAAAgsgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and cation distribution in some
 Mn-rich natural and synthetic spinels
 Sample: JBS3

qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAQAAAAAAACAAAAgAAAAACAAAEAAAAAQAAIAAAAEAAIAAAAgAEAAABAAQAAAQAEAAAQAIAAAgAgAAIAIAAEAIAAEAIAAAAgABAEAAQAgACAQABAIABAEAAAIACAQAAB==


formula: Mg.129 Mn.832 Fe2.004 Zn.007 Al.03 O4
compound: <missing>
formula_title: <missing>
a: 8.4956
b: 8.4956
c: 8.4956
alpha: 90
beta: 90
gamma: 90
cell_volume: 613.172
crystal_density: 4.896
atoms_sites: ["MgT", "MnT", "FeT", "ZnT", "MgM", "AlM", "FeM", "MnM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgAg7g8A
atoms_y: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgAg7g8A
atoms_z: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgAg7g8A
atoms_occupancy: YCkDAGDoKgCAmQ4AQGoAAJBZAgBA5wAA8Nk1AGDxAwAACT0A
atoms_u_iso: UKoAAFCqAABQqgAAUKoAABCkAAAQpAAAEKQAABCkAAAQvQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and cation distribution in some
 Mn-rich natural and synthetic spinels
 Sample: JBS4

qdat:
AAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAABAAAAABAAAAAAAAIAAACAAAAAAIAAAgAAAACAABAAAAAgABAAAAIAAgAAAIACAAACABAAACABAAAQAIAACAEAABACAACAEAAAAQAAgCAAEAQACAIABAEAAgEAAAEABAQAAAg==


formula: Mn.339 Fe2.266 Zn.298 Mg.019 Al.057 Ti.025 O4
compound: <missing>
formula_title: <missing>
a: 8.4576
b: 8.4576
c: 8.4576
alpha: 90
beta: 90
gamma: 90
cell_volume: 604.980
crystal_density: 5.090
atoms_sites: ["MnT", "FeT", "ZnT", "MgM", "AlM", "FeM", "MnM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgA49A8A
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgA49A8A
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgA49A8A
atoms_occupancy: wDwSAJC2GACQKxIAcJQAADC6AQCAyTgA8DYBAFDDAAAACT0A
atoms_u_iso: wI8AAMCPAADAjwAAUJEAAFCRAABQkQAAUJEAAFCRAABAnAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and cation distribution in some
 Mn-rich natural and synthetic spinels
 Sample: FRK1b

qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAgAAAAAAAEAAAAgAAAAACAAAIAAAAAgAAQAAAAIAAQAAABAAIAAACAAQAAAgAIAAAgAQAACABAAAQAQAAIAQAAQAgAAACAACAIAAQCAAIAgAEAQACAQAAAgAEBAAAC==


formula: (Mg.142 Al1.773 Mn.815 Fe.27) O4
compound: <missing>
formula_title: <missing>
a: 8.2226
b: 8.2226
c: 8.2226
alpha: 90
beta: 90
gamma: 90
cell_volume: 555.939
crystal_density: 4.185
atoms_sites: ["MgT", "AlT", "MnT", "FeT", "MgM", "AlM", "FeM", "MnM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgDoLxAA
atoms_y: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgDoLxAA
atoms_z: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgDoLxAA
atoms_occupancy: 0CgHAJD7AAAQfCgAkGgMADDAAABwmzUAcAsCAPChBAAACT0A
atoms_u_iso: IGcAACBnAAAgZwAAIGcAABBZAAAQWQAAEFkAABBZAACAiQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry and cation distribution in some
 Mn-rich natural and synthetic spinels
 Sample: SPN258

qdat:
AAAAAAAAAAAAAAAAAAAAAAgAAAAAAAAAAAAAgAAAAAIAAAAAAAAgAAAEAAAAAAIAAAQAAAAAgAAIAAAAEAAEAAAAQAAgAAAIABAAABAAQAAAgAIAAAgAgAAEAEAABACAABACAAAACAAEAIAAQCAAEAQABAEAAgCAAACAAQ==


formula: Pb2 Fe Cl3 (O5 H6)
compound: Tuscany, Italy
formula_title: Pb2FeCl3(OH)4.H2O
a: 8.033
b: 6.253
c: 9.221
alpha: 90
beta: 102.98
gamma: 90
cell_volume: 451.339
crystal_density: 4.876
atoms_sites: ["Pb1", "Pb2", "Fe", "Cl1", "Cl2", "Cl3", "O-H1", "O-H2", "O-H3", "O-H4", "Wat5"]
atoms_x: 4KUzAFBqEwDA4P//oFwIAKCcJwBgQhwAoCf8/wBrAwAgEgoAoFAKAICcGgA=
atoms_y: 0AQNADCYDwCAih0AIPoNAEDLDQCgYRwAYLkdAED6GgCghCsAYBMPAMD7OQA=
atoms_z: QFcxAPCNMQCg0h4AQIoDAKD3AwBg6RUAQDASAICtLABgNh4AAEAfAIBVEQA=
atoms_occupancy: 0
atoms_u_iso: YDUBALBiAQCgCQEAgDgBAMBXAQAA9AEAoA8AAAB3AQDgqwAAwFcBACA8AwA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Pb2FeCl3(OH)4.H2O, a newly discovered natural phase from Tuscany,
 Italy: physio-chemical data, crystal structure, and OD character

qdat:
AAAAAAAAAAACAIAAAAACIEAIABBACIAEAFAmgABQRADEUAiIMECOoEgMQobqD4CyJQJysp1tYYxDwv0CaOyLvK91X2xKnSOVt7edt9vSvM5x+d2n1btT8v/Pf/+H/v/m/3u1/7/v3/OHd5n29/f/nevf//33/9r59/VMpd==


formula: Ca.175 (Al.354 Si.646) O2.86 H1.72
compound: Synthetic
formula_title: <missing>
a: 9.873
b: 9.873
c: 10.288
alpha: 90
beta: 90
gamma: 90
cell_volume: 1002.834
crystal_density: 2.178
atoms_sites: ["Ca", "AlT", "SiT", "O1", "O2", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5"]
atoms_x: AAEEAKDEJwCgxCcA8AgqAABDKwAg0f//QBMCAECcAAAgywAA4LH//w==
atoms_y: EFQFAKCRIwCgkSMAYA4tACBPHQCgMDkAQHYwAKDXMgDAnR8AYAwlAA==
atoms_z: QJMnALDEJgCwxCYA4AUkADDOHwBgsx4AYL8cAOBiIQBAdxsAYFQZAA==
atoms_occupancy: YK4KAECbFQDAbScAAAk9AAAJPQDAtgYAAFMHAIBPEgDAJwkAgPwKAA==
atoms_u_iso: YFsDABC9AAAQvQAAsBECABDQAQDARQQAwCcJAMC2BgAA4gQAAMQJAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure analyses of a partially dehydrated synthetic
 Ca-garronite single crystal under different T, pH2O conditions
 Sample: GAR25/20, T = 25 C, 60% relative humidity

qdat:
AAAAAAAAAAAAAACAAAAAAQAAAJAAAAgAIIAAAACUCAIARBAEAoCAgIgAQBhAgQFCBYAwCCAJkEElELkAJEQuRATEJAhZMEbC2wdMSUHpClgwxRR6wTpcxHS1gtHGA8GARhwKIqgrCEIg0BASAoxBwJgEAAAEAQqEAAAAAA==


formula: (Al.354 Si.646) O2.86 Ca.175 H1.72
compound: Synthetic
formula_title: <missing>
a: 9.912
b: 9.912
c: 10.303
alpha: 90
beta: 90
gamma: 90
cell_volume: 1012.247
crystal_density: 2.158
atoms_sites: ["AlT", "SiT", "O1", "O2", "Ca", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5"]
atoms_x: oOcnAKDnJwDw7ykAsC4rAID0AwAg0f//wFcBAAB9AABg6gAAIFT//w==
atoms_y: CMAjAAjAIwDgTC0A8LodADBXBQBAwzgAoOMwACCZMgDgbh8A4M0kAA==
atoms_z: eI4mAHiOJgAA8CMAAFkfAIBOJwBgsx4AAM8cAMAOIgBAdxsAIDsYAA==
atoms_occupancy: QJsVAMBtJwAACT0AAAk9AGCuCgDAtgYAAFMHAIBPEgDAJwkAgPwKAA==
atoms_u_iso: EL0AABC9AAAA9AEA8MwBAMDIAwDARQQAQGAKAICLCABAfgUAwLYGAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure analyses of a partially dehydrated synthetic
 Ca-garronite single crystal under different T, pH2O conditions
 Sample: GAR25/27, T = 25 C, 80% relative humidity

qdat:
AAAAAAAAAAAAAACAAAAAAQAAASAAABAAIIAAAAEUCAIAiBAQBQEAgRAAgDCBAgJMFgBgEEASoISqYbQAiJC4mBKQiCFiwRkTVhURVorUVKGjIlGlBVHzIKPUD00QCgwDELBQkqCoohGFQIGIFLIKBIBAAABACFggAAAAAA==


formula: (Al.708 Si1.292) O4.888 Ca.354 H1.776
compound: Synthetic
formula_title: <missing>
a: 9.790
b: 9.790
c: 9.097
alpha: 90
beta: 90
gamma: 90
cell_volume: 871.894
crystal_density: 2.279
atoms_x: yFsiAMhbIgCQyyYAkMsmAFCOJgBQjiYA8B8iABDrIgBwOSQAAMohAHD7DADQGBIAoHwLACBxDwAAxAkA
atoms_y: yFsiAMhbIgCACAQAgAgEALB6FgCwehYAkHwqAJB/BADQbgwAYNEZAFCfOAAgxzsAANkSAECnEwAAIw8A
atoms_z: AAAAAAAAAADwOxUA8DsVAEBCDwBAQg8A0MQGAHCJHwBAjQ8AoB0GABC5CQDguw4AoJk0AKC5NwBA2zQA
atoms_occupancy: QJsVAMBtJwBAmxUAwG0nAECbFQDAbScAAAk9AAAJPQAACT0AAAk9ACBxDwAgKgYAADM2AAAzNgAAMzYA
atoms_u_iso: ENYAABDWAACA1AAAgNQAAKDwAACg8AAA8P4BAHDZAQAwHgIAwAYCAIC1AQCAJgQAgKMEAICLCACAiwgA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure analyses of a partially dehydrated synthetic
 Ca-garronite single crystal under different T, pH2O conditions
 Sample: GAR145/27, T = 145 C, 27 mbar pH2O

atoms_sites:
["AlT1", "SiT1", "AlT2", "SiT2", "AlT3", "SiT3", "O1", "O2", "O3", "O4", "Ca1", "Ca2", "OW", "H1", "H2"]

qdat:
AAAAAAAAAAAAAAASAAAAAIAAoIEEAAIAARgCQAkESghAYsgRMSBBAUGygSVwkIpLWxuSGsmOPTBL3Vu6Educvcbo1tFZ7uP6b/avBP730b/1/2323C93/kl+9lu5eu1tbf7pXupi3t8o69WTPiavkqp8r9AooU6zoBRQI4==


formula: Na1.18 Mg4.35 Mn.87 Al1.24 Ca1.41 Si6.92 O22 F2
compound: <missing>
formula_title: <missing>
a: 9.829
b: 18.024
c: 5.284
alpha: 90
beta: 104.66
gamma: 90
cell_volume: 905.627
crystal_density: 3.135
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The behaviour of Mn in amphiboles: Mn in synthetic
 fluor-edenite and synthetic fluor-pargasite
 Sample: MFE

atoms_sites:
["NaA", "NaAm", "NaA2", "MgM1", "MnM1", "AlM2", "MgM2", "MnM2", "MgM3", "MnM3", "MnM4", "CaM4", "NaM4", "MnM4*", "CaM4*", "NaM4*", "SiT1", "AlT1", "SiT2", "O1", "O2", "F3", "O4", "O5", "O6", "O7"]

atoms_x:
AAAAABCxAgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACBCEQAgQhEA8LwRAMjHBgCwVwcAYGIGALhPFgDYWBUACCkVANgNFQA=

atoms_y:
gIQeAICEHgDg5BwAqGsFAKhrBQDAywoAwMsKAMDLCgAAAAAAAAAAAEjUEABI1BAASNQQAGBjDwBgYw8AYGMPAOAkBQDgJAUAIHYKAAgvBQCYbAoAAAAAAKgvDwAAUggAMBQHAAAAAAA=

atoms_z:
AAAAAABABgAAAAAAgIQeAICEHgAAAAAAAAAAAAAAAAAAAAAAAAAAAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeABAzEgAQMxIAQBsxAIBUDQAAUSwAAH8rABDtLwBgKwYAoJAkAHAQEQA=

atoms_occupancy:
ADUMAAA1DAAANQwAIHU4AOCTBAAA4gQAAGMuAADECQCA0DsAgDgBAIAaBgDgqhUAAHECAEB+BQDAXBUAQA0DAECOLADAehAAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
uPABABjNAQCo9gEA0HAAANBwAACgggAAoIIAAKCCAAC4dAAAuHQAAIjlAACI5QAAiOUAAIiQAACIkAAAiJAAAAhhAAAIYQAAuHQAAKCCAABgmgAAGLAAAMjXAACo2QAAqNkAAPDDAAA=

qdat:
AAAAAAAAAAACEAAAAAAAGAgUBAIAAAAggGBCAICAEwUEgMEQsBBUslIIQKwwCP8GgPgaMxucBAzJDsGgBB6EdybYx0RQHxyIyLQOfuIrok5SSbS2kPAFGv5NgvrMEh/qQ9acNAXa6QYsCwE7hpC3UOHk5sn7RFgDPLwK8F==


formula: Na.87 Ca1.65 Mg3.38 Mn1.24 Al2.85 Si6.01 O22 F2
compound: <missing>
formula_title: <missing>
a: 9.812
b: 17.926
c: 5.308
alpha: 90
beta: 105.10
gamma: 90
cell_volume: 901.388
crystal_density: 3.213
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The behaviour of Mn in amphiboles: Mn in synthetic
 fluor-edenite and synthetic fluor-pargasite
 Sample: MFP

atoms_sites:
["NaA", "CaA", "NaAm", "CaAm", "NaA2", "CaA2", "MgM1", "MnM1", "AlM2", "MgM2", "MnM2", "MgM3", "MnM3", "MnM4", "CaM4", "MnM4*", "CaM4*", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "F3", "O4", "O5", "O6", "O7"]

atoms_x:
AAAAAAAAAACgsgIAoLICAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgRxEAIEcRACjfEQAo3xEAyJAGAKBJBwBwZgYAKIoWAIiKFQC4HhUAeP8UAA==

atoms_y:
gIQeAICEHgCAhB4AgIQeADjTHAA40xwAIIAFACCABQAIwAoACMAKAAjACgAAAAAAAAAAAGAHEQBgBxEAkDcQAJA3EACgNwUAoDcFAEiPCgBIjwoAOFkFAJiPCgAAAAAAmFgPACiYCABAHQcAAAAAAA==

atoms_z:
AAAAAAAAAADQFQYA0BUGAAAAAAAAAAAAgIQeAICEHgAAAAAAAAAAAAAAAAAAAAAAAAAAAICEHgCAhB4AgIQeAICEHgDocxIA6HMSAMCaMQDAmjEA0B0NALjZLAAoeisA2AEwADjfBgDIJiUAeMcQAA==

atoms_occupancy:
wJ4KAECWAQDAngoAQJYBAMCeCgBAlgEAAEUzAADECQDAPhoAgDEXAMCYCwCAXzkAgKkDAABTBwCAMRcAAFMHAIAxFwAgCyAA4P0cAHCpOwCQXwEAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==

atoms_u_iso:
aK8BAGivAQAQ1QEAENUBAGgOAgBoDgIAsHwAALB8AAD4ZgAA+GYAAPhmAADYcgAA2HIAACiqAAAoqgAA6MsAAOjLAAD4XAAA+FwAANBwAADQcAAAOKQAAFCgAADowQAAuNMAANjRAACA7QAA2NEAAA==

qdat:
AAAAAAAAAAACEAAAAAAAGAQMAgIAAAAwQDAiAEBAFkMCQKCgKAgqSLCEIC0UBN8BoLoMWYbOAQYqZyj4ASeCG0F9I9xMB8eRmUqC983K5Sn8od2beyYEq/9l0HqylgtUpPS0VkFX1UcGxaG8ooUcoRtEqPsmwFCAd45L8Q==


formula: (K.986 Na.014) (Al1.03 Si2.97) O8
compound: <missing>
pub_title: A high-pressure structural study of microcline (KAlSi3O8) to 7 GPa P = 0.0 GPa
formula_title: <missing>
a: 8.5733
b: 12.9375
c: 7.2075
alpha: 90.530
beta: 115.972
gamma: 87.968
cell_volume: 718.229
crystal_density: 2.572
atoms_x: EFcRABBXEQBgnwAAYJ8AAICJAACAiQAAkF0rAJBdKwBQJSsAUCUrAJAaAADACScAsB0yAEDOMgAwHgIAAFgCAMB/CwCAygoA
atoms_y: EJH//xCR//8QewsAEHsLAGDwMQBg8DEAYFwHAGBcBwAAGjYAABo2AOCUCAAgTgAAMCYJAOA7NADgnRMAADAqANClBwDAGTUA
atoms_z: 8FcIAPBXCABATg0AQE4NADAhDgAwIQ4AUMgUAFDIFAAQWBUAEFgVALAK//8wcxEAUHUNAMCGDgAgcQ8AwGEQAFCwGABgCRkA
atoms_occupancy: QC48AMDaAAAAnjkAAGsDAIAmBACA4jgAoIwAAGB8PACgjAAAYHw8AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 2IUBANiFAQAwAQEAMAEBADABAQAwAQEAMAEBADABAQAoCQEAKAkBAFhWAQDAKgEA0IMBAJCbAQAwYAEAkEYBALA6AQB4SgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["KM", "NaM", "AlT1o", "SiT1o", "AlT1m", "SiT1m", "AlT2o", "SiT2o", "AlT2m", "SiT2m", "Oa1", "Oa2", "Obo", "Obm", "Oco", "Ocm", "Odo", "Odm"]

qdat:
AAAAAAAAQAAAACAEQAgABABAIIIUQSAQIICBwRAAfMItACGQmQkySA7lWBRIME85z1Xg3ogKxfurnTskP3+2dOz/ar/4o3k5xvdPz2/vzKR89vjT+/3/a/Wu3vvTPl9v/e7/e7Q//3ff3peP4k+7lv/u3/8/91n5D/b/9Z==


formula: (K.986 Na.014) (Al1.03 Si2.97) O8
compound: <missing>
pub_title: A high-pressure structural study of microcline (KAlSi3O8) to 7 GPa P = 1.4 GPa
formula_title: <missing>
a: 8.4812
b: 12.930
c: 7.1784
alpha: 90.436
beta: 116.163
gamma: 87.97
cell_volume: 706.072
crystal_density: 2.616
atoms_x: gAoRAIAKEQDAXQAAwF0AAOBgAADgYAAA0BgrANAYKwBQ2ioAUNoqAPAjAABgaiYA0NUxAEBqMgCg0QEA8P4BAMCYCwDQrAoA
atoms_y: cLP//3Cz///gggsA4IILAKAPMgCgDzIA0FoHANBaBwBQFTYAUBU2ACCbCABghgAAsAAJALCONACgfhMAYDkqAFCABwDgTjUA
atoms_z: wF8IAMBfCAAASA0AAEgNACATDgAgEw4AsLgUALC4FADwOxUA8DsVAAAf///gdxEAcEYNAFA9DgAQfA8AcH8QACDRGABwMBkA
atoms_occupancy: QC48AMDaAAAAnjkAAGsDAIAmBACA4jgAoIwAAGB8PACgjAAAYHw8AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: cLEBAHCxAQAgEQEAIBEBAEAFAQBABQEAOAMBADgDAQD4GgEA+BoBAChoAQBwUgEAoEABAMjqAQCAQgEAMGABAFBeAQD4eQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["KM", "NaM", "AlT1o", "SiT1o", "AlT1m", "SiT1m", "AlT2o", "SiT2o", "AlT2m", "SiT2m", "Oa1", "Oa2", "Obo", "Obm", "Oco", "Ocm", "Odo", "Odm"]

qdat:
AAAAAAAAQAAAABACYAQABABAIEEEERAEEEBAwCQAFZINQCBYToi+CQMszBZZFCTR93jaH3SAfDnvPvOzJ2fG+ba+8/n5R+atvfvcef/8cMd37h7Vvv/V+J3v2e/fp7W/f7119+rJv//2fv3dPv2v1+nv79f7Z+2dOh/+//==


formula: (K.986 Na.014) (Al1.03 Si2.97) O8
compound: <missing>
pub_title: A high-pressure structural study of microcline (KAlSi3O8) to 7 GPa P = 2.9 GPa
formula_title: <missing>
a: 8.3722
b: 12.899
c: 7.1328
alpha: 90.38
beta: 116.290
gamma: 87.93
cell_volume: 690.128
crystal_density: 2.676
atoms_x: AMwQAADMEACAJQAAgCUAANA5AADQOQAAoNUqAKDVKgDAjSoAwI0qAEDt//9gBiYAIDsxABAOMgAAdwEAkMMBAABUCwDgugoA
atoms_y: kJ3//5Cd//8giQsAIIkLAPDxMQDw8TEAcFEHAHBRBwBAIDYAQCA2AFDFCACQfgAA8AYJALCONADQdhMAQE8qACCIBwBgWzUA
atoms_z: YFYIAGBWCAAwQA0AMEANAODzDQDg8w0AILcUACC3FABANxUAQDcVAHAd//+QfBEAIOcMAODaDQBAjQ8AMKsQAJDPGACgKBkA
atoms_occupancy: QC48AMDaAAAAnjkAAGsDAIAmBACA4jgAoIwAAGB8PACgjAAAYHw8AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: eKkBAHipAQBABQEAQAUBAAgVAQAIFQEAQPsAAED7AAAgEQEAIBEBAIBCAQBwUgEAGG4BANjkAQBwpwEAgEwBAMiLAQAwagEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["KM", "NaM", "AlT1o", "SiT1o", "AlT1m", "SiT1m", "AlT2o", "SiT2o", "AlT2m", "SiT2m", "Oa1", "Oa2", "Obo", "Obm", "Oco", "Ocm", "Odo", "Odm"]

qdat:
AAAAAAAAQAAAAAgBIAQAAgAgIBBDBQQBGCBgYASADlsCKBAWGaQKgKHJ36mhYpE9J87Nlf0UHw6J/uW/E9z73UNrK89j4y/8j3Wftjeb/62+7/Drwvv+3vHvffLu7a7/fn759/fqn38v/99/p/ef/b/HX776V9n9vnafv9==


formula: (K.986 Na.014) (Al1.03 Si2.97) O8
compound: <missing>
pub_title: A high-pressure structural study of microcline (KAlSi3O8) to 7 GPa P = 4.4 GPa
formula_title: <missing>
a: 8.276
b: 12.878
c: 7.0936
alpha: 90.38
beta: 116.372
gamma: 87.89
cell_volume: 676.845
crystal_density: 2.729
atoms_x: oHcQAKB3EAAg6v//IOr//9Du///Q7v//EIkqABCJKgCwTSoAsE0qACADAABAnyUA4OkwAMCVMQBgHAEAsGIBAHAHCwBwWAoA
atoms_y: YKX//2Cl///AfwsAwH8LAHAXMgBwFzIAgF8HAIBfBwCQGzYAkBs2AODfCADwhwAA0NEIAOBtNADgaxMA8DoqAKCUBwCAdzUA
atoms_z: MHcIADB3CABgOA0AYDgNABAFDgAQBQ4AAJsUAACbFACwNRUAsDUVALAj///wnhEAYHAMAEBODQAA0g8AAOUQAHDMGADwIxkA
atoms_occupancy: QC48AMDaAAAAnjkAAGsDAIAmBACA4jgAoIwAAGB8PACgjAAAYHw8AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: +HkBAPh5AQA4AwEAOAMBAAAdAQAAHQEA8BgBAPAYAQDQJAEA0CQBAMCJAQC4kQEAIGYBAHipAQBQswEA+HkBACBwAQDAkwEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAQAAAAAQAsAIAAQAgIAghIYIAkhAwKAEQDZNChggGTGoJ0BTUF+TQKSiWVVoqk2rQybVjb0aO8fXbPfjdqn92/pbt0b07t8Sn9+/O735rd/Pf/PTnnttX6mebv691+L1vzbv9X+8fv//P+/9/uN+//Put+utLvt==


formula: (K.986 Na.014) (Al1.03 Si2.97) O8
compound: <missing>
pub_title: A high-pressure structural study of microcline (KAlSi3O8) to 7 GPa P = 6.2 GPa
formula_title: <missing>
a: 8.1578
b: 12.8558
c: 7.0406
alpha: 90.49
beta: 116.616
gamma: 87.86
cell_volume: 659.648
crystal_density: 2.800
atoms_x: wC8QAMAvEABwmv//cJr//5Cd//+Qnf//MHMqADBzKgCgDSoAoA0qALBPAACADyUAwFAwADCzMABwrQAAsOUAALCQCgDg8gkA
atoms_y: gKj//4Co//+wowsAsKMLAEAGMgBABjIAEC8HABAvBwDQCDYA0Ag2AOD4CABQDgEAIP8IAHC6NAAwgBMAAK0qAECkBwDwjjUA
atoms_z: QJ4IAECeCADQHQ0A0B0NAPABDgDwAQ4AEJAUABCQFACwHBUAsBwVAJBS//8A3xEAQL4LAHCXDADQPRAAQDYRAADOGABgOxkA
atoms_occupancy: QC48AMDaAAAAnjkAAGsDAIAmBACA4jgAoIwAAGB8PACgjAAAYHw8AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: aK8BAGivAQBABQEAQAUBANgmAQDYJgEAoDYBAKA2AQCwMAEAsDABAEhcAQBQswEA+HkBAEBaAQCIowEAcLEBADBqAQBgrQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAQAAAAAIAKAEAAIAQEAIFCECAGIQUFgASBaqVEEIAhhUEPwDrAvY5AqYiw1Xx4+yjh5anLLMUPV/3jo8Tb4ln/k5/+8lb+vvEd+f1ov72STn3uv+/H5v9r78ot/vz+2y/u/5t591f7Oz7/b/fS/5PX7vzu+//vx==


formula: (K.986 Na.014) (Al1.03 Si2.97) O8
compound: <missing>
pub_title: A high-pressure structural study of microcline (KAlSi3O8) to 7 GPa P = 7.1 GPa
formula_title: <missing>
a: 8.0764
b: 12.8471
c: 6.9991
alpha: 90.548
beta: 116.830
gamma: 87.903
cell_volume: 647.584
crystal_density: 2.852
atoms_x: oMgPAKDIDwBwNv//cDb//zBJ//8wSf//ADAqAAAwKgCA2CkAgNgpAEAGAAAAAyUAMLkvAHAjMAAAZAAAQDIBADBrCgBgmwkA
atoms_y: UMn//1DJ///wqQsA8KkLABD1MQAQ9TEAcFEHAHBRBwAgHTYAIB02ABBVCQAQWQAAsBkJAECQNABQahMAAOUpAGB1BwAgoDUA
atoms_z: UMUIAFDFCABgBg0AYAYNAED9DQBA/Q0AUH0UAFB9FABANxUAQDcVAHAd///QtBEAsCYLAMAVDAAwqxAAMIwRAKDdGACgWhkA
atoms_occupancy: QC48AMDaAAAAnjkAAGsDAIAmBACA4jgAoIwAAGB8PACgjAAAYHw8AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: GG4BABhuAQBg+QAAYPkAANAkAQDQJAEAEA0BABANAQAQDQEAEA0BAJA8AQAI0wEAMGABAGBYAQDAkwEAkJsBAMiLAQAgZgEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAQAAAAAEAJACAAEAIEACCgVAgDEEREYAERKZCghiAY4NCDPAdgQ/bIDtQsK4uFD+0LVq9N2s4s/65+fxZ7vhvv2I1/a0t71ntw/7+6lvv5szpfcv/m3e9/Nf/+h7Nf/d63zvf140X2u+ff/d/G6/+mbvf/k/ftX==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.86145
b: 10.5839
c: 6.16980
alpha: 90
beta: 90
gamma: 90
cell_volume: 317.455
crystal_density: 4.245
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABANDsAQDQ7AAATGgBwky4A8AcNAICHEQA=
atoms_y: AAAAAAAAAADQNxEA0DcRALDgBQAwogUAwLUbAGD/CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAJBZAgA=
atoms_occupancy: QCMpAMDlEwBAIykAwOUTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: SEkAAEhJAABISQAASEkAAJgrAADobAAA+GYAAOhiAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 20 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAABwAAAAMYIAgRAIIQAoBYABqcAOoBAJCAKDHoCC6g7UKAWFQp0J5CKyFbLyaGSrT8aZqrFimfh3es23vZ72Sunwfr7/pfkJ+n7PRfat/71M8fI/z8l6b23/+k7d/xVO3P353l7==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.86394
b: 10.5915
c: 6.17510
alpha: 90
beta: 90
gamma: 90
cell_volume: 318.119
crystal_density: 4.236
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACAUzsAgFM7ALAXGgBghS4AQAMNADCMEQA=
atoms_y: AAAAAAAAAAAgZREAIGURANDjBQDAowUAoLIbABAECgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPANBfAgA=
atoms_occupancy: oBMpAGD1EwCgEykAYPUTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 8GQAAPBkAADwZAAA8GQAAChLAACIkAAAgI4AAHiMAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 100 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAIAQAAABwAAAAMYIAgRAIIQAoBYABycAPIBAKCAMDPoGC7ArYKAmFQpkTqELyF+P0yOS7S8SRLuLmm9ju3Y23/Rus0uvw+37/TbsL/NWaR+rv+35J8fY+35Gy//v+3k91/ztfdO/TunX==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.86743
b: 10.6011
c: 6.18226
alpha: 90
beta: 90
gamma: 90
cell_volume: 319.005
crystal_density: 4.224
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABggjsAYII7ACAWGgAQii4AsAENAHCSEQA=
atoms_y: AAAAAAAAAADgXhEA4F4RANDjBQBQpQUA4LgbAPAACgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAGBhAgA=
atoms_occupancy: YPQoAKAUFABg9CgAoBQUAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: mIoAAJiKAACYigAAmIoAAPhcAAAwrAAAOK4AADiuAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 200 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAIAQAAABQAAAAUYIAgSAIIgBIBwABSsAXIBAKCAMCPIGFWB1YUAsGgrsTyENiK+fk0Mkqn40xV+PNNfDu+otv+x3slbPg/d3/V/IX+P02je3Xuv3b4ez9f6X199f9vL7v7rWu6d63NP9==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.87189
b: 10.6134
c: 6.1905
alpha: 90
beta: 90
gamma: 90
cell_volume: 320.094
crystal_density: 4.210
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACgJDsAoCQ7ABAIGgDwhi4AYAYNABCJEQA=
atoms_y: AAAAAAAAAABweREAcHkRALDgBQBAsAUAcLobABAECgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAIBkAgA=
atoms_occupancy: QCMpAMDlEwBAIykAwOUTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: aJwAAGicAABonAAAaJwAANBwAADA1QAAuNMAAPDDAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 300 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAQAAADgAAAAUoIAgSAQYgBQCwADS4AdQBAUEAUGPQMF2BWokBMNBTYnkIXkT89EkdF3N4pi7eVKZ9Hd/R1e7n/ZJ+uhu/n+n+Yv8fstG9q9c7+/w9m+/Unr7+fbWTp/nW13d73u6m7==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.87650
b: 10.6249
c: 6.19849
alpha: 90
beta: 90
gamma: 90
cell_volume: 321.158
crystal_density: 4.196
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACgJDsAoCQ7ACAWGgCwgC4AQAMNAFCPEQA=
atoms_y: AAAAAAAAAABQjxEAUI8RALDgBQBgswUAIL8bABAECgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPABBmAgA=
atoms_occupancy: QCMpAMDlEwBAIykAwOUTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: GLoAABi6AAAYugAAGLoAALh+AABo8QAAYPkAAHjrAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 400 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAADgAAAAUoQAgiAQYgBQCwADk4AeQCAUEAYGeQMLmDVQoBINBnQnkIrMX4vJopLtXxpEu8aab+O7ej7d/P+qS69D8/P9PuxX4/R6F7f75n5th5P2+o3X3163srv/utqq566d419==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.87826
b: 10.6312
c: 6.20213
alpha: 90
beta: 90
gamma: 90
cell_volume: 321.653
crystal_density: 4.189
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAg5joAIOY6AOAPGgBQdy4AoAwNAMCNEQA=
atoms_y: AAAAAAAAAAAQohEAEKIRANDjBQCwrgUAQMIbAPAACgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAFBsAgA=
atoms_occupancy: YHEpAKCXEwBgcSkAoJcTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: kN0AAJDdAACQ3QAAkN0AAIiQAABABQEACBUBAED7AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 450 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAADgAAAAYwQAgiAQQgCQDwADlYAuQCAUEAYMeQILsDtQoBYVBmwnoQvMX5+RIpLOfzLF24qy16O7Wj2/7P+qV99D5/f9W9if4/R6NzVTrvZ9jzP+7JeX7V+n8u1/a5v3zv6Zo/7==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.88292
b: 10.6447
c: 6.21066
alpha: 90
beta: 90
gamma: 90
cell_volume: 322.813
crystal_density: 4.174
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAgaToAIGk6AGADGgBghS4A8AcNAKCKEQA=
atoms_y: AAAAAAAAAAAQ1BEAENQRACDfBQBgswUAsMAbABAECgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPALB1AgA=
atoms_occupancy: IM8pAOA5EwAgzykA4DkTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: SP0AAEj9AABI/QAASP0AADCsAADAKgEAoDYBAOggAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 550 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAACgAAAAowQBAkAQRACQFgAGlQA8gCAoIAoMsgYVMDtRICYqCuxPIRbYn5+TRaTKXjTJb5Ukr0d29H17uX9Ul66G6+f6tai3h+n0f2q9V+z/G0d++W83NffN1rv8uTe33b+3K3V==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.88544
b: 10.6499
c: 6.21456
alpha: 90
beta: 90
gamma: 90
cell_volume: 323.340
crystal_density: 4.167
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAg5joAIOY6AOAPGgDAdS4AYAYNAOCQEQA=
atoms_y: AAAAAAAAAAAwvhEAML4RANDjBQAwuwUAQMIbAKAFCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAJByAgA=
atoms_occupancy: QCMpAMDlEwBAIykAwOUTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: GA8BABgPAQAYDwEAGA8BAAjAAACAQgEAWFYBAKA2AQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 600 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAACgAAAAowQBAkAgRACQFgAHJwA8gEAoIAwM8gYXUHWhQCwqFOxPIReZvz8TReXc3mmLv5Vpt091tHtvufukn7sPze/y97Ffj9nkVs7tt/3+Gst36U1XfX6Lq3d0q3Mrvv1fU37==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.88766
b: 10.6543
c: 6.21842
alpha: 90
beta: 90
gamma: 90
cell_volume: 323.822
crystal_density: 4.161
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADgxjoA4MY6ADALGgBQdy4AQAMNACCXEQA=
atoms_y: AAAAAAAAAABQwREAUMERAEDiBQCguQUAgMgbAKAFCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPALB1AgA=
atoms_occupancy: AIcoAACCFAAAhygAAIIUAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 4B4BAOAeAQDgHgEA4B4BAOjLAABwUgEASFwBAHhKAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 650 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQAgAAACgAAAApQQBAkAgxACgFgAHJwA8gEAoIAwU9AoXYHahQEwqFNhfQRepPz0iS0Wc/GmLvxlpt46t2Ot38u6orr0Pz0/ze7F/jtHoXN/7r+3+For26t3etn6fLWfszndy+v7vluz==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.89032
b: 10.6595
c: 6.22274
alpha: 90
beta: 90
gamma: 90
cell_volume: 324.381
crystal_density: 4.154
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABANDsAQDQ7ADALGgAAfC4AsAENAACUEQA=
atoms_y: AAAAAAAAAACQlREAkJURANDjBQDAvAUAgMgbAFAKCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPALB1AgA=
atoms_occupancy: 4DgoACDQFADgOCgAINAUAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: cEgBAHBIAQBwSAEAcEgBANDPAAAYbgEAEHYBAEBkAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 700 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQAgAAACgAAAApQgBAkAgxACgGgAHKwBcgEAoIAwY9AoXYHahQEwsFNieQiuxPz0mi0mo/GmVayprXo7t6PrfY/cpPv0fm9/1b2K9D9No/X3fO/v8PZat0pu+9l2fVq753t+3df7+qt3==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.89292
b: 10.6653
c: 6.2270
alpha: 90
beta: 90
gamma: 90
cell_volume: 324.953
crystal_density: 4.147
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAkjsAAJI7AHARGgDgeC4A0AQNAGCdEQA=
atoms_y: AAAAAAAAAAAQiREAEIkRABDqBQAQ6gUAoMsbAOALCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAEB3AgA=
atoms_occupancy: gMsnAIA9FQCAyycAgD0VAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: YFgBAGBYAQBgWAEAYFgBAKDhAAAAcgEA0I0BAOB9AQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 750 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQAgAAAGgAAAApQgBBEAgxAEgLgAHKwBUgEBQQBQZdAwtYPdCgExMFdieQiqxfT8mikm5/MsXbzpTbx77aLb/pXdJX7ofq56l96LfHrPI9b7VN/3sfR/tdL/fbPc/m3/bnd9udvzdLXf==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.89570
b: 10.6711
c: 6.2309
alpha: 90
beta: 90
gamma: 90
cell_volume: 325.518
crystal_density: 4.140
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABAsTsAQLE7AFAOGgAwdC4AEAsNALCYEQA=
atoms_y: AAAAAAAAAACAoBEAgKARANDjBQCguQUAMM0bAOALCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAIB9AgA=
atoms_occupancy: YH0nAKCLFQBgfScAoIsVAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: EGwBABBsAQAQbAEAEGwBAJDnAAC4kQEAmJ0BAOCHAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 800 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQAgAAAHAAAAApggBBIAghAEgLgALKwB5AEBQQBQZpAwuQPVCgFhUGaiegi8zXnpEjss5+NMXfjTTvR270fXu5f5ZXfo/v5/q3aTeH+fQ2bq9d/dYeR+/6f1e9e5alv/yrb2u7+m5P/v==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.89828
b: 10.6766
c: 6.2354
alpha: 90
beta: 90
gamma: 90
cell_volume: 326.093
crystal_density: 4.132
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAkjsAAJI7ACAWGgCQfS4AsAENAPCeEQA=
atoms_y: AAAAAAAAAACQlREAkJURANDjBQDgvwUAwM4bAOALCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAMCDAgA=
atoms_occupancy: oB8nAGDpFQCgHycAYOkVAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: wIkBAMCJAQDAiQEAwIkBAEAFAQCgnwEAKMcBAICrAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 850 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQBAAAAHAAAABRggBBIAgiAEgLgAOTQB5AIBQQBgp5AwuwO1CgJhUKbE+hFdiXnpElpMy+VIWvjTivR3T0eX+x+6yfuo/Nz3r3sn+O+fRe3367/fY8z9ey3+fvf5/Nr/nWTk717v5e+9==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.9010
b: 10.6834
c: 6.2399
alpha: 90
beta: 90
gamma: 90
cell_volume: 326.717
crystal_density: 4.124
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABggjsAYII7AMAlGgAgfy4A8AcNAMCmEQA=
atoms_y: AAAAAAAAAABAgREAQIERAIDoBQCQxAUAwM4bAJAQCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAFCFAgA=
atoms_occupancy: wPAmAEAYFgDA8CYAQBgWAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: aK8BAGivAQBorwEAaK8BACAHAQAYzQEA+NgBACjHAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 900 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQBAAAAFAAAABRggCBIBAiAEgLAAOVgB5AIBQQBgq6Bg2wO1CgJiYM7E8hFdifrpNFpdz+WYu3nWmtTr3k6/fy3ayt/RfbT/N+4r0P0+h83n6/6741lt1Tes7e3Ttb7vlu3t93//yt9b==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.9041
b: 10.6899
c: 6.2441
alpha: 90
beta: 90
gamma: 90
cell_volume: 327.343
crystal_density: 4.116
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACAUzsAgFM7ADAkGgAAfC4AkP4MAICgEQA=
atoms_y: AAAAAAAAAACgihEAoIoRACDfBQBQvgUAANUbAHANCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPABB/AgA=
atoms_occupancy: wHMmAECVFgDAcyYAQJUWAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: OMEBADjBAQA4wQEAOMEBABgPAQAQywEAwOgBABDVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 950 C

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQBAAAAFAAAABSggCBIBBiAFALAAOVgCpAIBgQCgy6BhcwO5EgJioM7F8hF6m/PZJLJdj8aYtbGmneju3o+tdj9yk++R2b3uV3Yr8f8+i1vv1/23wvF62Vu93t+z5f3fO9/W679f1b+9==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.9067
b: 10.6964
c: 6.2491
alpha: 90
beta: 90
gamma: 90
cell_volume: 327.978
crystal_density: 4.108
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACgHjwAoB48AGAcGgAQii4AcPsMAHCrEQA=
atoms_y: AAAAAAAAAADgqREA4KkRALDgBQDgvwUAINgbALATCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAJCLAgA=
atoms_occupancy: IOclAOAhFwAg5yUA4CEXAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: sO4BALDuAQCw7gEAsO4BAIBCAQDQ4gEAQBgCAJj8AQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 1000 C

qdat:
AAAAAAAAAAAAAAAAAAAMAAAAAAAQBAAAAFAAAABSggCBIBBiAJAXAAOVgCxAICggCgyyBhdgb6FATCoU2J9CK6kvPSJLaam8qpVfOlNunutR83/jd1lbui+yner1pV4/t9D5vv5/nfxvL8unN16t/3a2u/M9vqr37/Zb92==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.8957
b: 10.6710
c: 6.2316
alpha: 90
beta: 90
gamma: 90
cell_volume: 325.551
crystal_density: 4.139
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAkjsAAJI7APAdGgBwei4AIAANAECaEQA=
atoms_y: AAAAAAAAAAAgZREAIGURAJDdBQCguQUA4NEbADAHCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAIB9AgA=
atoms_occupancy: wG0nAECbFQDAbScAQJsVAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: oJ8BAKCfAQCgnwEAoJ8BAHDpAAC4kQEAkJsBAKCVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 800 C, Data collected on cooling

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAQAgAAAHAAAAApggBBIAghAEgLgALKwB5AEBQQBQZ5AwuQPVCgFhUGak+gk8zXnpEllM5+NMXfjTTvR270fXu5f5ZXeo/t5/q3aTeH+fQ2b69f/dYeR+/qf1e9epelv/yrT2u7fm5Xv3==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.8850
b: 10.6490
c: 6.2141
alpha: 90
beta: 90
gamma: 90
cell_volume: 323.260
crystal_density: 4.168
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACA1joAgNY6AFAOGgCAiC4AoPMMAACUEQA=
atoms_y: AAAAAAAAAADAjREAwI0RAFDXBQCAtgUAgMgbAKAFCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPACB0AgA=
atoms_occupancy: QCMpAMDlEwBAIykAwOUTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: MAsBADALAQAwCwEAMAsBAOjBAACQRgEAeEoBAKBAAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 600 C, Data collected on cooling

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAACgAAAAowQBAkAgRACQFgAHJwA8gEAoIAwM8gYXUHWhQCoqFOxPIRaZvz8TReXc3mmLt5Upt091tHtvuf+kn7sOz+/617Ffj/n0Vu7td/VeGkt36U1XfX6Lq3d0q3s7vutXS37==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.8824
b: 10.6432
c: 6.2103
alpha: 90
beta: 90
gamma: 90
cell_volume: 322.714
crystal_density: 4.175
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADA7zsAwO87AIAGGgDwhi4AoAwNAFCPEQA=
atoms_y: AAAAAAAAAADAjREAwI0RAIDoBQBwwQUAIL8bAOALCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAEB3AgA=
atoms_occupancy: YO4pAKAaEwBg7ikAoBoTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: QPsAAED7AABA+wAAQPsAADikAADgKAEAgEwBAAgVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 550 C, Data collected on cooling

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAACgAAAAowQBAkAQRACQFgAGlQA8gCAoIAoMsgYVMDtRICYqCuxPIRXYl56RRaTKXjTJb5Ukn0d29H17uXdUV66G6+f6tai3x+n0b2u/X+z7G0d+2S83N7fN1rr8+Te33b63K9V==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.8798
b: 10.6376
c: 6.2060
alpha: 90
beta: 90
gamma: 90
cell_volume: 322.149
crystal_density: 4.183
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADA9ToAwPU6AFAOGgAQcS4AIBkNAHCSEQA=
atoms_y: AAAAAAAAAACAuREAgLkRACDfBQCAtgUA0MMbADAHCgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAJByAgA=
atoms_occupancy: 4CwqACDcEgDgLCoAINwSAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: kN0AAJDdAACQ3QAAkN0AAGicAAAQFwEA4CgBACAHAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 500 C, Data collected on cooling

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAADgAAAAowQBAkAQRACQFgADlYA6gCAoIAoMegYLsDtQoBYVCqxOoQvIn56RIrLufjTF740038e22i276VbUVt6H5/epe9ivxvT6PW/Xq/5bjSO3/Lu7vr3rVXf+VRVtzt2Tpr9==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.8776
b: 10.6325
c: 6.2019
alpha: 90
beta: 90
gamma: 90
cell_volume: 321.637
crystal_density: 4.189
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADgwDsA4MA7AIAGGgBwei4AoAwNAHCSEQA=
atoms_y: AAAAAAAAAAAglxEAIJcRACDfBQBAsAUAsMAbABAECgA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPALB1AgA=
atoms_occupancy: gDwqAIDMEgCAPCoAgMwSAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: oOEAAKDhAACg4QAAoOEAAKCCAABQ/wAA4B4BAGjxAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 450 C, Data collected on cooling

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAADgAAAAYwQAgiAQQgCQDwADlYAugCAUEAYMegMLsDtQoBYVCmwnoQvMX5+RopLufzLF28qy16O7Wj2/7P+qV99D5/f9W9hf4/R6NzfTrv59jxP+7JfX7V+n8u1/a5v3zu6Zo/7==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.8754
b: 10.6260
c: 6.1980
alpha: 90
beta: 90
gamma: 90
cell_volume: 321.094
crystal_density: 4.197
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADgQzsA4EM7ANAaGgBghS4A0AQNAFCPEQA=
atoms_y: AAAAAAAAAAAwcxEAMHMRALDgBQCQqwUAkL0bAGD/CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAABxAgA=
atoms_occupancy: gDwqAIDMEgCAPCoAgMwSAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 6MsAAOjLAADoywAA6MsAAJiAAABo8QAAYPkAAIDtAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 400 C, Data collected on cooling

qdat:
AAAAAAAAAAAAAAAAAAAGAAAAAAAIAgAAADgAAAAUoQAgiAQYgBQCwADk4AeQCAUEAYGeQMLmDXQoBINBnQnkIrsX4tJotLtPxpEu8aab6O7ej7d/P+qS69D8/P9PexX49R6F7f7539vh5L1+ovX/163srf/udnq57vV0t1==


formula: (Fe Mn) Si O4
compound: <missing>
formula_title: FeMnSiO4
a: 4.8671
b: 10.6043
c: 6.1828
alpha: 90
beta: 90
gamma: 90
cell_volume: 319.108
crystal_density: 4.223
atoms_sites: ["FeM1", "MnM1", "MnM2", "FeM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAg5joAIOY6AIAfGgCwgC4A8AcNACCXEQA=
atoms_y: AAAAAAAAAABQdhEAUHYRAJDdBQAQnwUA4LgbAND9CQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPADBpAgA=
atoms_occupancy: oA0qAGD7EgCgDSoAYPsSAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: qIQAAKiEAACohAAAqIQAAAhXAAAgsgAAELgAABiwAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Data collected at ISIS, Rutherford Appleton Laboratory
 Sample: T = 200 C, Data collected on cooling

qdat:
AAAAAAAAAAAAAAAAAAACAAAAAAAIAQAAABQAAAAUYIAgSAIIgBIBwABSsAbQBAKCAMGPQGFWB1oUAsGgrsTyENmK+fk0Mkyn40xW+PNNfD0uotv+zVslbfg+d3/W/IX+P02je3Xuv3b4ey/f6X199f9vL7v6rWq6d63JP9==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.81694
b: 10.4740
c: 6.13964
alpha: 90
beta: 90
gamma: 90
cell_volume: 309.761
crystal_density: 3.674
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAQ0jsAENI7AADIGQCwZy4AcMMNAGAHEQA=
atoms_y: AAAAAAAAAADw1hAA8NYQAGCzBQBwdgUA0HgbADDVCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAPBJAgA=
atoms_occupancy: gK0sAIBbEACArSwAgFsQAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: GFsAABhbAAAYWwAAGFsAANhoAAB4lgAAiIYAAHCUAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 20 C

qdat:
AAAAAAAAAAAAAAAAAAABgAAAAAACAIAAAAUAAAAElCAECQCBCAJAVAAOVQBogEBQIAwZUgoWoHeIoCYUhllPyJKsy61iik42X5Tg7fNHO7lpnxs3visyqtWpVr5369KlfHdfkzbZvn8+XP0bO6ben+b221V/7d3/Vvb79V==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.82397
b: 10.4977
c: 6.1515
alpha: 90
beta: 90
gamma: 90
cell_volume: 311.516
crystal_density: 3.653
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAQ6zsAEOs7AJDJGQDgXy4AkMYNABAMEQA=
atoms_y: AAAAAAAAAACQ5hAAkOYQACCtBQCQeQUAMIIbAMDWCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPABBNAgA=
atoms_occupancy: gK0sAIBbEACArSwAgFsQAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: cJQAAHCUAABwlAAAcJQAAKh6AADgyQAAKLQAALjTAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 200 C

qdat:
AAAAAAAAAAAAAAAAAAACgAAAAAACAIAAAAkAAAAFKCAEEgCDEAKAmAAcpgCxAIBgQAwp5AwtQG6hQEpJCLSfkSVVt1TJFdzsfynC28aMVtLTPjZv3H5mlb6S/WzXXW1U8Xa/Rub16fZtcdq6bk7pPZpe7Pe79929P/r+81==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.82822
b: 10.5114
c: 6.1582
alpha: 90
beta: 90
gamma: 90
cell_volume: 312.537
crystal_density: 3.641
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADg2TsA4Nk7APDSGQCQZC4AcMMNABAMEQA=
atoms_y: AAAAAAAAAABw/BAAcPwQAIC2BQCQeQUAUIUbAFDYCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPABBNAgA=
atoms_occupancy: 4BotACDuDwDgGi0AIO4PAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 6MEAAOjBAADowQAA6MEAAHiMAABo8QAAmN8AAHDpAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 300 C

qdat:
AAAAAAAAAAAAAAAAAAACgAAAAAAEAIAAAAoAAAAFKEAIEgECEASAqAAcqgCxAACgQBgq6BRNwNchQIxKGNSvIirpLp3LKbTM/lNDr8yc5qW2elzf6L9LJ9Ul2lmdatqp4t1+Tc3q2dz6Y7l9fpXaezb12d135+v6e/ftub==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.83184
b: 10.5276
c: 6.1653
alpha: 90
beta: 90
gamma: 90
cell_volume: 313.615
crystal_density: 3.629
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABg/zsAYP87AEDnGQDwVC4AkMYNAOATEQA=
atoms_y: AAAAAAAAAAAA5RAAAOUQAPC0BQBQcwUA4IYbADDVCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAFBTAgA=
atoms_occupancy: AGktAACgDwAAaS0AAKAPAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: cOkAAHDpAABw6QAAcOkAAEioAAAoCQEAYO8AACgJAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 400 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAIAAAAoAAAAJKEAIEgECIASAuAAozAFiAQDAgCgzyBhagd5CgJSUGWi/QkvTbzmSUyiZfpWGr5k5z8vs9LS9UP2NK25L9PO83pU65frcm9/N57n2x8n67We0vW7rut+vXdb09+5r01==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.83275
b: 10.5385
c: 6.1689
alpha: 90
beta: 90
gamma: 90
cell_volume: 314.182
crystal_density: 3.622
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAADzwAAA88AJDJGQBAUC4AYM4NAFASEQA=
atoms_y: AAAAAAAAAAAg6BAAIOgQAJCrBQCgbgUAcIgbADDVCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAMBRAgA=
atoms_occupancy: QIIuAMCGDgBAgi4AwIYOAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: YO8AAGDvAABg7wAAYO8AADiuAAAAEwEAYPkAAPgaAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 450 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAIAAAAoAAAAKMEAIEgECIASBOAAo1AFiAQDAgChVSBhage5CgJiUMak6QlXTb1siVWmZfKaL35k5X0tc6LW/UWqaTtpL5aNc9yVX5X69G7dZ53u9x9Pzu0+4+f/L69f2/374/25/1f==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.83551
b: 10.5439
c: 6.1727
alpha: 90
beta: 90
gamma: 90
cell_volume: 314.716
crystal_density: 3.616
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADA7zsAwO87AEDOGQAQWC4AIMgNACAaEQA=
atoms_y: AAAAAAAAAACA8RAAgPEQALCuBQDocQUAkIsbADDVCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAOBUAgA=
atoms_occupancy: QAUuAMADDwBABS4AwAMPAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: MAsBADALAQAwCwEAMAsBABiwAADQJAEAEA0BANAuAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 500 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAAAoAAAAKMEAIFAEGIAiBUAA41AFiAQFAgDBV0CiUge6DASiUMdE+RJbVflMil0mZ/KsNX5pzl0/cqSmroWsaTtyT7ad9vSl3y/+1F7+bz3NvTpXz8lbpervXbp1frq3xf9zdmd==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.83884
b: 10.5478
c: 6.17606
alpha: 90
beta: 90
gamma: 90
cell_volume: 315.221
crystal_density: 3.610
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABALjwAQC48ALDMGQCwTi4AoLsNALAbEQA=
atoms_y: AAAAAAAAAAAAzBAAAMwQAHCoBQAAeAUAsI4bAKDTCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAMBRAgA=
atoms_occupancy: wMwsAEA8EADAzCwAQDwQAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: YPkAAGD5AABg+QAAYPkAAAC+AAC4MgEA4B4BAHBIAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 550 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAAAoAAAAKUEAIJAEGIAkBUAA5WAHkAQFBADBVkCiVAXaDASkUM1F+hJbWXnMkl1My+K0PbxpzlpfZ6Wt6ofsUntSjy2Z5ripvi336Ny+rj9N/36X3clVJ9XfX3Z+//2+x+31vq3==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8423
b: 10.5515
c: 6.1795
alpha: 90
beta: 90
gamma: 90
cell_volume: 315.732
crystal_density: 3.604
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAg4DsAIOA7ACDLGQAQWC4AUMANAPAhEQA=
atoms_y: AAAAAAAAAABQ+RAAUPkQALCuBQAgewUAYJMbAJDeCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAABYAgA=
atoms_occupancy: 4CAsACDoEADgICwAIOgQAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: CBUBAAgVAQAIFQEACBUBANjHAABgWAEAyCwBAHBSAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 600 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAABQAAAAKUIAIJAEGIAkBUAAxWAGkAQFBADClkCi1AdqFASkkI1F6hKum6ndEplMz+S0avzJnnpaZ8VN/QrU0LfSn207balSrl/9yK3d2i/b/naum5u7R2a+mrbu/dVvT/r9N1f==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8459
b: 10.5566
c: 6.1830
alpha: 90
beta: 90
gamma: 90
cell_volume: 316.299
crystal_density: 3.598
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABggjsAYII7AODdGQAAYy4AMKQNAIA8EQA=
atoms_y: AAAAAAAAAADQoRAA0KEQANCxBQAgewUAkIsbAKDsCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPANBfAgA=
atoms_occupancy: 4KMrACBlEQDgoysAIGURAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: QGQBAEBkAQBAZAEAQGQBAIjlAAAoaAEAQFoBABhuAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 650 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAABQAAAAKUIAQJAEEQAkBcABRWALEAgGBAFCnkDE1A9yFAjEoY1K8iKus+rZIruI1+VYavzSnLr+z0dL3Q/Y0rrkv1k7zetVPluv0bm5dn+b/P0/L7b6zuavM21d6fv+j/yrbW/==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8495
b: 10.5610
c: 6.1873
alpha: 90
beta: 90
gamma: 90
cell_volume: 316.886
crystal_density: 3.591
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAgXTwAIF08ANDoGQBgbC4AIJYNAEA2EQA=
atoms_y: AAAAAAAAAABQfBAAUHwQAIC2BQCAhAUAsI4bAEDjCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPACBbAgA=
atoms_occupancy: wN4pAEAqEwDA3ikAQCoTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 4CgBAOAoAQDgKAEA4CgBAGD5AADwgQEA8HcBAMCJAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 700 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAABQAAAASUIAQJAIEQAkCcABRmALEAgKBAFCrkFEmA1yGAlFIY5L8iSrNuuZJLKZlWpoe3lTnNy0z4tb/ReppOulOlt119KVbH17kTv5tnc+2L4/Xa12lc3ddnr327f/F+nX+s/==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8530
b: 10.5664
c: 6.1908
alpha: 90
beta: 90
gamma: 90
cell_volume: 317.456
crystal_density: 3.585
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABggjsAYII7AFD1GQAwWy4AAJMNAGA5EQA=
atoms_y: AAAAAAAAAABgihAAYIoQANCxBQCAhAUAEJgbABDrCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAJBZAgA=
atoms_occupancy: 4CwqACDcEgDgLCoAINwSAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: oJ8BAKCfAQCgnwEAoJ8BADgDAQCAoQEA0IMBAIijAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 750 C

qdat:
AAAAAAAAAAAAAAAAAAADAAAAAAAEAQAAABQAAAASUIAQJAIMQAkCYAByqALEAgKBAGCrEFFmA3SKAlFIZaT8iS7NvOZJTaZn8pwdfmjNXS1zo+auhe5pW3FbpZnW/Kn+LdbkXbTLP9euXp2f2n1Pd9pvrLv3326P9uf81/==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8657
b: 10.5893
c: 6.2066
alpha: 90
beta: 90
gamma: 90
cell_volume: 319.791
crystal_density: 3.558
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADgPTwA4D08ADDZGQAQWC4AsH4NAIBVEQA=
atoms_y: AAAAAAAAAADAsg8AwLIPAPC0BQAglAUA8JQbAFDxCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPABBmAgA=
atoms_occupancy: oJApAGB4EwCgkCkAYHgTAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: wFECAMBRAgDAUQIAwFECAJA8AQDY5AEA4NwBAHgIAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 800 C

qdat:
AAAAAAAAAAAAAAAAAAAFAAAAAAAIAQAAABQAAAAUoQAgSAQIgBIE4AClMAWIBAUCAMGXQKJUBtoUBKKQi0nqIqqy6tkis0mX6Th7eVKc3LzPi5v/F6mla6U+mmbb8qV4t1+Tdvrs/ze52npebeU9m3rs9rv3X/4/863Vt7==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8592
b: 10.5772
c: 6.1988
alpha: 90
beta: 90
gamma: 90
cell_volume: 318.598
crystal_density: 3.572
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACgHjwAoB48AADhGQAQWC4AIJYNABBXEQA=
atoms_y: AAAAAAAAAACgXhAAoF4QAFC+BQDgjQUAII0bABDrCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAHBWAgA=
atoms_occupancy: oJYoAGByFACgligAYHIUAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: yIsBAMiLAQDIiwEAyIsBANgmAQCgnwEAeKkBAEi7AQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 850 C

qdat:
AAAAAAAAAAAAAAAAAAAFAAAAAAAIAQAAABQAAAASoIAQSAIMQBICoABisAVIAgMCAKFNIKFKBbkKBKJQzyW5ElVZecySWUzNdLQ6vMmOflpnx877C9zSttKvTTvt6VU+W6/Ru21efxp0dT87pvaLrb93qd377t6f/f9qv3==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8628
b: 10.5827
c: 6.2022
alpha: 90
beta: 90
gamma: 90
cell_volume: 319.175
crystal_density: 3.565
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAACgDwAAoA8AAODdGQBQXi4AwHMNAABJEQA=
atoms_y: AAAAAAAAAAAgBxAAIAcQAPC0BQCAhAUAEJgbAKDsCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPABBmAgA=
atoms_occupancy: YPQoAKAUFABg9CgAoBQUAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: ECoCABAqAgAQKgIAECoCAKg4AQBQswEAgKEBAODmAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 900 C

qdat:
AAAAAAAAAAAAAAAAAAAFAAAAAAAIAQAAABQAAAAUoQAgSAIIQBICoACisAWIBAMCAKFPIKJOBtkMBKKQi0X5Ep2bedyym0zP9Tg67NGc2u5Gx1/dD5lU6uS7WzXVWpVsXUuRM7v8/zb47X03JVSd1T5muvfz9f09+3bK39==


formula: (Mg Mn) Si O4
compound: <missing>
formula_title: MgMnSiO4
a: 4.8691
b: 10.5954
c: 6.2114
alpha: 90
beta: 90
gamma: 90
cell_volume: 320.447
crystal_density: 3.551
atoms_sites: ["MgM1", "MnM1", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAABALjwAQC48ADDZGQDgXy4AEIgNANBpEQA=
atoms_y: AAAAAAAAAAAw/A8AMPwPAHCoBQBwjwUAUJ4bAMDvCQA=
atoms_z: AAAAAAAAAABAQg8AQEIPAEBCDwBAQg8AQEIPAJByAgA=
atoms_occupancy: YH0nAKCLFQBgfScAoIsVAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 6D0CAOg9AgDoPQIA6D0CACBwAQDA6AEAsO4BACAuAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 High-temperature order-disorder in (Fe0.5Mn0.5)2SiO4 and (Mg0.5Mn0.5)2SiO4
 olivines: an in situ neutron diffraction study
 Sample: T = 1000 C

qdat:
AAAAAAAAAAAAAAAAAAAFAAAAAAAIAgAAACQAAAAUoQAgSAQYgBIEwADlUAeIBAUEAMKWQMTUD3IUBMUhjknyJKq265kitpmfanB1uZMtVLTNjpe6H7Kl1cl+tmutpKr4vtcid/Vo/n0z2Py6W857EvtN3dev9Xx/pz/qv2==


formula: Mn.196 Ca.716 Na.045 (Al1.911 Si2.089) O8
compound: <missing>
formula_title: <missing>
a: 8.131
b: 12.847
c: 7.069
alpha: 94.03
beta: 115.90
gamma: 90.72
cell_volume: 661.839
crystal_density: 2.797
pub_title:
 Crystal chemistry of synthetic Mn-bearing anorthite:
 Incorporation of MnAl2Si2O8 end-member into feldspar
 Note: U(1,1) for Obo altered to reproduce Uiso

atoms_sites:
["MnM1", "CaM1", "NaM1", "CaM2", "MnM3", "CaM3", "NaM3", "AlT1o", "SiT1o", "AlT1m", "SiT1m", "AlT2o", "SiT2o", "AlT2m", "SiT2m", "OA1", "OA2", "OBo", "OBm", "OCo", "OCm", "ODo", "ODm"]

atoms_x:
ILYQACC2EAAgthAAEF0QAEBuEABAbhAAQG4QAPBVAADwVQAAMBEAADARAAAAmikAAJopAOBLKQDgSykAkEwAAADdIgDgZjEAYIwxAPC5AAAQcgAAMC0MAKCVCwA=

atoms_y:
8EkCAPBJAgDwSQIA0J0AAFBS/v9QUv7/UFL+/zC8CQAwvAkA4MoxAODKMQBAkQYAQJEGAMCWNQDAljUAALcHAKBpPAAA9QUA0BQ0ABBwEQDQ0ykAUFQGAGDFNAA=

atoms_z:
8GkFAPBpBQDwaQUAcJYIAHAHCwBwBwsAcAcLAOASDQDgEg0AACkOAAApDgCwKBMAsCgTAOD1FQDg9RUAELk7AHDjEACQCgsAsNwOAECaEQAQjgwA0PoWAFByGgA=

atoms_occupancy:
AMoIAMDZFQAgSAEA4OwKAIAsAwDg7AoAAHcBACD/IQDgCRsAQH0aAMCLIgBgxRsAoEMhAKBhHABgpyAAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
MD0BADA9AQAwPQEAQF4CAOCfAgDgnwIA4J8CAGDRAABg0QAAMMAAADDAAADQzwAA0M8AAHDGAABwxgAA0GUBADDyAAAAkAEAoAMCABBsAQCwSQEAEGwBALD4AQA=

atoms_aniso_label:
["MnM1", "CaM1", "NaM1", "CaM2", "MnM3", "CaM3", "NaM3", "AlT1o", "SiT1o", "AlT1m", "SiT1m", "AlT2o", "SiT2o", "AlT2m", "SiT2m", "OA1", "OA2", "OBo", "OBm", "OCo", "OCm", "ODo", "ODm"]

atoms_aniso_u11:
ENYAABDWAAAQ1gAAsGgAADA9AQAwPQEAMD0BAJDJAACQyQAAgLsAAIC7AABwrQAAcK0AANC2AADQtgAAUCECACDkAABwdQEAcHUBAAAsAQAwCwEAMFYBAIBqAQA=

atoms_aniso_u22:
wIkBAMCJAQDAiQEAYEIDABC+BAAQvgQAEL4EACDkAAAg5AAAQM4AAEDOAACgpQAAoKUAAFCqAABQqgAAsGIBAJCwAADAJQEAcHUBALB7AQCgVAEAQEsBAKCGAQA=

atoms_aniso_u33:
oPAAAKDwAACg8AAAwFECABDQAQAQ0AEAENABAOCrAADgqwAA4JIAAOCSAACg8AAAoPAAALDMAACwzAAA4N0AAKAiAQDgOwIA8EMDAOCMAQDwHQEAkBQBAKC4AQA=

atoms_aniso_u12:
cHsAAHB7AABwewAAYIYAAMCb/v/Am/7/wJv+/yDR//8g0f//IDUAACA1AAAQDgAAEA4AALAEAACwBAAAwCsAAHD+///Ax///ADIAAPC///+QTAAAkAEAAOAuAAA=

atoms_aniso_u13:
MBEAADARAAAwEQAAgNr//3D4AABw+AAAcPgAANA5AADQOQAAECcAABAnAACwNgAAsDYAAHAwAABwMAAA0M8AAGBUAAAA+gAAYDUBAICJAADAKwAAsAQAADCU//8=

atoms_aniso_u23:
ILj//yC4//8guP//EDP+/zAE/v8wBP7/MAT+/6AoAACgKAAAIAMAACADAACADAAAgAwAAOAuAADgLgAAUC0AAIAlAABABgAA0CAAAPA8AADAx///8CMAAIDB//8=

qdat:
AAAAAAAAQAAAAAIANAAgAAIAUAQAigSAiiCAIJTAIoB00JCEEVNhMWDIwcqKNmAErNZKtoFGuWaDTaFW6VDzZKl19lf96/LdziX77v8nVz24///5SJu/j1/cV/rfRzP4tu771e30/fv277vf58e7+e196btu3d79/77d+3==


formula: Fe.51 Al.6 Mg.44 Ca.96 Si1.4 O6
compound: Chelyabinsk coal basin, Southern Urals
formula_title: <missing>
a: 9.786
b: 8.860
c: 5.338
alpha: 90
beta: 105.87
gamma: 90
cell_volume: 445.185
crystal_density: 3.419
atoms_sites: ["FeM1", "AlM1", "MgM1", "CaM2", "FeT", "SiT", "AlT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAODgDADg4AwA4OAMAIArGAAAyggAgAgJAA==
atoms_y: ANwFAADcBQAA3AUAoIoqAADnGAAA5xgAAOcYAIAlGQBAxQ4AoFsdAA==
atoms_z: wMYtAMDGLQDAxi0AwMYtAMA9LwDAPS8AwD0vAKDLNAAAjScAgDgBAA==
atoms_occupancy: wFwVAAA1DAAA2xoAAJg6AADiBACAuSoAADUMAAAJPQAACT0AAAk9AA==
atoms_u_iso: +MUAAPjFAAD4xQAASJ4AAPjFAAD4xQAA+MUAAIDtAAAgsgAAOE8AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Subsilicic ferrian aluminian diopside from the Chelyabinsk
 coal basin (Southern Urals) - an unusual clinopyroxene

qdat:
AAAAAAAAAAAAAAAAQAAAAAQCAAAAIAAQEAAIAQAABEABEQCYCAIEQAAATIJAUAEAEqyBQQhCgNYAAIfAAVBGA0WaywYApOsAC5oblBE1XKQmxEacvbBlck3RzhK4b4dnHJz94iQW+i9x49RWbUzDvDKPSevjbyj7AisQBR==


formula: Zn4 Si2 O9 H2
compound: <missing>
formula_title: <missing>
a: 8.181
b: 10.841
c: 5.081
alpha: 90
beta: 90
gamma: 90
cell_volume: 450.635
crystal_density: 3.418
atoms_sites: ["Zn", "Si", "O1", "O2", "O3", "O4", "H3", "H3*"]
atoms_x: 6DIwAAAAAACgCTMAAAAAAKCpKQAAAAAAQB0qAKC6IgA=
atoms_y: QGkzAEBKNADAmzAAAF4zAAAAAAAAAAAAAAAAAAAAAAA=
atoms_z: AAAAAMD0HQCQRRYAQFcxAFCyOQBwNhgAYFMuAIDQOwA=
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgIQeAICEHgA=
atoms_u_iso: OEoAAAA8AADAXQAAwF0AAJDJAAAgZwAAQA0DAEANAwA=
atoms_aniso_label: ["Zn", "Si", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: EF4AAEBRAABghgAAsGgAADB1AABgnwAA
atoms_aniso_u22: WDkAAKAoAACQZQAAIGcAAMBEAACgKAAA
atoms_aniso_u33: kEcAANA5AABAUQAAkEwAADChAQDwbgAA
atoms_aniso_u12: SPT//wAAAADAx///AAAAAAAAAAAAAAAA
atoms_aniso_u13: 6P7//wAAAACA8///AAAAABD1//8AAAAA
atoms_aniso_u23: QAEAAFD7//+ADAAAQAYAAAAAAAAAAAAA
pub_title:
 Proton disorder in dehydrated hemimorphite - IR spectroscopy
 and X-ray structure refinement at low and ambient temperatures
 T = 110 K

qdat:
AAAAAAAAAAAAAAAAgAAIAABAICAAAAAigAQEAACEAQADQGICUAgQ0ACAkQ0AACtYTCgKNAyQFIwaROEQxsEAiKofvoQuiyy8WgAzhFJl/iSorv9CypI3HjL20oTerzKqplitzPNJq5Yt1F0jN1fZ8PWD08d3zlAocKFSVS==


formula: Zn4 Si2 O9 H2
compound: <missing>
formula_title: <missing>
a: 8.191
b: 10.824
c: 5.088
alpha: 90
beta: 90
gamma: 90
cell_volume: 451.099
crystal_density: 3.414
atoms_sites: ["Zn", "Si", "O1", "O2", "O3", "O4", "H3", "H3*"]
atoms_x: 4D8wAAAAAACwFzMAAAAAAKDCKQAAAAAAQKwnAKC6IgA=
atoms_y: wGEzAOhCNACAlTAAIEgzAAAAAAAAAAAAAAAAAAAAAAA=
atoms_z: AAAAANACHgBQPxYAoEcxACDsOQCAXRgAgB4vAIBfOQA=
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgIQeAICEHgA=
atoms_u_iso: sJAAADhjAACAuwAAgKIAAOBBAQDwuQAAQA0DAEANAwA=
atoms_aniso_label: ["Zn", "Si", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: IKgAAHB7AABQ3AAAQJwAABDvAACgIgEA
atoms_aniso_u22: II8AADBcAABQ3AAAoPAAANCdAAAASwAA
atoms_aniso_u33: IHYAANBSAAAAfQAAMFwAAIAyAgDAwQAA
atoms_aniso_u12: uOP//wAAAADAlf//AAAAAAAAAAAAAAAA
atoms_aniso_u13: 4Pz//wAAAACA2v//AAAAAGC+//8AAAAA
atoms_aniso_u23: wAMAAEAGAACgKAAAEA4AAAAAAAAAAAAA
pub_title:
 Proton disorder in dehydrated hemimorphite - IR spectroscopy
 and X-ray structure refinement at low and ambient temperatures
 T = 293 K

qdat:
AAAAAAAAAAAAAAAAgAAIAACAQEAAAAAigAQEAACEAQAFQGICUAgQ0ACAkQ0AACtsTCgUUhRQHIwaSNEQ6cMBEKwq7UwrBzkYawBjiFOrb0VI6v6FUqRvFlPlUwjU/jS3LPXNmOJj/5pWZJoia+6pUWoDl42zlMBw4UVUml==


formula: Mg1.109 Mn.821 Ca.07 Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.758
b: 8.897
c: 5.283
alpha: 90
beta: 108.74
gamma: 90
cell_volume: 434.339
crystal_density: 3.472
atoms_sites: ["MgM1", "MnM1", "CaM2", "MnM2", "MgM2", "SiA", "SiB", "O1A", "O1B", "O2A", "O2B", "O3A", "O3B"]
atoms_x: oEsPAKBLDwCwcg8AsHIPALByDwBAkAIAYFYhAODqNAAAqBYA4DYHAHAUJgCwXQYA4OYkAA==
atoms_y: MOknADDpJwD4dAEA+HQBAPh0AQAg0BQA8DYzAACbFAAQITMAUKUeAGCuPACgyA8AcPArAA==
atoms_z: cHIOAHByDgCQXA4AkFwOAJBcDgDQbxAAoM4OAFDxCQCgXAgAkO0TALDLFQBQjSIAgGseAA==
atoms_occupancy: oCQ7AGDkAQDARQQAwDcwAICLCAAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: AF8AAABfAAD4uwAA+LsAAPi7AADIbgAA2HIAAJCIAACAjgAAGLAAAJjfAADwwwAA6MsAAA==
atoms_aniso_label: ["MgM1", "MnM1", "CaM2", "MnM2", "MgM2", "SiA", "SiB", "O1A", "O1B", "O2A", "O2B", "O3A", "O3B"]
atoms_aniso_u11: cGIAAHBiAAAAyAAAAMgAAADIAAAwXAAAYG0AAMBdAAAgTgAAgLsAAGDqAABgbQAA4KsAAA==
atoms_aniso_u22: AGQAAABkAADgxAAA4MQAAODEAAAQcgAA4HkAAIC7AADgqwAAAH0AACDLAABg6gAAQBkBAA==
atoms_aniso_u33: EFkAABBZAABQkQAAUJEAAFCRAAAAfQAAcHsAAKCMAABAnAAAwNoAAGDqAABg6gAAgLsAAA==
atoms_aniso_u12: oA8AAKAPAACQGgAAkBoAAJAaAAAw+P//QO3//wAAAABg8P//gMH//4A+AACAPgAAAAAAAA==
atoms_aniso_u13: sB0AALAdAADgFQAA4BUAAOAVAADwIwAAcDAAAOAuAABAHwAAIE4AAIA+AACAPgAAwF0AAA==
atoms_aniso_u23: YAkAAGAJAACgDwAAoA8AAKAPAAAQ9f//8PH//wAAAAAAAAAAwOD//0CcAABAnAAAwF0AAA==
pub_title:
 The temperature-dependent P2_1/c - C2/c phase transition in the
 clinopyroxene kanoite MnMg[Si2O6]: a single-crystal X-ray and optical study
 T = 200 C

qdat:
AAAAAAAAAAAIAAAAIAAAAACEgEQAAIAECAgCgoAAApkEIIDg0ggkYCRAClmgkJEhSI6kqgDdxCaUiic6VqSTm8jxj7nccf/Ql9pHzF6sGd95q9sar7tV9XeP31vb636vtf/VP+f+v9nebr+Da/b7lqZ9uX2uU3nYuubJu5==


formula: Mg1.123 Mn.807 Ca.07 Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.796
b: 8.880
c: 5.315
alpha: 90
beta: 109.26
gamma: 90
cell_volume: 436.467
crystal_density: 3.448
atoms_sites: ["MgM1", "MnM1", "CaM2", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAADw6REAYEMHALCTFgAgmBUA
atoms_y: kC43AJAuNwBAuRAAQLkQAEC5EAAQhgUAIGIFAGBFDwDAXQAA
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwAA0g8AYDcJAKDDFABAkAIA
atoms_occupancy: 4MA7ACBIAQDARQQAQPkvAADKCAAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: mIAAAJiAAACA7QAAgO0AAIDtAAB4jAAACLYAAFD/AACIRAEA
atoms_aniso_label: ["MgM1", "MnM1", "CaM2", "MnM2", "MgM2", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: QIMAAECDAAAQCAEAEAgBABAIAQAAfQAAUHgAAKAJAQDgqwAA
atoms_aniso_u22: MHUAADB1AAAA4QAAAOEAAADhAACAiQAAIMsAAIC7AADA1AEA
atoms_aniso_u33: 4HkAAOB5AABguAAAYLgAAGC4AACwmgAAwNoAAIA4AQCAOAEA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAABg8P//cP7//5C2//+wBAAA
atoms_aniso_u13: kBoAAJAaAABQFAAAUBQAAFAUAADAKwAAcDAAAEBqAABwMAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAACA8///YPD//5DP//+gFf//
pub_title:
 The temperature-dependent P2_1/c - C2/c phase transition in the
 clinopyroxene kanoite MnMg[Si2O6]: a single-crystal X-ray and optical study
 T = 270 C

qdat:
AAAAAAAAAAAAAAAAIAAAAACCAAAAAIAECAAAgQAAACCAIIBQwgAiICAAAFCgkAAgBICkwABsghJYggIQQtSMgUDRTYWCAGfRKgxC7DaUDB2pEVQUAasvu5QFs4jVA64bVG1QW/+ymbzADx9BkVUdvCLBgNsCRMjUQrfk0A==


formula: Ca Fe.77 Mg.22 Si O4
compound: <missing>
pub_title: Crystal chemistry of meteoritic kirschsteinite Sample: KIR1
formula_title: <missing>
a: 4.877
b: 11.166
c: 6.448
alpha: 90
beta: 90
gamma: 90
cell_volume: 351.136
crystal_density: 3.415
atoms_sites: ["CaM2", "FeM1", "MgM1", "Si", "O1", "O2", "O3"]
atoms_x: wNs7AAAAAAAAAAAAaGUZACC3LQCATg4AADARAA==
atoms_y: GOsQAAAAAAAAAAAASCYFACDlBACwjhsAsDIJAA==
atoms_z: QEIPAAAAAAAAAAAAQEIPAEBCDwBAQg8AMOYCAA==
atoms_occupancy: AAk9AED/LgCAbQ0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: QGoAAMB2AADAdgAAwF0AAACWAACwgQAAYIYAAA==
atoms_aniso_label: ["CaM2", "FeM1", "MgM1", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: gHAAAOBgAADgYAAAoEEAAIA+AAAQcgAAgIkAAA==
atoms_aniso_u22: wF0AAICJAACAiQAA4GAAAOCrAADgYAAAwI8AAA==
atoms_aniso_u33: gHAAAOB5AADgeQAAoHMAADDZAACQsAAA4HkAAA==
atoms_aniso_u12: YAkAAPDx///w8f//AAAAAJABAACQAQAAEA4AAA==
atoms_aniso_u13: AAAAAADn//8A5///AAAAAAAAAAAAAAAAgAwAAA==
atoms_aniso_u23: AAAAAGDw//9g8P//AAAAAAAAAAAAAAAAcBcAAA==
qdat:
AAAAAAAAAAAAAAAAAACAAAAAAAAgEAAAFAAAAEAggAAwgBRAgCAIAJiAcgAISgIEAyEWEgBkSAkgINkCxJBglFslioJFovDSwHFRUVDS0KFHyoQoXClSpV+uUXKjnlRQ3T6zhyzZx1xjrGvWe807xyrXONxm7EtZ9raNhD==


formula: Ca (Fe.69 Mg.31) Si O4
compound: <missing>
formula_title: <missing>
a: 4.875
b: 11.164
c: 6.447
alpha: 90
beta: 90
gamma: 90
cell_volume: 350.875
crystal_density: 3.374
atoms_sites: ["CaM2", "FeM1", "MgM1", "Si", "O1", "O2", "O3"]
atoms_x: ENc7AAAAAAAAAAAAaFsZAMCtLQCwXw4A8CERAA==
atoms_y: kOsQAAAAAAAAAAAA8CMFALDmBAAgjRsAkC8JAA==
atoms_z: QEIPAAAAAAAAAAAAQEIPAEBCDwBAQg8AEOMCAA==
atoms_occupancy: AAk9AEAdKgDA6xIAAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: gHAAAHB7AABwewAAkGUAAPCgAACAiQAAMI4AAA==
atoms_aniso_label: ["CaM2", "FeM1", "MgM1", "Si", "O1", "O2", "O3"]
atoms_aniso_u11: sIEAABByAAAQcgAAgFcAANBSAABghgAAQJwAAA==
atoms_aniso_u22: 4GAAAPCHAADwhwAAAGQAAHCtAAAwXAAAcJQAAA==
atoms_aniso_u33: gHAAAFB4AABQeAAAoHMAAMDaAABguAAA4HkAAA==
atoms_aniso_u12: 0AcAAPDx///w8f//IAMAAHD+//9w/v//wBIAAA==
atoms_aniso_u13: AAAAAADn//8A5///AAAAAAAAAAAAAAAA8AoAAA==
atoms_aniso_u23: AAAAAHD+//9w/v//AAAAAAAAAAAAAAAAIBwAAA==
pub_title:
 Crystal chemistry of meteoritic kirschsteinite
 Sample: KIR2
 Note: U(1,1) of O1 altered to reproduce Uiso

qdat:
AAAAAAAAAAAAAAAAAADAAAAAAAAgEAAAFAAAAEAggAAwgAxAgCAIAJiAMgAIRgICAyESEgBkTAkgIFkBRJBglEkUikElonDRQHFZcVDS0KHHSoYoXj1ypc6uUWqhnVQwrTq7gqy5x3RjrGtWas05pxrNONwjbEq5treNhj==


formula: Al2 Ge O6 H2
compound: <missing>
formula_title: <missing>
a: 4.804
b: 9.107
c: 8.551
alpha: 90
beta: 90
gamma: 90
cell_volume: 374.107
crystal_density: 3.987
atoms_sites: ["Al", "Ge", "O1", "O2", "O3", "O-H"]
atoms_x: ME76/0C7GABgVu//MK4DAOD5DABQ6yMA
atoms_y: IB4IAOBG/P/A1AEAYBMPAIDB//8AIw8A
atoms_z: 8AA2AUCK9wFAS0wAQFSJAMA4fwAwFLsA
atoms_occupancy: 0
atoms_u_iso: 8DwAAPA8AADwPAAA8DwAAPA8AADwPAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Ge-analogues of aluminium silicates: High-pressure synthesis
 and properties of orthorhombic Al2GeO4(OH)2
 Note: Space group setting altered to match standard

qdat:
AAAAAAAAAAAAAAAABAAAAAAgEgAEAAAABCiACAEAgACCQYiCEopIYCRiEgZACELJEi2UwlLCQcQx6lGCh2GCrYXY3cc88GH5zq/qr121WVU5Wj7T61nuu/f/1XflbuV//W3/7+e79/z+fuXdb2e9e199r3/2ffrR7zytv9==


formula: K.795 Na.62 Ca1.276 (Si7.928 Al4.072) O31 H13.94
compound: <missing>
formula_title: <missing>
a: 14.556
b: 13.206
c: 7.513
alpha: 90
beta: 110.75
gamma: 90
cell_volume: 1350.520
crystal_density: 2.308
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Symmetry reduction of the aluminosilicate framework of LAU topology
 by ordering of exchangeable cations: the crystal structure of primary leonhardite
 with a primitive Bravais lattice

atoms_sites:
["K1", "Na11", "Na12", "Ca1", "Si11", "Al11", "Si12", "Al12", "Si21", "Al21", "Si22", "Al22", "Al11", "Si11", "Al12", "Si12", "O1", "O21", "O22", "O31", "O32", "O41", "O42", "O51", "O52", "O6", "O71", "O72", "Wat1", "Wat2", "Wat3", "Wat4"]

atoms_x:
QEIPAMDGLQCQtCkAmIQfAHDHHQBwxx0AoOcdAKDnHQAgEhQAIBIUAPj9EwD4/RMAUEMXAFBDFwDIaxcAyGsXAIBlHwCQhRwACF4cACj8FwB4LhgAENMXAHAxGADonhkAaLUjAJDqEQD4ARAAQDIQAGCJJQAArCYAQHQoAMDGLQA=

atoms_y:
uLEiALBKBQCwcAcA4BoPAGhoFgBoaBYAECQIABAkCACgIAgAoCAIAFA/FgBQPxYAwIcDAMCHAwC43BoAuNwaAEBMDwBY4RYAgIwHACDYBwBwoRYA2IcYAJjkBQAAgyIAkCoEANAqDwB4hAMAQLQaAFBnBwBwmRQAIFgPAMDKCwA=

atoms_z:
AAAAAAAAAABgbjYAePEsALD2CACw9ggAuC8JALgvCQDgohMA4KITACBoEwAgaBMAwMcsAMDHLAC4eiwAuHosABA9DQBARjgA4G44ANBUIQAw+iAAMH4LAEBUDABAjiwAQG4QAAAdEADwqywAMJksAKATKQDQMCcAkKoBAICEHgA=

atoms_occupancy:
4IUwAMDfFADgewgAwPAmAEC3OgDAUQIAABU7AAD0AQDgQzsAIMUBAKAkOwBg5AEAQDo6AMDOAgAAGzoAAO4CAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AEA0OwA=

atoms_u_iso:
EGYCAEDXCwDA1AEA4CgBAPBuAADwbgAAgHAAAIBwAAAggAAAIIAAAJB+AACQfgAAIIAAACCAAADQhAAA0IQAAMDzAAAQ7wAAEO8AANABAQBQ9QAA8AQBAOAPAQDA8wAAIP0AAIAGAQDQAQEAkPsAAFA0AwDwEQMAIMUBACDxAgA=

qdat:
AAAAAAACgAAgAAAJBKAACBQhJgQAoFFDCZWoBgVeIzMG5Z1GXH2TpHl/6+rrT/13Wc/+Wu//956+c/v/H3/X3/n979d////9873/79m9//0//3/rd//7f+3vv7/fvf1u/0b/2+74W72/LMf353yL2b19/Z+7l+vfb33+/y==


formula: K Al1.788 Mg.64 Si3.572 O12 H2
compound: Dora-Maira massif, western Alps
formula_title: <missing>
a: 5.21379
b: 5.21379
c: 29.7382
alpha: 90
beta: 90
gamma: 120
cell_volume: 700.088
crystal_density: 2.827
atoms_sites: ["K", "AlM2", "AlM3", "MgM3", "SiT1", "AlT1", "SiT2", "O1", "O2", "O3", "O4", "O5", "O6", "H"]
atoms_x: oN8HAIAeLwDAuxoAwLsaAKDpLwCg6S8AQHEcAIAkLgDg9x0AIFgoAOCBBwAgaiUAAFMHAOD4CAA=
atoms_y: QL8PAMATNgDgXQ0A4F0NAKA3IwCgNyMAACc4AKC6IgDAATkAIKsvAAB1KwCAYQ8AIAYMAOCeFwA=
atoms_z: OCwKAAAAAAAAAAAAAAAAAOB0BQDgdAUA4I0FAJAnAgAAPwIAsNoGAJCMBgBA9QYA0C0CADBQAgA=
atoms_occupancy: AAk9AAAJPQAA+RUAABAnAED5LwDADw0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: QBMCAOAoAQCgAwIAoAMCACBIAQAgSAEAIEgBACBIAQCghgEAIEICAAB3AQAgSAEAgLUBACCzBAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Cation site ordering in phengite 3T from the Dora-Maira
 massif (western Alps): a variable-temperature neutron
 powder diffraction study
 Note: at T = 293 K

qdat:
AAAAAAAAAAEAAAAAAAAAAQAUQEAQAQAKABAAEAAIZEUBAINUEiAwEEIAQAQAANIhBAQEAipiCBAgEAgAKkQipUISQEBABpIQgggQAaiIgg9yIQgggAAA1JEIW5L1mVBCAdJEQhAAAAAdR5yVF0pEIQAA2UiIQAAADqe7WI==


formula: K2 Al2.798 Mg.63 Si3.572 O12 H2
compound: Dora-Maira massif, western Alps
formula_title: <missing>
a: 5.23169
b: 5.23169
c: 30.1227
alpha: 90
beta: 90
gamma: 120
cell_volume: 714.017
crystal_density: 3.233
atoms_x: YMAHAGDFGwBgxRsAgJsvAICbLwBgRzAAYEcwAADPHADAxi0AgAceAMDwJgDAsAcAQL4kAICRBwDg+AgA
atoms_y: IHEPAODaDQDg2g0AQFI2AEBSNgBglSMAYJUjAOBVOAAgfCIAoLM4AOCRLgDAzCwAAKYOAGAlDADgnhcA
atoms_z: OCwKAAAAAAAAAAAAAAAAAAAAAACgoAUAoKAFAEBMBQBgFgIAoE4CADDOBgCAfgYAEOQGAHAkAgAwUAIA
atoms_occupancy: AAk9AMD7OQBADQMAwK8cAEBZIABA+S8AwA8NAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: YNgDAIC7AACAuwAAgK8CAICvAgAA+gAAAPoAAOClAQDA1AEAoIYBAIC1AQAA7gIA4BYEAABxAgCgbgUA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Cation site ordering in phengite 3T from the Dora-Maira
 massif (western Alps): a variable-temperature neutron
 powder diffraction study
 Note: at T = 893 K

atoms_sites:
["K", "AlM2", "MgM2", "AlM3", "MgM3", "SiT1", "AlT1", "SiT2", "O1", "O2", "O3", "O4", "O5", "O6", "H"]

qdat:
AAAAAAAAAAEAAAAAAAAABAAYQIAgAgAYAEAAQABAyKICAQbIKIDAQggBABAAAciECBAQCKaEIECAgEAA6RCKlQhJAgIAGkhEECBADqRCEE1IiEIEAAAHpERCfJOcSkQQDVIiEIAAAADqTqSovlIiEAAGykhEAAAAal9TRE==


formula: Pb4.32 Sb3.68 S8.7 Cl2.3
compound: <missing>
formula_title: Pb4.32Sb3.68S8.68Cl2.32
a: 15.04
b: 15.51
c: 4.09
alpha: 90
beta: 90
gamma: 90
cell_volume: 954.076
crystal_density: 5.930
atoms_x: INMHAOCiDgCAIB4AgCAeAJANFwCQDRcAUMUIAOA9CgBwbRMAcG0TACA2BAAgNgQAAHEbAABxGwAAAAAA
atoms_y: 4C8EAPBgEwDQ/g0A0P4NAIAfAQCAHwEA8KMMAFBsGwCwcAcAsHAHAJAgGACQIBgAADcUAAA3FAAAAAAA
atoms_z: AAAAAAAAAACAhB4AgIQeAICEHgCAhB4AgIQeAICEHgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACAhB4A
atoms_occupancy: AAk9AAAJPQCAGgYAgO42AICpAwCAXzkAAAk9AAAJPQCAKi0AgN4PAMA3MABA0QwAgAwyAID8CgAACT0A
atoms_u_iso: cD0CAEATAgBABwQAQAcEALAeBACwHgQAMFYBANCwAQCAMgIAgDICAMBRAgDAUQIAwM4CAMDOAgDgnwIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of synthetic Pb4.32Sb3.68S8.68Cl2.32
 A chlorine-bearing alternative to Pb4Sb4S11

atoms_sites:
["Pb1", "Pb2", "PbM3", "SbM3", "PbM4", "SbM4", "S1", "S2", "S3", "ClS3", "S4", "ClS4", "S5", "ClS5", "Cl"]

qdat:
AAAAAAAAACAAAEgUAAAIAEgAFCApCxIgQKUGEZFCcRLjiMETE/DyZm1HzrbdVfJ89bvt9yn03l+6hft1eW3I1pve95F/93d3apWq6VPf/L9wq//sXryX/roq9KL3+HTEvlJ+la34zbruXy3Spv8ZRDSIWLd27Gn9MuX8+b==


formula: Na8 Al6 Si6 C O27
compound: <missing>
pub_title: Crystal structure of a carbonate-nosean Na8[AlSiO4]6CO3
formula_title: <missing>
a: 9.001
b: 9.001
c: 9.001
alpha: 90
beta: 90
gamma: 90
cell_volume: 729.243
crystal_density: 2.182
atoms_sites: ["Na1", "Na2", "Al", "Si", "C", "O1", "O2", "O3", "O4"]
atoms_x: oEoLAKB+LACgtQ4A4M4PAAAAAABgPQgAAI0nAKC5NwAgHggA
atoms_y: oEoLAKB+LACAhB4AAAAAAAAAAABAdxsAIOw5AOAKBgAAAAAA
atoms_z: oEoLAKB+LAAAAAAAgIQeAAAAAABAZgkAgE4nAKD3AwAAAAAA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9ADgsCgA4LAoA
atoms_u_iso: gO0AAKBBBQBgOwAA6GIAADABAQCA7QAAgO0AADABAQAwAQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAACAAAAEAAAQAAIAAgAEAAABABABAEAIAgEAAEAgICAgIEAAgQIEACCABBBBBBCAEEIIQhACEIgiEAhCIBCAREQiICIhEiAiIiJARIgRAkRIkCRJEgCSJIEkgiCSSSCSSSESgkFJAQCklBCikBSVAQRIQQKEg==


formula: Ca (Fe.994 Zn1.006) As2 (O10 H2)
compound: Tsumeb mine, Namibia
formula_title: <missing>
a: 9.010
b: 6.246
c: 7.391
alpha: 90
beta: 115.52
gamma: 90
cell_volume: 375.358
crystal_density: 4.187
atoms_sites: ["CaMe1", "FeMe2", "ZnMe2", "AsX", "O-H1", "O2", "O3", "O4"]
atoms_x: AAAAAEBCDwBAQg8AkNM3AHD9FABwbRMAsBECAFDTDgA=
atoms_y: AAAAAEBCDwBAQg8AgIQeAICEHgAAAAAA4BMRAICEHgA=
atoms_z: AAAAAICEHgCAhB4AeHsMALDrGADQGRYA0PgOAOBBAQA=
atoms_occupancy: AAk9AKBVHgBgsx4AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: CLYAAIiQAACIkAAAwHYAAAi2AACQ3QAAGLAAAFD1AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of the tsumcorite-group minerals. New data on ferrilotharmeyerite,
 tsumcorite, thometzekite, mounanaite, helmutwinklerite, and a redefinition of gartrellite

qdat:
AAAAAAAAAAAAAAACAAAAAQAAABAAAEAIAEAEAgAAAAYAAAgQFAEEgAABEBAggGDMAAEgDQA5ABkBANEAACiEVaEQIBgDMAQQZiGKrBOpAKGpNhTiIwJDIZmNiAJcGLPiFXnVKrSgqJrGbK2Sx5nNoyJOhA32dj3xuhTpn3==


formula: Pb Cu2 (As1.234 S.766) (O10 H2)
compound: Tsumeb mine, Namibia
formula_title: <missing>
a: 9.077
b: 6.300
c: 7.661
alpha: 90
beta: 116.99
gamma: 90
cell_volume: 390.380
crystal_density: 5.218
atoms_sites: ["PbMe1", "CuMe2", "AsX", "SX", "O-H1", "O2", "O3", "O4"]
atoms_x: AAAAAEBCDwBw8zcAcPM3ACDpFAAw0RIAQOEBAEC4DAA=
atoms_y: AAAAAEBCDwCAhB4AgIQeAICEHgAAAAAA8J4RAICEHgA=
atoms_z: AAAAAICEHgCQzAwAkMwMAMCoGQCw8BMAcAIQAEAZAQA=
atoms_occupancy: AAk9AAAJPQCgqCUAYGAXAAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 8NYBAAAdAQDgHgEA4B4BAPh5AQAwyQEAMGoBACAuAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of the tsumcorite-group minerals. New data on ferrilotharmeyerite,
 tsumcorite, thometzekite, mounanaite, helmutwinklerite, and a redefinition of gartrellite

qdat:
AAAAAAAAAAAAAAAIAAAAAgAAABAAAICAAIAECAAAABYAAQgAKACFAAAKBACAIORQAAFARhUYBQJICCEABCQGdiEBoBEuwAAFK5CChVYkIJLcFJPJckAwU+FhiJG0IZdQhm7mAzJb8b5mJ0qaJt2kCORNPNuRHw3MMqxtOV==


formula: Pb Fe2 V2 (O10 H2)
compound: Mounana, Gaboon
formula_title: <missing>
a: 9.294
b: 6.166
c: 7.713
alpha: 90
beta: 115.57
gamma: 90
cell_volume: 398.717
crystal_density: 4.854
atoms_sites: ["PbMe1", "FeMe2", "VX", "O-H1", "O2", "O3", "O4"]
atoms_x: AAAAAEBCDwDAUjgAgI4UAJBwEwBgegIAUPgMAA==
atoms_y: AAAAAEBCDwCAhB4AgIQeAAAAAAAQqBAAgIQeAA==
atoms_z: AAAAAICEHgAAxQ0A8IcZAKC3FgDwQBAAMK3//w==
atoms_occupancy: 0
atoms_u_iso: QGQBAOAoAQCA7QAACBUBAMiLAQAIFQEAaFABAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of the tsumcorite-group minerals. New data on ferrilotharmeyerite,
 tsumcorite, thometzekite, mounanaite, helmutwinklerite, and a redefinition of gartrellite

qdat:
AAAAAAAAAAAAAAAgAAAAAgAAAgAABAQAAAoAAQAAAwQAAYCAIggAEAEAkCgBYAAQCAAJGSAAqAMoWAAAGFsRIRDIQoJAjYAwmBQshZFkB8RPIgyF2mMHRKsULxJVD4XsEPiUwQWL2Y5y9KeadIDXHmtPypO6QfiiI5Zevx==


formula: Pb Fe Cu As2 (O10 H2)
compound: Tsumeb mine, Namibia
formula_title: <missing>
a: 5.431
b: 5.642
c: 7.573
alpha: 67.62
beta: 69.57
gamma: 70.31
cell_volume: 195.422
crystal_density: 5.425
atoms_sites: ["PbMe1", "FeMe2", "CuMe2", "AsX", "O-H1", "O2", "O3a", "O3b", "O4"]
atoms_x: AAAAAAAAAACAhB4AQAYZAEDpCACAVREA4FEPAMDeKQAg7g8A
atoms_y: AAAAAICEHgAAAAAAMIgaAOBvCgBArRIAIM8pAMAJDgDgyBAA
atoms_z: AAAAAICEHgCAhB4AAFcwAGCfGQDg5ygAcC4RALCeEADgOwIA
atoms_occupancy: 0
atoms_u_iso: 6A0AAAgVAQAIFQEA+MUAAKh6AACoegAAqHoAAKh6AACoegAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAEAAAACRBEABAAAAQiCAAAABAkgfMCBDJkBAADQAIIYAc0tVycAMIZEMUJgJHBsa05YlevnrXwXNCatTxoj/ffNSsv1ra/y8av+zfV++/+/zxf4sf29vZ537bvj3/+Z+1fd/frf/n/7/t///7f/71397==


formula: Pb Zn2 As2 (O10 H2)
compound: Tsumeb mine, Namibia
formula_title: <missing>
a: 5.606
b: 5.610
c: 7.617
alpha: 70.19
beta: 69.91
gamma: 69.18
cell_volume: 203.771
crystal_density: 5.296
atoms_sites: ["PbMe1", "Zn1", "Zn2", "AsX", "O-H1", "O2", "O3a", "O3b", "O4"]
atoms_x: AAAAAAAAAACAhB4ASLIZACB8CQAwHBMAcDoPAKDCKQAgAREA
atoms_y: AAAAAICEHgAAAAAAgNQZAECYCQDQ4BIAcLEpAPAUDwCgihEA
atoms_z: AAAAAICEHgCAhB4AeHYvADDGGABQuicA0MAPACDuDwDQhAAA
atoms_occupancy: 0
atoms_u_iso: SBoCAChoAQAQbAEAYFgBAHBlAgAQdgEAkPoBAOjeAQB44wMA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAQAAAACAIQAgAAAAQAwAAAABAAVaAAHqIAQBACAwAgJADTobwA8ABgnlBwAQRvs6MM0/HPygADDd3ICDmD/zoe8dusPj5M8FgP3Kf1/+dbnuOPqz9b/9q//+7uzy8z/9nnu1X9/nv3z5d7/9vT8hffv/==


compound: Kangerdlugssuaq intrusion, East Greenland
formula_title: <missing>
a: 14.1686
b: 14.1686
c: 30.0847
alpha: 90
beta: 90
gamma: 120
cell_volume: 5230.343
crystal_density: 2.927
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
formula:
Ca3.27 Mn3.68 Na14.48 Fe.79 Al.13 Mg.05 Nb.55 Zr2.93 Ti.23 Si25.1 Y.42 K.3 Sr.15 Hf.06 O75.81 F1.51 Cl.269 H.22

pub_title:
 Kentbrooksite from the Kangerdlugssuaq intrusion, East Greenland,
 a new Mn-REE-Nb-F end-member in a series within the eudialyte group:
 Description and crystal structure

atoms_sites:
["CaM1", "MnM1", "NaM1", "MnM2", "FeM2", "AlM2", "MgM2", "FeM2a", "NbM3", "ZrM3", "TiM3", "SiM4", "SiM4a", "Na1a", "Na1b", "Na2", "Na3a", "Na3b", "Na", "Y", "K", "Sr", "Na5", "Zr", "Hf", "Ti", "Si1", "Si2", "Si3", "Si4", "Si5", "Si6", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "O17", "O18", "O19", "O20", "F1a", "Cl1a", "O-H1a", "F1b", "Cl1b", "O-H1b", "F2a", "Cl2a", "O-H2a", "F2b", "Cl2b", "O-H2b", "F2c", "Cl2c", "O-H2c", "F2d", "Cl2d", "O-H2d", "F2e", "Cl2e", "O-H2e"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAAAAAAQEgAABAIIUIBAhCIDECEVAsCxLJRJJaEkhwtOUKp0S44qJoYqDxwr2QkIymfS3ysx2zXV5GJmasZ7nWeZ945Mma32W4zdoFltOWWEEzY2IFIASPZhqEEBNAhAUAAsmESBAAGUEQBAABQIAgAAAAAAAAAAAAAA==


formula: (Ba.9 Ca.1) Al2 Si3 O13.08 H6.16
compound: <missing>
formula_title: <missing>
a: 9.5374
b: 9.6127
c: 6.5233
alpha: 90
beta: 90
gamma: 90
cell_volume: 598.057
crystal_density: 2.673
atoms_sites: ["Ba", "Ca", "Al", "Si1", "Si2", "O1", "O2", "O3", "O4", "O5", "Wat1", "Wat2"]
atoms_x: gIQeAICEHgDwaQUAAAAAANBJ9f/wrwoAMI38/3BSCwDwMAIAwMX3/yBECgBgkhcA
atoms_y: AAAAAAAAAAAAQQoAAAAAAIDPBQBQtRMAADUMAIAyAgAgNwgAcG8CAJDtEwCgrQcA
atoms_z: IJYmACCWJgCQFyYAQFEAABCXFwAQCyYAMHwcAKB7IACQUzUAkJMJACBpCAAg1/7/
atoms_occupancy: gO42AIAaBgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AECOLABAcDEA
atoms_u_iso: ANsBAADbAQCQPAEAkDwBAJA8AQCo2QAAqNkAAKjZAACo2QAAqNkAAMBRAgDAUQIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 310 K

qdat:
AAAAAAAAAAAAAAAEgAAAABoAMAAwAYAgQAHCAAxMIAGDCwNaxwDKBg7Uoxa4BRYP07ppWqxdB/Qo0rP5r1I2/+h/u9l+/e08s/3e/b+93vdF79f////nf+e/u/uvP/f/P9v/fr/P2fYf55//fv+/9Xn+m5f31WnzuK893Z==


formula: (Ba.9 Ca.1) Al2 Si3 O12.46 H4.92
compound: <missing>
formula_title: <missing>
a: 9.4903
b: 9.5690
c: 6.5290
alpha: 90
beta: 90
gamma: 90
cell_volume: 592.916
crystal_density: 2.633
atoms_sites: ["Ba", "Ca", "Al", "Si1", "Si2", "O1", "O2", "O3", "O4", "O5", "Wat1", "Wat2"]
atoms_x: gIQeAICEHgCAUgUAAAAAANBJ9f9glQoAUF78/6AxCwBgLwIAUMf3/4AnCADgtxcA
atoms_y: AAAAAAAAAACANAoAAAAAADDUBQCAlBMAoHYMAKAcAgCAQAgA0PsBAKBfFADA4gcA
atoms_z: wFomAMBaJgCgVyYAYFQAANB3FwBg7SUAQNUcAICqIADggDUAEB0KAJDRBwAws/7/
atoms_occupancy: gO42AIAaBgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AEDoHQCAKi0A
atoms_u_iso: YBYCAGAWAgBoUAEAaFABAGhQAQD4xQAA+MUAAPjFAAD4xQAA+MUAADDcAgAw3AIA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 396 K

qdat:
AAAAAAAAAAAAAAAEgAAAABoAGAAYAIAQgADiAAZmMADBSUC5QoEjBgtrSYnoAUYG6q01XqseR3oOdLm7/rUVu7kdZvd/9T+1+fv/v//327+w//7//e93393//+//76/+59/z94/+/d+n7Pf8/z/7vf5+X5Pv99r0/3zP30==


formula: (Ba.9 Ca.1) Al2 Si3 O12.04 H4.08
compound: <missing>
formula_title: <missing>
a: 9.4393
b: 9.5089
c: 6.5042
alpha: 90
beta: 90
gamma: 90
cell_volume: 583.800
crystal_density: 2.631
atoms_sites: ["Ba", "Ca", "Al", "Si1", "Si2", "O1", "O2", "O3", "O4", "O5", "Wat1", "Wat2"]
atoms_x: gIQeAICEHgCAUgUAAAAAABA39f9ALgoAEIr8/7BYCwBQcgEAILb3/4AnCABQZRgA
atoms_y: AAAAAAAAAAAAcwoAAAAAAFC+BQCA+BMAYIkMAEATAgAwdwgAcAsCAKBfFAAgUAgA
atoms_z: 4KgmAOCoJgBwwyYA0FIAAHCHFwCQHSUA8MAcAJADIQAwYzUAkCkKAJDRBwCgZv7/
atoms_occupancy: gO42AIAaBgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AADECQCAfTQA
atoms_u_iso: 6D0CAOg9AgBoUAEAaFABAGhQAQAIFQEACBUBAAgVAQAIFQEACBUBAGgrAwBoKwMA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 451 K

qdat:
AAAAAAAAAAAAAAACQAAAAA0ADAAIAEAIQABxAAMxGAAgpGBWcMBZgQda1GFuAFGBuqst16bG2c6DlT1n216k9XtHbtb3/b+2vrb28/v9V/daG/7v/fv97t3f/3r///S/7Xz/m0z/39/8evtX5+n/XevH4fym//3f561K+P==


formula: (Ba.9 Ca.1) Al2 Si3 O10.68 H1.36
compound: <missing>
formula_title: <missing>
a: 9.3758
b: 9.4097
c: 6.5377
alpha: 90
beta: 90
gamma: 90
cell_volume: 576.779
crystal_density: 2.522
atoms_sites: ["Ba", "Ca", "Al", "Si1", "Si2", "O1", "O2", "O3", "O4", "O5", "Wat1", "Wat2"]
atoms_x: gIQeAICEHgCgVQUAAAAAAIBn9f9gYwoAQFD8/5CgCwAg3gEA8KT3/4AnCACw+BoA
atoms_y: AAAAAAAAAACwwgoAAAAAAHBdBQDwpRQA8FgMAFCFAgCwgwgAsMYBAKBfFAAwBgYA
atoms_z: 4F0mAOBdJgBgnCYAAOEAALDYFwAgziUAsOwcAAB/IQBgvzUAgBsKAJDRBwCwbv//
atoms_occupancy: gO42AIAaBgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AMDUAQDA6xIA
atoms_u_iso: wFECAMBRAgBQswEAULMBAFCzAQDIiwEAyIsBAMiLAQDIiwEAyIsBACBUBAAgVAQA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 An in situ study of the edingtonite dehydration process from
 X-ray synchrotron powder diffraction
 Sample: 643 K

qdat:
AAAAAAAAAAAAAAABgAAAAAMABgAEACAEgAAaAADgSAAIGhgOjBiMIgRjy0g+wAygo+lnzbHMcWfSFs7qv/vxh6u9Fvnf/+a92eWP73r9/q/f4Hv////v/+u6//jX//Qz/3++/nx7+/u/zcv6fl69vn/u3L8i/v//9md7/9==


formula: Ca Mg Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.7483
b: 8.9246
c: 5.2505
alpha: 90
beta: 105.882
gamma: 90
cell_volume: 439.355
crystal_density: 3.274
atoms_sites: ["CaM2", "MgM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAADAdBEAADoHAPAcFgBwSBUA
atoms_y: YGUSAGBoNwBAlwUA8FAFACA/DwAQOgEA
atoms_z: QEIPAEBCDwDgDA4AgL0IAPBgEwBw7jwA
atoms_occupancy: 0
atoms_u_iso: uH4AADhPAAAwTQAA6GIAADABAQDgagAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: Di#S2

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAACAAIIAAEAgAAAGABCEAqCAEIwAAAIxQiAQCARCk0CCYiCLIoAAowAjBogDQuroAiIVioUTOLnRCx+FclrAByHfccIJw8ocMhPrLNnbC8/oIyuHJVpNI7YfasBVVkqBc5SosjRKwcFB==


formula: Ca Mg.943 Fe.13 Si1.927 O6
compound: <missing>
formula_title: <missing>
a: 9.7433
b: 8.9410
c: 5.2511
alpha: 90
beta: 105.936
gamma: 90
cell_volume: 439.869
crystal_density: 3.328
atoms_sites: ["CaM2", "MgM1", "FeM1", "SiT", "FeT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAA4HcRAOB3EQDAGgcAkBMWAJBkFQA=
atoms_y: kF0SAABfNwAAXzcAgLYFAIC2BQCgVQUAkCQPABAIAQA=
atoms_z: QEIPAEBCDwBAQg8AIPoNACD6DQDgxggAYF8TAFCgPAA=
atoms_occupancy: AAk9AGCOOQCgegMAsM46AFA6AgAACT0AAAk9AAAJPQA=
atoms_u_iso: sHwAAEhJAABISQAAOEUAADhFAADwZAAAmIAAAMhuAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts6/#2

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAACAAIIAAEBAAAAGABCEBKEAEQwAAAIaQiAQEASBk0BCQiCTIoABIwAlCogDwsrYAiE3iQoTJTqqExeJsZrAChHbdUIZw84cqi95HVs1B8+kIrWSpeZMo+ofkoCXJk6BU6ZJVDhLwMFB==


formula: Ca Mg.895 Fe.205 Si1.9 O6
compound: <missing>
formula_title: <missing>
a: 9.7600
b: 8.9236
c: 5.2670
alpha: 90
beta: 105.890
gamma: 90
cell_volume: 441.198
crystal_density: 3.352
atoms_sites: ["CaM2", "MgM1", "FeM1", "SiT", "FeT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAsH8RALB/EQDgHQcAUA0WAJBkFQA=
atoms_y: EGoSAJBgNwCQYDcAYLMFAGCzBQCAUgUAcDoPAPAdAQA=
atoms_z: QEIPAEBCDwBAQg8AEAUOABAFDgBQrAgAYJETAGDHPAA=
atoms_occupancy: AAk9AGCgNgCgaAYAwPs5AEANAwAACT0AAAk9AAAJPQA=
atoms_u_iso: UEEAADhPAAA4TwAAKFUAAChVAACQKQAAOEUAAGA7AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts10/#2

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAAEAAIIAAEAgAAAMABCEA0EAEIgAAAQyQiAgEARCokCEVCEdKQABJgAjDZAGxVLoBII5pgUTsOtSCk0K5KfADiPe4oIbg1I05D/2Sbv1G5aghy8cSu5cly5vW4GWKm4Jay5jxbIhhwoK==


formula: Ca Mg.906 Fe.194 Si1.9 O6
compound: <missing>
formula_title: <missing>
a: 9.7578
b: 8.9226
c: 5.2639
alpha: 90
beta: 105.886
gamma: 90
cell_volume: 440.798
crystal_density: 3.350
atoms_sites: ["CaM2", "MgM1", "FeM1", "SiT", "FeT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAMHMRADBzEQCQIgcAkBMWAPBtFQA=
atoms_y: EGoSAKBuNwCgbjcAoLkFAKC5BQDAWAUA4DgPADAkAQA=
atoms_z: QEIPAEBCDwBAQg8AoO0NAKDtDQBwrwgAIIsTAODTPAA=
atoms_occupancy: AAk9AEBMNwDAvAUAwPs5AEANAwAACT0AAAk9AAAJPQA=
atoms_u_iso: +GYAABhRAAAYUQAAGFsAABhbAAB4NwAA6GIAAMB2AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts10/#3

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAAEAAIIAAEAgAAAKABCEA0EAEIwAAAIyQiAgEARCokCEUiCNJQABJgAjDZAGxTLoBII5pQUTcNtSCk0K1KbADiPe4YIbg9I05BezaZfVDo6QhysOSuVUjy5fS4CbJlcJ6y5jpPIwhQUG==


formula: Ca Mg.857 Fe.267 Si1.876 O6
compound: <missing>
formula_title: <missing>
a: 9.7646
b: 8.9200
c: 5.2709
alpha: 90
beta: 105.889
gamma: 90
cell_volume: 441.556
crystal_density: 3.377
atoms_sites: ["CaM2", "MgM1", "FeM1", "SiT", "FeT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAwHQRAMB0EQDgHQcAcBAWAAB8FQA=
atoms_y: cHMSACBiNwAgYjcAoLkFAKC5BQAgYgUAEEoPAFBAAQA=
atoms_z: QEIPAEBCDwBAQg8AsOINALDiDQCQsggAwJoTAADXPAA=
atoms_occupancy: AAk9AKBONABguggAQEA5AMDIAwAACT0AAAk9AAAJPQA=
atoms_u_iso: YDsAAFhDAABYQwAA8GQAAPBkAABgOwAASJ4AAOhiAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts15/#2

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAAEAAIIAAEAgAAAMABCIA0EAIIgAAAQyQiAgEARCokCEVCENKQACJgAjC5APRVLQBIIxqgUSsOpiCk0M6OvADkVe4YItg3I05DnqSbt2H5ehBU0YU86omy6rnoG2Km4L03ZGySJhBgwU==


formula: Ca Mg.805 Fe.445 Si1.75 O6
compound: <missing>
formula_title: <missing>
a: 9.7724
b: 8.9176
c: 5.2837
alpha: 90
beta: 105.881
gamma: 90
cell_volume: 442.881
crystal_density: 3.444
atoms_sites: ["CaM2", "MgM1", "FeM1", "SiT", "FeT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAsH8RALB/EQBADgcAECAWALBnFQA=
atoms_y: cHMSAOBbNwDgWzcAoLkFAKC5BQAQVAUAME0PAGA1AQA=
atoms_z: QEIPAEBCDwBAQg8AcPUNAHD1DQAggggAgK0TAADXPAA=
atoms_occupancy: AAk9ACAiMQDg5gsA4Gc1ACChBwAACT0AAAk9AAAJPQA=
atoms_u_iso: OEUAAAhXAAAIVwAAKFUAAChVAAA4TwAAOE8AAOhiAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts20/#2

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAAEAAQIAAIAgAAAUACEIAkEAIIgAAAQiRBBAEASExEEIlEIVKgACLAAiEpAOTWSQCgRSjAUXYK5iGp0KUKtAHIu7oYZPA2LnKHH3EyNWL/TCHU44q8VaOdZeXIWc5HwmqrzUjkmDDChI==


formula: Ca Mg.733 Fe.597 Si1.67 O6
compound: <missing>
formula_title: <missing>
a: 9.7844
b: 8.9132
c: 5.2989
alpha: 90
beta: 105.883
gamma: 90
cell_volume: 444.476
crystal_density: 3.499
atoms_sites: ["CaM2", "MgM1", "FeM1", "SiT", "FeT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAQIERAECBEQCg/gYAUCYWAGBsFQA=
atoms_y: 8H8SADBXNwAwVzcAwLwFAMC8BQDQZgUAQFsPAPBPAQA=
atoms_z: QEIPAEBCDwBAQg8AAN4NAADeDQCQNQgAIL0TACDzPAA=
atoms_occupancy: AAk9ACC9LADgSxAA4PYyACASCgAACT0AAAk9AAAJPQA=
atoms_u_iso: +GYAABBZAAAQWQAA2GgAANhoAAA4TwAAYDsAADhPAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts30/#2

qdat:
AAAAAAAAAAAAAAAAQAAAAAQEAAAAEAAQIAAIAgAAAkACEIBoEAIJgAAARERBBAEASFjEIIlEIdJAAEPAAmQqAcSUmgFAhTqASuQMjEKikYYsJAPJp/E4y1D+VGKLPOIsbU7emQZZyRP/LI07lWOJFyxdyNls7ZCaYDIIIR==


formula: Ca Mg.641 Fe.759 Si1.2 O6
compound: <missing>
formula_title: <missing>
a: 9.8007
b: 8.9002
c: 5.3214
alpha: 90
beta: 105.856
gamma: 90
cell_volume: 446.515
crystal_density: 3.388
atoms_sites: ["CaM2", "MgM1", "FeM1", "SiT", "FeT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAIH4RACB+EQDwEgcA8DUWAKCLFQA=
atoms_y: 4IoSADBXNwAwVzcAMLsFADC7BQAwcAUAIIoPANBlAQA=
atoms_z: QEIPAEBCDwBAQg8AQMsNAEDLDQCgjggAIHITAJC/PAA=
atoms_occupancy: AAk9AKAfJwBg6RUAAJ8kAAA1DAAACT0AAAk9AAAJPQA=
atoms_u_iso: GFEAABC4AAAQuAAAKFUAAChVAACYigAASJ4AAKjZAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Mossbauer spectroscopy and Rietveld refinement on synthetic
 ferri-Tschermak's molecule CaFe3+(Fe3+Si)O6 substituted diopside
 Sample: fts40/#1

qdat:
AAAAAAAAAAAAAAAAQAAAAAQEAAAAIAAQIAAIAgAAAoACEQCwEAIKgAAATISBEAIAKLKCQhGEgc0AAIOAAlBaA4MVbAMAmU4AK8wZyEitVhkMogsq9+FY0rHOyUGRephNMNm/SCRMxR9uQVTfY0mZOSBWyfXh3kmbApDCCb==


formula: Mg.9 Al4.39 Si1.96 O12
compound: <missing>
formula_title: <missing>
a: 7.8791
b: 16.5425
c: 5.6329
alpha: 90
beta: 90
gamma: 90
cell_volume: 734.192
crystal_density: 3.504
atoms_x: 0KkXANCpFwAANAgAADQIAICEHgCAhB4A8A4QAPAOEAAAAAAAAAAAAICEHgAQaQ4AcJ4PADBDAABQQAEA0A8gAA==
atoms_y: AAAAAAAAAACANAoAgDQKABCaCgAQmgoA0AcZANAHGQAAAAAAAAAAAAAAAAAAAAAAMO4JAIA5BQDATg8AYLMFAA==
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAQEIPAEBCDwAAAAAAAAAAAAAAAACgoTsAQLUAAEBCDwBAQg8AQEIPAA==
atoms_occupancy: QFkgAABxAgCA0DsAgDgBAEA0OwDA1AEAQDQ7AMDUAQDAPhoAwNQBAIBtDQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: MPIAADDyAACwNgAAsDYAACBOAAAgTgAAwF0AAMBdAAAQWQAAEFkAALCBAABghgAAwEQAAEBqAABwSQAAcEkAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure refinement of synthetic Fe- and Mg-staurolite by
 Rietveld analysis of X-ray powder-diffraction data
 Sample: Mg-staurolite synthesized at 25 kbar

atoms_sites:
["MgT2", "AlT2", "SiT1", "AlT1", "AlM1", "MgM1", "AlM2", "MgM2", "AlM3", "MgM3", "MgM4", "O1", "O2", "O3", "O4", "O5"]

qdat:
AAAAAAAAAAAACACAAAAAAAESAIEAAGAIAAJACQgooQIBUiIFABjAQQzAASFOYJFoBMzFTeQUkGIfEBlhjTvmKDEm9UyMYRX5KOQysdglGhoRK/7VXqvdiVHZzQGVY52mJZq21PDeSb9eIxbeKEc+GUllrUXSxdmJdjWjyx==


formula: Fe.44 Al2.305 Si.95 O6
compound: <missing>
formula_title: <missing>
a: 7.8719
b: 16.6231
c: 5.6583
alpha: 90
beta: 90
gamma: 90
cell_volume: 740.419
crystal_density: 3.758
atoms_x: YA8YAGAPGADAFAgAwBQIAICEHgCAhB4AEF0QABBdEAAAAAAAgIQeAABbDgBAdA8AMBEAAAAsAQDQcyAA
atoms_y: AAAAAAAAAABgGAoAYBgKAGCVCgBglQoAoA8ZAKAPGQAAAAAAAAAAAAAAAADg2QkAIGIFAHAIDwBQCQYA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAQEIPAEBCDwAAAAAAAAAAALAAOwBw3wAAQEIPAEBCDwBAQg8A
atoms_occupancy: wFUrAMAnCQDA+zkAQA0DAEA0OwDA1AEAQDQ7AMDUAQAATB0AQA0DAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0OgAANDoAADwPAAA8DwAACBOAAAgTgAAwF0AAMBdAACQZQAA8NIAAACWAADAXQAAQIMAADBcAAAwXAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure refinement of synthetic Fe- and Mg-staurolite by
 Rietveld analysis of X-ray powder-diffraction data
 Sample: Fe-staurolite synthesized at 25 kbar

atoms_sites:
["FeT2", "AlT2", "SiT1", "AlT1", "AlM1", "FeM1", "AlM2", "FeM2", "AlM3", "FeM4", "O1", "O2", "O3", "O4", "O5"]

qdat:
AAAAAAAAAAAACACAAAAAAAISAQCAAGAIAARAChBRIgQCVEwJADJAhSTAAmR0wyNgBalRq8hmYsgvIG2HFtfSsCRY7NYUwOa5RQqOtuksaqEUTujjj5V3QpxU2Y73h/hKhSZl36juDMu0LMs26i90tzdH3FMjdNKeKjGcqc==


formula: Fe.455 Al2.29 Si.95 O6
compound: <missing>
formula_title: <missing>
a: 7.8783
b: 16.6172
c: 5.6591
alpha: 90
beta: 90
gamma: 90
cell_volume: 740.863
crystal_density: 3.763
atoms_x: AB8YAAAfGAAw+gcAMPoHAICEHgCAhB4AgHQQAIB0EAAAAAAAgIQeANCtDgAAhw8AAAAAAOBaAQBgXCAA
atoms_y: AAAAAAAAAAAADwoAAA8KAICxCgCAsQoAEA4ZABAOGQAAAAAAAAAAAAAAAACg7AkAAEYFADDpDgAwBgYA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAQEIPAEBCDwAAAAAAAAAAAFD3OgCg1wAAQEIPAEBCDwBAQg8A
atoms_occupancy: gJsvAADiBADA+zkAQA0DAEA0OwDA1AEAQDQ7AMDUAQAAvR8AQJwAAAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0OgAANDoAADwPAAA8DwAACBOAAAgTgAAwF0AAMBdAACQZQAA8NIAAACWAADAXQAAQIMAADBcAAAwXAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-structure refinement of synthetic Fe- and Mg-staurolite by
 Rietveld analysis of X-ray powder-diffraction data
 Sample: Fe-staurolite synthesized at 5 kbar
 Note: These coordinates do not reproduce the reported bond lengths, but
 Koch-Muller tells me that the coordinates are correct, and the reported
 bond lengths were incorrect.

atoms_sites:
["FeT2", "AlT2", "SiT1", "AlT1", "AlM1", "FeM1", "AlM2", "FeM2", "AlM3", "FeM4", "O1", "O2", "O3", "O4", "O5"]

qdat:
AAAAAAAAAAAACACAAAAAAAISAQEAAGAIAARAChBRIgQCZEwJADNAhSTAAmJ0wyNgBSmRmshGYUgvIFeHGtfSsCRZ7NYUwedrSwyOp/EsasIUXuljlZ9/Qqy16Q/7jrjPB0Zu32juDU80TN86yi1YtjdOmNcidNKWMnOoqc==


formula: N2.24 (Si6.803 Al2.197) O22.88 H17.26
compound: <missing>
pub_title: X-ray single-crystal structure refinement of NH4-exchanged heulandite at 100 K
formula_title: <missing>
a: 17.738
b: 17.974
c: 7.416
alpha: 90
beta: 115.91
gamma: 90
cell_volume: 2126.725
crystal_density: 2.077
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["N1", "N3", "N14", "SiT1", "AlT1", "SiT2", "AlT2", "SiT3", "AlT3", "SiT4", "AlT4", "SiT5", "AlT5", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5", "Wat8", "Wat9", "Wat10", "Wat11", "Wat12", "Wat14", "H11", "H12", "H13", "H14", "H31", "H32", "H33"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAAAAABAACAQACAECEMAAIEAaQSBCIANB4gZI4CpHDQbKwMyaQPPZowcbrevxxVLa+8GcNzNaiRn98lLBK8rivZgPZzm7hurF4Ge6cv3FpJlHp+RoJb9M6iapu8zdLfBrp8BrEPMolhpJY4dyVPpD8vFfhZmWJtkL1hW==


formula: Mg.895 Fe.141 Zn.01 Mn.01 Al1.942 O4
compound: xenoliths of the Alban Hills, Italy volcanic region
pub_title: Crystal chemistry of spinels from xenoliths of the Alban Hills volcanic region Sample: SP182b
formula_title: <missing>
a: 8.1011
b: 8.1011
c: 8.1011
alpha: 90
beta: 90
gamma: 90
cell_volume: 531.658
crystal_density: 3.681
atoms_sites: ["MgT", "FeT", "ZnT", "MnT", "AlT", "SiT", "MgM", "FeM", "NiM", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgC4ABAA
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgC4ABAA
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgC4ABAA
atoms_occupancy: wOonANClBwCwmgAAIJkAAIBBDACQAQAACFoHAMh9AAB4BQAAeCU1ACADAAAACT0A
atoms_u_iso: 0FIAANBSAADQUgAA0FIAANBSAADQUgAA8DwAAPA8AADwPAAA8DwAAPA8AABQeAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAAEAAIAAACAAIAAAIABAAACAAgAACABAAAIAIAACACAABACAAAACAACAIAAQBAABAIAAgBAAIAgAAAg==


formula: Mg.934 Fe.119 Zn.004 Mn.006 Al1.936 O4
compound: xenoliths of the Alban Hills, Italy volcanic region
pub_title: Crystal chemistry of spinels from xenoliths of the Alban Hills volcanic region Sample: SP238a
formula_title: <missing>
a: 8.0996
b: 8.0996
c: 8.0996
alpha: 90
beta: 90
gamma: 90
cell_volume: 531.362
crystal_density: 3.654
atoms_sites: ["MgT", "FeT", "ZnT", "MnT", "AlT", "SiT", "MgM", "FeM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AwP0PAA==
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AwP0PAA==
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AwP0PAA==
atoms_occupancy: ALMpAPDmBQDwPAAAwF0AAADLDABgCQAAgKoHABirAACYqzQAAAk9AA==
atoms_u_iso: AEsAAABLAAAASwAAAEsAAABLAAAASwAAYDsAAGA7AABgOwAA4HkAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAAEAAIAAACAAIAAAEABAAACAAgAACABAAAIAIAACACAABACAAAACAACAIAAQBAABAEAAQBAAIAgAAAQ==


formula: Mg.875 Fe.214 Zn.004 Mn.01 Al1.896 O4
compound: xenoliths of the Alban Hills, Italy volcanic region
pub_title: Crystal chemistry of spinels from xenoliths of the Alban Hills volcanic region Sample: SP263b
formula_title: <missing>
a: 8.1093
b: 8.1093
c: 8.1093
alpha: 90
beta: 90
gamma: 90
cell_volume: 533.274
crystal_density: 3.716
atoms_sites: ["MgT", "FeT", "ZnT", "MnT", "AlT", "SiT", "MgM", "FeM", "AlM", "CrM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgBg/g8A
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgBg/g8A
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgBg/g8A
atoms_occupancy: 0OslAODyCQDwPAAAsJoAAMBHDADQBwAAILoHAFCLAQCAtTMAsAQAACADAAAACT0A
atoms_u_iso: EFkAABBZAAAQWQAAEFkAABBZAAAQWQAAMEMAADBDAAAwQwAAMEMAADBDAADQhAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAQAAAQAAAAAgAAIAAAACAACAAAAEAAIAAACAAQAAAIACAAAEABAAAEACAAAQAQAAEAEAACACAAAAEAAIAQAAQBAACAQAAgEAAQBAAABA==


formula: Mg.845 Fe.235 Zn.008 Mn.019 Al1.886 O4
compound: xenoliths of the Alban Hills, Italy volcanic region
pub_title: Crystal chemistry of spinels from xenoliths of the Alban Hills volcanic region Sample: SP264h
formula_title: <missing>
a: 8.1130
b: 8.1130
c: 8.1130
alpha: 90
beta: 90
gamma: 90
cell_volume: 534.004
crystal_density: 3.735
atoms_sites: ["MgT", "FeT", "ZnT", "MnT", "AlT", "SiT", "MgM", "FeM", "AlM", "CrM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAOAAEAA=
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAOAAEAA=
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAOAAEAA=
atoms_occupancy: kLkkAOChCgDgeQAAkC0BAICrCwCwBAAAcGoHAKjYAQAwujMACAcAAAAJPQA=
atoms_u_iso: wF0AAMBdAADAXQAAwF0AAMBdAADAXQAAMEMAADBDAAAwQwAAMEMAACCAAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAQAAAAAAQAAAgAAAAAgAAIAAAACAACAAAAEAAQAAACAAQAAAIACAAAEABAAAEAEAAAQAQAAEAEAACAEAAAAIAAIAQAAQBAAEAQAAgEAAQCAAABA==


formula: Mg.843 Fe.258 Zn.006 Mn.018 Al1.874 O4
compound: xenoliths of the Alban Hills, Italy volcanic region
pub_title: Crystal chemistry of spinels from xenoliths of the Alban Hills volcanic region Sample: SP264i
formula_title: <missing>
a: 8.1141
b: 8.1141
c: 8.1141
alpha: 90
beta: 90
gamma: 90
cell_volume: 534.221
crystal_density: 3.751
atoms_sites: ["MgT", "FeT", "ZnT", "MnT", "AlT", "SiT", "MgM", "FeM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AIAIQAA==
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AIAIQAA==
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AIAIQAA==
atoms_occupancy: MPskAABUCwCgWgAAYBwBAHA5CwDQBwAAADoHAGg2AgDIkDMAAAk9AA==
atoms_u_iso: oFoAAKBaAACgWgAAoFoAAKBaAACgWgAAEEAAABBAAAAQQAAAkH4AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAQAAAAAAQAAAgAAAAAgAAIAAAACAACAAAAIAAQAAAEAAQAAAIACAAAEABAAAEAEAAAQAQAAEAIAACAEAAAAIAAIAQAAgCAAEAQABAEAAQCAAACA==


formula: Mg.984 Fe.075 Mn.002 Al1.933 Ti.001 O4
compound: xenoliths of the Alban Hills, Italy volcanic region
pub_title: Crystal chemistry of spinels from xenoliths of the Alban Hills volcanic region Sample: SP266a
formula_title: <missing>
a: 8.0978
b: 8.0978
c: 8.0978
alpha: 90
beta: 90
gamma: 90
cell_volume: 531.008
crystal_density: 3.617
atoms_sites: ["MgT", "FeT", "ZnT", "MnT", "AlT", "SiT", "MgM", "FeM", "NiM", "AlM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgAI/A8A
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgAI/A8A
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgAI/A8A
atoms_occupancy: 4DksAMDIAwAQDgAAECcAADDDDACADAAA6OwHAHhpAABYAgAAUJ40ACgKAAAACT0A
atoms_u_iso: cEkAAHBJAABwSQAAcEkAAHBJAABwSQAAgD4AAIA+AACAPgAAgD4AAIA+AACQfgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAACAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAAEAAIAAACAAIAAAEABAAACAAgAACABAAAIAIAACACAABACAAAACAACAIAAIAgABAEAAQBAAIAgAAAQ==


formula: Mg1.004 Fe.071 Zn.003 Al1.911 Ti.008 O4
compound: xenoliths of the Alban Hills, Italy volcanic region
pub_title: Crystal chemistry of spinels from xenoliths of the Alban Hills volcanic region Sample: SP267e
formula_title: <missing>
a: 8.1017
b: 8.1017
c: 8.1017
alpha: 90
beta: 90
gamma: 90
cell_volume: 531.776
crystal_density: 3.612
atoms_sites: ["MgT", "FeT", "ZnT", "MnT", "AlT", "SiT", "MgM", "FeM", "NiM", "AlM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgDYAxAA
atoms_y: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgDYAxAA
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAgIQeAICEHgCAhB4AgIQeAICEHgDYAxAA
atoms_occupancy: 4AgwAPB7AgDAKwAA0AcAALBFCgBgCQAAUJ8GALjsAACQAQAA+DE1AKBBAAAACT0A
atoms_u_iso: wEQAAMBEAADARAAAwEQAAMBEAADARAAA8DwAAPA8AADwPAAA8DwAAPA8AAAQcgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAABAAAAAAAACAAAAIAAAAAAIAAAQAAAAAQAAEAAAABAABAAAAEAAIAAACAAIAAAIABAAACABAAACABAAAQAIAACAEAABACAAAACAAEAIAAQBAABAIAAgBAAIAgAAAg==


formula: (Fe1.22 Al.42 Mg.36) (Be3 Si6) Na.55 (O19 H2)
compound: <missing>
pub_title: Stoppaniite, a new member of the beryl group: crystal structure and crystal-chemical implications
formula_title: <missing>
a: 9.397
b: 9.397
c: 9.202
alpha: 90
beta: 90
gamma: 120
cell_volume: 703.706
crystal_density: 2.843
atoms_sites: ["FeM", "AlM", "MgM", "BeT*", "SiT*", "BeT*", "SiT*", "NaA*", "WatA*", "O1", "O2"]
atoms_x: VVgUAFVYFABVWBQAgIQeAICEHgDwLxcA8C8XAAAAAAAAAAAAUFcSAKDYHQA=
atoms_y: q7AoAKuwKACrsCgAAAAAAAAAAABQhgYAUIYGAAAAAAAAAAAAAMUNABBCCAA=
atoms_z: QEIPAEBCDwBAQg8AQEIPAEBCDwAAAAAAAAAAAAAAAABAQg8AAAAAAOD4CAA=
atoms_occupancy: QDslAEDRDACA/AoAuLAoAEhYFAA4LAoAyNwyAMCRIQAACT0AAAk9AAAJPQA=
atoms_u_iso: IMsAACDLAAAgywAAIMsAACDLAACAuwAAgLsAAMBRAgCgegMAQBkBAMBXAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAABAAAAAAAAAJAACQAAAABAAoBAACAAgAAFEIJQAiGIAAAZSAikAASIiJAakCDMkEQYQNZNVkEJcCIKSVk5HCFOZFxVZRpHM1alAuHdzPVjo3q4Ub9bnVa7Ey42SPv/O67M7O/m3ftFiaD59Q21L6xKq9psE==


formula: Fe2.57 Si.43 O4
compound: <missing>
pub_title: Crystal structure of spinelloid II in the system Fe3O4-Fe2SiO4
formula_title: <missing>
a: 5.85928
b: 17.9801
c: 8.38395
alpha: 90
beta: 90
gamma: 90
cell_volume: 883.253
crystal_density: 4.954
atoms_sites: ["FeM1", "FeM2", "FeM3", "FeM4", "SiT1", "FeT1", "SiT2", "FeT2", "O1", "O2", "O3", "O4", "O5"]
atoms_x: QEIPAEBCDwAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACg4Q8AACMPAA==
atoms_y: QEIPAOAkBQB4LQoAAAAAAECwGQBAsBkAQEIPAEBCDwCQyTIAiPr//1BuCgBAQg8AoPEEAA==
atoms_z: wMYtAMDGLQDwzAEAAAAAAAA5FwAAORcAuKgXALioFwCw4g0AWDkPAJDwEABg6///wMz//w==
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AMA+GgBAyiIAwD4aAEDKIgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: CMAAAODJAAAYsAAAGLoAAFiiAABYogAAaJIAAGiSAADYxwAAMAsBAOAoAQDA1QAAgOMAAA==
atoms_aniso_label: ["FeM1", "FeM2", "FeM3", "FeM4", "SiT1", "FeT1", "SiT2", "FeT2", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: WNkAAMDpAABAqwAAQKsAAIiVAACIlQAAmIoAAJiKAACgwwAAONEAADjRAABACgEAyCIBAA==
atoms_aniso_u22: OLgAAOC6AABgvQAAOLgAAOioAADoqAAA8JYAAPCWAAAo4QAAeFkBAAAhAgDgvwAAaKsAAA==
atoms_aniso_u33: ULQAAIC2AABopgAAOMcAAOCmAADgpgAAyJsAAMibAAAgsgAAUPoAAJiFAACYtwAAgN4AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAASPT//w==
atoms_aniso_u13: uAsAAKgCAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAY/P//oDIAAA==
atoms_aniso_u23: AAAAAAAAAADA/v//wP7///AFAADwBQAAAAAAAAAAAABo/P//0EgAACANAAAAAAAASO///w==
qdat:
AAAAAAAAAAACABAAAAAAAFAICgAEAAALAAQqACoAAeKyAQEHAEgsRJK7IASNGmeJH2kgJkCFVHy7DqV04kO5CNIWw88gYxq13KBKjOntRT1V+rSHHXPnTp9u2khu1+a/BfnZjs9ZqVmtZJo3c3n5nYLMmbE0binCS/R6k6==


formula: (K3.6 Na1.4) Fe4.95 Mn.72 Mg.63 Ca.18 Si20 O68 H30
compound: Kola Peninsula, Russia
formula_title: <missing>
a: 14.86
b: 20.54
c: 5.29
alpha: 95.6
beta: 92.3
gamma: 94.4
cell_volume: 1600.349
crystal_density: 2.274
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Kalifersite, a new alkaline silicate from Kola Peninsula (Russia)
 based on a palygorskite-sepiolite polysomatic series

atoms_sites:
["K1", "Na1", "K2", "Na2", "K3", "Na3", "Fe1", "Mn1", "Mg1", "Ca1", "Fe2", "Mn2", "Mg2", "Ca2", "Fe3", "Mn3", "Mg3", "Ca3", "Fe4", "Mn4", "Mg4", "Ca4", "Fe5", "Mn5", "Mg5", "Ca5", "Si1", "Si2", "Si3", "Si4", "Si5", "Si6", "Si7", "Si8", "Si9", "Si10", "O1", "O-H2", "O-H2", "O4", "O5", "O6", "O7", "O-H7", "O8", "O9", "O-H9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "O17", "O18", "O19", "O20", "O21", "O22", "O23", "O24", "O25", "O26", "O27", "O28", "Wat29", "Wat30", "Wat31", "Wat32", "Wat33", "Wat34"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

qdat:
AAAAAQAgAgIAAgQEAEQBE1aIJjYRYRrkSIq44S5DLW910d6vLH7JXvc9a/sz3fl+u/vv+/1+b67738dX9/7fex/3e9ffvdzf37a/3Ttud+0X1x/X3sv5z/mtz//z/qfj726t+8TcqZnG1Ju+O3Y6vx/u3r0qxGybu6759f==


formula: Ca2.864 Mn.025 Na.019 Ni.002 Mg.112 Al.222 V.144 Ti.827 Fe1.426 Si2.358 O12
compound: Baden-Wurtemburg, Germany
pub_title: Crystal chemistry of Ti-bearing andradites Note: sample KB166
formula_title: <missing>
a: 12.122
b: 12.122
c: 12.122
alpha: 90
beta: 90
gamma: 90
cell_volume: 1781.241
crystal_density: 3.805
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABg4xYAYOMWAGDjFgDAUQIA
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACg7gIA
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAgoQcAAAAAAAAAAAAAAAAAAAAAAAAAAABAQg8AQEIPAEBCDwDo5ScA
atoms_occupancy: MEU6ALCBAABwYgAA8AoAALAEAAAQ0AEAsLMAAGDGBgAAZQQAwOsSADA+HgBA+S8AIDYEAKDZCAAACT0A
atoms_u_iso: 0J0AANCdAADQnQAA0J0AANCdAADQnQAAaH4AAGh+AABofgAAaH4AAGh+AAAAfQAAAH0AAAB9AABguAAA
atoms_aniso_u11: QLUAAEC1AABAtQAAQLUAAEC1AABAtQAAkH4AAJB+AACQfgAAkH4AAJB+AACgcwAAoHMAAKBzAAAg5AAA
atoms_aniso_u22: QLUAAEC1AABAtQAAQLUAAEC1AABAtQAAkH4AAJB+AACQfgAAkH4AAJB+AACwgQAAsIEAALCBAACgpQAA
atoms_aniso_u33: 8G4AAPBuAADwbgAA8G4AAPBuAADwbgAAkH4AAJB+AACQfgAAkH4AAJB+AACwgQAAsIEAALCBAACAogAA
atoms_aniso_u12: cDAAAHAwAABwMAAAcDAAAHAwAABwMAAAsAQAALAEAACwBAAAsAQAALAEAAAAAAAAAAAAAAAAAADg4///
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAsAQAALAEAACwBAAAsAQAALAEAAAAAAAAAAAAAAAAAACgKAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAsAQAALAEAACwBAAAsAQAALAEAAAAAAAAAAAAAAAAAABQ+///
atoms_sites:
["CaX", "MnX", "NaX", "NiX", "KX", "MgX", "MgY", "AlY", "VY", "TiY", "FeY", "SiZ", "TiZ", "FeZ", "O"]

atoms_aniso_label:
["CaX", "MnX", "NaX", "NiX", "KX", "MgX", "MgY", "AlY", "VY", "TiY", "FeY", "SiZ", "TiZ", "FeZ", "O"]

qdat:
AAAAAAAAAAAAAAAAAAAAAQAAEAAAAAAAIAEAAACAEAIAgAAIBAAAAICAgACBAQIECAAAgQQQIIIAIIAQQggCCEIQQgCAIhCEAiAAiEQiIBEQCACIiAgBEAAiIEQAgAAgAAAgAAAAAAABIAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca2.895 Mn.024 Na.018 Mg.104 Al.224 Ti.703 Fe1.288 Si2.744 O12
compound: N'Zala, Atlas mountains, Morocco
pub_title: Crystal chemistry of Ti-bearing andradites Note: sample NZALA
formula_title: <missing>
a: 12.105
b: 12.105
c: 12.105
alpha: 90
beta: 90
gamma: 90
cell_volume: 1773.758
crystal_density: 3.752
atoms_sites: ["CaX", "MnX", "NaX", "MgX", "MgY", "AlY", "TiY", "FeY", "SiZ", "TiZ", "FeZ", "O"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABg4xYAYOMWAGDjFgD4WgIA
atoms_y: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABg8gIA
atoms_z: IKEHACChBwAgoQcAIKEHAAAAAAAAAAAAAAAAAAAAAABAQg8AQEIPAEBCDwAA8ScA
atoms_occupancy: IOY6AAB9AADAXQAAIEgBAFBAAQAA1gYAoCASABDSIgAw1DcAMDcCAKD9AgAACT0A
atoms_u_iso: iHcAAIh3AACIdwAAiHcAAChaAAAoWgAAKFoAAChaAACgWgAAoFoAAKBaAACgjAAA
atoms_aniso_label: ["CaX", "MnX", "NaX", "MgX", "MgY", "AlY", "TiY", "FeY", "SiZ", "TiZ", "FeZ", "O"]
atoms_aniso_u11: gIkAAICJAACAiQAAgIkAAChaAAAoWgAAKFoAAChaAADQUgAA0FIAANBSAADAqAAA
atoms_aniso_u22: gIkAAICJAACAiQAAgIkAAChaAAAoWgAAKFoAAChaAABQXwAAUF8AAFBfAADQhAAA
atoms_aniso_u33: YFQAAGBUAABgVAAAYFQAAChaAAAoWgAAKFoAAChaAABQXwAAUF8AAFBfAABQeAAA
atoms_aniso_u12: 8CMAAPAjAADwIwAA8CMAADgEAAA4BAAAOAQAADgEAAAAAAAAAAAAAAAAAAAQ9f//
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAADgEAAA4BAAAOAQAADgEAAAAAAAAAAAAAAAAAABwFwAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAADgEAAA4BAAAOAQAADgEAAAAAAAAAAAAAAAAAAAw+P//
qdat:
AAAAAAAAAAAAAAAAAAAAAQAAEAAAAAAAIACAAACACAIAQAAIAgAAAICAgACAgQIECAAAQQIIIEIAEIAIQQQBBCEIQgBAIQhEARAARCIhEAiICABERAQAiAAJECIAQAAQAAAQAAAAAAAAiAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca2.919 Mn.012 Na.003 Mg.048 Fe1.412 Al.278 Ti.328 Si3 O12
compound: Zermatt, Valais, Switzerland
pub_title: Crystal chemistry of Ti-bearing andradites Note: sample ZER1
formula_title: <missing>
a: 12.060
b: 12.060
c: 12.060
alpha: 90
beta: 90
gamma: 90
cell_volume: 1754.050
crystal_density: 3.765
atoms_sites: ["CaX", "MnX", "NaX", "MgX", "FeX", "AlY", "TiY", "FeY", "SiZ", "O"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABg4xYAgF8CAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwAAAAAAAAAAAAAAAAAAAAAAWPACAA==
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAAAAAAAAAAAAAAAABAQg8A4PInAA==
atoms_occupancy: IGM7AIA+AACgDwAAAPoAAMBdAADgewgAgAIKAKCKKgAACT0AAAk9AA==
atoms_u_iso: GG8AABhvAAAYbwAAGG8AABhvAABwTgAAcE4AAHBOAAAgTgAAAH0AAA==
atoms_aniso_label: ["CaX", "MnX", "NaX", "MgX", "FeX", "AlY", "TiY", "FeY", "SiZ", "O"]
atoms_aniso_u11: AH0AAAB9AAAAfQAAAH0AAAB9AAAgTgAAIE4AACBOAADARAAAYIYAAA==
atoms_aniso_u22: AH0AAAB9AAAAfQAAAH0AAAB9AAAgTgAAIE4AACBOAABAUQAAsIEAAA==
atoms_aniso_u33: 0FIAANBSAADQUgAA0FIAANBSAAAgTgAAIE4AACBOAABAUQAAEHIAAA==
atoms_aniso_u12: ABkAAAAZAAAAGQAAABkAAAAZAAB4AAAAeAAAAHgAAAAAAAAAUPv//w==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAB4AAAAeAAAAHgAAAAAAAAAYAkAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAB4AAAAeAAAAHgAAAAAAAAAAAAAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAIAAEAAAAAAAEACAAABACAEAIAAEAQAAAEBAIABAQICBAgAAIEECCCCACCAEEEIAQQhCEIAgCEIRAEQAEQiEQgIiAQAREQEAEQACIgRACAACAAACAAAAAAAAEQAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca2.934 Mn.048 Na.012 Mg.056 Al.496 V.056 Ti.299 Fe1.306 Si2.793 O12
compound: Schaffhausen area, Switzerland
pub_title: Crystal chemistry of Ti-bearing andradites Note: sample SCHAFF
formula_title: <missing>
a: 12.038
b: 12.038
c: 12.038
alpha: 90
beta: 90
gamma: 90
cell_volume: 1744.468
crystal_density: 3.775
atoms_sites: ["CaX", "MnX", "NaX", "MgX", "MgY", "AlY", "VY", "TiY", "FeY", "SiZ", "TiZ", "FeZ", "O"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAYOMWAGDjFgBg4xYAIFsCAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA4OoCAA==
atoms_z: IKEHACChBwAgoQcAIKEHAAAAAAAAAAAAAAAAAAAAAAAAAAAAQEIPAEBCDwBAQg8AwOonAA==
atoms_occupancy: QLE7AAD6AACAPgAAQB8AAKCGAQAAIw8AgLUBAADWBgDg0yMA4NI4AKCGAQCArwIAAAk9AA==
atoms_u_iso: cHsAAHB7AABwewAAcHsAAFhwAABYcAAAWHAAAFhwAABYcAAA8FUAAPBVAADwVQAA8IcAAA==
atoms_aniso_label: ["CaX", "MnX", "NaX", "MgX", "MgY", "AlY", "VY", "TiY", "FeY", "SiZ", "TiZ", "FeZ", "O"]
atoms_aniso_u11: wI8AAMCPAADAjwAAwI8AAIBwAACAcAAAgHAAAIBwAACAcAAAsE8AALBPAACwTwAAwI8AAA==
atoms_aniso_u22: wI8AAMCPAADAjwAAwI8AAIBwAACAcAAAgHAAAIBwAACAcAAAEFkAABBZAAAQWQAAMI4AAA==
atoms_aniso_u33: 0FIAANBSAADQUgAA0FIAAIBwAACAcAAAgHAAAIBwAACAcAAAEFkAABBZAAAQWQAA4HkAAA==
atoms_aniso_u12: ECcAABAnAAAQJwAAECcAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA4Pz//w==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA0AcAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAYAkAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAAEABAAABABACAIAACAQAAACAgIAAgIECAgQAAECCCBBBABBABCEEAIQQhCEAQBCEIQCEACEQiIQEQgIAIRIBACIAAkQIgBAABAAABAAAAAAAABIAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca1.588 Fe1.001 Mn.691 Mg.006 Al1.698 Ti.015 Si3 O12
compound: Okahandja, Namibia
pub_title: Crystal chemistry of Ti-bearing andradites Note: sample NAMIB
formula_title: <missing>
a: 11.764
b: 11.764
c: 11.764
alpha: 90
beta: 90
gamma: 90
cell_volume: 1628.040
crystal_density: 3.920
atoms_sites: ["CaX", "FeX", "MnX", "NaX", "MgX", "AlY", "TiY", "FeY", "SiZ", "O"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABg4xYACEECAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwAAAAAAAAAAAAAAAAAAAAAAENkCAA==
atoms_z: IKEHACChBwAgoQcAIKEHACChBwAAAAAAAAAAAAAAAABAQg8A2NInAA==
atoms_occupancy: 4E8gAMCGDgBwDg4AsAQAAEAfAAAQ0DMAMHUAAMDDCAAACT0AAAk9AA==
atoms_u_iso: YHwAAGB8AABgfAAAYHwAAGB8AACwTwAAsE8AALBPAAAgTgAAsIEAAA==
atoms_aniso_label: ["CaX", "FeX", "MnX", "NaX", "MgX", "AlY", "TiY", "FeY", "SiZ", "O"]
atoms_aniso_u11: AJYAAACWAAAAlgAAAJYAAACWAACwTwAAsE8AALBPAABwYgAAoKUAAA==
atoms_aniso_u22: AJYAAACWAAAAlgAAAJYAAACWAACwTwAAsE8AALBPAADARAAA4HkAAA==
atoms_aniso_u33: AEsAAABLAAAASwAAAEsAAABLAACwTwAAsE8AALBPAADARAAAAGQAAA==
atoms_aniso_u12: sB0AALAdAACwHQAAsB0AALAdAACQGgAAkBoAAJAaAAAAAAAAcBcAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAACQGgAAkBoAAJAaAAAAAAAAoPb//w==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAACQGgAAkBoAAJAaAAAAAAAA0AcAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAABAAAQAAAAAAAIACAAABABACAIAABAIAAABAICAAICAgQECAAAQQIEEEEACCAEEEEAIQQhBCAIAhCEIAiAAhEIhEAhEBAAiIgEAIQACIgJACAABAAAAgAAAAAAAASAAAAAAAAAAAAAAAAAAAAA==


formula: Ca Zn8 S2 O29 Cl2 H36
compound: slag dumps at Val Varenna, Italy
formula_title: Ca[Zn8(SO4)2(OH)12Cl2](H2O)9
a: 8.3797
b: 8.3797
c: 68.123
alpha: 90
beta: 90
gamma: 120
cell_volume: 4142.679
crystal_density: 2.882
atoms_sites: ["Ca", "Zn1", "Zn2", "S", "O1", "O2", "O3", "O4", "Cl", "Wat5", "Wat6", "H1", "H2", "H3"]
atoms_x: q7AoAKBxEQAAAAAAVVgUAFVYFACgzxIA0DodALB+9P8AAAAAALY1AKuwKAAATB0AgJLy/8CKNwA=
atoms_y: VVgUABBZGQAAAAAAq7AoAKuwKADw8TEAQOAWAKB6AwAAAAAAwNwhADAhJwAA+RUAAOIEAAAQJwA=
atoms_z: CBYFAADx///IZv7/yI8CAGA1AQDY/AIAqNQAAIjx/v94Xvz/YI0DAAgWBQAAdwEAwGn+/4CpAwA=
atoms_occupancy: 0
atoms_u_iso: MKEBAJAUAQCQFAEAACwBAPA2AQCw+AEAMPIAAOAoAQBwCwIA0KoCAMAyAwBADQMAQA0DAEANAwA=
atoms_aniso_label: ["Ca", "Zn1", "Zn2", "S", "O1", "O2", "O3", "O4", "Cl", "Wat5", "Wat6"]
atoms_aniso_u11: 4NcBAKC+AABw3wAAkBQBAJAtAQDQiwMAIOQAAEBLAQCQQAIAII0CADDHAwA=
atoms_aniso_u22: 4NcBAIDUAABw3wAAkBQBAJAtAQBQCAIAkMkAAJAUAQCQQAIAkEACAEDbAgA=
atoms_aniso_u33: sDABAGCyAQDQfgEAUFkBACBIAQAgLwEA0DMBAFByAQCgnwEA0MMCAPBDAwA=
atoms_aniso_u12: 8OsAANBrAADwbgAAEIsAAACWAABQCAIAMHUAAKDXAAAQIQEAAOEAANDiAQA=
atoms_aniso_u13: AAAAACADAAAAAAAAAAAAAAAAAACgkv//QO3//xD1//8AAAAAkH4AAKAoAAA=
atoms_aniso_u23: AAAAACAcAAAAAAAAAAAAAAAAAADwjf//wBIAAMASAAAAAAAAcGIAAFAUAAA=
pub_title:
 The crystal structure of Ca[Zn8(SO4)2(OH)12Cl2](H2O)9,
 a new phase from slag dumps at Val Varenna, Italy

qdat:
AAAAAAAAAQAAAABCAAAgAgAAAkCAEkAICAAAAAaiQQAIIAAAAAxB6UIAABgiAAA5SAZEAAAAYRA0fpAAKxAAAACh6QUQAAD1AAAAp9QA7QAAApAAD6HOkAaQAAANQr5APRQAcgAAAD0VAAegJQHoAAr0rcAAaAAAD0Do0A==


formula: Mg2.218 Ga3.557 Ge1.225 O10
compound: <missing>
pub_title: Crystal structures of sapphirine and surinamite analogues in the MgO-Ga2O3-GeO2 system
formula_title: <missing>
a: 8.822
b: 9.794
c: 10.256
alpha: 63.82
beta: 84.77
gamma: 65.32
cell_volume: 717.875
crystal_density: 5.097
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["MgM1", "GaM1", "MgM2", "GaM2", "MgM3", "GaM3", "MgM4", "GaM4", "MgM5", "MgM6", "MgM7", "GaM7", "MgM8", "GaM8", "MgM9", "GaM9", "GaT1", "GeT1", "GaT2", "GeT2", "GaT3", "GeT3", "GaT4", "GeT4", "GaT5", "GeT5", "GaT6", "GeT6", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "O17", "O18", "O19", "O20"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAAAAAAAAEAwQQAAIACCBFgooiIBJQHAYjj4QcIHILU/QzNdWJ2279d6g/Tfajv73uu77fqX+/53/3/v3//yv/6///9/7/v/////f99+9//////7//r//////2e/f/N/fP5v15vSP+wNNU7zIycOuBkAM0BCIIgGIAoC==


formula: Mg8.078 Ga7.842 Ge6.08 O32
compound: <missing>
pub_title: Crystal structures of sapphirine and surinamite analogues in the MgO-Ga2O3-GeO2 system
formula_title: <missing>
a: 10.320
b: 23.733
c: 10.073
alpha: 90
beta: 110.29
gamma: 90
cell_volume: 2314.039
crystal_density: 4.870
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["MgM1", "MgM2", "GaM2", "MgM3", "GaM3", "MgM4", "GaM4", "MgM5", "GaM5", "MgM6", "GaM6", "MgM7", "GaM7", "MgM8", "MgM9", "GaM9", "GaT1", "GeT1", "GeT2", "GaT3", "GeT3", "GeT4", "GaT5", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAAAAABAACAAQAASEABCYJEAEA/ABACAcugiyIieEKbcKSF4LKiBZ3bD8hYndejOm8NAV39Fttv8nlo556tUulO91sXW70F27p//+ZV5ZTd+d/9d2fN/397K5o07VqrmLs0mRzpLG9RpkG3ubLgspBBasrglAaABzMiB==


formula: Sb O2
compound: Cetine mine, Siena, Italy
formula_title: <missing>
a: 12.061
b: 4.836
c: 5.383
alpha: 90
beta: 104.60
gamma: 90
cell_volume: 303.836
crystal_density: 6.722
atoms_sites: ["Sb1", "Sb2", "O1", "O2"]
atoms_x: QEIPAAAAAADgtAsAMLsFAA==
atoms_y: QEIPALBmEQDQJwMAoCgZAA==
atoms_z: AAAAAEBCDwCgLCkAkOQ6AA==
atoms_occupancy: 0
atoms_u_iso: aDMAANhoAADobAAA8GQAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Clinocervantite, B-Sb2O4, the natural monoclinic polymorph
 of cervantite from the Cetine mine, Siena, Italy
 Note: z-coordinate to O2 altered by communications with R Basso, April, 2003

qdat:
AAAAAAAAAAAAAAAAAAgAAAAEAAAAAAAAIAEBAAAAQAAIAABBkBAABBAAQBggIACACCFAAoJBABRyAAQhIAADYFGAFiKKAGAEghAjMQgDAckUCMBDEINFKYYAHBFAC4IGwZg1CqRg1TkMCsARwuWIkEpJWdCgxasDRmnI6R==


formula: Cu3 Mo.742 S1.258 O9
compound: <missing>
formula_title: <missing>
a: 7.421
b: 6.754
c: 13.624
alpha: 90
beta: 90
gamma: 90
cell_volume: 682.854
crystal_density: 4.340
atoms_sites: ["Cu1", "Cu2", "Cu3", "Mo1", "S1", "S2", "O1", "O2", "O3", "O4", "O5", "O6", "O7"]
atoms_x: AAAAAHARMwAwFSkAIJ4tACCeLQAwehQAgHE2AKA6LwCAkSAAkAUQABDjNADw6SoAAE0hAA==
atoms_y: AAAAAMC98P/AvfD/QEIPAEBCDwDAvfD/wL3w/8C98P/AvfD/EJD7/9B4AgBAQg8AQEIPAA==
atoms_z: gIQeAMDQFACo6iEAqA0TAKgNEwDAShgAoEIdAJBoDAAw3xgAYEgbAKAnFQAwsAsAoNAWAA==
atoms_occupancy: AAk9AAAJPQAACT0AwEktAEC/DwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: oEABADjBAQAgxQEA0C4BANAuAQDYhQEA0CQBAMhmAwCQFwMAeAgCAHAGAgAw3AIA0KACAA==
atoms_aniso_label: ["Cu1", "Cu2", "Cu3", "Mo1", "S1", "S2", "O1", "O2", "O3", "O4", "O5", "O6", "O7"]
atoms_aniso_u11: kMkAAAD0AQBASwEAIMsAACDLAAAAEwEAAPoAAOCTBADgKAEAIEgBAIC1AQCAMgIAIMUBAA==
atoms_aniso_u22: kPsAADBWAQDwNgEAUPUAAFD1AAAARQEAAPoAAOAiAgAgQgIAwNQBAECWAQDgpQEAwFECAA==
atoms_aniso_u33: sDABAODdAABArwEAwAwBAMAMAQDgQQEAIMsAAGBnAQBg2AMAgLUBAKCGAQCg/QIAIEICAA==
atoms_aniso_u12: oPb//wAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgMH//+AuAAAAAAAAAAAAAA==
atoms_aniso_u13: oPb//xDc//8AlgAAMPj//zD4//+wHQAAgD4AAAAAAADA2gAAQB8AAGDw//9Aov//wNoAAA==
atoms_aniso_u23: sOv//wAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAoA8AAKCS//8AAAAAAAAAAA==
pub_title:
 The crystal structure of vergasovaite Cu3O[(Mo,S)O4SO4],
 and its relation to synthetic Cu3O[MoO4]2

qdat:
AAAAAAAAAAAAAAAIgIAABAIAAAghQQCwQRCiEYACA2ijGjQTQQSoohuml+EwPku7vkSidZ/4/Xe1fs8eNxft/r9v27XtJ29ff3n66enNv16+r/83de/1r/3oX+r+s/17/+/v/+6+v/f3++//Pe+/3+979/6v//7ff3a6z/==


formula: Si2 O8 Na H6
compound: <missing>
formula_title: <missing>
a: 4.946
b: 20.510
c: 7.277
alpha: 90
beta: 90
gamma: 90
cell_volume: 738.197
crystal_density: 1.918
atoms_sites: ["Si", "O1", "O2", "O3", "Na", "Wat4", "Wat5"]
atoms_x: ANUCAAAAAADw0RUAQDgAAAAAAADIzQAAAAAAAA==
atoms_y: MNcRAIAKKgCQUBAAUNsVAADIAADAwgQAQO8gAA==
atoms_z: IKv9/0BCDwAQFP//wMIEAEBCDwDgOv7/QEIPAA==
atoms_occupancy: 0
atoms_u_iso: wNoAAKCGAQCghgEAoIYBAEATAgCArwIAAFMHAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structure solution from powder data of the hydrous layer
 silicate kanemite, a precursor of the industrial ion exchanger SKS-6

qdat:
AAAAAAAAAAQAAAAAACAAEBAAAgQEBBGACRAKQQBBBUoNohApYQm0akcQA8XHGscTSethVC0m7yJT3mYXBgKmTrt56mxyNgk/eZdNrUPksut/v7aeSkv8a0v13t7yqbU27uv//39z/3T/5xVz6/fee75v+z33ffn7ov3o18==


formula: (Ca.483 Na.412 K.105) Li2 Al7 Si6 B3 F.327 O30.672 H3.291
compound: Madagascar
formula_title: <missing>
a: 15.880
b: 15.880
c: 7.118
alpha: 90
beta: 90
gamma: 120
cell_volume: 1554.496
crystal_density: 3.002
atoms_x: AAAAAAAAAAAAAAAAGEU5ABhFOQBQJRIAQLkLACCsBgBwWDwAcFg8AHBYPADwchAAMLMDAMilBQAQSQsAWAAMAJByEQDwywwA
atoms_y: AAAAAAAAAAAAAAAA6MMDAOjDAwCo4w8A4JsLAOBcNgCQsAAAkLAAAJCwAAB4OQgA0FU5AJBLCwCIpAUAmGYLAFBxEQBIfxAA
atoms_z: sEYOALBGDgCwRg4AkGImAJBiJgBoSiUAmO///wCjGwDABTAAwAUwAMAFMABQCR8A4C8dAHBjBACguQUA8E4vALDmBAAQ6RoA
atoms_occupancy: 4HodAIAlGQCgaAYAuLAoAEhYFAAACT0AAAk9AAAJPQAgpwYAYMAHAKDrBQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: MH8AADB/AAAwfwAAIIUAACCFAAAwXAAAiEoAAMhuAABQ9QAAUPUAAFD1AABApgAAkDwBAIiQAAB4lgAAoIIAANBwAACIhgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Homogeneous liddicoatite from Madagascar: a possible
 reference material? First EMPA, SIMS and SREF data
 Sample: 1

atoms_sites:
["CaX", "NaX", "KX", "LiY", "AlY", "AlZ", "Si", "B", "F1", "O1", "O-H1", "O-H1", "O2", "O3", "O4", "O5", "O6", "O7"]

qdat:
AAAAAAAAAAAAAQAAEAAAAQBAAgIAAAIQARBCIAAERAJAZCgESDAGhABIREgIFIaEhgqGlpQMGFxQUUOeXHPDDDliKrD1KFG8WwRdoBJYxvHuYxWJXwNQiAurLnMeKQ2LhVhBG0c5Cic1TAlQouAL0SJE0RJIkoTRBEyggS==


formula: Ca.452 Na.435 K.04 Li2 Al7 Si6 B3 F.327 O30.672 H3.39
compound: Madagascar
formula_title: <missing>
a: 15.882
b: 15.882
c: 7.115
alpha: 90
beta: 90
gamma: 120
cell_volume: 1554.232
crystal_density: 2.993
atoms_x: AAAAAAAAAAAAAAAAKEQ5AChEOQCIJBIAGLkLABCtBgAAWjwAAFo8AABaPACAdBAA2LADAHilBQAQSQsAsP0LANhwEQBozAwA
atoms_y: AAAAAAAAAAAAAAAA2MQDANjEAwAw4w8AkJsLAPBbNgAArwAAAK8AAACvAABAOggAKFg5APBKCwCIpAUAaGQLAIBuEQA4gBAA
atoms_z: EGkOABBpDgAQaQ4AQIAmAECAJgAIZCUA6AgAAEDCGwAgDzAAIA8wACAPMAAwHx8AAEwdAAB+BAAQ0QUAgGkvAEABBQBQCBsA
atoms_occupancy: gJYbAOCMGgAAcQIAuLAoAEhYFAAACT0AAAk9AAAJPQAgpwYAwLwFAEDvBwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: oIIAAKCCAACgggAA6IAAAOiAAAAYWwAAQEcAAOBqAAAgBwEAIAcBACAHAQAoqgAAkDwBAGiSAABwlAAAsHwAAMhuAACgggAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Homogeneous liddicoatite from Madagascar: a possible
 reference material? First EMPA, SIMS and SREF data
 Sample: 2

atoms_sites:
["CaX", "NaX", "KX", "LiY", "AlY", "AlZ", "Si", "B", "F1", "O1", "O-H1", "O-H1", "O2", "O3", "O4", "O5", "O6", "O7"]

qdat:
AAAAAAAAAAAAAQAAEAAAAQBAAgIAAAIQARBCIAAERAJAZCQESDAGiABIJEgIJIaEhgqGlpQMGFxwMUOeXHPCjDkhKrD1cFG8WwRdoBJYxvDuIxWJWwNQiAuvJjMdGQ2LRVxBG0c5CiM1RAnQYuBLsTJEqRJkkobRAkyggR==


formula: K.94 Na.03 Al2.43 Mg.04 Fe.34 Si3.24 O11.88 F.12 H1.88
compound: <missing>
formula_title: <missing>
a: 5.21397
b: 9.0521
c: 19.9968
alpha: 90
beta: 95.736
gamma: 90
cell_volume: 939.071
crystal_density: 2.887
atoms_x: AAAAAAAAAADwFA8A8BQPAPAUDwAQYBwAEGAcAHC6GwBwuhsAYE4aAHC9DgBgrw4AIPEbAFDoFwDAGRwAwBkcAAD5FQA=
atoms_y: QLAFAECwBQAwDAUAMAwFADAMBQCwwTgAsME4ANDADwDQwA8AsK4FAEDtMQDwHBYAIIg5APBfDwBQdCIAUHQiAIDLJwA=
atoms_z: QEIPAEBCDwDwCgAA8AoAAPAKAADwPggA8D4IAGBWCABgVggAAEEKAHDCCQDAUwoAIDwDAMBLAwBwHgMAcB4DABB5AwA=
atoms_occupancy: gF85AMDUAQDg9jIAgDgBAEBgCgDANzAAQNEMAMCoMgBAYAoAAAk9AAAJPQAACT0AAAk9AAAJPQCAXzkAgKkDAIBfOQA=
atoms_u_iso: wFcBAMBXAQDAiQEAwIkBAMCJAQBAGQEAQBkBAGDqAABg6gAAkJEBAGAvAgBg5AEAQJYBABAIAQBAlgEAQJYBAAASegA=
atoms_aniso_label: ["H"]
atoms_aniso_u11: YNIEAA==
atoms_aniso_u22: AGsDAA==
atoms_aniso_u33: 4BAFAA==
atoms_aniso_u12: gLsAAA==
atoms_aniso_u13: AIP//w==
atoms_aniso_u23: AAAAAA==
pub_title:
 Tetrahedral order in phengite 2M_1 upon heating, from powder
 neutron diffraction, and thermodynamic consequences
 Sample: T = 293 K
 Note: O5 z-coordinate altered.

atoms_sites:
["K", "Na", "AlM2", "MgM2", "FeM2", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O6", "F6", "H"]

qdat:
AAAAAAAAAAEAAAAAAAAAAgAaIEIAgQAMCAAgCAAQZAyFAQMMjRFAKSEJgEEaAbsnIcQlIf1UlSTESAmgqeWGveLTUEkimzOyU1RSL+54sJvv1LTvI6RLamKplUPYlhwuVevnXJ3ELQhUxt11YmbpI0sJmvkuxKiGIMRZk0==


formula: K.94 Na.03 Al2.43 Mg.04 Fe.34 Si3.24 O11.88 F.12 H1.88
compound: <missing>
formula_title: <missing>
a: 5.23899
b: 9.1048
c: 20.2440
alpha: 90
beta: 95.684
gamma: 90
cell_volume: 960.890
crystal_density: 2.822
atoms_x: AAAAAAAAAABwOg8AcDoPAHA6DwCwVhwAsFYcANB4GwBAkBsAUCQOAGAyDgBAWBwA8BAYAFDpGwBQ6RsAwFYWAA==
atoms_y: AF8FAABfBQAw8wQAMPMEADDzBABQnzgAUJ84APD1DwCAzwUAQDgyAOCRFQBQgDkAIHEPAKBvIgCgbyIAAHQnAA==
atoms_z: QEIPAEBCDwBAHwAAQB8AAEAfAACAJwgAgCcIAGA9CADAOgoAIK4JAIBNCgAQRwMAIFUDAND1AgDQ9QIAoPcDAA==
atoms_occupancy: gF85AMDUAQDg9jIAgDgBAEBgCgCA1yUAgDEXAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AIBfOQCAqQMAgF85AA==
atoms_u_iso: oP0CAKD9AgBQCAIAUAgCAFAIAgCghgEAoIYBAGDqAADAzgIAwEsDAGBhAgDgnwIAIMUBAGDeAgBg3gIAABJ6AA==
atoms_aniso_label: ["H"]
atoms_aniso_u11: wJgLAA==
atoms_aniso_u22: wEsDAA==
atoms_aniso_u33: wAkOAA==
atoms_aniso_u12: 4KsAAA==
atoms_aniso_u13: wNQBAA==
atoms_aniso_u23: wM4CAA==
pub_title:
 Tetrahedral order in phengite 2M_1 upon heating, from powder
 neutron diffraction, and thermodynamic consequences
 Sample: T = 873 K

atoms_sites:
["K", "Na", "AlM2", "MgM2", "FeM2", "SiT1", "AlT1", "SiT2", "O1", "O2", "O3", "O4", "O5", "O6", "F6", "H"]

qdat:
AAAAAAAAAAIAAAAAAAAABAAyQQQBAgAwEACAIABA8DEiBAo0OIUB5IgqBAigDqy4jjCxC9pUkRZCQIkJK4yvzxs8gpQp0asSTUMi67eJCe97Tk2iWsl17jU53F+ZYYdFu2rNkqhFkRI0Za0kbszUcWJyvqWxORGIKQ9qky==


formula: Si7 Al Mg5 Ca2 Na O22 F2
compound: <missing>
pub_title: A neutron powder diffraction study of cation ordering in high-temperature synthetic amphiboles
formula_title: <missing>
a: 9.8535
b: 18.0154
c: 5.2752
alpha: 90
beta: 104.892
gamma: 90
cell_volume: 904.973
crystal_density: 3.076
atoms_x: oCYRAKAmEQCAoBEAAAAAAAAAAAAAAAAAAAAAAAAAAABAwwYAoEkHAGBJBgDwNRYAAEoVAOAUFQDg4hQA
atoms_y: wCYFAMAmBQDQegoA8GkFAAC+CgAAAAAAAP4QAICEHgAALQUAEGgKAAAAAAAwNA8A4EkIAAAhBwAAAAAA
atoms_z: IF8SACBfEgCwVTEAgIQeAAAAAAAAAAAAgIQeAAAAAAAgZA0AgGIsAGCXKwCgNDAAAFkGAPCpJADwOhEA
atoms_occupancy: wMYtAEBCDwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: IBwAACAcAAAwKgAA0DkAAGA7AACwaAAAoL4AAADECQAQQAAAAGQAABByAADAXQAAsIEAANBrAABwlAAA
atoms_aniso_label: ["NaA2/m"]
atoms_aniso_u11: wJgLAA==
atoms_aniso_u22: AE0IAA==
atoms_aniso_u33: IHcOAA==
atoms_aniso_u12: AAAAAA==
atoms_aniso_u13: oMEMAA==
atoms_aniso_u23: AAAAAA==
atoms_sites:
["SiT1", "AlT1", "SiT2", "MgM1", "MgM2", "MgM3", "CaM4", "NaA2/m", "O1", "O2", "F3", "O4", "O5", "O6", "O7"]

qdat:
AAAAAAAAAAACEAAAAAAAEAgKBAIAAAAggGBCAIBAEwSEgEEQUCBMqXIIYG4YBHyGgDg1EZleBArJh0HgCB4iHZZ8isMoD57IpiwUOXGZoM5kGM6rrCgJitsbwTzVLJPqslOWHgDeriGegUCuYqTdsjRVHakq0Q0Ax6UB+g==


formula: Na Mg4 Al3 Ca2 Si6 O24 H2
compound: <missing>
pub_title: A neutron powder diffraction study of cation ordering in high-temperature synthetic amphiboles
formula_title: <missing>
a: 9.8930
b: 17.937
c: 5.2802
alpha: 90
beta: 105.518
gamma: 90
cell_volume: 902.819
crystal_density: 3.075
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["NaA2/m", "MgM1", "MgM2", "AlM2", "MgM3", "AlM3", "CaM4", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "H"]

atoms_x:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAPAhEQDwIREAQJoRAECaEQDghwYAcFEHANB5BgCgUxYAkEsVAMD4FABg1hQAUHsMAA==

atoms_y:
gIQeAJBgBQCQvwoAkL8KAAAAAAAAAAAAQB0RAFBBBQBQQQUAYJUKAGCVCgAgSQUA4IgKAAAAAACgSw8A8IkIAHDtBgAAAAAAAAAAAA==

atoms_z:
AAAAAICEHgAAAAAAAAAAAAAAAAAAAAAAgIQeAACOEgAAjhIAMN8xADDfMQAQVg0AIL0sAIDMKwDw/S8AUBwHAHDJJQAATxAAQJUvAA==

atoms_occupancy:
AAk9AAAJPQDAxi0AQEIPAICEHgCAhB4AAAk9AIBmIwCAohkAACc4AADiBAAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==

atoms_u_iso:
gCYEABBZAAAwEQAAMBEAALBoAACwaAAAgKIAAPAjAADwIwAAECcAABAnAABQkQAA4HkAAKAPAACAcAAAMFwAABCLAACwgQAAIL8CAA==

qdat:
AAAAAAAAAAACEAAAAAAACAgKBAEAAAAQgFAhAIAgCYJCgGCIKBAiVKkQSCcEAh5BQBglWKhnggSioah4BA+QhmUfiGDlAeqUTM4mLGo1NFN3Cxfl4psIYv+pWEbVsag+5Yxyw6AOycIayCwO2jgs8yJEytJWUxHQBHZ4GZ==


formula: Si3 Al3 O12 Na2.92
compound: <missing>
pub_title: The crystal structure of a low-silica dehydrated NaX zeolite
formula_title: <missing>
a: 25.104
b: 25.104
c: 25.104
alpha: 90
beta: 90
gamma: 90
cell_volume: 15820.812
crystal_density: 1.425
atoms_sites: ["Si", "Al", "O1", "O2", "O3", "O4", "Na1", "Na2", "Na3", "Na4"]
atoms_x: CLD8/6ih/P9gTPn/0O7///Dk/f8wxfv/MOYCADDvDQCAEhgAoKsYAA==
atoms_y: aKkHAFAwAgDg/P//sNL//+CTBADAdwQAMOYCADDvDQAAWQYAoPcDAA==
atoms_z: MCMCAKiRBwAgdQYAYKEIAGBVBAAg8woAMOYCADDvDQBA6QgAgCYEAA==
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AQDQ7AEDDOAAAxAkAgPwKAA==
atoms_u_iso: 0
atoms_aniso_label: ["Si", "Al", "O1", "O2", "O3", "O4", "Na1", "Na2", "Na3", "Na4"]
atoms_aniso_u11: UHIBAFByAQBg5AEAIMUBAGBbAwDgIgIAQIoDAEATAgCAqQMAgDgBAA==
atoms_aniso_u22: kC0BAEDnAABAigMAYOQBAMDUAQDAUQIAQIoDAEATAgCAGgYAgN4PAA==
atoms_aniso_u33: kPsAAEAZAQAA9AEAIEICACDFAQBgYQIAQIoDAEATAgCAGgYAQNEMAA==
atoms_aniso_u12: MK3//2AJAABAJf//oIwAAIDB///A4P//QJwAAOCrAACAx/7/AAAAAA==
atoms_aniso_u13: 8AoAADDG///A4P//IFT//2Dw//9g8P//QJwAAOCrAACAOAEAwGP//w==
atoms_aniso_u23: 4Mr//0DU///AY///gET//8BdAABAqP7/QJwAAOCrAAAAcQIAwEUEAA==
qdat:
AAAAAAAQAAABABAACAQAECACCAIIBBAQgIQIQIgRBEEQCCIRCQiEgIkBAhAgEIAAAgABAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: O23.978 F.014 Cl.008 Si6.168 Al2.512 Mg4.13 Ti.43 Ca1.675 Na.889 K.199 H1.356
compound: <missing>
formula_title: <missing>
a: 9.860
b: 17.984
c: 5.291
alpha: 90
beta: 105.24
gamma: 90
cell_volume: 905.218
crystal_density: 3.092
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Detection, crystal-chemical mechanisms and petrological implications of
 Ti partitioning in pargasite and kaersutite
 Sample: K1

atoms_sites:
["O1", "O2", "O3", "F3", "Cl3", "O-h3", "O4", "O5", "O6", "O7", "SiT1", "AlT1", "SiT2", "AlT2", "MgM1", "TiM1", "MgM2", "TiM2", "AlM2", "MgM3", "TiM3", "AlM3", "MgM4", "CaM4", "NaM4", "MgM4*", "CaM4*", "NaM4*", "NaA", "KA", "NaAm", "KAm", "NaA2", "KA2", "H"]

atoms_x:
4IcGAHA4BwBAkQYAQJEGAECRBgBAkQYA4FkWABBYFQCACxUAcMsUADAoEQAwKBEA8LcRAPC3EQAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAcLoCAHC6AgAAAAAAAAAAAEBtDAA=

atoms_y:
QEwFAKCCCgAAAAAAAAAAAAAAAAAAAAAAgEgPAPCJCACAFAcAAAAAAGA2BQBgNgUAkI0KAJCNCgAARgUAAEYFAIDKCgCAygoAgMoKAAAAAAAAAAAAAAAAAPAIEQDwCBEA8AgRAJChDwCQoQ8AkKEPAICEHgCAhB4AgIQeAICEHgAgoBwAIKAcAAAAAAA=

atoms_z:
EFYNACCLLAAwnysAMJ8rADCfKwAwnysAcAowAGDGBgCAQSUAgPEQABCDEgAQgxIAAIMxAACDMQCAhB4AgIQeAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAAAAAAAAAAAAkJIFAJCSBQAAAAAAAAAAAFDuLwA=

atoms_occupancy:
AAk9AAAJPQDAYSkAYG0AAIA+AABg+xIAAAk9AAAJPQAACT0AAAk9AOAOLwAg+g0A4A4vACD6DQAARTMAAMQJAADyKwDgIgIAIPQOAED/LgAAcQIAwJgLAICpAwDAjxkAQEsBAICpAwDAjxkAQEsBAIBbEADwCwQAwC0IAMAGAgDALQgAwAYCAMBhKQA=

atoms_u_iso:
QKYAAFCgAADIzQAAyM0AAMjNAADIzQAA0M8AAMDVAACA7QAAOAMBAOhsAADobAAAyG4AAMhuAADwwwAA8MMAAMh4AADIeAAAyHgAAHiMAAB4jAAAeIwAAFiYAABYmAAAWJgAAKg4AQCoOAEAqDgBACDFAQAgxQEAUL0BAFC9AQCY/AEAmPwBADBNAAA=

qdat:
AAAAAAAAAAACEAAAAAAAGAgKBAIAAAAwgFAiAIBAEoSCgEGQWBBMWPEIUGYIBH6DQFgvGYlWAgakw6BgBA9CGpG+xeM0B4rEdTYSOOnM2aUeKnan3FoFQ32NsJ6SloWyiLLXDIB77RDHweAzqME9GSpaXmzqkEqAN6NA9J==


formula: O23.984 F.014 Cl.002 Si6.131 Al2.319 Mg4.12 Ti.57 Ca1.742 Na.913 K.193 H1.305
compound: <missing>
formula_title: <missing>
a: 9.906
b: 18.015
c: 5.296
alpha: 90
beta: 105.35
gamma: 90
cell_volume: 911.391
crystal_density: 3.083
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Detection, crystal-chemical mechanisms and petrological implications of
 Ti4+ partitioning in pargasite and kaersutite
 Sample: K2

atoms_sites:
["O1", "O2", "O3", "F3", "Cl3", "O-h3", "O4", "O5", "O6", "O7", "SiT1", "AlT1", "SiT2", "AlT2", "MgM1", "TiM1", "MgM2", "TiM2", "AlM2", "MgM3", "TiM3", "AlM3", "MgM4", "CaM4", "NaM4", "MgM4*", "CaM4*", "NaM4*", "NaA", "KA", "NaAm", "KAm", "NaA2", "KA2", "H"]

atoms_x:
QJEGAJA7BwBwiQYAcIkGAHCJBgBwiQYA8E4WAEBQFQDQBhUAMMUUAPAhEQDwIREAkK4RAJCuEQAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAsHUCALB1AgAAAAAAAAAAAGDUDAA=

atoms_y:
AEYFAGB8CgAAAAAAAAAAAAAAAAAAAAAAsEAPAECFCABADgcAAAAAAEAzBQBAMwUAUIcKAFCHCgDQTQUA0E0FABDMCgAQzAoAEMwKAAAAAAAAAAAAAAAAAPAIEQDwCBEA8AgRAJChDwCQoQ8AkKEPAICEHgCAhB4AgIQeAICEHgBwghwAcIIcAAAAAAA=

atoms_z:
YGoNAOCELAAwuCsAMLgrADC4KwAwuCsA8BYwACDZBgDgSiUAgPEQAOCKEgDgihIA8I0xAPCNMQCAhB4AgIQeAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAAAAAAAAAAAA4EIFAOBCBQAAAAAAAAAAAIAFLwA=

atoms_occupancy:
AAk9AAAJPQBQ0ycAYG0AAKAPAACwuBQAAAk9AAAJPQAACT0AAAk9AADHLgAAQg4AAMcuAABCDgBA4TMAwCcJAED/LgAgMAUAoNkIAIAqLQCAGgYAAMQJAOAiAgCwlBoA8MwBAOAiAgCwlBoA8MwBAKAsEACw7AMAUBYIACD3AQBQFggAIPcBAFDTJwA=

atoms_u_iso:
YJoAAGicAAAQuAAAELgAABC4AAAQuAAA8MMAAMjXAACI5QAAIAcBAOhsAADobAAA2GgAANhoAAAYsAAAGLAAALB8AACwfAAAsHwAAHiWAAB4lgAAeJYAAEioAABIqAAASKgAAKg4AQCoOAEAqDgBAFi1AQBYtQEAENUBABDVAQBIuwEASLsBADikAAA=

qdat:
AAAAAAAAAAACIAAAAAAAGAgMBAIAAAAggJBCAQBAEwSFAMEQcCBIqXIQoE4YBHyGgFBVMbGWBBNJhuDgEC5CGaJ7E4JoB56RNihIcbHZoY7cOHcvlFghiv0rwTqtSSHvFGMmGgB2yiGWQUBs4sLrESRMrJlnMJ0AR2WAmS==


formula: O23.989 F.009 Cl.002 Si5.967 Al2.463 Mg4.082 Ti.64 Ca1.734 Na.932 K.226 H1.403
compound: <missing>
formula_title: <missing>
a: 9.907
b: 18.019
c: 5.304
alpha: 90
beta: 105.38
gamma: 90
cell_volume: 912.931
crystal_density: 3.089
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Detection, crystal-chemical mechanisms and petrological implications of
 Ti4+ partitioning in pargasite and kaersutite
 Sample: K3

atoms_sites:
["O1", "O2", "O3", "F3", "Cl3", "O-h3", "O4", "O5", "O6", "O7", "SiT1", "AlT1", "SiT2", "AlT2", "MgM1", "TiM1", "MgM2", "TiM2", "AlM2", "MgM3", "TiM3", "AlM3", "MgM4", "CaM4", "NaM4", "MgM4*", "CaM4*", "NaM4*", "NaA", "KA", "NaAm", "KAm", "NaA2", "KA2", "H"]

atoms_x:
cIkGAOA2BwAAiwYAAIsGAACLBgAAiwYAgFAWANBRFQBgCBUAMMUUANAeEQDQHhEAILARACCwEQAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAkIsCAJCLAgAAAAAAAAAAAOAYDAA=

atoms_y:
IEkFAPB9CgAAAAAAAAAAAAAAAAAAAAAA0EMPAPCJCAAgCwcAAAAAAEAzBQBAMwUA4IgKAOCICgDQTQUA0E0FABDMCgAQzAoAEMwKAAAAAAAAAAAAAAAAABAMEQAQDBEAEAwRAJChDwCQoQ8AkKEPAICEHgCAhB4AgIQeAICEHgCQnhwAkJ4cAAAAAAA=

atoms_z:
IGQNAJCJLADQrisA0K4rANCuKwDQrisAoBswAFDqBgBgVyUAIOgQANCVEgDQlRIAUJcxAFCXMQCAhB4AgIQeAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAAAAAAAAAAAAoIcFAKCHBQAAAAAAAAAAACDdLwA=

atoms_occupancy:
AAk9AAAJPQDw0CoAUEYAAKAPAAAg4hEAAAk9AAAJPQAACT0AAAk9ALCGLQBQgg8AsIYtAFCCDwAARTMAAMQJAMDGLQDAtgYAgIsIAMDGLQCAGgYAwCcJAMBRAgBwdRoAUL0BAMBRAgBwdRoAUL0BAPCkEACQmAQAsFEIABBNAgCwUQgAEE0CAPDQKgA=

atoms_u_iso:
aJwAAFiYAAAgsgAAILIAACCyAAAgsgAACMAAALDbAACw2wAAUP8AAPBkAADwZAAACGEAAAhhAAAYsAAAGLAAAMB2AADAdgAAwHYAAHCUAABwlAAAcJQAACiqAAAoqgAAKKoAAKg4AQCoOAEAqDgBAKCfAQCgnwEA8OABAPDgAQCw7gEAsO4BAPBkAAA=

qdat:
AAAAAAAAAAACIAAAAAAAGAgUBAIAAAAggKBCAQBAEwUFAMEQcCBIqXIQoE4YCH0HAHBVUrGeBBVJh0HAED6CGSZ/EoZoDx6RaihIcdPpo474aLZPmOgjDP0ywj1NSiPKNEcsGgDsmkMcg4DOYwTOUmjk2ammQTkA3scB8k==


formula: O23.983 F.014 Cl.003 Si5.86 Al2.61 Mg3.976 Ti.67 Ca1.789 Na.901 K.215 H1.378
compound: <missing>
formula_title: <missing>
a: 9.903
b: 17.995
c: 5.304
alpha: 90
beta: 105.44
gamma: 90
cell_volume: 911.084
crystal_density: 3.098
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Detection, crystal-chemical mechanisms and petrological implications of
 Ti4+ partitioning in pargasite and kaersutite
 Sample: K4

atoms_x:
UIYGAFA1BwDghwYA4IcGAOCHBgDghwYAwFYWAIBWFQDQBhUAMMUUABAlEQAQJREAQLMRAECzEQAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAsI4CALCOAgAAAAAAAAAAAGBwDAA=

atoms_y:
0E0FABCBCgAAAAAAAAAAAAAAAAAAAAAAgEgPABCNCAAgCwcAAAAAANA0BQDQNAUAcIoKAHCKCgBATAUAQEwFAKDNCgCgzQoAoM0KAAAAAAAAAAAAAAAAAMAQEQDAEBEAwBARAJChDwCQoQ8AkKEPAICEHgCAhB4AgIQeAICEHgCQnhwAkJ4cAAAAAAA=

atoms_z:
4F0NAFCcLAAQtSsAELUrABC1KwAQtSsAUCAwAMABBwBwZSUAYO4QABCcEgAQnBIA0KMxANCjMQCAhB4AgIQeAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAAAAAAAAAAAA8GkFAPBpBQAAAAAAAAAAAJAmMAA=

atoms_occupancy:
AAk9AAAJPQCgDSoAYG0AAHAXAACQdhIAAAk9AAAJPQAACT0AAAk9AFC1LACwUxAAULUsALBTEAAARTMAAMQJAMBVKwAgoQcAIBIKAABjLgCAGgYAgIsIACDFAQAQTRsAMG8BACDFAQAQTRsAMG8BACBrEABQYAQAkDUIAGAvAgCQNQgAYC8CAKANKgA=

atoms_u_iso:
SJ4AAGCaAAAotAAAKLQAACi0AAAotAAA8MMAAKjZAACA4wAAMAEBAPBkAADwZAAAAF8AAABfAAAgsgAAILIAAMB2AADAdgAAwHYAAGiSAABokgAAaJIAAEioAABIqAAASKgAAKg4AQCoOAEAqDgBAKCfAQCgnwEAANEBAADRAQAA2wEAANsBAJiKAAA=

qdat:
AAAAAAAAAAACEAAAAAAAGAgMBAIAAAAwgFAiAQBAEwUFgMEQcCBMqXIQYE4IBH0GgHBNMZGWBAtJhuDgCB6CHaJ7E8JsBxeItixMMcqo8o5cVH8nVLQDjv8TYT7lThNmEmOmGQB2ySGOQsBvMYK+MWTU3JmXIKiAa2aBuU==


formula: Mg.963 Fe.717 Cr.018 Ti.07 Mn.005 Al.226 B O4
compound: Inglefield Land, North-West Greenland
formula_title: <missing>
a: 9.198
b: 3.091
c: 9.355
alpha: 90
beta: 90
gamma: 90
cell_volume: 265.972
crystal_density: 3.719
atoms_sites: ["MgM1", "FeM1", "CrM1", "TiM1", "MgM2", "FeM2", "MnM2", "AlM2", "B", "O1", "O2", "O3", "O4"]
atoms_x: CAAHAAgABwAIAAcACAAHADhJBgA4SQYAOEkGADhJBgBgGAoA4CgBALAODwDQYg4A4KsAAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAA==
atoms_z: WMEiAFjBIgBYwSIAWMEiADC6CwAwugsAMLoLADC6CwCwbzUAoP00APC+LQCAcAAA8GEXAA==
atoms_occupancy: QBIXAKBJIABAGQEAwEUEAKC0IwCAeQsAIE4AAEDLDQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 6GIAAOhiAADoYgAA6GIAAMh4AADIeAAAyHgAAMh4AADYaAAAKKoAAGicAACAjgAAkIgAAA==
atoms_aniso_label: ["MgM1", "FeM1", "CrM1", "TiM1", "MgM2", "FeM2", "MnM2", "AlM2", "B", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: iHIAAIhyAACIcgAAiHIAAIhoAACIaAAAiGgAAIhoAACQdAAAcGIAAPCRAACohAAAGJwAAA==
atoms_aniso_u22: KFUAAChVAAAoVQAAKFUAALByAACwcgAAsHIAALByAADoYgAAYO8AAFD1AADQzwAASJ4AAA==
atoms_aniso_u33: CGEAAAhhAAAIYQAACGEAAACMAAAAjAAAAIwAAACMAAAIYQAAsKkAABhRAADIWgAA2F4AAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: WO7//1ju//9Y7v//WO7//3gFAAB4BQAAeAUAAHgFAABI6v//YPD//yAXAACY4P//uBUAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
pub_title:
 Crystal structure and chemistry of yuanfuliite
 and its relationships with warwickite
 Sample: 425359

qdat:
AAAAAAAAAAAAAAAAgAAAAAJAAYAAAAAAgAAGgEAAFAYABEVDAoSABgAANZiAMwABAGoRYahNYBIoWgE3kWnoKMWI6ULppRKJX9VyEPL4zS9jGtUrf/sC7ubZ13ss/HdqNyr9Vset2pcb9MK7P2T+WBV/zvpmRczbJCNrxB==


formula: Mg.969 Al.283 Fe.665 Cr.005 Ti.077 B O4
compound: Inglefield Land, North-West Greenland
formula_title: <missing>
a: 9.174
b: 3.084
c: 9.337
alpha: 90
beta: 90
gamma: 90
cell_volume: 264.168
crystal_density: 3.698
atoms_sites: ["MgM1", "AlM1", "FeM1", "CrM1", "TiM1", "MgM2", "FeM2", "AlM2", "B", "O1", "O2", "O3", "O4"]
atoms_x: mPwGAJj8BgCY/AYAmPwGAJj8BgDYSQYA2EkGANhJBgCgHgoA4CgBALAODwDQYg4A0LYAAA==
atoms_y: QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAA==
atoms_z: 2MMiANjDIgDYwyIA2MMiANjDIgDwuAsA8LgLAPC4CwBAcTUA0PU0APC+LQAwdQAAgGMXAA==
atoms_occupancy: 4BsYAOAuAABAXx8AIE4AACCzBADACCMAYDcJAAAXEQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0HAAANBwAADQcAAA0HAAANBwAACgggAAoIIAAKCCAAC4fgAAyM0AAOjBAAAoqgAASJ4AAA==
atoms_aniso_label: ["MgM1", "AlM1", "FeM1", "CrM1", "TiM1", "MgM2", "FeM2", "AlM2", "B", "O1", "O2", "O3", "O4"]
atoms_aniso_u11: mHYAAJh2AACYdgAAmHYAAJh2AACYbAAAmGwAAJhsAAD4iQAAiHwAAPCvAAD4kwAA2LMAAA==
atoms_aniso_u22: 6GIAAOhiAADoYgAA6GIAAOhiAACoegAAqHoAAKh6AACgeAAAuCgBABAXAQBQ9QAAILIAAA==
atoms_aniso_u33: MHoAADB6AAAwegAAMHoAADB6AAAooAAAKKAAACigAAAAeAAAUMMAAEB+AACQdAAAiHIAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: aPL//2jy//9o8v//aPL//2jy//94BQAAeAUAAHgFAABo8v//WO7//5gNAAC43v//KBkAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
pub_title:
 Crystal structure and chemistry of yuanfuliite
 and its relationships with warwickite
 Sample: 425360

qdat:
AAAAAAAAAAAAAAAAgAAAAAFAAUAAAAAAgAAFgEAACgIABCKhgUJAAwAAHUxAGYAAgHUJUJQmuAkkfIBbyJT0FGLEfKFu0YlEsqq4iFV8c09ZhvVL3b/Bv/HqdV7Tbxbamcq+V6JPnz/E/RE/z24ZGwVUstqbSO69sRxf8Q==


formula: Pb4 S (O12 C2) H2
compound: Leadhills, Scotland
pub_title: Crystal structure of susannite, Pb4SO4(CO3)2(OH)2: a trimorph with macphersonite and leadhillite
formula_title: <missing>
a: 9.0718
b: 9.0718
c: 11.570
alpha: 90
beta: 90
gamma: 120
cell_volume: 824.614
crystal_density: 6.518
atoms_occupancy: 0
atoms_aniso_label: ["Pb1", "Pb2", "Pb3", "Pb4", "S1", "S2", "S3"]
atoms_aniso_u11: IBYBAEAAAQAgrQUAoFwIAGDeAgCAMgIAIEICAA==
atoms_aniso_u22: wPMAAEAAAQAABwMAkKQCAGDeAgCAMgIAIEICAA==
atoms_aniso_u33: QAABAFDcAAAgrAEAUEABAGBtAADgKAEAIEgBAA==
atoms_aniso_u12: gIkAALBoAAAwGAMAAOgDAAB3AQBAGQEAQBkBAA==
atoms_aniso_u13: 4Pz//yADAABAHwAAsOv//wAAAAAAAAAAAAAAAA==
atoms_aniso_u23: QO3//wAAAADw0gAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_sites:
["Pb1", "Pb2", "Pb3", "Pb4", "S1", "S2", "S3", "O-H1", "O-H2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "C1", "C2", "C3", "C4", "C5", "C6"]

atoms_x:
0MAoABAmFQAQ+SgAQFsoAKuwKABVWBQAAAAAAKCWKAAg3BIAoE40AMAsHQAAhygAIB0dAMDg//8gCyAAq7AoAOD2MgBVWBQAoNIeAAAAAACgUAoAAAAAAFVYFACrsCgAVVgUAAAAAACrsCgA

atoms_y:
cE///zDAAADgszkA0FUlAFVYFACrsCgAAAAAAIAsAwDA5v7/QFX3/wD76/9A7hwAAEj0/wA29/8AghQAVVgUAMBQFwCrsCgAYNAuAAAAAADAtgYAAAAAALin6/9VWBQAuKfr/wAAAABVWBQA

atoms_z:
IBYBAICoMQBA9iMA4IkOAMA+GgCAJRkA4BUZACCDDADgxyUAgKkDAICpAwDgnwIAIC4vAGBNLwCAJC4AAI4SAOCAHABgpyAA4KQWACCIIACghRYAoHQEAMBFBABg3gIAoGwvACCrLwAAYy4A

atoms_u_iso:
QAABALD+AACwCwMA8I4DAEATAgDA1AEAAPQBAAB3AQBg3gIAIMsAAKAJAQDgqwAAYGcBAAB3AQBg5AEAAHECAEDvBwBAfgUAgIsIAICpAwBA0QwAIMsAAKAJAQDgqwAAYGcBAAB3AQBg5AEA

qdat:
AAAAAAAAAgAAAIAAQAQAAAEgBACQQIQAQAAKYAkCggAhEwQwpCFIEMoQoIThdhAKWAjMGpk6tCaj4QYskmnrGXhFjpFFpPrgebE5yzviWrT/yU6BvF59VsVvpvU9iZxcdNo+8Odu8j9X99y7YvLMXdN+/JnSRUyFL7b1lW==


formula: Zn.616 Mn.374 Mg.035 Al.034 Fe1.94 O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK2
formula_title: <missing>
a: 8.4654
b: 8.4654
c: 8.4654
alpha: 90
beta: 90
gamma: 90
cell_volume: 606.656
crystal_density: 5.145
atoms_sites: ["ZnT", "MnT", "MgT", "AlT", "FeT", "ZnM", "MnM", "MgM", "AlM", "FeM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeANDyDwA=
atoms_y: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeANDyDwA=
atoms_z: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeANDyDwA=
atoms_occupancy: IHYjAOC8EgBAEwIAQBkBAICpAwBwEQEAcAsCANAHAAAAfQAAgF85AAAJPQA=
atoms_u_iso: 0J0AANCdAADQnQAA0J0AANCdAABgnwAAYJ8AAGCfAABgnwAAYJ8AAPCgAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAgAAAAAAAEAAABAAAAAACAAAIAAAAAgAAQAAAAIAAQAAACAAIAAAEAAgAAAgAQAAAgAQAACACAAAgAgAAQAQAAQAgAAACAAEAQAAgEAAIBAAEAgAEAgAAAgAICAAAE==


formula: (Zn.616 Mn.37 Mg.043 Al.034 Fe1.937) O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK3
formula_title: <missing>
a: 8.4641
b: 8.4641
c: 8.4641
alpha: 90
beta: 90
gamma: 90
cell_volume: 606.376
crystal_density: 5.143
atoms_sites: ["ZnT", "MnT", "MgT", "AlT", "FeT", "ZnM", "MnM", "MgM", "AlM", "FeM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAGD0DwA=
atoms_y: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAGD0DwA=
atoms_z: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAGD0DwA=
atoms_occupancy: oCslAOA5EwCgCQEAoAMCAOClAQCwNgAAsK0BACDLAADQBwAA4Ek6AAAJPQA=
atoms_u_iso: MI4AADCOAAAwjgAAMI4AADCOAAAwjgAAMI4AADCOAAAwjgAAMI4AAJCXAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAgAAAAAAAEAAAAgAAAAACAAAIAAAAAgAAQAAAAIAAQAAACAAIAAAEAAgAAAgAIAAAgAQAACACAAAgAgAAQAQAAQAgAAACAAEAQAAgCAAIBAAEAgAEAgAAAgAIBAAAE==


formula: Zn.638 Mn.351 Mg.044 Al.141 Fe1.785 Ti.024 O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK5
formula_title: <missing>
a: 8.4434
b: 8.4434
c: 8.4434
alpha: 90
beta: 90
gamma: 90
cell_volume: 601.939
crystal_density: 5.092
atoms_sites: ["ZnT", "MnT", "MgT", "AlT", "FeT", "ZnM", "MnM", "MgM", "AlM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgDw9Q8A
atoms_y: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgDw9Q8A
atoms_z: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgDw9Q8A
atoms_occupancy: IGolACBlEQBgZwEAIMUBAAD0AQBQwwAAoAMCABCkAAAAawMAUH81AIC7AAAACT0A
atoms_u_iso: oIwAAKCMAACgjAAAoIwAAKCMAABQkQAAUJEAAFCRAABQkQAAUJEAAFCRAACQlwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAQAAAAAQAAAAAAACAAAAgAAAAABAAAEAAAAAQAAAAAAAEAAIAAAAgAEAAABAAQAAAQAEAAAQAEAAAgAgAAIAIAAEAIAAEAIAAAAgABAEAAIAgACAQABAIABAEAAAIABAQAAB==


formula: Zn.697 Mn.333 Al.143 Fe1.761 Mg.042 Ti.026 O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK6
formula_title: <missing>
a: 8.4431
b: 8.4431
c: 8.4431
alpha: 90
beta: 90
gamma: 90
cell_volume: 601.874
crystal_density: 5.128
atoms_sites: ["ZnT", "MnT", "AlT", "FeT", "ZnM", "MnM", "MgM", "AlM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAID3DwA=
atoms_y: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAID3DwA=
atoms_z: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAID3DwA=
atoms_occupancy: INUoAIDeDwBgZwEAAO4CAMDaAABQOgIAIEgBAICpAwDQRjQAIMsAAAAJPQA=
atoms_u_iso: MI4AADCOAAAwjgAAMI4AAICJAACAiQAAgIkAAICJAACAiQAAgIkAACCZAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAQAAAAAQAAAAAAACAAAAgAAAAABAAAEAAAAAQAAIAAAAEAAIAAAAgACAAABAAQAAAQAEAAAIAEAAAgAgAAIAIAAEAEAAEAIAAAAgABAEAAIAgACAQABAIABAEAAAIABAQAAB==


formula: Zn.698 Mn.326 Mg.037 Al.141 Fe1.772 Ti.026 O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK7
formula_title: <missing>
a: 8.4428
b: 8.4428
c: 8.4428
alpha: 90
beta: 90
gamma: 90
cell_volume: 601.810
crystal_density: 5.131
atoms_sites: ["ZnT", "MnT", "MgT", "AlT", "FeT", "ZnM", "MnM", "MgM", "AlM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgCA9w8A
atoms_y: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgCA9w8A
atoms_z: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgCA9w8A
atoms_occupancy: 4DgoAKAsEADAXQAA4CgBAOAcAwCwMAEAkNwBADDyAAAguQMAUIU0ACDLAAAACT0A
atoms_u_iso: 8G4AAPBuAADwbgAA8G4AAPBuAADQawAA0GsAANBrAADQawAA0GsAANBrAAAAfQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAQAAAAAQAAAAAAACAAAAgAAAAABAAAEAAAAAQAAIAAAAEAAIAAAAgACAAABAAQAAAQAEAAAIAEAAAgAgAAIAIAAEAEAAEAIAAAAgAAgEAAIAgACAQABAIABAEAAAIABAQAAB==


formula: Zn.602 Mn.426 Mg.035 Al.028 Fe1.91 O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK8
formula_title: <missing>
a: 8.4688
b: 8.4688
c: 8.4688
alpha: 90
beta: 90
gamma: 90
cell_volume: 607.387
crystal_density: 5.141
atoms_sites: ["ZnT", "MnT", "MgT", "AlT", "FeT", "ZnM", "MnM", "FeM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCw7w8A
atoms_y: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCw7w8A
atoms_z: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCw7w8A
atoms_occupancy: YBIkAIBPEgDgIgIAgLUBAGDeAgDwVQAAYNgDALDaOAAACT0A
atoms_u_iso: IJkAACCZAAAgmQAAIJkAACCZAADQnQAA0J0AANCdAACAogAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAgAAAAAAAEAAABAAAAAAEAAAIAAAAAgAAQAAAAQAAgAAACAAIAAAEAAgAABAAQAAAgAQAACACAAAgAgAAQAgAAQAgAAACAAIAQABAEAAQBAAEBAAEBAAABAAICAAAE==


formula: Zn.658 Mn.328 Mg.038 Al.129 Fe1.832 Ti.016 O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK10
formula_title: <missing>
a: 8.4466
b: 8.4466
c: 8.4466
alpha: 90
beta: 90
gamma: 90
cell_volume: 602.623
crystal_density: 5.126
atoms_sites: ["ZnT", "MnT", "MgT", "AlT", "FeT", "ZnM", "MnM", "MgM", "AlM", "FeM", "TiM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgDw9Q8A
atoms_y: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgDw9Q8A
atoms_z: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAICEHgDw9Q8A
atoms_occupancy: YAAnAGCEEQCAPgAAAPQBAMBRAgBwlAAAUEABAKAJAQDQ9QIAoL82AAB9AAAACT0A
atoms_u_iso: AJYAAACWAAAAlgAAAJYAAACWAAAAlgAAAJYAAACWAAAAlgAAAJYAAACWAABAnAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAQAAAAAAAEAAAAgAAAAACAAAEAAAAAQAAAAAAAIAAIAAABAAEAAABAAQAAAQAEAAAQAIAABAAgAAIAIAAEAIAAEAIAAAAgABAEAAQAgAEAQABAIABAIAAAIACAQAAB==


formula: Zn.67 Mn.317 Mg.056 Al.031 Fe1.924 O4
compound: <missing>
pub_title: Cation distribution in natural Zn-spinels: franklinite Sample: FRK12
formula_title: <missing>
a: 8.4585
b: 8.4585
c: 8.4585
alpha: 90
beta: 90
gamma: 90
cell_volume: 605.174
crystal_density: 5.156
atoms_sites: ["ZnT", "MnT", "MgT", "AlT", "FeT", "ZnM", "MnM", "MgM", "AlM", "FeM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAEDxDwA=
atoms_y: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAEDxDwA=
atoms_z: IKEHACChBwAgoQcAIKEHACChBwCAhB4AgIQeAICEHgCAhB4AgIQeAEDxDwA=
atoms_occupancy: 4LUoAOBXDgBg5AEAQJYBAABxAgBwFwAAoIACAFDDAAAQJwAAwH45AAAJPQA=
atoms_u_iso: EIsAABCLAAAQiwAAEIsAABCLAAAQiwAAEIsAABCLAAAQiwAAEIsAAOCSAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAAgAAAAAgAAAAAAAEAAAAgAAAAACAAAIAAAAAgAAQAAAAIAAQAAACAAIAAACAAQAAAgAIAAAgAQAACABAAAQAQAAIAQAAQAgAAACAACAIAAQCAAIAgAEAQACAQAAAgAIBAAAC==


formula: Pb Al3 (P1.38 S.62) O14 H6
compound: <missing>
pub_title: Hinsdalite and plumbogummite, their atomic arrangements and disordered lead sites
formula_title: <missing>
a: 7.029
b: 7.029
c: 16.789
alpha: 90
beta: 90
gamma: 120
cell_volume: 718.361
crystal_density: 4.028
atoms_sites: ["Pb", "Al", "P", "S", "O1", "O2", "O-H3"]
atoms_x: gOcBAICEHgAAAAAAAAAAAAAAAACwMw0AILoHAA==
atoms_y: gOcBAAAAAAAAAAAAAAAAAAAAAABQzPL/4EX4/w==
atoms_z: AAAAAICEHgDgxhIA4MYSAADRJADgePz/sFEIAA==
atoms_occupancy: OCwKAAAJPQBAHSoAwOsSAAAJPQAACT0AAAk9AA==
atoms_u_iso: QK8BAFDcAADwuQAA8LkAABAIAQDw0gAAIP0AAA==
atoms_aniso_label: ["Pb", "Al", "P", "S"]
atoms_aniso_u11: sK0BAHDGAADgqwAA4KsAAA==
atoms_aniso_u22: sK0BAEDOAADgqwAA4KsAAA==
atoms_aniso_u33: AKkBANABAQAQ1gAAENYAAA==
atoms_aniso_u12: IMsAACBnAADwVQAA8FUAAA==
atoms_aniso_u13: MPj//yADAAAAAAAAAAAAAA==
atoms_aniso_u23: 0AcAALAEAAAAAAAAAAAAAA==
qdat:
AAAAAAAAAAAAAAAAAAKAAIAAAAAAABIAAAAyCEAAAAEAAAkxAAAChABSQAACCAMeCABEAooQAQANwQBiA1AAAgJQgMgdBAIA3EAoCgARBMQEgxIAAuIEgkAQGxAoagEAhBIVACFSCBRBA8AoIAIeQ4cgg6hwwCiyBAYAWR==


formula: Pb Al3 (P1.9 As.1) O14 H6
compound: <missing>
pub_title: Hinsdalite and plumbogummite, their atomic arrangements and disordered lead sites
formula_title: <missing>
a: 7.039
b: 7.039
c: 16.761
alpha: 90
beta: 90
gamma: 120
cell_volume: 719.205
crystal_density: 4.049
atoms_sites: ["Pb", "Al", "P", "As", "O1", "O2", "O-H3"]
atoms_x: EH8CAICEHgAAAAAAAAAAAAAAAADgEg0AwLAHAA==
atoms_y: EH8CAAAAAAAAAAAAAAAAAAAAAAAg7fL/QE/4/w==
atoms_z: AAAAAICEHgAQ7BIAEOwSAHCEJAAgf/z/6GQIAA==
atoms_occupancy: OCwKAAAJPQDA+zkAQA0DAAAJPQAACT0AAAk9AA==
atoms_u_iso: UIsBABByAABguAAAYLgAAKAJAQBAAAEAIMsAAA==
atoms_aniso_label: ["Pb", "Al", "P", "As"]
atoms_aniso_u11: 8OUBACBOAADwoAAA8KAAAA==
atoms_aniso_u22: 8OUBAGBUAADwoAAA8KAAAA==
atoms_aniso_u33: EDoBANC2AADQ6AAA0OgAAA==
atoms_aniso_u12: wD4BADAqAACwTwAAsE8AAA==
atoms_aniso_u13: 4OP//yADAAAAAAAAAAAAAA==
atoms_aniso_u23: IBwAALAEAAAAAAAAAAAAAA==
qdat:
AAAAAAAAAAAAAAAAAAKAAQAAAAAAABIAAAAyEEAAAAEAABExAAAFBABSQAAECAYSBABEApIIAQAVIICiA1AAAgTQgMgaBAIBfEBIDAAiDUQMgiIABKIJAoAgFSBQ1AIChCQqACJkMDhCBYBQoARMhRpBB5GjgEj0CBQAsj==


formula: Cu3 As O7 H3
compound: <missing>
pub_title: Gilmarite, Cu3(AsO4)(OH)3, a new mineral: its description and crystal structure
formula_title: <missing>
a: 5.445
b: 5.873
c: 5.104
alpha: 114.95
beta: 93.05
gamma: 91.92
cell_volume: 147.494
crystal_density: 4.285
atoms_sites: ["Cu1", "Cu2", "Cu3", "As", "O1", "O2", "O-H3", "O4", "O-H5", "O-H6", "O7"]
atoms_x: wAADAJCAIQAw7iIAsOv//0DjCQCAeQsAYOgqAGBZLQDgpBYA4HodAKA8NwA=
atoms_y: QNckAHApFgAwxzUAsAQAAGCKEAAgIjEAwBQhAICpAwCgEykAYJwNAID6NAA=
atoms_z: gK0TAADHFQBQnRcAkAEAAGBVBABAhAQAQGYJAEBaCwBA1iAAwHMmACDbJwA=
atoms_occupancy: 0
atoms_u_iso: IJkAALCaAACwmgAAEIsAAGDqAABAGQEAQJwAACDLAACgjAAAIMsAAAD6AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAKAACAAAAAEABAAAABAACEAAgAIoQAAACAAQBADBgQAKIKAAAAQAESyAACQQFADEoAwQACFBRAsAQGEgEKiUCAgCOEgWSQCeIBcoSSgg2c7gSmpUCbR4Bg4THgWs08o2QAMib9ZGOKP2jPlOUd0w==


formula: Ca2.751 Mg.051 Mn.069 Fe1.338 Al.67 Ti.211 Si2.88 O12 H.168
compound: Mt. Vulture, Southern Italy
pub_title: Crystal chemistry of melanites from Mt. Vulture (Southern Italy) Sample: LC2
formula_title: <missing>
a: 11.999
b: 11.999
c: 11.999
alpha: 90
beta: 90
gamma: 90
cell_volume: 1727.568
crystal_density: 3.777
atoms_sites: ["CaX", "MgX", "MnX", "FeX", "AlY", "FeY", "TiY", "SiZ", "FeZ", "TiZ", "O", "O-H"]
atoms_x: IKEHACChBwAgoQcAIKEHAAAAAAAAAAAAAAAAAGDjFgBg4xYAYOMWAOBZAgDgWQIA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIDmAgCA5gIA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAAEBCDwBAQg8AQEIPAHDqJwBw6icA
atoms_occupancy: IPg3AKAJAQBgZwEA4J8CAGByFACgtCMAAOIEAACYOgAgywAAoAkBAEAuPADA2gAA
atoms_u_iso: 6GwAAOhsAADobAAA6GwAADhPAAA4TwAAOE8AABhRAAAYUQAAGFEAAKh6AAAAEnoA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAACABAAAAgAgCAEAABAIAAABAQEAAQECAgQIAACBBAggggAggAghBACEIIQhAEAQhEEAhAAhEIhEBCICABERAQASAAJEBEAIAAIAAAIAAAAAAAAJAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca2.751 Mg.051 Mn.069 Fe1.339 Al.67 Ti.21 Si2.871 O12 H.192
compound: Mt. Vulture, Southern Italy
pub_title: Crystal chemistry of melanites from Mt. Vulture (Southern Italy) Sample: LC6
formula_title: <missing>
a: 11.995
b: 11.995
c: 11.995
alpha: 90
beta: 90
gamma: 90
cell_volume: 1725.841
crystal_density: 3.779
atoms_sites: ["CaX", "MgX", "MnX", "FeX", "AlY", "FeY", "TiY", "SiZ", "FeZ", "TiZ", "O", "O-H"]
atoms_x: IKEHACChBwAgoQcAIKEHAAAAAAAAAAAAAAAAAGDjFgBg4xYAYOMWAABYAgAAWAIA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAADDmAgAw5gIA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAAEBCDwBAQg8AQEIPADDpJwAw6ScA
atoms_occupancy: IPg3AKAJAQBgZwEA4J8CAGByFABgGCMAQH4FACBpOgCAOAEAQJwAAAAPPAAA+gAA
atoms_u_iso: +GYAAPhmAAD4ZgAA+GYAAEhJAABISQAASEkAAFhDAABYQwAAWEMAANhyAADYcgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAACAAgAAAgAgBAEAABAIAAABAQEAAQECAgQIAACBBAggQQAggAghBACEIIQhAEAQhCEAhAAhEIhEBCIBABERAQARAAIiBEAIAAIAAAEAAAAAAAAJAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca2.781 Mg.06 Mn.069 Fe1.408 Al.55 Ti.261 Si2.85 O12 H.12
compound: Mt. Vulture, Southern Italy
pub_title: Crystal chemistry of melanites from Mt. Vulture (Southern Italy) Sample: LC9
formula_title: <missing>
a: 12.015
b: 12.015
c: 12.015
alpha: 90
beta: 90
gamma: 90
cell_volume: 1734.488
crystal_density: 3.790
atoms_sites: ["CaX", "MgX", "MnX", "FeX", "AlY", "FeY", "TiY", "SiZ", "FeZ", "TiZ", "O", "O-H"]
atoms_x: IKEHACChBwAgoQcAIKEHAAAAAAAAAAAAAAAAAGDjFgBg4xYAYOMWACBbAgAgWwIA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAADDmAgAw5gIA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAAEBCDwBAQg8AQEIPADDpJwAw6ScA
atoms_occupancy: YJQ4AIA4AQBgZwEAwNQBAODIEACA1yUAoGgGAMD7OQBAlgEAoAkBAMBsPABAnAAA
atoms_u_iso: qHoAAKh6AACoegAAqHoAABhbAAAYWwAAGFsAAChVAAAoVQAAKFUAANhyAADYcgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAACABAAAAgBACAEAABAIAAACAQEAAQICBAgQAACCBBBAggAggBBBCAEIIQhCAIAhCEIBCABCIREIBEQEACIiAgAkAARECQAgAAQAAAQAAAAAAAAiAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca2.799 Mg.051 Mn.069 Fe1.432 Al.55 Ti.231 Si2.85 O12 H.12
compound: Mt. Vulture, Southern Italy
pub_title: Crystal chemistry of melanites from Mt. Vulture (Southern Italy) Sample: LC10
formula_title: <missing>
a: 12.013
b: 12.013
c: 12.013
alpha: 90
beta: 90
gamma: 90
cell_volume: 1733.622
crystal_density: 3.795
atoms_sites: ["CaX", "MgX", "MnX", "FeX", "AlY", "FeY", "TiY", "SiZ", "FeZ", "TiZ", "O", "O-H"]
atoms_x: IKEHACChBwAgoQcAIKEHAAAAAAAAAAAAAAAAAGDjFgBg4xYAYOMWAKhaAgCoWgIA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAMDnAgDA5wIA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAAEBCDwBAQg8AQEIPAODtJwDg7ScA
atoms_occupancy: IPI4AKAJAQBgZwEA4KUBAODIEADgwSYAQH4FAMD7OQDgpQEAoAkBAMBsPABAnAAA
atoms_u_iso: 6GwAAOhsAADobAAA6GwAAChVAAAoVQAAKFUAAEBHAABARwAAQEcAALh0AAC4dAAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAACABAAAAgBACAEAABAIAAACAQEAAQICBAgQAACCBBBAggAggBBBCAEIIQhBAIARCEIBCABCIRCIBEQEACIiAgAkAARECIAQAAQAAAQAAAAAAAASAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca2.781 Mg.06 Mn.06 Fe1.411 Al.56 Ti.251 Si2.85 O12 H.156
compound: Mt. Vulture, Southern Italy
pub_title: Crystal chemistry of melanites from Mt. Vulture (Southern Italy) Sample: LC13
formula_title: <missing>
a: 12.014
b: 12.014
c: 12.014
alpha: 90
beta: 90
gamma: 90
cell_volume: 1734.055
crystal_density: 3.787
atoms_sites: ["CaX", "MgX", "MnX", "FeX", "AlY", "FeY", "TiY", "SiZ", "FeZ", "TiZ", "O", "O-H"]
atoms_x: IKEHACChBwAgoQcAIKEHAAAAAAAAAAAAAAAAAGDjFgBg4xYAYOMWAMhdAgDIXQIA
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABjqAgAY6gIA
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAAEBCDwBAQg8AQEIPANjrJwDY6ycA
atoms_occupancy: YJQ4AIA4AQCAOAEAoAMCAAAXEQCA1yUAgBoGAMD7OQAAdwEAoAkBAOA9PAAgywAA
atoms_u_iso: qHoAAKh6AACoegAAqHoAAABfAAAAXwAAAF8AABhbAAAYWwAAGFsAAKCCAACgggAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAAIAACAAAAAAACABAAAAgBACAEAABAIAAACAQEAAQICBAgQAACCBBBAggAggBBBCAEIIQhCAIARCEIBCABCIRCIBEQEACIiAgAkAARECQAQAAQAAAQAAAAAAAASAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ba Mn9 (V5.382 As.618) O26 H2
compound: Central Pyrenees, France
formula_title: <missing>
a: 12.832
b: 12.832
c: 12.832
alpha: 90
beta: 90
gamma: 90
cell_volume: 2112.920
crystal_density: 4.307
atoms_sites: ["Ba", "Mn1", "Mn2", "Mn3", "V", "As", "O1", "O2", "O3", "O4", "O5", "H"]
atoms_x: AAAAAIB74f9gNuz/0GDt/yB88P8gfPD/QM/r//B49v9Q3ev/MJ71/wDo6v/g2Oz/
atoms_y: AAAAAAAAAADgugoAYFQAAGBuBABgbgQAINH//+A9CgBg+QoAYKEIAICT9v+govT/
atoms_z: AAAAAAAAAACgyRMAYLQJAOBS+v/gUvr/YIz//4D4EwAA+x0AkLz+/4BsCQBgXQsA
atoms_occupancy: AAk9AAAJPQAACT0AAAk9AKC/NgBgSQYAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: oAkBAOCrAACAuwAAwNoAAKCMAACgjAAAIMsAAMDaAADA2gAAAPoAAMDaAACAtQEA
atoms_aniso_label: ["Ba", "Mn1", "Mn2", "Mn3", "V", "As", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: oAkBACCyAABguAAAQAABAOCSAADgkgAAwNoAAIC7AADA2gAAAPoAAGDqAAA=
atoms_aniso_u22: oAkBACCyAABguAAA8NIAADCOAAAwjgAAwNoAAGDqAABg6gAAoAkBAGDqAAA=
atoms_aniso_u33: oAkBACCyAABguAAAkMkAAJCXAACQlwAAgLsAAMDaAACAuwAAYOoAAGDqAAA=
atoms_aniso_u12: 4C4AAAAAAADA+f//gPP//8D5///A+f//oA8AAGDw//8AAAAAYPD//+AuAAA=
atoms_aniso_u13: 4C4AAAAAAADA+f//ENz//7AEAACwBAAAAAAAAAAAAAAAAAAAYPD//yDR//8=
atoms_aniso_u23: 4C4AAAAAAABABgAAAOf//0AGAABABgAAQB8AAEAfAADgLgAAwOD//+AuAAA=
pub_title:
 Description and crystal structure of nabiasite, BaMn9[(V,As)O4]6(OH)2,
 a new mineral from the Central Pyrenees (France)

qdat:
AAAAAAAAAAAAAAQAIAQAgAAgEAAgIEEACCCEEIIAhCIAiARAIiICRERIESJIgiCCIJJJIKSSglJKEpCQpSkSlSCVKJUSKGUVVJSijKCFVRKqDVQiUSFGEQkgwAKRAIASBAAASAAABAAAAIAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Ca (Al.099 Ti.901) Si O4.901 F.099
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF09
formula_title: <missing>
a: 7.0541
b: 8.6925
c: 6.5445
alpha: 90
beta: 113.903
gamma: 90
cell_volume: 366.876
crystal_density: 3.517
atoms_sites: ["Ca", "Aloct", "Tioct", "Si", "O1", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgCAhB4AwMYtAMDGLQDAxi0A4Fs3ACBzFwA=
atoms_y: ICsKAAAAAAAAAAAAYEQLAKAQBACgEAQA4BYEAGC7DAA=
atoms_z: AAAAAICEHgCAhB4AAAAAAICEHgCAhB4AgC4LAJBrGAA=
atoms_occupancy: AAk9AOAKBgAg/jYAAAk9ACD+NgDgCgYAAAk9AAAJPQA=
atoms_u_iso: 6H8BAOCHAQDghwEAoEABAJiAAACYgAAAmIAAAJiAAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAQAAAQAAAABCAEAAgAAACEAEAABAAQgQIAAAAEhQMCEYAIgEAIIhKIAqAgGA4JAQCgriAboFFJAAQqYkBLfsIwoFCmDgBiVZGyoVaMPIwbGA/zJf3YiRIj7EIv+0WYkyry6FCoJE71kzZPSoo6Z==


formula: Ca (Al.182 Ti.818) Si O4.818 F.182
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF18
formula_title: <missing>
a: 7.0511
b: 8.6722
c: 6.5325
alpha: 90
beta: 114.026
gamma: 90
cell_volume: 364.845
crystal_density: 3.510
atoms_sites: ["Ca", "Aloc", "Tioct", "Si", "O1", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgCAhB4AwMYtAMDGLQDAxi0AgIQ3AFCEFwA=
atoms_y: MCAKAAAAAAAAAAAAEDALAJA0BACQNAQAgA0EAIC+DAA=
atoms_z: AAAAAICEHgCAhB4AAAAAAICEHgCAhB4AEEkLANBYGAA=
atoms_occupancy: AAk9AMAbCwBA7TEAAAk9AEDtMQDAGwsAAAk9AAAJPQA=
atoms_u_iso: UF4BAIhEAQCIRAEAELgAANARAADQEQAA0BEAANARAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAQAAAQAAAABBAEAAQAAACEACAABgAIQIIAAAACQwKBCMAEgCAEIQmEAVAQDAUEgQBQVxAK0ChkgAEKqRAVV7EIKBQrBwA4lkRscF8jGyYGxgN9in+qFCKQ0pCZttvmQrJs3hQWBRa3kszbynJaR==


formula: Ca (Al.291 Ti.709) Si O4.709 F.291
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF29
formula_title: <missing>
a: 7.0462
b: 8.6529
c: 6.5231
alpha: 90
beta: 114.143
gamma: 90
cell_volume: 362.925
crystal_density: 3.493
atoms_sites: ["Ca", "Aloct", "Tioct", "Si", "O1", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgCAhB4AwMYtAMDGLQDAxi0AcF03AFBSFwA=
atoms_y: QBUKAAAAAAAAAAAAoDELACAdBAAgHQQAUBUEAPDVDAA=
atoms_z: AAAAAICEHgCAhB4AAAAAAICEHgCAhB4AwE0LABBfGAA=
atoms_occupancy: AAk9AODCEQAgRisAAAk9ACBGKwDgwhEAAAk9AAAJPQA=
atoms_u_iso: GG4BAEBaAQBAWgEAsDoBAAhhAAAIYQAACGEAAAhhAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAIAAAQAAAABBAEAAQAAABCACAAAwAIIIEAAAABIoFBBGACQBACEISiAKgEBgOCQIAoKcQFZBQqQACFXMQKVbhGFAYNgcAMJqEaHBqQitGAswFdYp/vCQkkdqgl5nzokKxfbYkFQMjX3rK26ZpWm==


formula: Ca (Al.372 Ti.628) Si O4.628 F.372
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF37
formula_title: <missing>
a: 7.0368
b: 8.6360
c: 6.5135
alpha: 90
beta: 114.232
gamma: 90
cell_volume: 360.948
crystal_density: 3.485
atoms_sites: ["Ca", "Aloct", "Tioct", "Si", "O1", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgCAhB4AwMYtAMDGLQDAxi0AYB03AEArFwA=
atoms_y: sBMKAAAAAAAAAAAAUDYLAKBCBACgQgQA4P0DALC2DAA=
atoms_z: AAAAAICEHgCAhB4AAAAAAICEHgCAhB4AoEoLAMAYGAA=
atoms_occupancy: AAk9AIC0FgCAVCYAAAk9AIBUJgCAtBYAAAk9AAAJPQA=
atoms_u_iso: SP0AALA6AQCwOgEAOKQAAChLAAAoSwAAKEsAAChLAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAIAAAIAAAAAggCAAIAAABCABAAAQAEIECAAAAAkUCggjABIAgBCEKRAFQCAwFBIEAUCuICsgoMkABCrmIDLrwhBQKGQOAHE7iKjgakY3RgbMBfaM37w0IqHKoRu6WrJC433NIhMClXt7Rsq2akp==


formula: Ca (Al.489 Ti.511) Si O4.511 F.489
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF49
formula_title: <missing>
a: 7.0229
b: 8.6130
c: 6.5023
alpha: 90
beta: 114.344
gamma: 90
cell_volume: 358.342
crystal_density: 3.472
atoms_sites: ["Ca", "Aloct", "Tioct", "Si", "O1", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgCAhB4AwMYtAMDGLQDAxi0AwD83AOBsFwA=
atoms_y: 8AAKAAAAAAAAAAAAgEcLACAdBAAgHQQAkBsEABCODAA=
atoms_z: AAAAAICEHgCAhB4AAAAAAICEHgCAhB4AUIELAJCEGAA=
atoms_occupancy: AAk9AKDYHQBgMB8AAAk9AGAwHwCg2B0AAAk9AAAJPQA=
atoms_u_iso: iEQBAMgsAQDILAEAeOsAAOhiAADoYgAA6GIAAOhiAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAIAAAIAAAAAgQCAAIAAAAhABAAAIACECBAAAAASKBQQRgAkAQAhCCogC0BAYBwkCAFBPCAvQKGKAAQqxiBWq8IwoChkDgBxE4ioUFxGN2YDSgX2in+2NCKQ7qCJmXrzIbE9JqIKglV9/aNvWy0V==


formula: Ca (Al.672 Ti.328) Si O4.328 F.672
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF67
formula_title: <missing>
a: 6.9904
b: 8.5759
c: 6.4798
alpha: 90
beta: 114.480
gamma: 90
cell_volume: 353.537
crystal_density: 3.457
atoms_sites: ["Ca", "Aloct", "Tioct", "Si", "O1", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgCAhB4AwMYtAMDGLQDAxi0AwCY3AKB/FwA=
atoms_y: APYJAAAAAAAAAAAAAFQLAMAsBADALAQAoPcDAJCBDAA=
atoms_z: AAAAAICEHgCAhB4AAAAAAICEHgCAhB4A0I0LAFCwGAA=
atoms_occupancy: AAk9AAAEKQAABRQAAAk9AAAFFAAABCkAAAk9AAAJPQA=
atoms_u_iso: cEgBAGhQAQBoUAEAaPEAAFCgAABQoAAAUKAAAFCgAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAAEAAAIAAAAAQIAgAEAAAAQgAQAAEABBBAgAAAAEjAIEEQAJAEAEQgpQAdAIFAaEAQBQR4QFUAgRQAEGXKgJ2vhGFAKOQaAKExCbjglEQ7agWSA+qSn60sExDmUInfeVWROLbmiQlAprj3MaT8lZ==


formula: Ca (Al.819 Ti.181) Si O4.181 F.819
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF82
formula_title: <missing>
a: 6.9580
b: 8.5445
c: 6.4612
alpha: 90
beta: 114.585
gamma: 90
cell_volume: 349.312
crystal_density: 3.449
atoms_sites: ["Ca", "Aloct", "Tioct", "Si", "O1", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgCAhB4AwMYtAMDGLQDAxi0AQBo3ANB3FwA=
atoms_y: 8OcJAAAAAAAAAAAAEGILAKBCBACgQgQAAM8DAMBgDAA=
atoms_z: AAAAAICEHgCAhB4AAAAAAICEHgCAhB4AUJoLAJC2GAA=
atoms_occupancy: AAk9AOD8MQAgDAsAAAk9ACAMCwDg/DEAAAk9AAAJPQA=
atoms_u_iso: AHIBAFCzAQBQswEA4B4BAPi7AAD4uwAA+LsAAPi7AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAACAAAEAAAAAIIAQACAAAAIQAIAADAAggQQAAAABRQGBBMACQBABEIMUALQCBIGiICAMEKEBWgEEKAAhi6UCK1YIwoBSyGQBxFMjOaE0mHJuDyID6xE7jUgVCNZRFt/5tpEc1mWJCKCTHTukzN6G==


formula: Ca Al Si F O4
compound: <missing>
pub_title: Crystal structural changes in titanite along the join TiO-AlF Sample: AlF100
formula_title: <missing>
a: 6.9157
b: 8.5076
c: 6.4391
alpha: 90
beta: 114.683
gamma: 90
cell_volume: 344.236
crystal_density: 3.437
atoms_sites: ["Ca", "Aloct", "Si", "F1", "O2", "O3"]
atoms_x: QEIPAICEHgDAxi0AwMYtAIA5NwCgyhcA
atoms_y: oAUKAAAAAAAwZQsAYDwEAGAKBABAVAwA
atoms_z: AAAAAICEHgAAAAAAgIQeANB0CwBgvhgA
atoms_occupancy: 0
atoms_u_iso: KAkBAAgVAQDoywAAyG4AAMhuAADIbgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAAAAAAAAACAAACAAAAAECAIABAAAAEEAEAAAgAIIEIAAAAAUkBgQTAAiAQAQiDDAC0AgJAkRAQChDQgG4BghQAIEOjAR1/AlFAFVEzANEo8VvkW6QIjUeQQebkraGyBSEvokT++yLRI991NFIYEibrnVsW1==


compound: western Alps
formula_title: <missing>
a: 10.862
b: 7.483
c: 5.150
alpha: 90
beta: 90
gamma: 90
cell_volume: 418.594
crystal_density: 4.868
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
formula:
Y.639 Ce.005 Pr.001 Nd.011 Sm.01 Gd.068 Dy.065 Er.034 Yb.025 Th.06 U.004 Ca.01 (Ti1.95 Nb.05) W.03 O6

pub_title:
 Crystal chemistry of aeschynite-(Y) from the Western Alps:
 residual electron density on difference-Fourier map
 Sample: TR1

atoms_sites:
["YA", "CeA", "PrA", "NdA", "SmA", "GdA", "DyA", "ErA", "YbA", "ThA", "UA", "CaA", "TiB", "NbB", "WC", "O1", "O2", "O3", "O4"]

atoms_x:
8HsbAPB7GwDwexsA8HsbAPB7GwDwexsA8HsbAPB7GwDwexsA8HsbAPB7GwDwexsAEO4VABDuFQCgzQoAQIERAOAdIADgxyUAIGYVAA==

atoms_y:
QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AkFofAJBaHwBAQg8AIJMaAIDhGwBAQg8AQEIPAA==

atoms_z:
UAgCAFAIAgBQCAIAUAgCAFAIAgBQCAIAUAgCAFAIAgBQCAIAUAgCAFAIAgBQCAIAYD0hAGA9IQDgzSQAoJM1AFAALQCgARMAEJ4aAA==

atoms_occupancy:
YAAnACBOAACgDwAA4KsAAECcAACAJgQAoPcDAEATAgCghgEAgKkDAIA+AABAnAAAYII7AKCGAQDA1AEAAAk9AAAJPQAACT0AAAk9AA==

atoms_u_iso:
YOoAAGDqAABg6gAAYOoAAGDqAABg6gAAYOoAAGDqAABg6gAAYOoAAGDqAABg6gAAwD4BAMA+AQBgZwEAAHcBAKCGAQAAdwEAYGcBAA==

qdat:
AAAAAAAAAAAAAAAAAAAIAAEBCAEAgAAIAAgJAAkCChACgxSSAJMBIgRAgxAcMNCoqUQtgxmlzUqpmaJ1kt2+tw9feaxqpt/dneP9/h7m2/3zKrq39611kvH23n/VK//rv+P3e7at7tvv7/3643+v365Uv/5O3H3xux3vPf==


compound: western Alps
formula_title: <missing>
a: 10.803
b: 7.532
c: 5.180
alpha: 90
beta: 90
gamma: 90
cell_volume: 421.487
crystal_density: 5.105
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
formula:
Y.54 La.001 Ce.009 Pr.003 Nd.032 Sm.034 Gd.072 Dy.071 Er.043 Yb.03 Th.12 U.02 Ca.01 (Ti1.95 Nb.03 W.02) O6.02

pub_title:
 Crystal chemistry of aeschynite-(Y) from the Western Alps:
 residual electron density on difference-Fourier map
 Sample: MI

atoms_sites:
["YA", "LaA", "CeA", "PrA", "NdA", "SmA", "GdA", "DyA", "ErA", "YbA", "ThA", "UA", "CaA", "TiB", "NbB", "WB", "OC", "O1", "O2", "O3", "O4"]

atoms_x:
8HsbAPB7GwDwexsA8HsbAPB7GwDwexsA8HsbAPB7GwDwexsA8HsbAPB7GwDwexsA8HsbADDxFQAw8RUAMPEVAEDdCgCQfBEAUBwgAMDdJQDAQxUA

atoms_y:
QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAJBzHwCQcx8AkHMfAEBCDwAgrBoAMOYbAEBCDwBAQg8A

atoms_z:
kNwBAJDcAQCQ3AEAkNwBAJDcAQCQ3AEAkNwBAJDcAQCQ3AEAkNwBAJDcAQCQ3AEAkNwBAMAtIQDALSEAwC0hAMB/JABAijUAEOEsAFAfEwCAtRoA

atoms_occupancy:
gPUgAKAPAACgjAAA4C4AAAD0AQBAEwIAAGUEAGBVBADgnwIAwNQBAABTBwCAOAEAQJwAAGCCOwBg6gAAQJwAAIA4AQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
MHUAADB1AAAwdQAAMHUAADB1AAAwdQAAMHUAADB1AAAwdQAAMHUAADB1AAAwdQAAMHUAAKC+AACgvgAAoL4AAOCrAADA2gAAAPoAAAD6AAAA+gAA

qdat:
AAAAAAAAAAAAAAAAAAAIAAIBEAIBgAAIABAKAAhEEUADBhoqAhwDFAKCgiRJoWcyGwgtClBE5qai0WhyVsf69Wo+0OrlrzacT1f73OtvT93Ur9Wz59/X63Pvtvfnf975+1rtcv3vPdpvfX1e//S/Fr/N77P9vH7fJ6/v99==


compound: western Alps
formula_title: <missing>
a: 10.904
b: 7.490
c: 5.189
alpha: 90
beta: 90
gamma: 90
cell_volume: 423.791
crystal_density: 5.293
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
formula:
Y.55 Ce.011 Pr.002 Nd.026 Sm.016 Gd.091 Dy.079 Er.034 Yb.022 Th.1 U.03 Ca.02 Ti1.81 Nb.09 Ta.01 W.11 O6

pub_title:
 Crystal chemistry of aeschynite-(Y) from the Western Alps:
 residual electron density on difference-Fourier map
 Sample: TR2

atoms_sites:
["YA", "CeA", "PrA", "NdA", "SmA", "GdA", "DyA", "ErA", "YbA", "ThA", "UA", "CaA", "TiB", "NbB", "TaB", "WB", "WC", "O1", "O2", "O3", "O4"]

atoms_x:
kIsbAJCLGwCQixsAkIsbAJCLGwCQixsAkIsbAJCLGwCQixsAkIsbAJCLGwCQixsAQOYVAEDmFQBA5hUAQOYVAOBvCgAQiREA0CggAGC7JQBAghUA

atoms_y:
QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AcD4fAHA+HwBwPh8AcD4fAEBCDwBQvRoAAO4bAEBCDwBAQg8A

atoms_z:
gBkCAIAZAgCAGQIAgBkCAIAZAgCAGQIAgBkCAIAZAgCAGQIAgBkCAIAZAgCAGQIAsB8hALAfIQCwHyEAsB8hAKArJQDAljUA8PYsAFBREwAQ0BoA

atoms_occupancy:
wJEhAOCrAABAHwAAQJYBAAD6AADgjQUAYNIEAEATAgDAVwEAgBoGAMDUAQCAOAEAoDw3ACC/AgAgTgAAIL8CAIA4AQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
wCUBAMAlAQDAJQEAwCUBAMAlAQDAJQEAwCUBAMAlAQDAJQEAwCUBAMAlAQDAJQEAsGIBALBiAQCwYgEAsGIBAIA4AQCghgEAQJYBACDFAQBAlgEA

qdat:
AAAAAAAAAAAAAAAAAAAQAAIBEAIBgAAQAAgRABIEJEAJCiVEAUoGiAhChmA4YofEogh5GqZOHqaOVos3KJdqzKhd6rW0N2mst1za6Jrrx1u3neP3K3pdbo/s2+7cet1/P1rt/+ZP37Pf39v/bvbrNdV17du1ty6/ZO/Z/7==


formula: Y.61 Ce.001 Nd.005 Sm.013 Gd.056 Dy.076 Er.041 Yb.025 Th.04 U.08 Fe.01 Ti1.8 Nb.17 Ta.01 W.06 O6
compound: western Alps
formula_title: <missing>
a: 10.881
b: 7.484
c: 5.156
alpha: 90
beta: 90
gamma: 90
cell_volume: 419.871
crystal_density: 5.206
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of aeschynite-(Y) from the Western Alps:
 residual electron density on difference-Fourier map
 Sample: CE
 - note: O1 z coordinate altered to match reported bond lengths

atoms_sites:
["YA", "CeA", "NdA", "SmA", "GdA", "DyA", "ErA", "YbA", "ThA", "UA", "FeA", "TiB", "NbB", "TaB", "WB", "WC", "O1", "O2", "O3", "O4"]

atoms_x:
oIAbAKCAGwCggBsAoIAbAKCAGwCggBsAoIAbAKCAGwCggBsAoIAbAKCAGwDQ5xUA0OcVANDnFQDQ5xUAQN0KAICHEQBQHCAAkLMlAPCGFQA=

atoms_y:
QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwDAOR8AwDkfAMA5HwDAOR8AQEIPAGCAGgAA1RsAQEIPAEBCDwA=

atoms_z:
YC8CAGAvAgBgLwIAYC8CAGAvAgBgLwIAYC8CAGAvAgBgLwIAYC8CAGAvAgAANCEAADQhAAA0IQAANCEAQL4kAPDANQDAFy0AcNcSAMBwGgA=

atoms_occupancy:
QDslAKAPAAAgTgAAIMsAAABrAwCAowQAoIACAKCGAQAAcQIAAOIEAECcAACA7jYAIDAFACBOAABAnAAAAHECAAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
cK0AAHCtAABwrQAAcK0AAHCtAABwrQAAcK0AAHCtAABwrQAAcK0AAHCtAACA7QAAgO0AAIDtAACA7QAAAHcBAAD6AACgCQEAQBkBAGDqAAA=

qdat:
AAAAAAAAAAAAAAAAAAAIAAEBCAEAgAAIAAgJAAkECiAEgiSiAJMBQghAgyAYMWFxUYQvBTtHjkyqkqLXJV086x1qc1zspva3Wafb3Btt8vnyS/Lrdy7vNuPn/n+uT+/v/8Pr6+1d57PX3fn3521r+9bsvdyPrP/3/jX+9/==


compound: western Alps
formula_title: <missing>
a: 11.031
b: 7.448
c: 5.188
alpha: 90
beta: 90
gamma: 90
cell_volume: 426.240
crystal_density: 5.574
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
formula:
Y.65 La.001 Ce.005 Pr.001 Nd.015 Sm.017 Gd.042 Dy.042 Er.023 Yb.018 Th.07 U.04 Ca.01 Fe.03 Ti1.41 Nb.36 Ta.22 W.05 O6

pub_title:
 Crystal chemistry of aeschynite-(Y) from the Western Alps:
 residual electron density on difference-Fourier map
 Sample: VV

atoms_sites:
["YA", "LaA", "CeA", "PrA", "NdA", "SmA", "GdA", "DyA", "ErA", "YbA", "ThA", "UA", "CaA", "FeA", "TiB", "NbB", "TaB", "WB", "WC", "O1", "O2", "O3", "O4"]

atoms_x:
kKQbAJCkGwCQpBsAkKQbAJCkGwCQpBsAkKQbAJCkGwCQpBsAkKQbAJCkGwCQpBsAkKQbAJCkGwAw2BUAMNgVADDYFQAw2BUA4G8KAGCdEQDAGiAAEKclAMCnFQA=

atoms_y:
QEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEBCDwDQ/B4A0PweAND8HgDQ/B4AQEIPACB6GgAwzRsAQEIPAEBCDwA=

atoms_z:
IHQCACB0AgAgdAIAIHQCACB0AgAgdAIAIHQCACB0AgAgdAIAIHQCACB0AgAgdAIAIHQCACB0AgDALSEAwC0hAMAtIQDALSEA4FAkALC6NQCwCS0A8GATAJB4GgA=

atoms_occupancy:
QKwnAKAPAAAgTgAAoA8AAGDqAACgCQEAQJACAECQAgBgZwEAQBkBAMBFBAAAcQIAQJwAAMDUAQCgBysAgPwKAMC2BgAgTgAAAHECAAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
EL0AABC9AAAQvQAAEL0AABC9AAAQvQAAEL0AABC9AAAQvQAAEL0AABC9AAAQvQAAEL0AABC9AACgvgAAoL4AAKC+AACgvgAA4CgBACBIAQDgKAEAQBkBAIA4AQA=

qdat:
AAAAAAAAAAAAAAAAAAAgAAICCAICQAAgAAhBACgEMEAhDQJKAYUKCEBERwDYcI7FAgSlIfBVDTJq5yUxi/G85GlVF/cqX+2ti5/5d5KXdXlHvd92Xm6tn1ft3+Lpf96m3Wvdb7fXPwdPbu/7/67/32de6vv7Z339enb593==


formula: Na.66 Ca.86 K.64 Mg.26 Si18 O49.42 H26.84
compound: volcanoclastites of North-Western Sardinia
formula_title: <missing>
a: 17.6750
b: 17.9572
c: 7.4091
alpha: 90
beta: 116.304
gamma: 90
cell_volume: 2108.105
crystal_density: 2.212
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-chemistry and synchrotron Rietveld refinement
 of two different clinoptilolites from volcanoclastites
 of North-Western Sardinia
 Sample: LAC1

atoms_sites:
["Na1", "Ca2", "K3", "Mg4", "Si1", "Si2", "Si3", "Si4", "Si5", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5", "Wat6", "Wat7", "Wat8", "Wat9", "Wat10"]

atoms_x:
QGwIAGDeAgBAxQ4AAAAAAPDhCgDw7gwAIM4MAOAvBAAAAAAA0NgLAMAiDgAgPgsAsC0OAAAAAACQygQAkLgHACCyAACQ5QwAkCIHAKCXEwDg/gcAoPEEAICEHgAA+gAA4I0FACAwBQDgHAMAIBgJAAB9AAA=

atoms_y:
AAAAAICEHgCAhB4AAAAAAIBmCgBgIhkAoK4LAGBMEgAQVg0AgIQeAKCUBwDwnAkAYGIGADD9EwBwwgkAYEsOAJDmEADgag8AQPkWAAAAAAAAAAAAwEQZAAAAAAAA3AUAAAAAAAAAAAAAAAAAAAAAAAAAAAA=

atoms_z:
gDwqAID2CwCggAIAgIQeAGD+BQBA4h4AcForAACWGQAAAAAA0A4cALC8JACw0zUAUDcPAICEHgDwpwMA0AMiAGArCwCwPwsAYLgZAKB0BADAhDgAoKc6AICEHgDARBkAgEkTAAD4KgDgCgYAABYmAKD1LQA=

atoms_occupancy:
QCQUAMA+GgAAiBMAgN4PAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AACBKQCATxIAAAk9AAAJPQCAhB4AgIQeAICEHgBA6B0AAEwdAIDeDwA=

atoms_u_iso:
QA0DAMBFBADA1AEAgKkDAECcAACAOAEAgDgBAECcAABAnAAAgDgBAIA4AQDA1AEAwNQBAMDUAQBAnAAAwNQBAECcAACAOAEAgDgBAABTBwDARQQAwLYGAMDUAQDARQQAADUMAABTBwDAJwkAQGAKAEDvBwA=

qdat:
AAAAAAAABAACAQABACCCGAAICANIRBBEAGg8IIYSAohRkOiYGMXEHG2a4DJRu+6qyj9ffA1CbG7p8V3PCpQJ33olbMB7uW/8Fv6KhZq/Ou4lV2I9XqNRDa0TuGlNrlXSc6KrN4FMYZJ9tD8Txhzp2fiHucUfBbiYNW0L8T==


formula: Na.26 Ca.74 K1.22 Si18 O50.12 H28.24
compound: volcanoclastites of North-Western Sardinia
formula_title: <missing>
a: 17.6589
b: 17.9241
c: 7.4034
alpha: 90
beta: 116.243
gamma: 90
cell_volume: 2101.790
crystal_density: 2.243
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-chemistry and synchrotron Rietveld refinement
 of two different clinoptilolites from volcanoclastites
 of North-Western Sardinia
 Sample: ZC16

atoms_sites:
["Na1", "Ca2", "K3", "Si1", "Si2", "Si3", "Si4", "Si5", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5", "Wat6", "Wat7", "Wat8", "Wat9"]

atoms_x:
IJUJAOCfAgBASA4AsPQKAPDVDACgqAwAoCkEAAAAAAAAbQsAcHIOAFCzCwBQVg4AAAAAAHDgBAAwyAcAgAYBADAODQCQIgcAYHIUAMAzBwBAAQUAgIQeAOClAQAgoQcAAGUEAGBbAwAgGAkA

atoms_y:
AAAAAICEHgCAhB4AkHQKAPAjGQBAjAsAkEQSAKA+DQCAhB4AgJEHAKBWCQCwdgYAIAgUADC8CQAwUw4AsOkQAEB0DwBA+RYAAAAAAAAAAAAA5xgAAAAAAICXBgAAAAAAAAAAAAAAAAAAAAAA

atoms_z:
wAIkAODsCgDAUQIA4AoGADC7HgAwIisAwI8ZAAAAAABg2BwAkB0lAEBrNgDweA8AgIQeABB5AwDQ0SEAoBgLAPDCCwBguBkAgJ0FAAC8NACA1joAgIQeAIArGAAgyhUA4K8pAEBmCQBAoCkA

atoms_occupancy:
QO8HAECVFgBAOyUAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgDEXAADbGgBAFkAAAAk9AMAgHwBAlRYAQB0qAEDDOABAjiwA

atoms_u_iso:
AHECAIAaBgDARQQAQJwAAIA4AQCAOAEAQJwAAECcAACAOAEAwNQBAMDUAQDA1AEAAHECAECcAADA1AEAQJwAAIA4AQDA1AEAQH4FAICpAwCAiwgAwNQBAABxAgBADQMAgG0NAEBgCgDAtgYA

qdat:
AAAAAAAABAACAQABACCCGAAICANIRAhEAGg8IMUaAsRRUOicGMXEHn2aYDN52t6eTjdd3A/CalrY0L9PipYJ32slbMB7mWrsF9aKhZqvKu4VS2I9TaHRD+0ZqGlPplWyc6KtN4HMUZJ9tDsRpgzluXSHucUXBbicNSsL0T==


formula: K.632 As15 Cu18 O88.3 H65.017
compound: <missing>
pub_title: Crystal structure of pushcharovskite
formula_title: <missing>
a: 13.6164
b: 15.6672
c: 19.1869
alpha: 106.933
beta: 91.531
gamma: 98.401
cell_volume: 3863.296
crystal_density: 3.241
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["K", "As1", "As2", "As3", "As4", "As5", "As6", "As7", "As8", "As9", "As10", "As11", "As12", "As13", "As14", "As15", "Cu1", "Cu2", "Cu3", "Cu4", "Cu5", "Cu6", "Cu7", "Cu8", "Cu9", "Cu10", "Cu11", "Cu12", "Cu13", "Cu14", "Cu15", "Cu16", "Cu17", "Cu18", "O1", "O-H2", "O-H3", "O4", "O-H5", "O6", "O7", "O-H8", "O-H9", "O-H10", "O11", "O12", "O13", "O14", "O15", "O-H16", "O17", "O18", "O19", "O-H20", "O21", "O22", "O23", "O-H24", "O25", "O26", "O27", "O-H28", "O29", "O30", "O31", "O32", "O33", "O34", "O35", "O-H36", "O-H37", "O38", "O39", "O40", "O-H41", "O42", "O43", "O44", "O-H45", "O46", "O47", "O48", "O-H49", "O50", "O51", "O52", "O-H53", "O54", "O55", "O-H56", "O-H57", "O58", "O59", "O60", "O-H61", "Wat61", "O-H62", "Wat62", "O-H63", "Wat63", "O-H64", "Wat64", "O-H65", "Wat65", "O-H66", "Wat66", "O-H67", "Wat67", "O-H68", "Wat68", "O-H69", "Wat69", "O-H70", "Wat70", "O-H71", "Wat71", "O-H72", "Wat72", "O-H73", "Wat73", "O-H74", "Wat74", "O-H75", "Wat75", "O-H76", "Wat76", "O-H77", "Wat77", "O-H78", "Wat78", "O-H79", "Wat79", "O-H80", "Wat80", "O-H81", "Wat81", "O-H82", "Wat82", "Wat83", "Wat84", "Wat85", "Wat86", "Wat87", "Wat88a", "Wat88b", "Wat89a", "Wat89b", "Wat90a", "Wat90b", "Wat91a", "Wat91b", "Wat92a", "Wat92b", "Wat92c"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAACAhAAoMABYSBwwKmQDbmNh3KU92T1sPP+a1vv/39f//q/vv/f9/+//nv////v/7/v////////9///f/////f/////v//v3///+3/t3efn7et81X6KXDNMgNyojAPAwAgGAQAAEAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Na.06 Ca.94) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.8475
b: 9.0277
c: 5.2495
alpha: 90
beta: 104.805
gamma: 90
cell_volume: 451.189
crystal_density: 3.637
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAA0IIRAOCBBwDAPRYA8CIVAA==
atoms_y: wFUSAMBVEgCQYDcAsK4FAECXBQAQ/w4AIEgBAA==
atoms_z: QEIPAEBCDwBAQg8AcCcOABBVCQDAsxMAQB8AAA==
atoms_occupancy: gKkDAIBfOQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: QEcAAEBHAAD4XAAAeDcAACiqAADA1QAAkOcAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: hd/6

qdat:
AAAAAAAAAAAAAAAAgAAAAAgQAAAAQAAggAAgEAAAAoAIiAJIgCBMAAAEUYggQAQEkgyEEKkEKiUAAPQAiguAWarPgICkh2CpXgxuIFOiom50hMhn85LDiZ6I56w5eDhjkVzWQ+4Yk7HmMepHXERJ94ZHzMm2WJGBqIQgm9==


formula: (Na.1 Ca.9) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.8472
b: 9.0288
c: 5.2466
alpha: 90
beta: 104.789
gamma: 90
cell_volume: 451.014
crystal_density: 3.629
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAYIQRANCMBwAgYBYAwBEVAA==
atoms_y: sGASALBgEgAAXzcA0JgFAAB4BQAg2w4AQDIBAA==
atoms_z: QEIPAEBCDwBAQg8A4CUOAEAbCQAgvRMAEMw8AA==
atoms_occupancy: gBoGAIDuNgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: 0M8AANDPAADI1wAAiIYAAGD5AAAQFwEAqDgBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: hd/10

qdat:
AAAAAAAAAAAAAAAAgAAAAAgQAAAAQAAggAAgEAAAAoAIiAJIgCBMAAAEUYggQAQEkgyEEKkEKiMAAPQAihuAWarPgICkh2CpXwxuIFOhoj50hMhn85LDiZ6I56w5+Dhjkvy1Iu4Yi7H2EaonXEJJdYZHzMl2WJGBqIQQm9==


formula: (Na.25 Ca.75) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.7951
b: 8.9698
c: 5.2634
alpha: 90
beta: 105.523
gamma: 90
cell_volume: 445.574
crystal_density: 3.635
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAoLwRAKAXBwCAHhYAcOQUAA==
atoms_y: kCsSAJArEgAgMDcAAHgFABC4BQAwNA8AACwBAA==
atoms_z: QEIPAEBCDwBAQg8AMJ4OAMCkCQDQ+RIAQKs8AA==
atoms_occupancy: QEIPAMDGLQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: oIIAAKCCAAAIVwAAME0AANhyAABYmAAAmIAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae25/20

qdat:
AAAAAAAAAAAAAAAAQAAAAAQIAAAAEAAQQAAIBAAAAIACIQCkIAQjAAAAjFCICAIBESVQQRkQR0kgACuAEIGoAbKw+AIhGUpCi7B5sQcfRjJfYA4h/aHCG8NSPHRZz1Vj9hWc8CdMmZO1Zoe4LqaAsTSMjpIzR4ixio4JAd==


formula: (Na.4 Ca.6) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.7598
b: 8.9277
c: 5.2748
alpha: 90
beta: 106.041
gamma: 90
cell_volume: 441.712
crystal_density: 3.628
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAsJgRAKBJBwAg4xUA0IMVAA==
atoms_y: gDYSAIA2EgAQCTcA0GYFAIA5BQCwJw8AYNEAAA==
atoms_z: QEIPAEBCDwBAQg8A4FcOAIAICQBQgxMAIBwAAA==
atoms_occupancy: AGoYAACfJAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: CGEAAAhhAAD4XAAA8AUAAODJAAAItgAAsB0AAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae40/20

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAAEAAQIAAEBAAAAKABCEBUEAEIwAAAIyQiAgEARCokCEYiCLKQACJgAjDZAHQ9ToAoIbogUTqLtSGVUK1NOADiM64oIag4o8xB9lRZt9Dt+QhisMK+5Ml2pfWYGXJm0J2tZipbJhgwYU==


formula: (Na.5 Ca.5) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.7441
b: 8.9103
c: 5.2791
alpha: 90
beta: 106.225
gamma: 90
cell_volume: 440.091
crystal_density: 3.615
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAA4KkRAOAEBwAwChYAYAgVAA==
atoms_y: gDYSAIA2EgCw/zYAUHMFALAYBQDATg8AwPMAAA==
atoms_z: QEIPAEBCDwBAQg8AEFAOAAD8CACAmhIAANc8AA==
atoms_occupancy: gIQeAICEHgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: oIIAAKCCAAAIVwAAME0AANhyAABYmAAAmIAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae50/20

qdat:
AAAAAAAAAAAAAAAAQAAAAAIEAAAACAAIEAAEAgAAAKABBCA0CAEIwAAAEaIRAQCAJBYyBCURBFlIABEQASisgDoVZ0AUEJ4wKJ0lVVDKdEqmSgAxDPsUGF4KSWsQ2z0q9vg3/ERYzDCu8XUTLl1HEzqVzC9yWVJdy0wGER==


formula: (Na.6 Ca.4) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.7189
b: 8.8818
c: 5.2835
alpha: 90
beta: 106.598
gamma: 90
cell_volume: 437.075
crystal_density: 3.614
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAUKgRAOA2BwBQDRYAgFYVAA==
atoms_y: YDMSAGAzEgDQAjcAcHYFALAxBQBAQg8AYNEAAA==
atoms_z: QEIPAEBCDwBAQg8AAHQOAFD3CADwFRMAkEwAAA==
atoms_occupancy: AJ8kAABqGAAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: oIIAAKCCAAAIVwAAME0AANhyAABYmAAAmIAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae60/1

qdat:
AAAAAAAAAAAAAAAAIAAAAAECAAAACAAICAACAQAAAJAAghAaBABEYAAACFEEgECAEQIVAIlEQTSiAAhGAEqJIB6HicgCAnqSEiMlPVIxlxmVj8AKFbtjgx2j5UphVvcipm6GfUYJiymM/g7CokeMJKjQ2MP3F9Yzq6XAcU==


formula: (Na.75 Ca.25) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.6977
b: 8.8519
c: 5.2861
alpha: 90
beta: 106.765
gamma: 90
cell_volume: 434.488
crystal_density: 3.597
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAQJoRALAlBwCwZxUA0FEVAA==
atoms_y: cCgSAHAoEgBg6zYAsGMFAOAQBQCASA8AYLgAAA==
atoms_z: QEIPAEBCDwBAQg8AEGkOAPA+CACAFxMAEKQAAA==
atoms_occupancy: wMYtAEBCDwAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: oIIAAKCCAAAIVwAAME0AANhyAABYmAAAmIAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae75/20

qdat:
AAAAAAAAAAAAAAAAIAAAAAECAAAABAAECAABAQAAAIgAQQgOAgAiMAAABCiCQCBACIGKQESiIItSAAgjACWCyAvE5nQBgK7JBInJTlSIRsxXIvACx7NcoMZpVWOoYu/IYdvhXrmEoSoy7oLyrGjahjJcOTm2w26L+fDIFu==


formula: (Na.9 Ca.1) Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.6714
b: 8.8152
c: 5.2926
alpha: 90
beta: 107.166
gamma: 90
cell_volume: 431.122
crystal_density: 3.585
atoms_sites: ["NaM2", "CaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAILARAMAaBwCw/RUAoFkVAA==
atoms_y: IEYSACBGEgAA4jYAUHMFAEDPBABgkA8AoL4AAA==
atoms_z: QEIPAEBCDwBAQg8AIEUOACBpCABgyRIA0LYAAA==
atoms_occupancy: gO42AIAaBgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: oIIAAKCCAAAIVwAAME0AANhyAABYmAAAmIAAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae90/13

qdat:
AAAAAAAAAAAAAAAAIAAAAACBAAAAAgAEBAAAgIAAAIIAIIIFAIARDAAAARQgkAggAiFokBEohBZYgAQI4AVgkgZyGlSAUDO0IKExGcqiCc4EyLUAVcpvtAjK1nxponv4lBm+f3TJDRLim6ieLMbdKWKEjJGxNFZI+6YMQT==


formula: Na Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.6549
b: 8.7947
c: 5.2938
alpha: 90
beta: 107.394
gamma: 90
cell_volume: 428.952
crystal_density: 3.577
atoms_sites: ["NaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAQuxEA0PYGACDjFQBgUxUA
atoms_y: MFQSADDaNgDwaQUAQLYEAGCQDwBwlAAA
atoms_z: QEIPAEBCDwCATg4A4GIIAOA/EgBwrQAA
atoms_occupancy: 0
atoms_u_iso: WPcAAPhmAABYOQAAWJgAAFCgAAD4ZgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae100/12

qdat:
AAAAAAAAAAAAAAAAEAAAAACBAAAAAgAEAgAAQEAAAEIAEEEDAIAIhAAAAIoQSAQQARCUSASUIgs8QAIEOAKwTIK9BpsgJAi6CFBchGqpBtaDMk6gF6q+2QIyVZ07YJfuJQMu3+Yyg06oVp4njij75ZbBSxF6b5LXO7HFkB==


formula: Na Fe Si2 O6
compound: <missing>
formula_title: <missing>
a: 9.6543
b: 8.8070
c: 5.2943
alpha: 90
beta: 107.316
gamma: 90
cell_volume: 429.748
crystal_density: 3.570
atoms_sites: ["NaM2", "FeM1", "SiT", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAQuxEA4NIGAHD3FQCQSxUA
atoms_y: 8DQSABDXNgAQbQUAQLYEAMCADwDQtgAA
atoms_z: QEIPAEBCDwBALw4AIGkIACB4EgDAdgAA
atoms_occupancy: 0
atoms_u_iso: KFUAAIheAACoGwAAeOsAALh0AABYQwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthesis and structural properties of clinopyroxenes of the
 hedenbergite CaFeSi2O6 - aegirine NaFeSi2O6 solid-solution series
 Sample: ae100/F3d

qdat:
AAAAAAAAAAAAAAAAEAAAAACBAAAAAgAEBAAAQEAAAEIAIEIHAIAJDAAAAIogUAQQAhEkUAiYRAtogAIEcAVQmQVZDS1AJAm0CJCYjNKxBqcCZJ1ALa09ugZkqx5WoT+8Swa9n+QkhZ1QbaxPGlG9yylCnjL03yS+M2NKkF==


formula: Ca2 Fe1.865 Al.135 O5
compound: <missing>
formula_title: <missing>
a: 5.420
b: 14.743
c: 5.597
alpha: 90
beta: 90
gamma: 90
cell_volume: 447.240
crystal_density: 3.979
atoms_sites: ["Ca", "Fe", "FeT", "AlT", "O1", "O2", "O3"]
atoms_x: EJkfAICEHgDAwyEAwMMhAAAaHQCAXRgAoBQtAA==
atoms_y: cOsXAICEHgBAQg8AQEIPAEDmFQBAQg8AQHgfAA==
atoms_z: IJU7AICEHgCAahoAgGoaAIDpIgBQywcAwHUuAA==
atoms_occupancy: AAk9AAAJPQCgyzQAYD0IAAAJPQAACT0AAAk9AA==
atoms_u_iso: IE4AAAAyAADQIAAA0CAAACBnAACwTwAAwEQAAA==
atoms_aniso_label: ["Ca", "Fe", "FeT", "AlT", "O1", "O2", "O3"]
atoms_aniso_u11: kH4AAFAUAADAKwAAwCsAABCkAABgVAAAYDsAAA==
atoms_aniso_u22: cDAAAEBqAAAQDgAAEA4AAMBEAAAgTgAAQGoAAA==
atoms_aniso_u33: QDgAAFAUAADwIwAA8CMAAHBJAABwSQAAgCUAAA==
atoms_aniso_u12: kAEAADD4//8AAAAAAAAAAAAAAAAAAAAAQB8AAA==
atoms_aniso_u13: MBEAAJABAACQAQAAkAEAAMD5//+Qz///oN3//w==
atoms_aniso_u23: YPD//yADAAAAAAAAAAAAAPAjAAAAAAAAoPb//w==
pub_title:
 Crystal growth and cation distribution in doped dicalcium ferrite
 Ca2(Fe1-xMex)2O5 (Me=Al,Ga)
 Sample: Me = Al

qdat:
AAAAAAAAAAAAAAQAAAAAgAAAAABBMAEAAAIAAECYwQSkUQAxgAJEERIiHFAJloFwETKQ26G0QxLg1qOF7xcsc9RwfYUIlHrnkjP6qX41Gzj/EH4+zaxrxP+qjf63q/dcX0G3Pa/L+3+0f8l7pqm3p2Pm+X2z54z7+e5p2z==


formula: Ca2 (Fe1.445 Ga.555) O5
compound: <missing>
formula_title: <missing>
a: 5.420
b: 14.721
c: 5.599
alpha: 90
beta: 90
gamma: 90
cell_volume: 446.732
crystal_density: 4.156
atoms_sites: ["Ca", "Fe", "Ga", "FeT", "GaT", "O1", "O2", "O3"]
atoms_x: wJ0fAICEHgCAhB4AMKkhADCpIQAQ9hwAsG4YADAWLQA=
atoms_y: cOsXAICEHgCAhB4AQEIPAEBCDwAg4xUAQEIPALB2HwA=
atoms_z: wIs7AICEHgCAhB4AYGcaAGBnGgBg/yIAwLAHAHB6LgA=
atoms_occupancy: AAk9AOBnNQAgoQcAQMoiAMA+GgAACT0AAAk9AAAJPQA=
atoms_u_iso: EFkAALA2AACwNgAAMCoAADAqAABAagAAkEwAAEBRAAA=
atoms_aniso_label: ["Ca", "Fe", "Ga", "FeT", "GaT", "O1", "O2", "O3"]
atoms_aniso_u11: YIYAAGAiAABgIgAA0DkAANA5AACAuwAAwEQAADBDAAA=
atoms_aniso_u22: QDgAAJBlAACQZQAAwBIAAMASAABAHwAAsE8AAJB+AAA=
atoms_aniso_u33: cEkAAJAaAACQGgAAMCoAADAqAADgYAAA4GAAAKAoAAA=
atoms_aniso_u12: AAAAAFD7//9Q+///AAAAAAAAAABg8P//AAAAAKAPAAA=
atoms_aniso_u13: MBEAAJABAACQAQAAAAAAAAAAAABABgAAYNf//0DU//8=
atoms_aniso_u23: YPD//0AGAABABgAAAAAAAAAAAABAHwAAAAAAAKD2//8=
pub_title:
 Crystal growth and cation distribution in doped dicalcium ferrite
 Ca2(Fe1-xMex)2O5 (Me=Al,Ga)
 Sample: Me = Ga

qdat:
AAAAAAAAAAAAAAQAAAAAgAAAAABBMAEAAAIAAICYwQSkWQAwgAFEERITHDAJloEgERGIX+FcQZLgzuOF7xaucdR4dUUIin7nkhPaqX4tGhi3EH4/zbprxP/ulP63q/dsX0G3vq3b27+0f6l5pqm3q6Pm+X+z54r3q/5puz==


formula: Al3.983 Fe1.038 Mg.97 Si2 (O14 H4)
compound: <missing>
formula_title: <missing>
a: 9.467
b: 5.466
c: 9.140
alpha: 96.67
beta: 101.04
gamma: 90.0
cell_volume: 460.949
crystal_density: 3.409
atoms_x: QEIPAEBCDwAAAAAAIGIFACBiBQBAQg8AQEIPAMD6HABARgYAUP8PAAB3GgAQfhcAEC0YAID1BwBg0wgA
atoms_y: QEIPAEBCDwCAhB4AUMgtAFDILQBAQg8AwMYtABDpGgDAjxkAcNQ4AGAWGwAgEw4AoMgoAPBVAADwJB0A
atoms_z: AAAAAAAAAACAhB4AAEsAAABLAACAhB4AgIQeAHBtEwAAXwUA4I0FAPAlCAAAPhcAcIEYAFDcGQDwVBUA
atoms_occupancy: kPc7AHARAQAACT0AwCAfACCaHQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthetic and natural Fe-Mg chloritoid: structural, spectroscopic and
 thermodynamic studies
 Sample: MKM-97-4

atoms_sites:
["AlM1A", "FeM1A", "AlM2A", "FeM1B", "MgM1B", "AlM2B1", "AlM2B2", "SiT", "O-H1A", "O-H1B", "O1C", "O2A", "O2B", "O2C", "O2D"]

qdat:
AAAAAAAAAAAJAAAAABAIAAEGAAAMgAgAQBEOABEoECwEhcAkDE0RBIDKoBJZoY+ioyBiCwH6icwNi27Uji8K5yKx2v5hv+jjXv1OZ867tj328fe3/DVFf3n/9dy5+5+7v9/l/r15v97v99vfvdXs8X7v+e+ud9/f+7Z8+P==


formula: Al3.985 Fe.875 Mg1.12 Si2 (O14 H4)
compound: <missing>
formula_title: <missing>
a: 9.451
b: 5.4674
c: 18.159
alpha: 90
beta: 101.4
gamma: 90
cell_volume: 919.807
crystal_density: 3.378
atoms_x: QEIPAEBCDwAAAAAAIDAFACAwBQDQdQ8AUH8cAKD+BgCA9w8AkF8aAOA0GAAgOxgAoKcIABAKCQA=
atoms_y: QEIPAEBCDwDQARoAECwtABAsLQDA0ScAQKIYALBVGAAgCzkA8DwZABBPCgDg8yYA4GE2AJBMGQA=
atoms_z: AAAAAAAAAABAQg8AIDUAACA1AADQKg8AIMcJAMBLAwBQ0AIAECgEADD7CwBQ/gsAMLALAGAlDAA=
atoms_occupancy: oB48AGDqAAAACT0AwD4aAAAuIgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Synthetic and natural Fe-Mg chloritoid: structural, spectroscopic and
 thermodynamic studies
 Sample: RO2

atoms_sites:
["AlM1A", "FeM1A", "AlM2A", "FeM1B", "MgM1B", "AlM2B1", "SiT", "O-H1A", "O-H1B", "O1C", "O2A", "O2B", "O2C", "O2D"]

qdat:
AAAAAAAAAAABAAAAAAAAAASEAAQEABAAAAgKAALgoAUEE0AwLkAAqAgiRAF2apSkoomlREzcFEBDn1GRarWgNYHhA/FLMcakGL1pIn5sVr0GoTU10wZ2pf2e/Tsfd78LS4LwAs1a7rau2otcolVhU0HULLcyqIGxZ+R400==


formula: Ca5 Si6 O22 H10
compound: <missing>
formula_title: <missing>
a: 11.274
b: 7.344
c: 11.468
alpha: 99.18
beta: 97.19
gamma: 90.02
cell_volume: 929.775
crystal_density: 2.611
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of clinotobermorite and tobermorite 9 A:
 OD character, polytypes, and structural relationships
 Sample: MDO2 data collected at Pisa

atoms_sites:
["Ca1", "Ca1A", "Ca3", "Ca3A", "Ca2", "Si1", "Si1A", "Si2", "Si2A", "Si3", "Si3A", "O1", "O1A", "O11", "O11A", "O2", "O2A", "O21", "O21A", "O3", "O3A", "O31", "O31A", "O4", "O4A", "O5", "Wat5", "O6", "O6A", "Wat6", "Wat6A", "Wat7", "Wat8"]

atoms_x:
gDcWAODR6f/w+DQAENXK/xAAEwCwgjYAsG3J/zDPPAAgRcP/0J42AOBlyf+guTcAgBfI/2AXOAAAVsj/4A4vAKAv0f8gsS4AoC/R/yBOAADgLgAAQB8AACBOAADgYTYAoF/J/6CMAABAXx8AYMAHAIBu+P+gjev/wN8UAIDeDwCA3g8A

atoms_y:
AIsGAOCj+f9gFwYA8OP5/3Dr/v/gfAwAADXz/2DK/f9wVgIAIELp/4CCFgCAkQcAADD4/+AF8v/g2g0AoBDr/yBNFQAgGAkAoMj2/yBV6v8gyhUA4HUJAGAs9v9gThoAAKLl/8Dg//+gjAAAYH/9/yA8AwAg4/z/4J8CAEB58f+grw8A

atoms_z:
wFI4ACBAyP/Q0DYAsKXI/5AtGgBwOQsAcMP0/5CvFQCA+un/UGgLAFCn9P/A6xIA4CPt/4BJEwDgI+3/4AQHAIBo+f9AeAYAoDn5/2DGBgDAh/n/4AoGAGCX+f8gdw4AQHnx/6BVHgBgMB8AYPsSAKCH7P8gUNb/4KkqAKDGIABgpyAA

atoms_u_iso:
8CMAAPAjAACAJQAAgCUAAKCGAQDgFQAA4BUAAIBXAACAVwAAIBwAACAcAAAgywAAIMsAAECcAABAnAAAgD4AAIA+AAAAfQAAAH0AACBOAAAgTgAAgD4AAIA+AACgjAAAoIwAAMDaAABgZwEAwNoAAMDaAACAnQUAgJ0FAMBLAwCgegMA

qdat:
AAAAAAAAAIAAAAkAAIKAAJgBAIAIxAGBAmBHBNCHWAStURTdjNWqcpLV5F7CudAevvz5W+9K/re8e+s9v/mz9/v/6v3f//7+37f+f////+3f//ez//d36P//339f8//y/N2///d29Z/+3/OT//f///tv3N1udn//97n5uZ==


formula: Ca5 Si6 O22 H10
compound: <missing>
formula_title: <missing>
a: 11.273
b: 7.350
c: 11.498
alpha: 99.17
beta: 97.19
gamma: 89.97
cell_volume: 932.930
crystal_density: 2.602
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of clinotobermorite and tobermorite 9 A:
 OD character, polytypes, and structural relationships
 Sample: MDO2 data collected at Bern

atoms_sites:
["Ca1", "Ca1A", "Ca3", "Ca3A", "Ca2", "Si1", "Si1A", "Si2", "Si2A", "Si3", "Si3A", "O1", "O1A", "O11", "O11A", "O2", "O2A", "O21", "O21A", "O3", "O3A", "O31", "O31A", "O4", "O4A", "O5", "Wat5", "O6", "O6A", "Wat6", "Wat6A", "Wat7", "Wat8"]

atoms_x:
kBMWANDD6f/QJzUAoO/K/+AHEwDQhTYAIIXJ/5DYPADgV8P/0J42AOBMyf+guTcAwDbI/0DJNwCAF8j/QP8uAGAQ0f+AoS4AYBDR/+AuAACgDwAAQB8AAIA+AADgYTYAoF/J/6CMAACAAR8AQHIHAAAw+P+gjev/YHIUAEC/DwDA/Q8A

atoms_y:
QJEGAMCg+f/ABwYA4NX5/yDX/v+wnQwA8Fjz/7Cs/f+ASwIA0Ebp/2CYFgAgoQcAwI34/+CC8v/ACQ4A4LLq/0AeFQCgVgkAgPf2/6CT6v/A2RUAQGYJAGAs9v8gLxoAAKLl/+Cx//+gjAAAYH/9/8DOAgCgJ/z/oIACAKDm8f9AQg8A

atoms_z:
kFo4ALAoyP8AyTYAALrI/5AUGgDQKQsAcMP0/xDVFQDgHOr/0HQLAACT9P9g+xIAwFLt/0AqEwAA9ez/wLYGAMAK+f/AtgYAYJf5/6DlBgDAh/n/4AoGAACn+f+AZw4A4Ijx/0BlHgCAAR8AwOsSAAB47P8g09X/YGsqAMAUIQCAeCAA

atoms_u_iso:
UC0AAFAtAAAQJwAAECcAAECWAQAAGQAAABkAACBnAAAgZwAAsE8AALBPAACgjAAAoIwAAIC7AACAuwAAgD4AAIA+AABgbQAAYG0AACBOAAAgTgAAIE4AACBOAAAAfQAAAH0AAKAJAQBAlgEAQJwAAECcAAAAZQQAAGUEACC/AgCgegMA

qdat:
AAAAAAAAAIAAAAkAAIKAAJgBAIAJxAGDAsDGBWCGaAkvUSltjNbKtpOV6P+HsvAv3Xn6l9v3X259X+t9/9l/r///z+++//a19f9e//+///tfv+/n/+/v6///v/79Z//n/ft3//dr7T7u789irn/fX/f/27/99N7f+7fj93==


formula: Ca5 Si6 O22 H10
compound: <missing>
formula_title: <missing>
a: 11.276
b: 7.343
c: 22.642
alpha: 90
beta: 97.28
gamma: 90
cell_volume: 1859.637
crystal_density: 2.611
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of clinotobermorite and tobermorite 9 A:
 OD character, polytypes, and structural relationships
 Sample: MDO1 data collected at Pisa

atoms_sites:
["Ca1", "Ca1A", "Ca3", "Ca3A", "Ca2", "Si1", "Si1A", "Si2", "Si2A", "Si3", "Si3A", "O1", "O1A", "O11", "O11A", "O2", "O2A", "O21", "O21A", "O3", "O3A", "O31", "O31A", "O4", "O4A", "O5", "Wat5", "O6", "O6A", "Wat6", "Wat6A", "Wat7", "Wat8"]

atoms_x:
MM00AKBcCABw7DQAgNwHAICPMQDAXjYAgGUGAODsPACwaAAAwMI2AJBzBgAgezcAoPEEACB1OADgjQUAoO8uAMAJDgDAwC4AQEgOAMBdAACAPgAAYPD//8Dg//8ggTYAgJcGAKCMAABg6gAAQO8HAMCWNQDgdQkAwCUzAIAkLgAAYy4A

atoms_y:
gDEXAAB2FgCgxTUAwBk1AKACFwCgVDMAoNcyAOCBBwCg3wcAILIZAEAGGQBANDsAYBE5AGD7EgDAbhIA4KQWAADzFgCgQjYAALw0AMBQFwBAlRYAQNs0AMAfNABggyYAQDUmAMA5BgCAMRcAYLoIAICRBwBAoCkAQLImAICXBgCA3SQA

atoms_z:
wDIcADCbAgAgWxsA0NwCALAaDQCgGCQAkJI3ADBgKQDwCjIAsFgkAHBENwAg2ycAwKIzACBYKAAgkzMAYKEhAEBAOQAg/yEAYAs6AMAOIgDA+zkAgHIhAGCOOQBAuCUAQNU1ACC3LQBgkA8AYPonAGA1MwBg+icAoNEzAKAsEAAAmhAA

atoms_u_iso:
UF8AAFBfAABgVAAAYFQAAIC1AQCgDwAAoA8AAECcAABAnAAA4C4AAOAuAACAPgAAgD4AAECcAABAnAAAIE4AACBOAACAPgAAgD4AAKCMAACgjAAAoA8AAKAPAAAgywAAIMsAAECcAADgpQEAYOoAAGDqAADAyAMAwMgDAABxAgCAqQMA

qdat:
AAAAAAAAAIAAAAAAAgiAgAhAAAQAlBgFIBxFhNICgQSJUiKhhmXWOAmbSzaSoeyujrwrXGVPyGzFnudXz1d5mP/duywOKefc1vd59lb+v9nWpX67ja172G+PtV6TMGlcjdW+k1cn3dT0WRW5/sYumatIoPkwzg4YFl0MgQ==


formula: Ca2.5 Si3 O9 H
compound: <missing>
formula_title: <missing>
a: 11.156
b: 7.303
c: 9.566
alpha: 101.08
beta: 92.83
gamma: 89.98
cell_volume: 763.870
crystal_density: 2.865
atoms_x: kKkWAOB0HgBwQhYAsI0XAFBqEwAwsxcAwM0XAMDNFwDgdB4AwKMeAIBbEADgSxAA4JgYAODsCgAARwkA
atoms_y: 0PwFAIATHADgaSQA4CsNAHDS/v8AKScAwCcJAGA+8/9gdygAAEcJAKCcJwDg8gkAoOoaAACP/f8AyR0A
atoms_z: AKf5/8CjHgAQ1Pj/oKINAPCBGgBQQw0AoAIXAOCkFgCgYgcAAE0IAMAzBwAgHggAIOgQAABwFwDAzRcA
atoms_occupancy: AAk9AICEHgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: oAkBAOAiAgCgCQEAIMsAAKCGAQBg6gAAwNQBAAB3AQAAdwEAQBkBACDLAABAGQEAwFcBAKCAAgBADQMA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of clinotobermorite and tobermorite 9 A:
 OD character, polytypes, and structural relationships
 Sample: MDO2

atoms_sites:
["Ca1", "Ca2", "Ca3", "Si1", "Si2", "Si3", "O1", "O11", "O2", "O21", "O3", "O31", "O4", "O6", "O-H6"]

qdat:
AAAAAAAAAIAQAACgAEBAgAIBCAAAwxBBAUBYBCEynMARTgQpNbByLhgFaR8pe2FHWVUtZNsarju71c98o/dpWLpbef++++/7zrnf9//+e/9/7997/6TPv////77//79f/9v//tXb+/2/7p+3p//P//73v/+6f++fff9+v5==


formula: Na2 Ca2 Al6 Si9 O38 H16
compound: <missing>
formula_title: <missing>
a: 18.4049
b: 56.655
c: 6.5443
alpha: 90
beta: 90
gamma: 90
cell_volume: 6823.935
crystal_density: 2.268
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Zeolites of NAT topology: Structure refinement of mesolite from single crystal
 X-ray data and comparison with the structures of natrolite and scolecite

atoms_sites:
["Na", "Ca", "Al1", "Al10", "Al100", "Si1", "Si10", "Si2", "Si20", "Si200", "O1", "O10", "O100", "O2", "O20", "O200", "O3", "O30", "O300", "O4", "O40", "O400", "O5", "O50", "O500", "O6", "O60", "O600", "O7", "H61", "H62", "H601", "H602", "H6001", "H6002", "H71", "H72"]

atoms_x:
uAw7APjqDQCgBzAAWBM6ALg2AgDAxi0AWEMAAOB1CQCYXQUAaAs3ANBlAQDYHTwAQOEuAJhEMgDIKAoAOG4EAEjfBQCgRzYAwHozACDJDAC4VQEAsFY6AHg1OQDIpgQAyP8KAPCyLwAwQQwAiEIDAADsMQAgLi8AYDsyAADECQCgPg0AwM4CAGDMBQDAnDQAICIxAA==

atoms_y:
2HEuAPh/MgBAny8AOKI0APj0MADAxi0ACMUyAFimLgBYsDMAOAkyABhSMQDwEjQAaCwvAFBWMQC4cjQAyDovAABBMgAQYjMAsE4uALDjLwDQtDQAAN4wAJCIMgDQMzMA0DMuAEDPMQAgxTMACOcuAEhMNADAGDEA8AoyALB7MwCASzQAULwvAJD6LgDAHzQAEC41AA==

atoms_z:
wIwmAHDNNQCwayUAIIE2ACCBNgAAAAAA8O8QACA8NQCgzicAoLUnALBLCQCw1AcAEMo0AFBoJADw9SgAwLU0ADCBMAAA7TAAkHMfABCNOgAw0SsAoPUtALB7GgBAOBkAACknAICjBAAwMwsAMAQXAABEFgCgjAAAwFECAEBIDgAgaxAAgEkTAMA+GgDgORMAQCQUAA==

atoms_u_iso:
ACwBAEC1AAAAZAAAIGcAACBnAABgbQAAQGoAAOBgAAAgZwAAAGQAAIC7AACw5QAAkMkAAICJAABAnAAAoIwAALCzAACgvgAAMMAAAOCrAADgxAAAAMgAAGDRAACAuwAAsMwAACApAgBg5AEAsEkBANCXAQAAcQIAgPwKAICLCACAqQMAQA0DAEANAwCAiwgAAMQJAA==

qdat:
AAAAAAAIAAAAgEBBARCIAKBlgYCQCIAASR5zCwDEhAgpBGxpqQoxEGkRWqzBAAKikeylpEZITIhAAAHI6RpEA7tCANJAAAA1WpFpIB0kAANJAAADdakGqABqgAAdIAAAvp1IGqABqQAAVIAAa8jZAGoAB5AAAAAAtnyDqA==


formula: Fe5.34 P3.62 V.38 O26.8 H17.6
compound: <missing>
pub_title: Structure solution from powder data of the phosphate hydrate tinticite
formula_title: <missing>
a: 7.965
b: 9.999
c: 7.644
alpha: 103.94
beta: 115.91
gamma: 67.86
cell_volume: 505.086
crystal_density: 2.881
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["Fe1", "Fe2", "Fe3", "Fe4", "P1", "V1", "O1", "O2", "O3", "Wat4", "P2a", "O5a", "O6a", "O7a", "Wat8a", "P2b", "Wat9b", "O10b", "Wat11b", "O12b", "O-H13", "O-H14"]

atoms_x:
gNIRAKDWFQAAAAAAsBECADDl/v8w5f7/cIQLACDJ+P8woQEAANL2/5BrGAAASxkAkCMLAOCaIADAqR0AAMcuADBrPACAKzEAcPslAEBoKgCgaB8AkI0KAA==

atoms_y:
gNQAACDlHQAAAAAAUFQfAPCjDADwowwA0AMJACD2FgAgXQoA4E8HAKAaEwAw0hYAMGgXAMC6FgBw+ggA0CQQACArCgDgIRcA4DMUALA4CACwCwMAANsaAA==

atoms_z:
wKgAAKDJLACAhB4AAGENACAZDQAgGQ0AEFwMAOCVDABgThoAMEoDAMDIAwCgM/r/AO4CAMDFEACAigQAoIkmAFCpLgDA3CEAcDssAIDCHADw1ikA4FYjAA==

atoms_occupancy:
AAk9AIB9NACAuSoAgBMcAEBwMQDAmAsAAAk9AAAJPQAACT0AAAk9AICEHgAACT0AAAk9AAAJPQAACT0AgIQeAIC5KgAACT0AgLkqAAAJPQAACT0AAAk9AA==

atoms_u_iso:
gO0AAIDtAACA7QAAgO0AAIDtAACA7QAAgO0AAIDtAACA7QAAgO0AAIDtAACA7QAAgO0AAIDtAACA7QAAgO0AAIDtAACA7QAAgO0AAIDtAACA7QAAgO0AAA==

qdat:
AAAAAAAAAAAIAAAIgAABAACQAEEAEIFBiCgAAAWbQgAQqJYBowDgI3hEJkUiY2gackL8VOwRmRQD9zNEUjaHysNZXvP1v3IuW53ZBf7uLn13udylftt/z996/7rx+zPv/381//P82zv/3/d/bu/u/+uV/7+3/3q/e3fs99==


formula: (Na.75 La.19 Ca.06) (Nb.5 Ti.5) O3
compound: <missing>
pub_title: Crystal structure of isolueshite and its synthetic compositional analogue Sample: isolueshite
formula_title: <missing>
a: 3.909
b: 3.909
c: 3.909
alpha: 90
beta: 90
gamma: 90
cell_volume: 59.731
crystal_density: 4.571
atoms_sites: ["Na", "La", "Ca", "Nb", "Ti", "O"]
atoms_x: AAAAAAAAAAAAAAAAgIQeAICEHgDgViMA
atoms_y: AAAAAAAAAAAAAAAAgIQeAICEHgAAAAAA
atoms_z: AAAAAAAAAAAAAAAAgIQeAICEHgCAhB4A
atoms_occupancy: wMYtAMCYCwCAqQMAgIQeAICEHgBAQg8A
atoms_u_iso: YBwBAGAcAQBgHAEAYNEAAGDRAAAgxQEA
atoms_aniso_label: ["Na", "La", "Ca", "Nb", "Ti", "O"]
atoms_aniso_u11: YBwBAGAcAQBgHAEAYNEAAGDRAACghgEA
atoms_aniso_u22: YBwBAGAcAQBgHAEAYNEAAGDRAACAuwAA
atoms_aniso_u33: YBwBAGAcAQBgHAEAYNEAAGDRAABADQMA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAAAAAAAAAAAAAAAEAAAAAAAAAAACAAAAAAAAABAAAAAAAACAAAAAAABAAAAAAAIAAAAAAQAAAAACAAAAABAAAAACAAAAAQAAAACAAAAAAAAACAAAAEAAAAQAAACAAAAQ==


formula: (Na.75 La.25) (Nb.5 Ti.5) O3
compound: <missing>
formula_title: <missing>
a: 7.7842
b: 7.8033
c: 7.7828
alpha: 90
beta: 90
gamma: 90
cell_volume: 472.746
crystal_density: 4.787
atoms_sites: ["NaA1", "LaA1", "NaA2", "LaA2", "NbB", "TiB", "O1", "O2", "O3"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAEBCDwBAQg8AYB8NAAAAAABAMBIA
atoms_y: QB8AAEAfAADgdB4A4HQeAEBCDwBAQg8AAAAAAAApDgAgdw4A
atoms_z: QEIPAEBCDwBAQg8AQEIPAAAAAAAAAAAAAAAAACBOAABAQg8A
atoms_occupancy: wMYtAEBCDwDAxi0AQEIPAICEHgCAhB4AAAk9AAAJPQAACT0A
atoms_u_iso: 8CIBAPAiAQDwIgEA8CIBAPAYAQDwGAEAYBYCAGhQAQDAdgAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of isolueshite and its synthetic compositional analogue
 Sample: synthetic (Na.75La.25)(Nb.5Ti.5)O3

qdat:
AAAAAAAAAAAAAAAAAAAgAAAIAABAAAgAAgAAAAgAIAEAGAEAEAIAADAMAgGAwGAgABAQGDgAMGAAwYIGGCBgBQwwQ4wYAQwxxhDAGEYYAjgKcZTmEAzHMZiAZlO5mATuoFYFMzdyh3M3ZwDm/9Q5sQZg2ZsmDcvVYfMgzD==


formula: Cu2 Pb6 Bi8 S19
compound: <missing>
pub_title: The crystal structure of Cu2Pb6Bi8S19
formula_title: <missing>
a: 27.637
b: 4.0499
c: 20.741
alpha: 90
beta: 131.258
gamma: 90
cell_volume: 1745.167
crystal_density: 6.949
atoms_x: CFoCAHipCwA4RhgAMK3///g7EgCw6gUAaGYYANDOEAAAAAAAOFQAABA1BgCoVwUAwFQEAOAYDAA4zwwAgCcSAOjRGAAw8xMA
atoms_y: gIQeAICEHgCAhB4AgIQeAAAAAAAAAAAAgIQeAICEHgCAhB4AgIQeAAAAAAAAAAAAgIQeAICEHgAAAAAAAAAAAICEHgAAAAAA
atoms_z: 4JwFAKhADQBY6RgAqEcVAOA/HACYChIA8MsCAPA7BgCAhB4AOMkNAHiPGwCQ8gkA8HMAANi7FgCoAAcAkEwUAHjgEADI/AMA
atoms_occupancy: 0
atoms_u_iso: IMUBAIDOAQDgjAEAsEkBAPAdAQAg/QAAsGIBAHBcAQCQFAEAoCIBABA6AQAg5AAAMAsBABBsAQDQGgEAwCUBACDFAQAA4QAA
atoms_aniso_u11: ENABAGDkAQDw5QEAMKEBAJBfAQCwYgEAQMgBAMCiAQBQpAEAYE4BAGCyAQBQcgEAoIYBAOBzAQCw3wEAoJ8BAGD9AQBgAwEA
atoms_aniso_u22: QMgBALCUAQBwdQEAABMBALDlAAAQ7wAAECEBAJBfAQCABgEAoFQBAJAtAQBwrQAAwAwBAOBBAQBg6gAAcMYAAABeAQDQAQEA
atoms_aniso_u33: ANsBADCCAgCQwwEAAJABAMBXAQDgDwEAwAYCAJB4AQAg5AAAQDIBAHAqAQCAOAEA4FoBAJB4AQAQUwEAIEgBALBJAQAAEwEA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u13: AEUBAECvAQDwaAEAEDoBAGADAQAg/QAAQJYBAEAyAQDg9gAAYAMBALAXAQDgKAEA0EwBAPDrAADQZQEAUA4BALDMAACQ4gAA
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA
atoms_sites:
["Cu", "Pb1", "Pb2", "Pb3", "Bi1", "Bi2", "Bi3", "Bi4", "S1", "S2", "S3", "S4", "S5", "S6", "S7", "S8", "S9", "S10"]

atoms_aniso_label:
["Cu", "Pb1", "Pb2", "Pb3", "Bi1", "Bi2", "Bi3", "Bi4", "S1", "S2", "S3", "S4", "S5", "S6", "S7", "S8", "S9", "S10"]

qdat:
AAAAAACAAAgAAEAIAAAAQEAAAQJBgAygBCIwSAACooAigwUmBIZCyGwmqmaFVG9KIPgdGqy0wMU9lrIvZVSch5iLijksdQpwZi0C0giHNLVbixgolXEhFUCzqBoNQMBIhpdHHw9KNxHwsZFCOIEKkUAiCAIfWWzYorRydS==


formula: Pb14 Sb30 O5 S54
compound: Tuscany, Italy
formula_title: <missing>
a: 51.996
b: 8.148
c: 24.311
alpha: 90
beta: 104.09
gamma: 90
cell_volume: 9989.811
crystal_density: 5.562
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Lead-antimony sulfosalts from Tuscany (Italy):
 II - Crystal structure of scainiite, Pb14Sb30S54O5,
 an expanded monoclinic derivative of Ba12Bi24S48
 hexagonal sub-type (zinkenite group)

atoms_sites:
["Pb1", "Sb1", "Pb2", "Sb2", "Pb3", "Sb3", "Pb4", "Sb4", "Pb5", "Sb5", "Sb6", "Pb6", "Pb7", "Pb8", "Pb9", "Pb10", "Pb11", "Pb12", "Pb13", "Pb14", "Pb15", "Pb16", "Sb7", "Sb8", "Sb9", "Sb10", "Sb11", "Sb12", "Sb13", "Sb14", "Sb15", "Sb16", "Sb17", "Sb18", "Sb19", "Sb20", "O1", "O2", "O3", "O4", "S1", "S2", "S3", "S4", "S5", "S6", "S7", "S8", "S9", "S10", "S11", "S12", "S13", "S14", "S15", "S16", "S17", "S18", "S19", "S20", "S21", "S22", "S23", "S24", "S25", "S26", "S27", "S28", "S29", "S30", "S31", "S32", "S33", "S34", "S35", "S36", "S37", "S38", "S39", "S40", "S41"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

qdat:
AAAAUABAJAKAEtZImrQ4vIfGkG27mrX0plz2Rsqv89nVLPdV2rJv9f9en5cb+ClSd95pWTO6sSYKl/d179j2daZkQ0993VmdksWYzQh//28/N1PI8xhD/XXa5WbjaIhAH7/9U/TopGIQAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: Na Mn Fe2 P3 O12
compound: <missing>
formula_title: NaMnFe2(PO4)3
a: 12.018
b: 12.565
c: 6.415
alpha: 90
beta: 114.33
gamma: 90
cell_volume: 882.672
crystal_density: 3.571
atoms_sites: ["NaA2*", "NaA1", "MnM1", "FeM2", "P1", "P2", "O1", "O2", "O3", "O4", "O5", "O6"]
atoms_x: AAAAAICEHgAAAAAAmCQRAAAAAABwwg4A0KobAGAXBgAQExQAgHgHADC9DQDwFRMA
atoms_y: 0Fj//wAAAACIAxAAiNInADiO7v/gXfn/AKwrAFAGJwB4hygA4EgYAKgvMgCwpB4A
atoms_z: QEIPAAAAAABAQg8A6KEWAEBCDwBIAAgAQIsgANDGDgAQTgYAwDYTABBkEwCw9xYA
atoms_occupancy: wK8cAEBZIAAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: qLQCAPj1AgBApgAA6GwAAChVAADoYgAAAL4AAIDtAADY0QAAOAMBANDPAAAwAQEA
atoms_aniso_label: ["NaA2'", "NaA1", "MnM1", "FeM2", "P1", "P2", "O1", "O2", "O3", "O4", "O5", "O6"]
atoms_aniso_u11: QBkBAOCfAgAggAAA8FUAAFBGAADAXQAAMI4AAFCRAABA5wAAAJYAAIC7AACQ+wAA
atoms_aniso_u22: QJACAKBzAACQlwAAUF8AAJBMAADgRwAAEL0AABCkAACwmgAAcK0AAADIAABAgwAA
atoms_aniso_u33: gDICAJCqAQBQkQAA8FUAAFAtAADARAAA0GsAAJDiAACQZQAA8DYBAOB5AAAA4QAA
atoms_aniso_u12: AAAAAEAGAAAAAAAAkO3//wAAAACg9v//4Pz//zAqAAAQ3P//wBIAAGDw//+A2v//
atoms_aniso_u13: oA8AABCX/v+AVwAAOCwAAKAPAABgIgAAMCoAAJAzAABAOAAAEHIAANBSAABwYgAA
atoms_aniso_u23: AAAAAPDx//8AAAAAAOz//wAAAACg9v//ENz//wDO//8g6v//cP7//yAcAABgIgAA
pub_title:
 First experimental evidence of alluaudite-like phosphates with high
 Li-content: the (Na1-xLix)MnFe2(PO4)3 series (x= 0 to 1)
 Sample: NaMnFe2(PO4)3

qdat:
AAAAAAAAAAAACAAACAAQAAAAEoBAABAAAIIJAB0EEGCAACBhEgiQAUggIOZxAEJ8EgaEHqG2QEDGVAN1o0kcFflppiC+GCd3F5YxMcuk26tGrlkqWT17PTE7QqIDHX9lj1IJokb4ykVUlYwLIhKRETsH9dBFcUzwwEbOln==


formula: Li.5 Na.5 Mn Fe2 P3 O12
compound: <missing>
formula_title: Na.5Li.5MnFe2(PO4)3
a: 11.988
b: 12.500
c: 6.392
alpha: 90
beta: 114.67
gamma: 90
cell_volume: 870.416
crystal_density: 3.560
atoms_sites: ["LiA2*", "NaA2*", "NaA1", "MnM1", "FeM2", "P1", "P2", "O1", "O2", "O3", "O4", "O5", "O6"]
atoms_x: AAAAAAAAAACAhB4AAAAAALAbEQAAAAAAwMIOAFCeGwAwBgYAQAsUANBzBwBAsg0AwDYTAA==
atoms_y: YFr//2Ba//8AAAAAkB4QAIjXJwB4du7/KGb5/8C5KwDw6CYAsIsoAKBgGABQLTIAcKgeAA==
atoms_z: QEIPAEBCDwAAAAAAQEIPAKCAFgBAQg8AIB4IAMB+IAAgkA4A4DwGAIDlEgDAaBMAwAUXAA==
atoms_occupancy: gIQeAMAJDgDAehAAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: UI4DAFCOAwCgQQUASKgAAABfAAAYWwAA+FwAAAjAAABw6QAAsNsAAOAoAQDowQAAQPsAAA==
atoms_aniso_label: ["LiA2'", "NaA2'", "NaA1", "MnM1", "FeM2", "P1", "P2", "O1", "O2", "O3", "O4", "O5", "O6"]
atoms_aniso_u11: wNQBAMDUAQCg9wMAoIwAADBcAACAVwAAIGcAAOCrAACgjAAAoAkBAIC7AADgqwAAQBkBAA==
atoms_aniso_u22: YN4CAGDeAgDAXQAAcJQAAMBEAABAOAAAQDgAAOCrAABAnAAAoIwAAIC7AACAuwAAYG0AAA==
atoms_aniso_u33: wM4CAMDOAgBgWwMAMI4AALBPAADQOQAAwEQAAGBtAADA2gAAwF0AAMBXAQBgbQAAIMsAAA==
atoms_aniso_u12: AAAAAAAAAABAHwAAAAAAABD1//8AAAAAcP7//zD4//+gDwAAUOL//4AMAACA8///4OP//w==
atoms_aniso_u13: wOD//8Dg//+A0/z/UF8AAHAwAADAEgAAoCgAAEA4AADgLgAAQDgAAPCHAABQRgAAEFkAAA==
atoms_aniso_u23: AAAAAAAAAABg8P//AAAAAIDz//8AAAAAUPv//5Do//8Qw///8PH//2Dw//9wFwAAoA8AAA==
pub_title:
 First experimental evidence of alluaudite-like phosphates with high
 Li-content: the (Na1-xLix)MnFe2(PO4)3 series (x= 0 to 1)
 Sample: Na.5Li.5MnFe2(PO4)3

qdat:
AAAAAAAAAAAABAAACAAQAAAACUBAAAgAAEEEgA2CBBggABAURQJiAJQICDmcoBCbAoChAqhXSBgd1oC1aF1jgb1LOuQTYwJ3cjmjCzpWW3ysUnfK52PP6enI2zaoGGtdKn7QTJwbpRkmVJVwJ0SKimLkHtfgheKzooCVnS==


formula: Mg2.42 Al2.58 Si3 O14 H3.42
compound: <missing>
formula_title: <missing>
a: 8.5424
b: 5.7117
c: 9.6484
alpha: 90
beta: 108.298
gamma: 90
cell_volume: 446.958
crystal_density: 3.270
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of the high-pressure phase Mg4(MgAl)Al4[Si6O21/(OH)7]:
 an analogue of sursassite
 Sample: A53

atoms_sites:
["MgM1", "MgM2", "AlM3", "MgM3", "AlM4", "AlM5", "SiT1", "SiT2", "SiT3", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "H1", "H2", "H3", "H4"]

atoms_x:
wAILAFDgEACAhB4AgIQeAICEHgAAAAAAQK0SAECfDABAGwkA4FEPAKCVCwCASRMAYNcYAKDkGwCgbgUAQPoaAADiBACAowQAwGn+/0CJGACg2QgAoAgWACB4+f8ATB0A

atoms_y:
QEIPAEBCDwAAAAAAAAAAAAAAAAAAAAAAwMYtAMDGLQDAxi0AgAEfAEDcHwBAXx8AwMYtAMDGLQBAQg8AQEIPAMDGLQDAxi0AwMYtAEBCDwBAQg8AQEIPAMDGLQBAQg8A

atoms_z:
IEATAOAAKQCAhB4AgIQeAAAAAAAAAAAAwOMLALA8MQAgFx4AQGUeADBrCgCwTzIAUKsEACDjFQBwojgAACsWANDpNgDQzCYAUKkVAPALBABAEwIAYA0QAKCvDwDAIQoA

atoms_occupancy:
AAk9AAAJPQCAZiMAgKIZAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AgKIZAAAJPQAACT0A

atoms_u_iso:
IE4AAMBdAABAGQEAQBkBACBOAACAPgAAAK8AAACvAAAArwAAYFQAAGBUAABgVAAAYFQAAGBUAABgVAAAYFQAAGBUAABgVAAAYFQAAGBUAABAnAAAQJwAAECcAABAnAAA

qdat:
AAAAAAAAAAAEBAAAAAACACFAABAgAMAKAAJAKALEICBWRCAYQoRKIJlAcwGUhRmoFoAbWiYkqKV1hXX7nx8/RqLZ/f6Esq/1tvlX/2F539XHk3jtcuvVb+O+v/991p/OH3/6/xf///99fq/yz/+517r/4nb/196/o+6q+/==


formula: Fe1.581 Al7.419 Si6 B3 O31 H3.58
compound: <missing>
formula_title: <missing>
a: 15.964
b: 15.964
c: 7.119
alpha: 90
beta: 90
gamma: 120
cell_volume: 1571.206
crystal_density: 3.136
atoms_sites: ["FeY", "AlY", "AlZ", "SiT", "B", "O1", "O-H1", "O2", "O-h3", "O4", "O5", "O6", "O7", "O8", "H3"]
atoms_x: ID05ACA9OQAQEy0AgHYxAOC5BgAAAAAAAAAAADDHAwCQ7zQAcMEFADA+NwCgqzEAsJIrAMCBLAAgCjUA
atoms_y: 4MsDAODLAwDA2CoAsFUxACBPNgAAAAAAAAAAANBBOQBwGQgAkEc3ANDKBQAw/jAAoJ0rAFA5MADg/gcA
atoms_z: cK8hAHCvIQDQviAAIKc4ABBMFwBQ8yoAUPMqAMCoGQBQchoAkL88ACAvAQCg1SoAcEkAACBgFgCATxIA
atoms_occupancy: YCogAKDeHAAACT0AAAk9AAAJPQCAohkAgGYjAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A
atoms_u_iso: oIwAAKCMAADAXQAAAH0AAAB9AADgpQEA4KUBAAD6AAAgywAAgLsAAOCrAACgjAAAAH0AAKCMAADA1AEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural investigations on a synthetic alkali-free
 hydrogen-deficient Fe-tourmaline (foitite)
 Locvality: synthetic

qdat:
AAAAAAAAAAAAAQAAEAAAAQCABAQAAAIgASCCQAAISASASEgIoCANEACgUSAYTg4KDC4OXIgQIligwwu1eVKFNOjEOIeTw47pTCluQJDad6do1a0NfBeLUBa8VO5yIj4bc5ESaiZkJRZIiBGCJECJEmxRko0SJBmSCyRAgs==


formula: K.964 Al1.368 Mg.73 Fe.038 Si3.808 O11.2 F.8 H1.2
compound: <missing>
formula_title: <missing>
a: 5.2046
b: 9.0368
c: 19.886
alpha: 90
beta: 95.615
gamma: 90
cell_volume: 930.809
crystal_density: 2.833
atoms_x: AAAAAHAIDwBwCA8AcAgPADAxHAAwMRwAwJwbAMCcGwAQFRwAUMANAADFDQAgphsAAIMYADDNGwAwzRsA4BsYAA==
atoms_y: gLYFAMD5BADA+QQAwPkEAKCkOACgpDgACMAPAAjADwCwrgUAUPUyAGA6FQDQDzkAkFYPAFCNIgBQjSIAQLImAA==
atoms_z: QEIPAEABAABAAQAAQAEAAFhACABYQAgA0EAIANBACABgTwoAyOwJAGBUCgD4WQMA0FQDACBVAwAgVQMAQIoDAA==
atoms_occupancy: gNY6AIDjIwAgRxYA4CgBAAAbOgAA7gIAABs6AADuAgAACT0AAAk9AAAJPQAACT0AAAk9AACfJAAAahgAAJ8kAA==
atoms_u_iso: oOoBAADhAAAA4QAAAOEAAPDSAADw0gAAwNoAAMDaAAAwJAEAsBcBAJAtAQBgHAEAABMBANCXAQDQlwEAYGcBAA==
atoms_aniso_u11: cNkBAPAEAQDwBAEA8AQBAPDrAADw6wAAkOIAAJDiAAAwbwEAkMkAAJBGAQDwHQEAgB8BACApAgAgKQIA
atoms_aniso_u22: cKcBAEC1AABAtQAAQLUAAFCRAABQkQAAEL0AABC9AADAwQAAYDUBAIA4AQBgNQEAoCIBAFBAAQBQQAEA
atoms_aniso_u33: IEICACDkAAAg5AAAIOQAAAD6AAAA+gAAEO8AABDvAAAQOgEAsEkBAPAEAQBgAwEAgO0AAEBkAQBAZAEA
atoms_aniso_u12: AAAAACADAAAgAwAAIAMAAFD7//9Q+///UPv//1D7//8w+P//oMT//+BHAADA4P//UPv//7BoAACwaAAA
atoms_aniso_u13: MCoAAEAGAABABgAAQAYAABAOAAAQDgAAEA4AABAOAACQGgAA0CAAAPAKAACwHQAAkOj//zBDAAAwQwAA
atoms_aniso_u23: AAAAANAHAADQBwAA0AcAACADAAAgAwAAIAMAACADAAAQDgAAwPn//9Du//8gAwAAQB8AALDr//+w6///
pub_title:
 Crystal structures and compressibilities of synthetic 2M_1 and 3T phengite micas
 Sample: synthetic 2M_1

atoms_sites:
["K", "AlM2", "MgM2", "FeM2", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O-h6", "F6", "H"]

atoms_aniso_label:
["K", "AlM2", "MgM2", "FeM2", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O-h6", "F6"]

qdat:
AAAAAAAAAAEAAAAAAAAAAQAZIEIAQIAJBAAQCAAIVgZCgIKMKwkgFpBEwBCLANnTEUMUkOsqilKiFARQZPOD1fGpqCUSLZj1Gakpl9s8WG336lp3kUoVsrF0yqHsZ44OpvXR6kZRGkIpYasauWqy0eNErX6TREojECIa6a==


formula: K Al.998 Mg.5 Fe.026 Si3.808 O11.2 F.8 H1.2
compound: <missing>
formula_title: <missing>
a: 5.2110
b: 5.2110
c: 29.689
alpha: 90
beta: 90
gamma: 120
cell_volume: 698.181
crystal_density: 2.727
atoms_aniso_u11: gLUBAKC+AACgvgAAoL4AAGDqAABg6gAAYOoAAGAcAQBgHAEA4BUAAOAVAAAAfQAAQBkBAAD6AABg6gAAQJACAAD0AQAA9AEA
atoms_aniso_u22: wFECAKC+AACgvgAAoL4AALDMAACwzAAAsMwAADBWAQAwVgEA4BUAAOAVAAAAfQAA4KsAAIC1AQBg6gAAwNQBACDFAQAgxQEA
atoms_aniso_u33: UIUCAADIAAAAyAAAAMgAAKCGAQCghgEAoIYBANBrAADQawAAIMUBACDFAQDAVwEAQBkBAECWAQAgSAEAIEgBAGBnAQBgZwEA
atoms_aniso_u12: cCoBAFBfAABQXwAAUF8AADB1AAAwdQAAMHUAAKClAACgpQAA0O7//9Du//+Awf//YPD//wD6AAAgVP//APQBAMBXAQDAVwEA
atoms_aniso_u13: 4OP//wAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEDt//9A7f//0O7//9Du//+gDwAAAAAAAMDg//+gDwAAwOD//8Dg///A4P//
atoms_aniso_u23: AAAAAKD2//+g9v//oPb//6APAACgDwAAoA8AANAHAADQBwAA8PH///Dx//+gDwAAIE4AACDR//+gDwAAYPD//yDR//8g0f//
pub_title:
 Crystal structures and compressibilities of synthetic 2M_1 and 3T phengite micas
 Sample: synthetic 3T

atoms_sites:
["K", "AlM2", "MgM2", "FeM2", "AlM3", "MgM3", "FeM3", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O-h6", "F6", "H"]

atoms_x:
8I8HABDy8/8Q8vP/EPLz/2DFGwBgxRsAYMUbAMA3MADANzAAoMUcAKDFHADAKi4AUFoeADAhJwAQxQcAAJklACAeCAAgHggAgKMEAA==

atoms_y:
UB4PAAj5+f8I+fn/CPn5/7DiDQCw4g0AsOINAPB9IwDwfSMA0Ec4ANBHOAAgxyIAsI84AAAxLgBg3CwAgGEPAMAVDADAFQwAABcRAA==

atoms_z:
OCwKAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAPCCBQDwggUAQH4FAEB+BQAQNAIAcD0CABDkBgBAqgYAQNwGADA3AgAwNwIAYGECAA==

atoms_occupancy:
AAk9AOCYGABAQg8AIMsAAOCYGABAQg8AIMsAAAAbOgAA7gIAABs6AADuAgAACT0AAAk9AAAJPQAACT0AAAk9AACfJAAAahgAAJ8kAA==

atoms_u_iso:
MB4CAMDBAADAwQAAwMEAAHARAQBwEQEAcBEBAHD4AABw+AAAsLMAALCzAAAA+gAA4CgBACBIAQCgCQEAoIYBAAB3AQAAdwEAwNQBAA==

atoms_aniso_label:
["K", "AlM2", "MgM2", "FeM2", "AlM3", "MgM3", "FeM3", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O-h6", "F6"]

qdat:
AAAAAAAAAAEAAAAAAAAAAQAUIEAQAQAKABAAEAAIZESBAIEyESAwEEIAQAIAANIhAgQEASlhBBAQEAgAOiIS5UIRIEBABVEQggQIAaSIQgtZIQgggAAA1IiIPtJ1iKhCAaokQggAAAAcpdzTCskiIQAAdSREQAAABqfptE==


formula: Cu3 As2 O12 H8
compound: <missing>
pub_title: Rollandite, Cu3(AsO4)2.4H2O, a new mineral: its description and crystal structure
formula_title: <missing>
a: 5.6906
b: 17.061
c: 9.732
alpha: 90
beta: 90
gamma: 90
cell_volume: 944.854
crystal_density: 3.800
atoms_sites: ["Cu1", "Cu2", "As", "O1", "O2", "O3", "Wat4", "O5", "Wat6", "Wat7"]
atoms_x: gAYaAGBnAQCQRRYA4CgBAAB3AQCAFAcA4MgQAAAXEQDADw0AAPkVAA==
atoms_y: +FsfAEBCDwD4TAYA8O0IAHAkAgCwugMAoGMkAJCmCgBAQg8AQEIPAA==
atoms_z: YGwVAGCDDQA4IQYAcO0fAEB1EwBQOgIAIJAOAGAfDQBgOzIAcJUdAA==
atoms_occupancy: 0
atoms_u_iso: sJoAAIBwAABQXwAAIMsAAKCMAABAnAAA4KsAAAB9AACghgEA4KsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAAAAAAAAAIAAAAAAAAMQAHAAAYgBAHBAABeJQIVGgdEFR48MEtWRA/zwVEKoE++OfVrx+oTf7G/tbO6e/m9z5/9K9n/fdd3/aPfftf+1P+f6337/3fLP+t/Ll9s/q/3e3L/7r4/ue/X+7fof777/X/vf+7/mVl7Xj09==


formula: (Si7.123 Al1.877) O22.52 Na.106 K.03 Mg.047 Ca.162 Ba.002 N1.315 H9.04
compound: <missing>
formula_title: <missing>
a: 13.601
b: 18.232
c: 17.810
alpha: 90
beta: 90
gamma: 90
cell_volume: 4416.406
crystal_density: 1.956
atoms_aniso_u11: 4KUBAOClAQCAtQEAgLUBAAB3AQAAdwEAgDgBAIA4AQDAzgIAoIACAADoAwAA9AEAoAMCAGDeAgBgZwEAQIoDAA==
atoms_aniso_u22: gDICAIAyAgDgIgIA4CICACBCAgAgQgIAoHoDAKB6AwBg2AMAYNgDAOCZAwBAigMA4J8CACBCAgAAawMAoP0CAA==
atoms_aniso_u33: AHECAABxAgAAcQIAAHECAIAyAgCAMgIAIMUBACDFAQBgWwMAQIoDAMBFBAAguQMA4JMEAOCTBADASwMAQO8HAA==
atoms_aniso_u12: AAAAAAAAAAAg0f//INH//8BdAADAXQAAAAAAAAAAAAAgVP//YHP//2Bz//8AAAAA4LH//wAAAAAAAAAAAAAAAA==
atoms_aniso_u13: wOD//8Dg//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACgFf//AIP//wB3AQAAAAAAAAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: wOD//8Dg//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACgCQEAIEgBAIDH/v8g0f//AAAAAAAAAAAAAAAAAAAAAA==
pub_title:
 Single crystal neutron diffraction study of the natural zeolite barrerite
 in its ND4-exchanged form

atoms_sites:
["SiT1", "AlT1", "SiT3", "AlT3", "SiT4", "AlT4", "SiT5", "AlT5", "O1", "O3", "O4", "O7", "O8", "O9", "O10", "Wat1", "Wat2", "Wat3", "Wat4", "Wat6", "Wat8", "Wat11", "NaC1", "KC1", "MgC1", "CaC1", "BaC1", "NH4C2", "ND42", "ND43", "ND44"]

atoms_x:
AIkXAACJFwAgXxIAIF8SAKCxFwCgsRcAQEIPAEBCDwCAYhMAgLQWADC/FQCAhB4AkD4TANDgEgCAhB4AICMcAICEHgBA7hwAILgYACC+FwCAhB4AwEoYAICEHgCAhB4AgIQeAICEHgCAhB4A4MIRAICEHgCgkRQAQKEUAA==

atoms_y:
0McSANDHEgAwERkAMBEZAAA7CwAAOwsAQEIPAEBCDwAgkRIA4CUOAPAvFwCgTBMAIPIGAICEHgAgMQkAQHIHAEDvBwAAAAAAAAAAAAAAAACAhB4AwLwFAAAAAAAAAAAAAAAAAAAAAAAAAAAAQIoDAEB+BQCAtQEAgCYEAA==

atoms_z:
kPQWAJD0FgCAhB4AgIQeAICEHgCAhB4AQEIPAEBCDwDQYxIAAPoZAPDrGQCQSxUAgIQeAICEHgCAhB4AQK0SAOC8EgBgThoAQI8XAGB4EwCAtBYAgEkTAODCEQDgwhEA4MIRAODCEQDgwhEAgNIRAKCpEABASA4A4DMUAA==

atoms_occupancy:
ME8wANC5DAAwTzAA0LkMADBPMADQuQwAME8wANC5DAAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AQNEMAEBCDwCAwBQAgN4PAMCYCwAACT0AwCcJACh8BgDA1AEAMOYCABDrCQAQJwAAuIgAAABTBwDAtgYAwCcJAA==

atoms_u_iso:
ABJ6AAASegAAEnoAABJ6AAASegAAEnoAABJ6AAASegAAEnoAABJ6AAASegAAEnoAABJ6AAASegAAEnoAwMgDAIAyAgCAiwgAwLYGAMBFBAAAEnoAAOIEAMDUAQDA1AEAwNQBAMDUAQDA1AEAQO8HAMCYCwAAUwcAQH4FAA==

atoms_aniso_label:
["SiT1", "AlT1", "SiT3", "AlT3", "SiT4", "AlT4", "SiT5", "AlT5", "O1", "O3", "O4", "O7", "O8", "O9", "O10", "Wat8"]

qdat:
AAAAAAAAAAANAAAIEAAZQAEkEBQCQKpgBhFoMZOMVbeAFqz2dvJbaxFY/u797L23mz9vwd9nCObvV/LAPa8Kf8iNRC0tCQIBvEBEAYLAAAAwAAAACAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Mg.93 Mn.07) Al2 S4 O38 H44
compound: <missing>
formula_title: <missing>
a: 6.1844
b: 24.2715
c: 21.2265
alpha: 90
beta: 100.326
gamma: 90
cell_volume: 3134.592
crystal_density: 1.824
atoms_u_iso: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal structure of the hydrated sulphate pickeringite (MgAl2(SO4)4.22H2O):
 X-ray powder diffraction study

atoms_sites:
["Mg", "Mn", "Al1", "Al2", "S1", "S2", "S3", "S4", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5", "Wat6", "Wat7", "Wat8", "Wat9", "Wat10", "Wat11", "Wat12", "Wat13", "Wat14", "Wat15", "Wat16", "Wat17", "Wat18", "Wat19", "Wat20", "Wat21", "Wat22"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

qdat:
AAAAAACACAggARACIagJmFRRI1MHyk+dj3vN7/2fb73+rf/z5X5/v1+/1/nt9f3/b3/t/6v//d0/Yt/8p177nP29/vd7+vqve6vvhfyefvt/P377Htm/T7mY1fb/e7tOvas/lTVpqzv/dtz3s56beWbSu51/5vvXLb1ss9==


formula: Si4 B Al2 Mg.96 Mn.035 V.015 Cr.005 Ca1.975 O16 H.95
compound: <missing>
formula_title: <missing>
a: 7.1381
b: 9.1626
c: 8.9421
alpha: 91.903
beta: 98.105
gamma: 77.468
cell_volume: 565.206
crystal_density: 3.170
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Structural study of magnesioaxinite and its crystal-chemical relations
 with axinite-group minerals

atoms_sites:
["Si1", "Si2", "Si3", "Si4", "B", "Al1", "Al2", "Mg", "Mn", "V", "Cr", "Ca1", "Ca2", "Mn2", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "O16", "H"]

atoms_x:
UN8MAHBVDQBYtCoAADMnALA9HAAYPwMAwHAVACDALgAgwC4AIMAuACDALgDAgC0AiCELAIghCwDAGQMAYEsOAOCSGQAwdwgAcEMBAFC1EwAQTBcA0IwgANCLNQBg6S4AMC0lADCIGgBAESwAEGUwAPDdEwDg2AUAIF08AA==

atoms_y:
IHQbAAi6EACAwA8AaBQBADC9JgCQyzAACCg5ADhYJAA4WCQAOFgkADhYJACoMxUAQEYGAEBGBgCAxCQAQOwUALC0HQCgbBYAIMIOAKA0FwBAvQcA4OIUADCKCQBwvxYAwC0IAJD3OwCgBAYA8BE1ACCFLQCwwjwAoKc6AA==

atoms_z:
sBkOAGDaHwBQrwAA8BUOADBzEQDgkg8AMKwZAIg5BwCIOQcAiDkHAIg5BwBA/RcASBwFAEgcBQBAvgsAUHMFADADEwDwThYAIEoiAOBwJwCAUh4AcII1AADvOAAwRQgAgGsFAODUDgDwehcAMOgKAOCqFQCQohMA4MclAA==

atoms_occupancy:
AAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AACYOgCAOAEAYOoAACBOAAAACT0AYII7AGDqAAAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AwPs5AA==

atoms_u_iso:
gD4AAJAzAAAQQAAA0DkAAJBMAADQOQAAgD4AAPBuAADwbgAA8G4AAPBuAACgcwAAIIAAACCAAABAUQAA0GsAANBSAAAwjgAAsE8AACBOAABwSQAAIE4AACBOAADwbgAA0IQAAJBMAAAASwAAUF8AABBAAABwSQAAYG0AAA==

qdat:
AAAAAAAAAAADAAAQCgAAEAgGAgMAEBZAAJwVAtAAFwMFkUlKtGgWdIwoARF/aHx/BBzGXI+7oZ7vHorsz9lq3afWmu5r3ue++9a9/9/+9u/z+3ft0r//fv////vv+///f////+//////1/9v/2/5/f/+z/+v3f/b//9b3z==


formula: (Ca.84 Sr.45 Na.71) Mg.19 Fe.29 Mn.03 Zn.02 Al.47 Ti.01 Si1.99 O7
compound: nephelinite lava of Mt. Etinde, Cameroon
formula_title: <missing>
a: 7.754
b: 7.754
c: 5.101
alpha: 90
beta: 90
gamma: 90
cell_volume: 306.695
crystal_density: 3.186
atoms_x: 4JcUAOCXFADglxQAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAI4IAACOCACAhB4AsLAIAGgGBQA=
atoms_y: oOwJAKDsCQCg7AkAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgPYVAID2FQAAAAAA0NMVALAICwA=
atoms_z: oBgfAKAYHwCgGB8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEAs6ABALOgAwBwoASLwPAKCNMQA=
atoms_occupancy: gKIZAKC7DQDgqhUAwJgLAECzEQDA1AEAgDgBAIATHABAnAAA4Lo8ACBOAAAACT0AAAk9AAAJPQA=
atoms_u_iso: wHABAMBwAQDAcAEAsDABALAwAQCwMAEAsDABALAwAQCwMAEAACwBAAAsAQDgCQIA4CICANAUAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of strontian soda melilite from nephelinite
 lava of Mt. Etinde, Cameroon
 Sample: ET1

atoms_sites:
["CaX", "SrX", "NaX", "MgT1", "FeT1", "MnT1", "ZnT1", "AlT1", "TiT1", "SiT2", "AlT2", "O1", "O2", "O3"]

qdat:
AAAAAAAAAAAAAAAAAAAQEAAAAAAggAQAAAgAEAQAAgCIAIAICQAgBAgCQJAYJCADEAANDQEBGgAiIAFwQpQmaIOFBAHJNABOAKYU0BjAlOc0hGjYQTEc5UmpBCdSuhxKwppWEjW/LxIxU3cSAsTcmbF27F2pdk3KIsTz3t==


formula: (Ca.83 Sr.45 Na.72) Mg.2 Fe.29 Mn.03 Zn.01 Al.46 Ti.02 Si1.99 O7
compound: nephelinite lava of Mt. Etinde, Cameroon
formula_title: <missing>
a: 7.764
b: 7.764
c: 5.095
alpha: 90
beta: 90
gamma: 90
cell_volume: 307.125
crystal_density: 3.178
atoms_x: eJYUAHiWFAB4lhQAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEI0IABCNCACAhB4AqK4IANACBQA=
atoms_y: CO4JAAjuCQAI7gkAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAcPcVAHD3FQAAAAAA2NUVAOgCCwA=
atoms_z: wBYfAMAWHwDAFh8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAiAs6AIgLOgDgBgoAaLoPAIiMMQA=
atoms_occupancy: YFQZAKC7DQAA+RUAADUMAECzEQDA1AEAQJwAAEB3GwCAOAEA4Lo8ACBOAAAACT0AAAk9AAAJPQA=
atoms_u_iso: 8GgBAPBoAQDwaAEAYDUBAGA1AQBgNQEAYDUBAGA1AQBgNQEAUCcBAFAnAQCAAAIAgAACACAQAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of strontian soda melilite from nephelinite
 lave of Mt. Etinde, Cameroon
 Sample: ET2

atoms_sites:
["CaX", "SrX", "NaX", "MgT1", "FeT1", "MnT1", "ZnT1", "AlT1", "TiT1", "SiT2", "AlT2", "O1", "O2", "O3"]

qdat:
AAAAAAAAAAAAAAAAAAAgEAAAAAAggAQAAAgAEAQAAQCIAIAICQAgBAgCQSAYJCACEAANCQEBGgAkIAGgQpwkcIOFDAHJLACeAKYI4BjBFKcZCHCYQXEc5jEZCC5bJhw8hWnsFGbet0Jid+4bB5+8ZylFyjtxxrvWMYbnkX==


formula: (Pb.83 Sr.17) Mn2 V2 (O10 H2)
compound: <missing>
formula_title: <missing>
a: 9.2953
b: 6.2894
c: 7.6906
alpha: 90
beta: 118.068
gamma: 90
cell_volume: 396.728
crystal_density: 4.693
atoms_sites: ["Pb", "Sr", "Mn", "V", "O-H1", "O2", "O3", "O4"]
atoms_x: AAAAAAAAAABAQg8AUDs4ANCJFADgORMAAKMCAOBdDQA=
atoms_y: AAAAAAAAAABAQg8AgIQeAICEHgAAAAAAkLQQAICEHgA=
atoms_z: AAAAAAAAAACAhB4AUFwNAICiGQBgbBUA0CQQAIC7AAA=
atoms_occupancy: wKgyAEBgCgAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: UFkBAFBZAQDAwQAAMKcAAAD6AACAOAEAoAkBAOClAQA=
atoms_aniso_label: ["Pb", "Sr", "Mn", "V", "O-H1", "O2", "O3", "O4"]
atoms_aniso_u11: 8GgBAPBoAQCgvgAA0J0AAECcAADAVwEAAPoAAKCGAQA=
atoms_aniso_u22: kBQBAJAUAQCQsAAAYJ8AAMDaAACAOAEAYOoAAOClAQA=
atoms_aniso_u33: MIgBADCIAQCg1wAAIMsAAIA4AQBgZwEAQBkBAMBXAQA=
atoms_aniso_u12: AAAAAAAAAAAw+P//AAAAAAAAAAAAAAAAoA8AAAAAAAA=
atoms_aniso_u13: UKoAAFCqAADgYAAAwF0AACBOAAAgywAAAH0AACBOAAA=
atoms_aniso_u23: AAAAAAAAAADQ7v//AAAAAAAAAAAAAAAAwOD//wAAAAA=
pub_title:
 Description, crystal structure, and paragenesis of krettnichite,
 PbMn2(VO4)2(OH)2, the Mn3+ analogue of mounanaite

qdat:
AAAAAAAAAAAAAAAEAAAAAgAAAEAAAIBAAIAECAAAABgAAIIAGAIkAAAEggBBAiEwAAiAMgToAYMECyEAAwIEzkCAwFBKkAARJLIhjV4QFAl0iieiykgTlNXjQAzEor1DNcV9jYSLyZA2QrnXhZfyFQp1iT/wxZnZgbTLbZ==


formula: (Nb.52 Ta.48) B O4
compound: <missing>
pub_title: Schiavinatoite, (Nb,Ta)BO4, the Nb analogue of behierite
formula_title: <missing>
a: 6.219
b: 6.219
c: 5.487
alpha: 90
beta: 90
gamma: 90
cell_volume: 212.215
crystal_density: 6.572
atoms_sites: ["NbM", "TaM", "B", "O"]
atoms_x: AAAAAAAAAAAAAAAAAAAAAA==
atoms_y: AAAAAAAAAAAAAAAAAPAKAA==
atoms_z: AAAAAAAAAACAhB4A8MQTAA==
atoms_occupancy: AL0fAABMHQAACT0AAAk9AA==
atoms_u_iso: yDIAAMgyAAAIVwAAKEsAAA==
atoms_aniso_label: ["NbM", "TaM", "B", "O"]
atoms_aniso_u11: QDMAAEAzAADAXQAAMHUAAA==
atoms_aniso_u22: QDMAAEAzAADAXQAAoCgAAA==
atoms_aniso_u33: UDIAAFAyAADAXQAAEEAAAA==
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAA==
atoms_aniso_u23: AAAAAAAAAAAAAAAAQAYAAA==
qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAEAAAAAAACAAAAAAAAQAAgACAAAAAAgAAAACAAACAEAIEAAAgAAIIAAAAgAEAAIAAAgACAgQBAAAAhCAQIEQgEAAAQEAAogIAEgAQgKIAAAiBBDoAQBAgABUgQCJACHCCABIIQkBgEkAQV==


formula: Ni Bi As O5
compound: Johanngeorgenstadt, Saxony, Germany
formula_title: <missing>
a: 6.7127
b: 6.8293
c: 5.2345
alpha: 107.625
beta: 95.409
gamma: 111.158
cell_volume: 207.616
crystal_density: 6.760
atoms_sites: ["Ni", "Bi", "As", "O1", "O2", "O3", "O4", "O5"]
atoms_x: IC4WAMBoDgCAYAsAIJQeAIDqDQDgVw4AIO/6/+AtFQA=
atoms_y: kNQsAOAWOwCwphcAQA0DAIBUJgBg0RkAQFQMAODIEAA=
atoms_z: sLMyAKj9GACgoQkAQP8uAABkGQAAvDQAgCAFAIBbEAA=
atoms_occupancy: 0
atoms_u_iso: 0M8AAHDGAADAqAAAYLgAAPC5AADwBAEAkOIAALD+AAA=
atoms_aniso_label: ["Ni", "Bi", "As", "O1", "O2", "O3", "O4", "O5"]
atoms_aniso_u11: sJoAAFB4AACAcAAAYG0AAKC+AAAAEwEAcK0AAPCHAAA=
atoms_aniso_u22: oAkBAPAdAQAA4QAAUHIBANDoAABA5wAAYAMBAMA+AQA=
atoms_aniso_u33: kMkAAGDRAADAqAAAYG0AAADIAAAgLwEAAPoAAFByAQA=
atoms_aniso_u12: EFkAALBoAACwTwAAcJQAAPCHAACQlwAA8FUAAAB9AAA=
atoms_aniso_u13: 8CMAAEA4AABwFwAAgCUAAABLAAAgNQAAUEYAAABLAAA=
atoms_aniso_u23: kEwAAPBVAABgOwAAcEkAAJBlAACwTwAAUF8AAPCgAAA=
pub_title:
 Paganoite, NiBiAsO5, a new mineral from Johanngeorgenstadt,
 Saxony, Germany: description and crystal structure

qdat:
AAAAAAAAAAAAAAAAASAAAEAAAAAAAQEAEAIIAAAAAAgQGQAEAAgEQgAIBAEAoggAjAAACQGIB0oACCAVAgAQ8AoBQcIGAQkQFMYhIMG4KlEhAgTeCiqEJgh2cIgGgrRgkdiGTDJpqUPCXYeQtG5AjXtEvYT+GQ/hMtdsZM==


formula: Bi2.94 Te1.01 Se1.73 S.32
compound: <missing>
pub_title: Telluronevskite, Bi3TeSe2, a new mineral
formula_title: <missing>
a: 4.264
b: 4.264
c: 23.25
alpha: 90
beta: 90
gamma: 120
cell_volume: 366.090
crystal_density: 8.075
atoms_sites: ["Bi1", "Te1", "Bi2", "Te2", "Bi3", "Te3", "Te1", "Se1", "Se1", "S1", "Se2", "S2"]
atoms_x: AAAAAAAAAABVWBQAVVgUAKuwKACrsCgAVVgUAFVYFACrsCgAq7AoAAAAAAAAAAAA
atoms_y: AAAAAAAAAACrsCgAq7AoAFVYFABVWBQAq7AoAKuwKABVWBQAVVgUAAAAAAAAAAAA
atoms_z: kLgHAJC4BwDg9BEA4PQRAFACHABQAhwAYHQDAGB0AwBQKg0AUCoNAGB/FgBgfxYA
atoms_occupancy: gNA7AIA4AQCA0DsAgDgBAIDQOwCAOAEAwPs5AEANAwAARTMAAMQJAABFMwAAxAkA
atoms_u_iso: 4GoAAOBqAADgagAA4GoAAOBqAADgagAAIBEBACARAQAgEQEAIBEBACARAQAgEQEA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
qdat:
AAAAEAAAAgAAAEAAAAgAAAEAAAAgKBAMACAAwAAQEAIAAhAAAcggIQgAjEIEBgBCBACQACAAIAAyQQIBAIAQAcQkgIBAIAIAIAaRBBKRCCQgoAgCANJCCCAgEAgCoiEEBAqVCCBAgEAAABkiIIIPFR6SFIoECA1EQgggQA==


formula: Mg7 P2 O16 H8
compound: Modum, Norway
pub_title: Raadeite, Mg7(PO4)2(OH)8: a new dense-packed phosphate from Modum (Norway)
formula_title: <missing>
a: 5.250
b: 11.647
c: 9.655
alpha: 90
beta: 95.94
gamma: 90
cell_volume: 587.202
crystal_density: 2.806
atoms_x: AAAAAAAEEABwOg8A8PsOACDFAQBgFhsAIKADAJB/BADABzgAEIwEAHDnIADwzDMAwCMSAAB9AACA/AoA4PEeAOBEJgA=
atoms_y: AAAAABDMCgAARRoAsM8MAKBpIwAQURIAENIiAGCZMwCgoyoAcOYDALANCwCAox0AIMciAOClAQAAOTUAgMYTAKAyDwA=
atoms_z: AAAAAFDfDAAQszwAcEQeAOBYKwBgrQYAYFs1AOCNNwBgDSkAALsXALDeFgCweCcAMGYoACBZEwAAPzQAYCsLAIAxFwA=
atoms_occupancy: 0
atoms_u_iso: AGQAACCAAADQawAAcHsAAIBXAACAiQAAwHYAAECDAACAiQAAgIkAAMB2AACQfgAAYJ8AAMDUAQCAOAEAAHECAABxAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["Mg1", "Mg2", "Mg3", "Mg4", "P", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "H1", "H2", "H3", "H4"]

qdat:
AAAAAAAAAAAAAAQAAAgAghgCAEAgIRAQICiAgKAAQQoSkAIWORnIAhirGUQibE7RBdiZGI/tiWC5vBNs7qdf7LK/G1dO0vL6Hecn/pvfn+8X6/V/tb98qHuvvu49P/E6dX61fpTPm9pv7v33dsK6Hb9fK/x3rnkTO/zZ/d==


formula: O11.995 Cl.005 Si3.11 Al2.748 Ti.003 Fe.039 Cr.062 Mg.081 Ba.044 Na.103 K.857 H1.829
compound: Westland
pub_title: Chromium-containing muscovite: crystal chemistry and XANES spectroscopy
formula_title: <missing>
a: 5.192
b: 9.011
c: 20.028
alpha: 90
beta: 95.74
gamma: 90
cell_volume: 932.314
crystal_density: 2.884
atoms_sites:
["O11", "O21", "O22", "O31", "O32", "O4", "O-H4", "Cl4", "SiT1", "AlT1", "SiT2", "AlT2", "AlM1", "TiM1", "FeM1", "CrM1", "MgM1", "AlM2", "TiM2", "FeM2", "CrM2", "MgM2", "BaA", "NaA", "KA"]

atoms_x:
YNYtAIBIDwDQaxkAUIQXAMCqOgBwZDoAcGQ6AHBkOgBQjxsAUI8bAJDkOgCQ5DoAwMYtAMDGLQDAxi0AwMYtAMDGLQBQQQ8AUEEPAFBBDwBQQQ8AUEEPAAAAAAAAAAAAAAAAAA==

atoms_y:
IPUSADCgFgCwrgUAYF4PAEATGwAg0gMAINIDACDSAwAAyA8AAMgPABA6GgAQOhoAQEIPAEBCDwBAQg8AQEIPAEBCDwDQFgUA0BYFANAWBQDQFgUA0BYFADgIBgA4CAYAOAgGAA==

atoms_z:
WKgJABhWCgAwTQoA4EQDAPhFAwBgFQMAYBUDAGAVAwAISggACEoIAGhJCABoSQgAAAAAAAAAAAAAAAAAAAAAAAAAAADIAAAAyAAAAMgAAADIAAAAyAAAAEBCDwBAQg8AQEIPAA==

atoms_occupancy:
AAk9AAAJPQAACT0AAAk9AAAJPQDgEAUAENE3ABAnAABwdC8AkJQNAHB0LwCQlA0AoLM4AHAXAACwMAEAYOQBANB4AgDQWRwA8AoAACCZAAAw8gAAoDsBAICvAgBgSQYAoE40AA==

atoms_u_iso:
cOkAANDPAADIzQAAqIQAAKCCAABwlAAAcJQAAHCUAAD4XAAA+FwAABhbAAAYWwAA6GIAAOhiAADoYgAA6GIAAOhiAADwZAAA8GQAAPBkAADwZAAA8GQAALAwAQCwMAEAsDABAA==

atoms_aniso_label:
["O11", "O21", "O22", "O31", "O32", "O4", "O-H4", "Cl4", "SiT1", "AlT1", "SiT2", "AlT2", "AlM2", "TiM2", "FeM2", "CrM2", "MgM2", "BaA", "NaA", "KA"]

atoms_aniso_u11:
aMQAACi+AAAgGwEAAJYAAEh2AACwfAAAsHwAALB8AABQUAAAUFAAAIhUAACIVAAAkFYAAJBWAACQVgAAkFYAAJBWAAAQPwEAED8BABA/AQA=

atoms_aniso_u22:
aBQBANDtAADQkwAA0GYAAGiNAAA4mgAAOJoAADiaAACYUwAAmFMAADBNAAAwTQAAAFoAAABaAAAAWgAAAFoAAABaAAAAOwEAADsBAAA7AQA=

atoms_aniso_u33:
ANwAAJi8AACYvAAAMJ0AAMh9AAAwnQAAMJ0AADCdAADIfQAAyH0AAMh9AADIfQAAyH0AAMh9AADIfQAAyH0AAMh9AAD4GgEA+BoBAPgaAQA=

atoms_aniso_u12:
WMH//0BCAABYBwAAwAMAABgLAACo+P//qPj//6j4///AAwAAwAMAAAAAAAAAAAAAQPz//0D8//9A/P//QPz//0D8//8AAAAAAAAAAAAAAAA=

atoms_aniso_u13:
wO///wAAAADIKAAAAAAAAEAQAACoIAAAqCAAAKggAAAAAAAAAAAAACAIAAAgCAAAIAgAACAIAAAgCAAAIAgAACAIAABgGAAAYBgAAGAYAAA=

atoms_aniso_u23:
4DgAAJDj//84DgAAAAAAADgOAABY1f//WNX//1jV//8AAAAAAAAAADgOAAA4DgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA=

qdat:
AAAAAAAAAAEAAAAAAAAAAgAZIEEAQIAMBAAQCAAQNgxEgQHGhRCgHJEEwECKAPzTiOMLCO1VTZEiFgRIS1xjbnjJVBJQp068SLUIjVqONjV16xUbxKUK/ZSaU7jfGsOHyb38SpS4hRESVGunJm7MlDVRmbejSEyIogxFlT==


formula: O11.969 F.031 Si3.069 Al2.774 Ti.019 Fe.021 Cr.099 Mg.02 Ca.004 Na.268 K.725 H1.92
compound: Northwest Nelson - Campbell Creek
pub_title: Chromium-containing muscovite: crystal chemistry and XANES spectroscopy
formula_title: <missing>
a: 5.175
b: 8.979
c: 19.915
alpha: 90
beta: 95.66
gamma: 90
cell_volume: 920.865
crystal_density: 2.867
atoms_sites:
["O11", "O21", "O22", "O31", "O32", "O4", "O-H4", "F4", "SiT1", "AlT1", "SiT2", "AlT2", "AlM2", "TiM2", "FeM2", "CrM2", "MgM2", "CaA", "NaA", "KA"]

atoms_x:
QOwtAGBeDwDAEhkAIHMXAEC3OgCwajoAsGo6ALBqOgDAgxsAwIMbAFDeOgBQ3joAID8PACA/DwAgPw8AID8PACA/DwAAAAAAAAAAAAAAAAA=

atoms_y:
0McSAHC/FgAAqgUAYF4PAKAcGwDgywMA4MsDAODLAwBYxQ8AWMUPAKA2GgCgNhoAMBYFADAWBQAwFgUAMBYFADAWBQCw+QUAsPkFALD5BQA=

atoms_z:
CK0JAEBgCgBwWAoA6EsDAEBJAwDAGQMAwBkDAMAZAwDgUwgA4FMIAPBSCADwUggAKAAAACgAAAAoAAAAKAAAACgAAABAQg8AQEIPAEBCDwA=

atoms_occupancy:
AAk9AAAJPQAACT0AAAk9AAAJPQDQfgEAAJg6ADDyAAAQ1S4A8DMOABDVLgDwMw4AcD44AHCUAAAQpAAAcAUDAECcAACAPgAAgFsQACBALAA=

atoms_u_iso:
gO0AAMDVAAC40wAAmIAAAIiQAAB4lgAAeJYAAHiWAADgagAA4GoAANhoAADYaAAA0HAAANBwAADQcAAA0HAAANBwAAAQbAEAEGwBABBsAQA=

atoms_aniso_label:
["O11", "O21", "O22", "O31", "O32", "O4", "O-H4", "F4", "SiT1", "AlT1", "SiT2", "AlT2", "AlM2", "TiM2", "FeM2", "CrM2", "MgM2", "CaA", "NaA", "KA"]

atoms_aniso_u11:
oIwAANiQAAAw7QAAkGAAANhPAAAYVgAAGFYAABhWAADAOgAAwDoAADBDAAAwQwAAOEUAADhFAAA4RQAAOEUAADhFAAD4UQEA+FEBAPhRAQA=

atoms_aniso_u22:
sOUAADjMAACInwAA+FIAABCGAABAeQAAQHkAAEB5AAAoRgAAKEYAAIA5AACAOQAAKEYAAChGAAAoRgAAKEYAAChGAABYZQEAWGUBAFhlAQA=

atoms_aniso_u33:
CFYBANgXAQDA+AAAqNkAAKjZAADA+AAAwPgAAMD4AACQugAAkLoAAJC6AACQugAAkLoAAJC6AACQugAAkLoAAJC6AAA4lAEAOJQBADiUAQA=

atoms_aniso_u12:
WND//zgdAADwCgAAuO3//0gSAABQ8f//UPH//1Dx//8AAAAAAAAAAGj8//9o/P//aPz//2j8//9o/P//aPz//2j8//8AAAAAAAAAAAAAAAA=

atoms_aniso_u13:
IAgAAAAAAAB4KAAA4Pf//xgQAABYIAAAWCAAAFggAAAgCAAAIAgAABgQAAAYEAAAGBAAABgQAAAYEAAAGBAAABgQAABwMAAAcDAAAHAwAAA=

atoms_aniso_u23:
MCoAAPDx//8AAAAAEA4AAAAAAADQ1f//0NX//9DV//8AAAAAAAAAABAOAAAQDgAAEA4AABAOAAAQDgAAEA4AABAOAAAAAAAAAAAAAAAAAAA=

qdat:
AAAAAAAAAAEAAAAAAAAAAQANECEAQIAGBAAIBAAIGgIiQEHjIoiQDihBYCBGgFVkpFiExD9qo8RYhQEUEpUo+5o2dQSkKfO/EjVFJNajhoVfeqXGWR1im3USVFoV5nhwul+3mqRqiTIkTQ1Uo4aZk4amNTlybwuRFEGQsx==


formula: O11.958 F.041 Cl.001 Si3.135 Al2.691 Ti.033 Fe.102 Cr.108 Mg.11 (Ba.012 Na.029 K.959) H1.456
compound: Northwest Nelson - Anatoki River
pub_title: Chromium-containing muscovite: crystal chemistry and XANES spectroscopy
formula_title: <missing>
a: 5.206
b: 9.040
c: 20.058
alpha: 90
beta: 95.79
gamma: 90
cell_volume: 939.159
crystal_density: 2.897
atoms_sites:
["O11", "O21", "O22", "O31", "O32", "O4", "O-H4", "F4", "Cl4", "SiT1", "AlT1", "SiT2", "AlT2", "AlM1", "TiM1", "FeM1", "CrM1", "MgM1", "MnM1", "AlM2", "TiM2", "FeM2", "CrM2", "MgM2", "MnM2", "BaA", "NaA", "KA"]

atoms_x:
ILctAJALDwDAqBkA0JAXAOCtOgDgYjoA4GI6AOBiOgDgYjoAgJYbAICWGwDQ6joA0Oo6AMDGLQDAxi0AwMYtAMDGLQDAxi0AwMYtAOA4DwDgOA8A4DgPAOA4DwDgOA8A4DgPAAAAAAAAAAAAAAAAAA==

atoms_y:
YBQTABBrFgBwjwUAsFkPAAD0GgAwxwMAMMcDADDHAwAwxwMAMMoPADDKDwAwRxoAMEcaAEBCDwBAQg8AQEIPAEBCDwBAQg8AQEIPAEAaBQBAGgUAQBoFAEAaBQBAGgUAQBoFAJD2BQCQ9gUAkPYFAA==

atoms_z:
YLQJAIBNCgBgSgoAgEUDAKBIAwCAEwMAgBMDAIATAwCAEwMAYEcIAGBHCAAgRggAIEYIAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAEABAABAAQAAQAEAAEABAABAAQAAQAEAAEBCDwBAQg8AQEIPAA==

atoms_occupancy:
AAk9AAAJPQAACT0AAAk9AAAJPQDgUQ8AAG8sAFBAAQDQBwAA4NYvACAyDQDg1i8AIDINAKC5NwDQAQEA4BwDAMBLAwBgWwMA0AcAANDcGwCwgQAAcI4BAOClAQCwrQEAIAMAAIC7AAAgxQEAYIg6AA==

atoms_u_iso:
kDwBACAHAQC4MgEAQPsAANDPAAB46wAAeOsAAHjrAAB46wAACLYAAAi2AABApgAAQKYAALiRAQC4kQEAuJEBALiRAQC4kQEAuJEBAKjZAACo2QAAqNkAAKjZAACo2QAAqNkAAEC5AQBAuQEAQLkBAA==

atoms_aniso_label:
["O11", "O21", "O22", "O31", "O32", "O4", "O-H4", "F4", "Cl4", "SiT1", "AlT1", "SiT2", "AlT2", "AlM2", "TiM2", "FeM2", "CrM2", "MgM2", "MnM2", "BaA", "NaA", "KA"]

atoms_aniso_u11:
WNQAAMDaAAAwOAEACPIAAIjWAACI1gAAiNYAAIjWAACI1gAAaKEAAGihAACgpQAAoKUAAFjUAABY1AAAWNQAAFjUAABY1AAAWNQAAJiEAQCYhAEAmIQBAA==

atoms_aniso_u22:
sBwBAGhQAQC4DwEAIBYBALCuAACwrgAAsK4AALCuAACwrgAAGLUAABi1AAD4egAA+HoAALCuAACwrgAAsK4AALCuAACwrgAAsK4AANi3AQDYtwEA2LcBAA==

atoms_aniso_u33:
QLkBADD8AAC4WgEAoNwAAKDcAAAoOwEAKDsBACg7AQAoOwEAEL0AABC9AACg3AAAoNwAADD8AAAw/AAAMPwAADD8AAAw/AAAMPwAAGD4AQBg+AEAYPgBAA==

atoms_aniso_u12:
KPH//5BRAABIIQAAMBYAANgOAACwHQAAsB0AALAdAACwHQAAGAsAABgLAAAAAAAAAAAAAMADAADAAwAAwAMAAMADAADAAwAAwAMAAAAAAAAAAAAAAAAAAA==

atoms_aniso_u13:
AAAAAPAoAACYSQAAAAAAAGgQAABYOQAAWDkAAFg5AABYOQAAaBAAAGgQAABoEAAAaBAAACAIAAAgCAAAIAgAACAIAAAgCAAAIAgAAPAoAADwKAAA8CgAAA==

atoms_aniso_u23:
AAAAAMjx//9o4///OA4AAMjx//8AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA4DgAAOA4AADgOAAA4DgAAOA4AADgOAAA4DgAAOA4AAAAAAAAAAAAAAAAAAA==

qdat:
AAAAAAAAAAEAAAAAAAAAAgAZIEIAgQAMCAAgCAAQVAhFAQKMixFAPKEFgIEUAdmXEcYWEftKmyKkJAiQpbiH3NGzyC0iXZnpMrQyJ3442E3X6lRrEtIltnGpzuP8Sw4fJ3XxNk7hHkIpYasWsWsy0eNEzVqTRFIjECIa6Z==


formula: (Mg Al2) O4
compound: <missing>
formula_title: <missing>
a: 8.0855
b: 8.0855
c: 8.0855
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.592
crystal_density: 3.575
atoms_sites: ["MgT", "AlT", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwCAhB4AgIQeAMj/DwA=
atoms_y: IKEHACChBwCAhB4AgIQeAMj/DwA=
atoms_z: IKEHACChBwCAhB4AgIQeAMj/DwA=
atoms_occupancy: gKEuAIBnDgDAMwcAQNU1AAAJPQA=
atoms_u_iso: oEEAAKBBAAAwQwAAMEMAADB1AAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Compositional dependence of cation distribution in some synthetic
 (Mg,Zn)(Al,Fe)2O4 spinels
 Sample: Sp3/10a

qdat:
AAAAAAAAAAAAAAAAAAAAAAEAAAAAAAAAAAAACAAAAAAgAAAAAAABAAAAEAAAAAAEAAAIAAAAAQAACAAAABAAAgAAACAAEAAAAgAEAAAEAAgAABAAQAABAAgAAEAEAABABAAAQAgAAAAgAAgCAAEAQAAgCAAEAgACAQAAAI==


formula: Mg.355 Zn.647 Al1.998 O4
compound: <missing>
formula_title: <missing>
a: 8.0870
b: 8.0870
c: 8.0870
alpha: 90
beta: 90
gamma: 90
cell_volume: 528.886
crystal_density: 4.241
atoms_sites: ["MgT", "ZnT", "AlT", "MgM", "AlM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgB4ExAA
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgB4ExAA
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgB4ExAA
atoms_occupancy: oLsNAGB9JwAA0AcAoPcDAGAROQAACT0A
atoms_u_iso: 4HkAAOB5AADgeQAAkGUAAJBlAABwewAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Compositional dependence of cation distribution in some synthetic
 (Mg,Zn)(Al,Fe)2O4 spinels
 Sample: Gah1a/a


formula: Mg Al1.788 Fe.202 O4
compound: <missing>
formula_title: <missing>
a: 8.1174
b: 8.1174
c: 8.1174
alpha: 90
beta: 90
gamma: 90
cell_volume: 534.873
crystal_density: 3.671
atoms_sites: ["MgT", "AlT", "FeT", "MgM", "AlM", "FeM", "O"]
atoms_x: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AuPsPAA==
atoms_y: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AuPsPAA==
atoms_z: IKEHACChBwAgoQcAgIQeAICEHgCAhB4AuPsPAA==
atoms_occupancy: AG8sACAMCwDgjQUAAE0IALAKMQAwYwMAAAk9AA==
atoms_u_iso: kEwAAJBMAACQTAAAcEkAAHBJAABwSQAAQIMAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Compositional dependence of cation distribution in some synthetic
 (Mg,Zn)(Al,Fe)2O4 spinels
 Sample: MgF1a/6a


formula: Mg.851 Zn.148 Al1.763 Fe.238 O4
compound: <missing>
formula_title: <missing>
a: 8.1242
b: 8.1242
c: 8.1242
alpha: 90
beta: 90
gamma: 90
cell_volume: 536.219
crystal_density: 3.845
atoms_sites: ["MgT", "ZnT", "AlT", "FeT", "MgM", "AlM", "FeM", "O"]
atoms_x: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeALgAEAA=
atoms_y: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeALgAEAA=
atoms_z: IKEHACChBwAgoQcAIKEHAICEHgCAhB4AgIQeALgAEAA=
atoms_occupancy: QLglAIAICQBgNwkA4BAFAFAcBwDAMTEA8LoEAAAJPQA=
atoms_u_iso: 4EcAAOBHAADgRwAA4EcAACBOAAAgTgAAIE4AACCAAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Compositional dependence of cation distribution in some synthetic
 (Mg,Zn)(Al,Fe)2O4 spinels
 Sample: Frk1a/d

qdat:
AAAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAAAEAAAAACAAAAAAAAEAAAAQAAAAAAQAAAgAAAABAAAQAAAAEAAEAAAAIAAgAAAEAAgAAAQAEAAAIACAAAIAEAABAAgAAIAIAAEAIAAAAIAAQAgABAEAAIAgACAQABAIAAAEA==


formula: Ca (Al1.817 Fe.183) O4
compound: Synthetic
formula_title: <missing>
a: 8.758
b: 8.112
c: 15.311
alpha: 90
beta: 90.21
gamma: 90
cell_volume: 1087.761
crystal_density: 2.992
pub_title:
 On the Al/Fe substitution in iron doped monocalcium
 aluminate - the crystal structure of CaAl1.8Fe0.2O4

atoms_sites:
["Ca1", "Ca2", "Ca3", "AlT1", "FeT1", "AlT2", "FeT2", "AlT3", "FeT3", "AlT4", "FeT4", "AlT5", "FeT5", "AlT6", "FeT6", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12"]

atoms_x:
kKcOABBdEABAJC0AwNoZAMDaGQDQnRkA0J0ZAHCEJABwhCQAgFolAIBaJQDgHTkA4B05AMBMOQDATDkA8LoEAJAUAQBgWwMAwBwPALB7GgCQRhoA0H4aAPCvIwAweSkAABguAGCLLQAQHDgA

atoms_y:
ACYCABCrHAAgPSAAYPUTAGD1EwBQUSwAUFEsACCZMgAgmTIA4I8NAOCPDQDghCwA4IQsAABpFAAAaRQAwJ8OAABsIAAw5jQAcO8OAMDLDwAwNzQAkAkgAODaDQCgbQEA4PUVAMBoLACQCw8A

atoms_z:
MHAFAMBeBABgEw8AAI0OAACNDgDAOw4AwDsOAFDEBABQxAQAEPAEABDwBACwlQUAsJUFAKCgBQCgoAUAAHcBAKDMBgBwEwkAEFwMACCsAQDglAgAYHYLAGDzCwDgTgMAkNYCANA7CABACQwA

atoms_occupancy:
AAk9AAAJPQAACT0AwIQ4AECEBAAALTcAANwFAEDPNgDAOQYAYJo3AKBuBQBgIzYAoOUGAIBlOACAowQAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
kLAAABDWAAAwJAEA4HkAAOB5AABAgwAAQIMAAMB2AADAdgAAoIwAAKCMAAAwdQAAMHUAALCBAACwgQAAEL0AABAIAQCQ+wAAUNwAADDZAAAw8gAAYBwBAIAGAQCABgEAEAgBAOD2AACg8AAA

atoms_aniso_label:
["Ca1", "Ca2", "Ca3", "AlT1", "FeT1", "AlT2", "FeT2", "AlT3", "FeT3", "AlT4", "FeT4", "AlT5", "FeT5", "AlT6", "FeT6", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12"]

atoms_aniso_u11:
gLsAAKC+AACABgEAcHsAAHB7AABAagAAQGoAAFB4AABQeAAAYG0AAGBtAAAQWQAAEFkAAFB4AABQeAAAUMMAAKAiAQAAEwEAYJ8AAODEAAAA+gAAcHUBAGDRAABg6gAAwCUBALDMAABAtQAA

atoms_aniso_u22:
UJEAAGDRAADwHQEAgIkAAICJAABwrQAAcK0AAAB9AAAAfQAA4MQAAODEAAAwpwAAMKcAAGCGAABghgAAsMwAAFDcAABQDgEA0AEBANDoAADQAQEAcPgAAACQAQDA2gAA4MQAAJBGAQDgcwEA

atoms_aniso_u33:
AMgAADDyAABASwEAsGgAALBoAAAwdQAAMHUAABByAAAQcgAAUHgAAFB4AABQXwAAUF8AAICJAACAiQAAUKoAANAaAQCA1AAAwPMAAHDfAACg8AAAQOcAAACvAABgTgEAIC8BAIDUAADAqAAA

atoms_aniso_u12:
YAkAALAdAACwBAAAsOv//7Dr//9gCQAAYAkAAHAXAABwFwAAgPP//4Dz///wCgAA8AoAAKAPAACgDwAAQB8AAKD2//9ws///MBEAAMArAAAgNQAAgPP//6BaAACADAAAsOv//2AiAADA+f//

atoms_aniso_u13:
oEEAANDu//+wBAAAIAMAACADAAAAGQAAABkAAFAUAABQFAAA4BUAAOAVAAAQDgAAEA4AAHAXAABwFwAAoEEAAKDd//+ADAAAUBQAADARAACQMwAA4BUAAOAuAABAagAAsB0AAHAXAABg8P//

atoms_aniso_u23:
cBcAAMASAABg8P//MPj//zD4//9gCQAAYAkAAJABAACQAQAAYPD//2Dw//8gAwAAIAMAAGAJAABgCQAAkBoAAEAGAABw/v//cP7//xDc//8QQAAA4Pz//1AUAAAg6v//4C4AAOAuAABAOAAA

qdat:
AAAAAAAAAAAAgCCAACRAAAIBQBC6kZMCEgQRMDXMFwBrXUolF9guh+fW7uUHM+jwt/3/f2e/H74bfvv8a/fn3/3f+/79+u/Wf/f++/f+7r/fv+77zvv75/3+9/vf/3//v////+/fq/++95u/v1eP9b/6v9l8/G7pbexqY1==


formula: Na.86 K.2 Ca1.325 Ba.015 Sr.435 (Al4.46 Si13.54) O49 H26
compound: <missing>
pub_title: High-pressure structural behaviour of heulandite Sample: P = .0001 GPa
formula_title: <missing>
a: 17.729
b: 17.909
c: 7.433
alpha: 90
beta: 116.52
gamma: 90
cell_volume: 2111.715
crystal_density: 2.252
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["NaCS1", "KCS1", "CaCS1", "BaCS1", "SrCS1", "CaCS2", "AlT1", "SiT1", "SiT2", "AlT2", "SiT3", "AlT3", "SiT4", "AlT4", "SiT5", "AlT5", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5", "Wat6"]

atoms_x:
sEsJALBLCQCwSwkAsEsJALBLCQDgbQIAsPQKALD0CgBQ3wwAUN8MAEC4DABAuAwA0O8DANDvAwAAAAAAAAAAAEDXCwBQJA4A0CkLAECTDgAAAAAA0AIFAIDDBwBAgwAAENkMAMABBwAgrw0AAOIEANC3BAAAAAAAAAAAAGDMBQA=

atoms_y:
AAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AIF0KACBdCgAgAxkAIAMZAHCdCwBwnQsAIC0SACAtEgDg+QwA4PkMAICEHgBgQwcAUFsJAMCEBgBA2RMAMKMJAFBWDgCwOhAAwIAPAMC6FgCAhB4AAAAAAFB4GQCAhB4A4I0FAAAAAAA=

atoms_z:
cBspAHAbKQBwGykAcBspAHAbKQCAWgwAYOUFAGDlBQDAcR4AwHEeAGDJKwBgySsAQAYZAEAGGQAAAAAAAAAAAGDFGwBwfiUAkAI2APCqDwCAhB4AIOsDADB3IQCQPAsAYK4KAKAuGABgc///ALY1AEA0OwCAhB4AgIQeAACUEQA=

atoms_occupancy:
wD4aAIAaBgAQ6wkAMHUAAHBGDQCAhB4AALgLAABRMQAg4SYA4CcWAKDjMABgJQwAwDExAEDXCwBApigAwGIUAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
IL8CACC/AgAgvwIAIL8CACC/AgCgAwIAAOEAAADhAABg6gAAYOoAAJDiAACQ4gAAIOQAACDkAACg8AAAoPAAACDFAQBg5AEAgLUBAOClAQAA9AEAYGcBACBCAgDA1AEAIMUBAECWAQCALAMAQHgGAKD3AwAgswQAwJgLAKBiBwA=

qdat:
AAAAAAAABAACAQACACCCGAAICANIRAhEAGg4IMUSAsRRUOlUCIXkHn2aYDNy2u88yj913B/C6m7Y0L/PipQK368l7MB/uUv8F/6ehpKuKrQ2V2ZdXcOSDq07sHmVLnkyU8WLLYJMk5Jq5C4TThzrkfIG+ck7BuiYafUb4n==


formula: Na.86 K.2 Ca1.325 Ba.015 Sr.435 (Al4.46 Si13.54) O49 H26
compound: <missing>
pub_title: High-pressure structural behaviour of heulandite Sample: P = 1.45 GPa
formula_title: <missing>
a: 17.481
b: 17.625
c: 7.345
alpha: 90
beta: 116.73
gamma: 90
cell_volume: 2021.179
crystal_density: 2.352
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["NaCS1", "KCS1", "CaCS1", "BaCS1", "SrCS1", "CaCS2", "AlT1", "SiT1", "SiT2", "AlT2", "SiT3", "AlT3", "SiT4", "AlT4", "SiT5", "AlT5", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5", "Wat6"]

atoms_x:
cCwJAHAsCQBwLAkAcCwJAHAsCQCgAwIAoBgLAKAYCwDwowwA8KMMAIClDACApQwA4LIDAOCyAwAAAAAAAAAAAGCoCwAg+g0AwBsLAAAjDwAAAAAAYE8FAGDABwDgLgAAYKIMAADWBgBgnA0AYNIEAMDCBAAAAAAAAAAAACAqBgA=

atoms_y:
AAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AgAIKAIACCgCg9hgAoPYYACCJCwAgiQsAYAESAGABEgAggwwAIIMMAICEHgAAUwcAAMoIAKBoBgCgFBQAQOkIAACmDgAg7g8AoK8PAGBmFgCAhB4AAAAAAADnGACAhB4AgCAFAAAAAAA=

atoms_z:
4DIpAOAyKQDgMikA4DIpAOAyKQCgSgsAICoGACAqBgBA6B0AQOgdAICzKwCAsysA4JgYAOCYGAAAAAAAAAAAAOCGGwBgDCUAgPQ1AAAdEACAhB4AIDAFAMCRIQCgSgsAQGAKAADzFgAg0f//4Gc1AIDcOQCAhB4AgIQeAKCXEwA=

atoms_occupancy:
wD4aAIAaBgAQ6wkAMHUAAHBGDQCAhB4AALgLAABRMQAg4SYA4CcWAKDjMABgJQwAwDExAEDXCwBApigAwGIUAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
4J8CAOCfAgDgnwIA4J8CAOCfAgCAtQEAwNoAAMDaAADgKAEA4CgBAIC7AACAuwAAQBkBAEAZAQBAGQEAQBkBAABxAgCAOAEAYOQBAIA4AQAgxQEA4KUBACC/AgAgxQEAoAMCAIAyAgAAcQIAAOIEAICpAwDARQQAQNEMAMBFBAA=

qdat:
AAAAAAAAAgABAIAAgAghBgABAgDKCIEIgAkHhAyjQExFDQaNQMRPIHL0s4Haz2u7UzjtTuhfhdTb8fF72xy6Cr+dQvZAfOyrdhPezcU9L49tFVfW+q+w8oOpxWYGqPfGMzU8WK5YJOislddC0ExplSyOiBvPSEoaw+FWs1==


formula: Na.86 K.2 Ca1.325 Ba.015 Sr.435 (Al4.46 Si13.54) O49 H26
compound: <missing>
pub_title: High-pressure structural behaviour of heulandite Sample: P = 3.4 GPa
formula_title: <missing>
a: 17.124
b: 17.376
c: 7.237
alpha: 90
beta: 116.93
gamma: 90
cell_volume: 1919.837
crystal_density: 2.477
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["NaCS1", "KCS1", "CaCS1", "BaCS1", "SrCS1", "CaCS2", "AlT1", "SiT1", "SiT2", "AlT2", "SiT3", "AlT3", "SiT4", "AlT4", "SiT5", "AlT5", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "Wat1", "Wat2", "Wat3", "Wat4", "Wat5", "Wat6"]

atoms_x:
8LsIAPC7CADwuwgA8LsIAPC7CADgpQEAYCsLAGArCwDgSgwA4EoMADCqDAAwqgwAsG8DALBvAwAAAAAAAAAAAABBCgDg2g0A4OwKAACgDwAAAAAAAF8FAABTBwCgkv//oMEMAEB4BgAg+g0AYNIEAABfBQAAAAAAAAAAAABZBgA=

atoms_y:
AAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AwCEKAMAhCgBgVBkAYFQZACCJCwAgiQsAIOIRACDiEQBgJQwAYCUMAICEHgAgJAcAgAgJACAqBgBAoRQAAMoIAGCWDgAAIw8AgGEPAGDpFQCAhB4AAAAAAGDXGACAhB4AIK0FAAAAAAA=

atoms_z:
oBMpAKATKQCgEykAoBMpAKATKQDApAkAYEkGAGBJBgBgPB0AYDwdAGDiKwBg4isAoPwXAKD8FwAAAAAAAAAAAGDXGACAWiUAYCM2AAAdEACAhB4AANwFAIByIQCgzQoAYK4KAMBcFQAgTgAAgPQ1AMB+OQCAhB4AgIQeAGB4EwA=

atoms_occupancy:
wD4aAIAaBgAQ6wkAMHUAAHBGDQCAhB4AALgLAABRMQAg4SYA4CcWAKDjMABgJQwAwDExAEDXCwBApigAwGIUAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
wFECAMBRAgDAUQIAwFECAMBRAgBAfgUAIMsAACDLAADA2gAAwNoAAKAJAQCgCQEAoAkBAKAJAQDgKAEA4CgBAICpAwCggAIA4KUBAOClAQBADQMA4CgBAADuAgBg5AEAAPoAAKADAgDA1AEAQH4FAEB+BQBAfgUAAOIEAEANAwA=

qdat:
AAAAAAAAAQAAgCAAQAIIQUAAQEAeIghAkADQeCDGMQLEOKhyaQTY2EPU2VwC6x6t73xpOKzcX86YbOPwr02DLIJZ7+E8kCsNXc6SP1Y5IlJw39JGdztla4aYHyZGoDJjNp7axfzFmxmcUNqaJ0bIjPMM6pHQK2zIZYTg8G==


formula: Na.86 K.2 Ca1.325 Ba.015 Sr.435 (Al4.46 Si13.54) O49 H26
compound: <missing>
pub_title: High-pressure structural behaviour of heulandite Sample: P = .0001 GPa (after compression)
formula_title: <missing>
a: 17.774
b: 17.824
c: 7.438
alpha: 90
beta: 116.38
gamma: 90
cell_volume: 2111.009
crystal_density: 2.252
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_x:
8GoJAPBqCQDwagkA8GoJAPBqCQCAfQIAQPYKAED2CgBQ3wwAUN8MAIC+DACAvgwAsOwDALDsAwAAAAAAAAAAAJDrCwDAIg4A4FALALCqDgAAAAAAkBUFAPDBBwDgkgAAsM8MAHAGBwBwkQ0AMNoEAJCxBAAAAAAAAAAAAKDrBQA=

atoms_y:
AAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AIEQKACBECgAgAxkAIAMZAGCoCwBgqAsAgDYSAIA2EgCw6AwAsOgMAICEHgBgXAcAQE0JALB2BgAg7xMAYIIJAMBUDgAgORAAQHQPAOC9FgCAhB4AAAAAAMB2GQCAhB4AUIwFAAAAAAA=

atoms_z:
0D0pANA9KQDQPSkA0D0pANA9KQCwOQwAUNcFAFDXBQAQbR4AEG0eAHDXKwBw1ysAcBcZAHAXGQAAAAAAAAAAAEB3GwBAVCUA8As2AGCpDwCAhB4AINIDAGDTIQDwXgsAwLcKAPBCGABgc///4Gc1AKAkOwCAhB4AgIQeAODCEQA=

atoms_u_iso:
gK8CAICvAgCArwIAgK8CAICvAgCAtQEA4N0AAODdAABw3wAAcN8AAKDXAACg1wAAkOIAAJDiAADQAQEA0AEBAIC1AQAgxQEAIMUBAOClAQBAEwIAoIYBAMBRAgDgIgIA4KUBAIC1AQAA7gIAYMYGAMDIAwBAhAQAQNEMAEDvBwA=

qdat:
AAAAAAAABAABAQACACBCKAAEEAMwJAREAMgoQKi8BSSw4Hk4HcmkDtO0MGJ89f5KvjvXuj3Ds32p0b19pTgi3b9F+IBXMZuwW/YuDnq3F6htK4z7OwVEP7pi4alW3mZpzQqdfAcxT4lW0JhOHHKdw6Iaxxj8LcphZ1xLkZ==


formula: K.004 (Mg1.3 Fe.7) Al3.94 Si4 O19.896 F.304 H7.896
compound: Monte Argentario
formula_title: <missing>
a: 13.716
b: 20.084
c: 5.110
alpha: 90
beta: 90
gamma: 90
cell_volume: 1407.663
crystal_density: 2.933
atoms_sites: ["K", "MgM1", "FeM1", "Al1", "Al2", "Si", "O1", "O2", "O3", "O-h1", "F1", "O-h2", "F2", "H1", "H2"]
atoms_x: AAAAAAAAAAAAAAAAgKYLAAAAAAA40AsAmJIMAFjpBAAoIw8ASBYGAEgWBgAQKAQAECgEAOBS+v/ALQgA
atoms_y: wMYtAOBnNQDgZzUAwMYtAHisOgAIszUAmNIwAAjkNgC4tTcA0GwxANBsMQAI9DoACPQ6AKDjMADgxjoA
atoms_z: QEIPAMDGLQDAxi0AwMYtAEBCDwDwbhkAYE4aANDuGADw9SgA8Kc1APCnNQAQmTgAEJk4AEDiHgCA6DcA
atoms_occupancy: gD4AAECsJwDAXBUAoB48AKAePAAACT0AAAk9AAAJPQAACT0A4D08AMBRAgDgPTwAwFECAOA9PADgPTwA
atoms_u_iso: QJwAAECDAABAgwAAwF0AACBnAAAwXAAAkH4AAECDAAAwjgAAkLAAAJCwAACwgQAAsIEAACC5AwAAdwEA
atoms_aniso_label: ["MgM1", "FeM1", "Al1", "Al2", "Si", "O1", "O2", "O3", "O-h1", "F1", "O-h2", "F2"]
atoms_aniso_u11: QGoAAEBqAADAXQAAEFkAALBPAADQhAAAYG0AAJCXAADAqAAAwKgAAKBaAACgWgAA
atoms_aniso_u22: MI4AADCOAABQXwAAMHUAAJBlAABgbQAAAJYAAACWAADgxAAA4MQAAPCgAADwoAAA
atoms_aniso_u33: 4JIAAOCSAADAXQAAIGcAAOBgAAAQiwAA8IcAAAB9AACgpQAAoKUAAPCHAADwhwAA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAANAHAADQBwAA4BUAAHD+//9wMAAAcDAAAGAJAABgCQAA
atoms_aniso_u13: 4BUAAOAVAAAAAAAAAAAAAAAAAADwCgAAIAMAAPDY///QBwAA0AcAABAOAAAQDgAA
atoms_aniso_u23: AAAAAAAAAABABgAAAAAAACADAACQAQAAcBcAAFD7//+wBAAAsAQAAIAMAACADAAA
pub_title:
 Crystal-chemistry of magnesiocarpholite: controversial X-ray
 diffraction, Mossbauer, FTIR and Raman results

qdat:
AAAAAAAAAAEAAAAIAAEABAEAABBAAAEYIAlAAgAAIiMCEhgiEAMXQBIUSEEIsk5BFBoVioEBEsogNiAQuimokGqtQ5QA9VkBQwIwARTFIQxEQkMQkghqKAEkAQAtKCTRKBGShKJAAyAgBQAGFoxE0SCQDRAKAEARQQAQqx==


formula: K.004 (Mg1.3 Fe.7) Al3.96 Si4 O19.92 F.24 H7.92
compound: Monte Leoni
formula_title: <missing>
a: 13.726
b: 20.099
c: 5.112
alpha: 90
beta: 90
gamma: 90
cell_volume: 1410.293
crystal_density: 2.926
atoms_sites: ["K", "MgM1", "FeM1", "Al1", "Al2", "Si", "O1", "O2", "O3", "O-h1", "F1", "O-h2", "F2", "H1", "H2"]
atoms_x: AAAAAAAAAAAAAAAACKsLAAAAAACYzwsA4JUMAADnBAB4KA8AsBcGALAXBgCwKAQAsCgEAIARyf+g3wcA
atoms_y: wMYtAKBrNQCgazUAwMYtAACsOgCQsjUAMNEwAEDjNgD4tjcAUG8xAFBvMQCg8joAoPI6AKDjMABgiDoA
atoms_z: QEIPAMDGLQDAxi0AwMYtAEBCDwDwbhkAEFMaACADGQBA8SgAcII1AHCCNQDgoDgA4KA4AGA2HgAgdTgA
atoms_occupancy: gD4AAECsJwDAXBUAwGw8AMBsPAAACT0AAAk9AAAJPQAACT0AwGw8AMDUAQDAbDwAwNQBAMBsPADAbDwA
atoms_u_iso: QJwAABByAAAQcgAAgFcAANBSAAAASwAA0GsAABByAADgeQAA0J0AANCdAADwbgAA8G4AAIAmBABg5AEA
atoms_aniso_label: ["MgM1", "FeM1", "Al1", "Al2", "Si", "O1", "O2", "O3", "O-h1", "F1", "O-h2", "F2"]
atoms_aniso_u11: oFoAAKBaAABgVAAAAEsAABBAAABgbQAAQFEAAGCGAACgjAAAoIwAAOBHAADgRwAA
atoms_aniso_u22: cHsAAHB7AABAUQAAEFkAANBSAADwVQAAgIkAAKBzAAAQpAAAEKQAAICJAACAiQAA
atoms_aniso_u33: QIMAAECDAABQXwAAgFcAAEBRAACQfgAA4HkAAKBzAAAwpwAAMKcAAHB7AABwewAA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAIAMAABgCQAA4BUAAMD5//+APgAAgD4AAKAPAACgDwAA
atoms_aniso_u13: UBQAAFAUAAAAAAAAcP7//5ABAADQBwAAAAAAAMDg//8AAAAAAAAAAIAMAACADAAA
atoms_aniso_u23: AAAAAAAAAABABgAAAAAAACADAAAgAwAAUBQAAIAMAABQ+///UPv//7AEAACwBAAA
pub_title:
 Crystal-chemistry of magnesiocarpholite: controversial X-ray
 diffraction, Mossbauer, FTIR and Raman results

qdat:
AAAAAAAAAAIAAAAIAAEABAEAABBAAAEYQAlAAgAAIiMCIhgiEAMmQCIUiEEJIlZBFBoVkoEBEtwgdiAROknIkGzWQxQApVkBRgIwAhTJIgxIQkIQtBCyUAEkAQBNKCjiMBGVBMJAAyBABQAKKoyE0SGgCRASAIARggAQ0x==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2173
b: 9.0493
c: 19.989
alpha: 90
beta: 95.734
gamma: 90
cell_volume: 939.017
crystal_density: 2.732
atoms_x: AAAAAAAAAABAxQ4AQMUOAEDFDgDAMhwAwDIcAICWGwCAlhsAoOQbAEAMGADAtRsAwLUbACAvGgBgGQ4AACMPAMBcFQA=
atoms_y: YE8FAGBPBQAgFwUAIBcFAGCzBQAgdTgAIHU4AIDeDwCA3g8AYFw5AIB6DwBATSIAQE0iADDUBQBQFDIAwD0WAAAKKAA=
atoms_z: QEIPAEBCDwAQDgAAEA4AABAOAABgPQgAYD0IAJBnCACQZwgAkCEDABAuAwCALAMAgCwDAIBNCgDwtQkAUFUKAIAsAwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: wFcBAMBXAQAgTgAAIE4AACBOAABg6gAAYOoAAMBdAADAXQAAIMsAAOCrAACAuwAAgLsAAOAoAQCAtQEAAPoAAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: ILkDAA==
atoms_aniso_u22: YN4CAA==
atoms_aniso_u33: 4J8CAA==
atoms_aniso_u12: AO4CAA==
atoms_aniso_u13: IDwDAA==
atoms_aniso_u23: 4CICAA==
pub_title:
 Thermal response of structure and hydroxyl ion of
 phengite-2M_1: an in situ neutron diffraction and FTIR study
 Sample: T = 20 C

atoms_sites:
["K", "Na", "Al", "Mg", "Fe", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "F3", "O4", "O5", "O6", "H1"]

qdat:
AAAAAAAAAAEAAAAAAAAAAgAaIEIAgQAKCAAgCAAQZAyFAQMMlRJAKKEJgEEaAbunIcQlIfVUlSLEKAmgqeWH/aLTUEoimzvyU1RSL+54sKvu1LTrQqxT7qKqlkNZzhw+VdWm3R2kaQiUx3p5Yu7JQ1MZrdFWiKiKIIh6l5==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2196
b: 9.0550
c: 20.010
alpha: 90
beta: 95.746
gamma: 90
cell_volume: 940.990
crystal_density: 2.726
atoms_x: AAAAAAAAAACAZw4AgGcOAIBnDgDgAxwA4AMcACCmGwAgphsAYMUbAEAMGADgAxwA4AMcAICcGgAgdw4AwAMPAMDfFAA=
atoms_y: oOsFAKDrBQDg9wQA4PcEAOD3BACgNjgAoDY4ACDuDwAg7g8AkIY5AHCeDwCgPSIAoD0iAFDXBQCQGjIAkPoVAGB9JwA=
atoms_z: QEIPAEBCDwBw5f//cOX//3Dl//+wOAgAsDgIACBQCAAgUAgAoC8DAOBOAwBQGwMAUBsDAPBLCgCgugkAgGYKAABrAwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: AHcBAAB3AQDgqwAA4KsAAOCrAADgpQEA4KUBAGBtAABgbQAAIMsAAAB9AADA2gAAwNoAAGDqAACAtQEAgLsAAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: oPEEAA==
atoms_aniso_u22: YN4CAA==
atoms_aniso_u33: wD8FAA==
atoms_aniso_u12: YN4CAA==
atoms_aniso_u13: gK8CAA==
atoms_aniso_u23: AAAAAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T = 100 C

atoms_sites:
["K", "Na", "Al", "Mg", "Fe", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "F3", "O4", "O5", "O6", "H1"]

qdat:
AAAAAAAAAAEAAAAAAAAAAgASIIIAgQAMCAAgCAAQbAyFAQcclRJAKSEJgEIaAbsmIoQlIb5UlSVESAmgqesK9eNjUFokm1PSYqRWLvx5UK/+3SjdRaxTzsLLroX5njw2m9VmqStASRClh6za46zJRVIatfFbCUiMQYhtrx==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2230
b: 9.0618
c: 20.044
alpha: 90
beta: 95.738
gamma: 90
cell_volume: 943.925
crystal_density: 2.718
atoms_x: AAAAAAAAAACAZw4AgGcOAIBnDgBA9BsAQPQbAMC1GwDAtRsAYMUbAEAMGADAMhwAwDIcACCsGgBgGQ4AwAMPAOCwFAA=
atoms_y: YMwFAGDMBQAw8wQAMPMEADDzBAAAJzgAACc4ACDuDwAg7g8AwH45AMCyDwDQNSIA0DUiAADcBQCwNjIAsOQVAGB9JwA=
atoms_z: QEIPAEBCDwAg6v//IOr//yDq///wJQgA8CUIALBRCACwUQgAMDEDAFBNAwAwGAMAMBgDACBECgAQuQkA8GQKAKB6AwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: IMUBACDFAQDA2gAAwNoAAMDaAAAA9AEAAPQBAGBtAABgbQAAYOoAAKCMAABg6gAAYOoAAKAJAQDA1AEAIMsAAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: 4BAFAA==
atoms_aniso_u22: gKkDAA==
atoms_aniso_u33: gCAFAA==
atoms_aniso_u12: QIoDAA==
atoms_aniso_u13: wM4CAA==
atoms_aniso_u23: wOD//w==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T = 200 C

atoms_sites:
["K", "Na", "Al", "Mg", "Fe", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "F3", "O4", "O5", "O6", "H1"]

qdat:
AAAAAAAAAAEAAAAAAAAAAgASIIIAgQAUCAAgEAAgaAiFAQUYliJAWUEKgII0A/NGIoQqIu5ZNkWIUBFBS8sL1+VmoFREtmPUZqimX1zxYT/XqXHuRUiWzMWTPI6zPDhsq1vNWjVIiREqjuyyxd2ThqY1W/KuElEYgxDbXR==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2276
b: 9.0701
c: 20.083
alpha: 90
beta: 95.726
gamma: 90
cell_volume: 947.481
crystal_density: 2.708
atoms_x: AAAAAAAAAADgVw4A4FcOAOBXDgCg5BsAoOQbACCmGwAgphsAQPQbAOAbGACAExwAgBMcAGDLGgDACQ4AwAMPAEChFAA=
atoms_y: oOsFAKDrBQCA7gQAgO4EAIDuBABARjgAQEY4AMD9DwDA/Q8AoJQ5AGCpDwAQPCIAEDwiAADcBQDAXTIAoNYVAMBtJwA=
atoms_z: QEIPAEBCDwBg8P//YPD//2Dw//9wGQgAcBkIACBQCAAgUAgAQD8DAJBTAwBwHgMAcB4DAFA8CgBAsQkAIHYKAKB6AwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: wFECAMBRAgAA+gAAAPoAAAD6AAAgxQEAIMUBACBOAAAgTgAAwFcBACDLAADAVwEAwFcBACBIAQAA9AEAgDgBAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: AFkGAA==
atoms_aniso_u22: 4J8CAA==
atoms_aniso_u33: YFUEAA==
atoms_aniso_u12: oHoDAA==
atoms_aniso_u13: 4KUBAA==
atoms_aniso_u23: oA8AAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T1 = 300 degrees C

qdat:
AAAAAAAAAAEAAAAAAAAAAgASQIIAgQAUCAAgEAAgqAiKAQUZFiKAcUITAII4A/ZKI4hMQ/yqKkaIUCNBUtUfe8bFILSJNmakyzDMrfjioX1eutO8ipEluYmmVQvjOHBpN7+bcmaIsiJVFflVi3unFSxmr6UyJKIxAiFumi==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2279
b: 9.0745
c: 20.096
alpha: 90
beta: 95.727
gamma: 90
cell_volume: 948.607
crystal_density: 2.705
atoms_x: AAAAAAAAAACAZw4AgGcOAIBnDgCg5BsAoOQbAICWGwCAlhsAQPQbAEAMGADgAxwA4AMcAED6GgBgGQ4A4NQOAGDvFAA=
atoms_y: QPsFAED7BQDw7AQA8OwEAPDsBACAZTgAgGU4AGANEABgDRAAYI45ADCYDwDwOCIA8DgiAODYBQCwTzIAYNAVAOA+JwA=
atoms_z: QEIPAEBCDwBA7f//QO3//0Dt//8AGwgAABsIADBFCAAwRQgAEC4DAEBYAwAwGAMAMBgDAGBKCgAwowkAcHEKAECKAwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: gK8CAICvAgBAGQEAQBkBAEAZAQBAEwIAQBMCAAB9AAAAfQAA4CgBAAD6AABAlgEAQJYBAKCGAQCgAwIAgDgBAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: IKcGAA==
atoms_aniso_u22: gCwDAA==
atoms_aniso_u33: gBoGAA==
atoms_aniso_u12: gKkDAA==
atoms_aniso_u13: 4KsAAA==
atoms_aniso_u23: QB8AAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T2 = 300 degrees C

qdat:
AAAAAAAAAAEAAAAAAAAAAgAyQIIBAQAUCABAEAAgqBCKAgUZFiKAckITAQIoA/ZKQwhMQ/yqLEqQkCJCktUd9crNIKSJNGqkzVFIvrniwn2WstO8jpEtuosqVQ9neHD5V9ebtGUApCJWFalnmqutFRRG16kyRSIxBiJumm==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2321
b: 9.0784
c: 20.125
alpha: 90
beta: 95.715
gamma: 90
cell_volume: 951.168
crystal_density: 2.697
atoms_x: AAAAAAAAAACgOA4AoDgOAKA4DgAA1RsAANUbAOCGGwDghhsAQPQbAOAbGADgAxwA4AMcAKDqGgDg2g0A4NQOAOCwFAA=
atoms_y: ANwFAADcBQAw2gQAMNoEADDaBACgNjgAoDY4AGANEABgDRAA4Jo5ADCxDwDwOCIA8DgiAEDiBQBQeDIA4MMVAIBOJwA=
atoms_z: QEIPAEBCDwCA8///gPP//4Dz//9AIQgAQCEIACA3CAAgNwgAwDIDAHBQAwAwGAMAMBgDAOA9CgDgpwkAYHwKAKB6AwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: AO4CAADuAgCgCQEAoAkBAKAJAQAA9AEAAPQBAAB9AAAAfQAAYGcBAGDqAABAlgEAQJYBAECWAQBg5AEAYGcBAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: gJEHAA==
atoms_aniso_u22: gCwDAA==
atoms_aniso_u33: 4AQHAA==
atoms_aniso_u12: gCYEAA==
atoms_aniso_u13: QIoDAA==
atoms_aniso_u23: APoAAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T1 = 400 degrees C

qdat:
AAAAAAAAAAEAAAAAAAAABAAyQIIBAQAYEABAEAAgyBEKAgcZLESAskQVAQRoB1ZMRwhMR+0yLIsQoCJCl6Y298qNQakKdO/JllFJP7nmwq+9U2N5FKFPspNOuhXmePDab16W5K0hSESmKunLF3dNGmjM39GkRkRRCkfctN==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2324
b: 9.0787
c: 20.129
alpha: 90
beta: 95.718
gamma: 90
cell_volume: 951.438
crystal_density: 2.696
atoms_x: AAAAAAAAAACAZw4AgGcOAIBnDgBgxRsAYMUbAICWGwCAlhsAgBMcAOAbGACg5BsAoOQbAGDLGgBAyw0A4NQOAEChFAA=
atoms_y: QPsFAED7BQBgBAUAYAQFAGAEBQBARjgAQEY4AAAdEAAAHRAAMJY5AOC1DwCAOiIAgDoiAIDoBQCAcDIAcMUVAIBOJwA=
atoms_z: QEIPAEBCDwBA7f//QO3//0Dt//8QEAgAEBAIABBCCAAQQggAgCwDAOBOAwDQDgMA0A4DAMA6CgBwqQkAYHwKAOCZAwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: QJACAECQAgAA+gAAAPoAAAD6AAAA9AEAAPQBAKCMAACgjAAAIEgBAMDaAABAGQEAQBkBAECWAQBg5AEAIEgBAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: IBgJAA==
atoms_aniso_u22: QIoDAA==
atoms_aniso_u33: AE0IAA==
atoms_aniso_u12: ILMEAA==
atoms_aniso_u13: 4BAFAA==
atoms_aniso_u23: AH0AAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T2 = 400 degrees C

qdat:
AAAAAAAAAAEAAAAAAAAABAAyQIIBAQAYEABAEAAgyBEKAgcZLESAskQVAQRoB1ZMRwhMR+0ybIsQoCKCl6Y294qNQakKdO/JllGJX7nmwq+9U6N5FKFfspNOuhfGePDab16U5K0hSESmKunLF1dOGqjM3dGkTkRRCkdctN==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2360
b: 9.0862
c: 20.169
alpha: 90
beta: 95.707
gamma: 90
cell_volume: 954.791
crystal_density: 2.687
atoms_x: AAAAAAAAAABASA4AQEgOAEBIDgAA1RsAANUbAOCGGwDghhsAQPQbAOAbGACAExwAgBMcAOAJGwCguw0AQMUOAMDfFAA=
atoms_y: YMwFAGDMBQBQ3QQAUN0EAFDdBAAAJzgAACc4AAAdEAAAHRAAcJw5AKCvDwCQSCIAkEgiABDqBQAwjjIAMKYVACBeJwA=
atoms_z: QEIPAEBCDwAQ9f//EPX//xD1//8gHggAIB4IAOAwCADgMAgAEC4DAABSAwDgHAMA4BwDADA5CgBQpgkAkHQKAOCZAwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: gCwDAIAsAwBAGQEAQBkBAEAZAQBAEwIAQBMCAAB9AAAAfQAAgLUBAAD6AABAlgEAQJYBAMDUAQAA9AEAoIYBAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: IJsIAA==
atoms_aniso_u22: AO4CAA==
atoms_aniso_u33: oNkIAA==
atoms_aniso_u12: wEUEAA==
atoms_aniso_u13: wMgDAA==
atoms_aniso_u23: oAkBAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T1 = 500 degrees C

qdat:
AAAAAAAAAAEAAAAAAAAABAAyQIQBAgAYEABAIABA2DESAg46LESA8oQWAgRQB+ScRxiYi+1SWRIhIESEpUY65o2dQUkS7M+JGqGSbVPFRP9+pabZHSKfZRac9irM8OFyv6s1SVRCiIksNdOSJmaaNTGVq5NonEjCFId5aZ==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2356
b: 9.0893
c: 20.177
alpha: 90
beta: 95.707
gamma: 90
cell_volume: 955.423
crystal_density: 2.685
atoms_x: AAAAAAAAAACAZw4AgGcOAIBnDgBgxRsAYMUbAEB3GwBAdxsA4AMcAEAMGADgAxwA4AMcAMA4GwBAyw0AoLUOAAD/FAA=
atoms_y: IK0FACCtBQBA6AQAQOgEAEDoBABARjgAQEY4AAAdEAAAHRAA8Kg5AACgDwAQPCIAEDwiABDqBQDAdjIAwKcVAKAfJwA=
atoms_z: QEIPAEBCDwDw8f//8PH///Dx///QCQgA0AkIAMAtCADALQgA0EADAJBTAwAQFQMAEBUDAGBKCgAQoAkA4G8KAOCZAwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: AGsDAABrAwAgSAEAIEgBACBIAQCAMgIAgDICAIC7AACAuwAAIMUBAEAZAQAgxQEAIMUBAGDkAQBAEwIAgLUBAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: gA4IAA==
atoms_aniso_u22: gK8CAA==
atoms_aniso_u33: QN0KAA==
atoms_aniso_u12: 4JkDAA==
atoms_aniso_u13: wFECAA==
atoms_aniso_u23: gD4AAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T2 = 500 degrees C

qdat:
AAAAAAAAAAEAAAAAAAAABAAyQIQBAgAYEABAIABA2DESBA46LESA8oQWAgRQC+ScRxCYi+1UWRIhYESErUQ+5o2eQUkS7NeJGqESrVPFhPt+pUbpHSKfZxac7CvE8OGy37slSVRCiIksVdeSJmaaNLGVr5NonEjCFId5aR==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2356
b: 9.0893
c: 20.177
alpha: 90
beta: 95.707
gamma: 90
cell_volume: 955.423
crystal_density: 2.685
atoms_x: AAAAAAAAAACAZw4AgGcOAIBnDgBgxRsAYMUbAEB3GwBAdxsA4AMcAEAMGADgAxwA4AMcAMA4GwBAyw0AoLUOAAD/FAA=
atoms_y: IK0FACCtBQDQ6QQA0OkEANDpBABARjgAQEY4AAAdEAAAHRAA8Kg5AACgDwCAOiIAgDoiABDqBQDAdjIAwKcVAKAfJwA=
atoms_z: QEIPAEBCDwDw8f//8PH///Dx//9ACAgAQAgIADAsCAAwLAgAYEIDAJBTAwAQFQMAEBUDAPBLCgAQoAkA4G8KAOCZAwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: AGsDAABrAwAgSAEAIEgBACBIAQCAMgIAgDICAIC7AACAuwAAIMUBAOAoAQAgxQEAIMUBAGDkAQBAEwIAgLUBAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: IB4IAA==
atoms_aniso_u22: gK8CAA==
atoms_aniso_u33: gPwKAA==
atoms_aniso_u12: gKkDAA==
atoms_aniso_u13: IEICAA==
atoms_aniso_u23: QB8AAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T = 600 C

qdat:
AAAAAAAAAAEAAAAAAAAABAAyQIQBAgAYEABAIABA2DESBA46LESA8oQWAgRQC+ScRxCYi+1UWRIhYESErUQ+5o2eQUkS7NeJGqESrVPFhPt+pUbpHSKfZxac7CvE8OGy37slSVRCiIksVdeSJmaaNLGVr5NonEjCFId5aR==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2412
b: 9.0983
c: 20.242
alpha: 90
beta: 95.690
gamma: 90
cell_volume: 960.504
crystal_density: 2.671
atoms_x: AAAAAAAAAADgVw4A4FcOAOBXDgBgxRsAYMUbAOCGGwDghhsAgBMcAEAMGADgAxwA4AMcAEB3GwAArA0AYJYOACDQFAA=
atoms_y: QH4FAEB+BQDw7AQA8OwEAPDsBACgNjgAoDY4AKAsEACgLBAAsKI5ADCxDwCgPSIAoD0iALD5BQCgjDIAkJYVAEAvJwA=
atoms_z: QEIPAEBCDwDw8f//8PH///Dx//+ADggAgA4IAPAlCADwJQgAsD0DAMBLAwCwCwMAsAsDAPBLCgCgoQkAQGAKAKB6AwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: YNgDAGDYAwDAVwEAwFcBAMBXAQCAMgIAgDICAMDaAADA2gAAAPQBAIA4AQBg5AEAYOQBACBCAgAgQgIAoAMCAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: oM0KAA==
atoms_aniso_u22: IEICAA==
atoms_aniso_u33: gG0NAA==
atoms_aniso_u12: IDYEAA==
atoms_aniso_u13: YEkGAA==
atoms_aniso_u23: 4CgBAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T = 650 C

qdat:
AAAAAAAAAAIAAAAAAAAABAAyQIQBAgAwEACAIABA8DEiBAo0KIUB5QgqBAigC6y4jjCxDtpU0RYhQIkJK4ytzxk6gtQluaqTLUMkzvOJDe96y0yyWoVW6k0p3H+ZYcNpv1pKkrRJERJUZq0cfsy4cWJTvSmxKRGIKg1qky==


formula: K.475 Na.025 Al2.28 Mg.2 Fe.28 Si3.24 O11.96 F.04 H1.96
compound: <missing>
formula_title: <missing>
a: 5.2328
b: 9.0948
c: 20.207
alpha: 90
beta: 95.694
gamma: 90
cell_volume: 956.932
crystal_density: 2.681
atoms_x: AAAAAAAAAABASA4AQEgOAEBIDgAA1RsAANUbAKBnGwCgZxsAICMcAKD8FwCg5BsAoOQbAEB3GwBAyw0AYJYOAOAtFQA=
atoms_y: AF8FAABfBQBw4AQAcOAEAHDgBABARjgAQEY4AAAdEAAAHRAAYKc5ANCnDwAQPCIAEDwiAPD/BQCgczIAUKkVAEAvJwA=
atoms_z: QEIPAEBCDwDA+f//wPn//8D5///QCQgA0AkIAMAUCADAFAgAUE0DADBKAwDgAwMA4AMDAMBTCgBgmwkAgGYKAKB6AwA=
atoms_occupancy: 4P0cAKCGAQAAYy4AgBoGAICLCABAcDEAwJgLAEBwMQDAmAsAAAk9AAAJPQCA0DsAgDgBAAAJPQAACT0AAAk9AIDQOwA=
atoms_u_iso: AOgDAADoAwDAVwEAwFcBAMBXAQBAkAIAQJACACDLAAAgywAAwNQBAIA4AQDgpQEA4KUBAIAyAgCAMgIAQBMCAAASegA=
atoms_aniso_label: ["H1"]
atoms_aniso_u11: ADUMAA==
atoms_aniso_u22: gLUBAA==
atoms_aniso_u33: AKYOAA==
atoms_aniso_u12: AOgDAA==
atoms_aniso_u13: 4AoGAA==
atoms_aniso_u23: oAkBAA==
pub_title:
 Thermal response of structure and hydroxyl ion of phengite-2M_1:
 an in situ neutron diffraction and FTIR study
 Sample: T = 700 C
 Note: y-coordinate altered

qdat:
AAAAAAAAAAIAAAAAAAAABAAyQIQBAgAwEABAIABA0DESBAoyLIUA1IgmAgjQC+ScRjCwjtVU2RIhYESEvURupY2aQUoU6NeLKqEQvVPNhN89p0axNWS35p6c7C/EsMPi3b0lSlRCiIosNJaSJkaaGLEZr5LIjEjCEodYpZ==


formula: Ca2 Si3 O11 H3
compound: Wessels mine, South Africa
formula_title: <missing>
a: 11.265
b: 7.386
c: 44.970
alpha: 90
beta: 90
gamma: 90
cell_volume: 3741.652
crystal_density: 2.439
atoms_x: AEsAAADwPABAQg8AAL4KAGBeDwAATQgAQGwIAIDXJQCA1yUAYCsLAOBRDwAAIw8AgOQOAEATAgCAyjwAgDwqAABkGQA=
atoms_y: EOU8AJCSHgBAsxEAYPD//9AxKwBgDRAAIDQuAKDSHgDgLgAAAAAAAOB0HgDg7AoAAEsyAGBtAACAAR8AAAAAAEAwEgA=
atoms_z: oE8GACBDBgBg0gQAQCwCANDQBADgIwYAcPMFAPA4CQDQZwkAAAAAADASBAAw5gIAwOcCABDKAgDg6gIAAAAAAKAPAAA=
atoms_occupancy: 0
atoms_u_iso: 4HkAAKBzAADAXQAAAH0AAIA+AADgLgAAYG0AAOCrAABgbQAAoAkBAECcAADgKAEA4KsAAAB3AQCArwIAgKkDAICpAwA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of tobermorite 11A: normal and anomalous forms,
 OD character and polytypic modifications
 Note: sample MD01

atoms_sites:
["Ca1", "Ca3", "Si1", "Si2", "Si3", "O1", "O1b", "O2", "O2b", "O3", "O5", "O6", "O6b", "O7", "O7b", "Wat2", "Wat3"]

qdat:
AAAAAAAAAIAAAAAAAQKQEAAMAAAgCBAKgIwYCSKAASACQQFiLQpIQkAgiEADMIG4woKlkJIHEIMgWhkn1DBgB2YcQgQAB/2bc6UiojSZIQAAArdKA5FpIIDPVCAAAA9a0jrWIAADrKAAABE6RgDpEAAAOkwAAAAAaRAAAA==


formula: Ca2 Si3 O11 H5
compound: Wessels mine, South Africa
formula_title: <missing>
a: 6.735
b: 7.385
c: 22.487
alpha: 90
beta: 90
gamma: 123.25
cell_volume: 935.351
crystal_density: 2.453
atoms_x: MC4QADDFLQBQRS4AcHY3AIBWLgDgDi8AYFMuAKAePABgrR8AwJA2AIB5CwDAehAAQP8uAODrHwDgPTwA4A8aAGCmNQDAwRkA
atoms_y: gGoaAMBSOABgkhcAMPctAJAvOwCw4B4AQN0KABDFIADwsRIAQIgtACCBNgBAfRoAEH80AOB/MQAwzQIA4F0NACB3DgAA1DAA
atoms_z: CIwMAKDpEQAQmwkACFgEAIigCQDgvwUAcBkIAOAYDABg2gsAAAAAAMC8BQAwuwUA8M0FAODmCwCQHQwAAAAAAAAAAAAAAAAA
atoms_occupancy: 0
atoms_u_iso: 0IQAAKBzAABgVAAAYIYAAIBXAADA2gAAcMYAADCOAACAuwAAoAkBAEAZAQAgvwIAYOoAAOCrAABAnAAAgIsIAICpAwBA7wcA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of tobermorite 11A: normal and anomalous forms,
 OD character and polytypic modifications
 Note: sample MD02

atoms_sites:
["Ca1", "Ca3", "Si1", "Si2", "Si3", "O1", "O2", "O3", "O4", "O5", "O6", "Wat6", "O7", "O8", "O9", "Wat1", "Wat2", "Wat3"]

qdat:
AAAACAAAAIAAAAgAAACAAAAIAAAAgAAKCA4QGUKiASgBgQEgCEIAKBAAwCACAAFyUKDZk4MiRYcqKIqFAQIQAIABAAAAAHqqebwoyzXedlBiIBgPEYggQCAQBAAANd/MfdSZxftqszMEXYgpAgICDZEIQIEHf0xdZjsf+Z==


formula: Ca2.25 Si3 O11 H5
compound: Bascenov, Urals, Russia
formula_title: <missing>
a: 6.732
b: 7.369
c: 22.680
alpha: 90
beta: 90
gamma: 123.18
cell_volume: 941.668
crystal_density: 2.507
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of tobermorite 11A: normal and anomalous forms,
 OD character and polytypic modifications
 Note: sample MDO2 - conventional X-ray source

atoms_sites:
["Ca1", "Ca2", "Ca3", "Si1", "Si2", "Si3", "O1", "O2", "O3", "O4", "O5", "O6", "Wat6", "O7", "O8", "O9", "Wat1", "Wat2", "Wat3"]

atoms_x:
gBAQAGAeIgBw5C0AIDQuAODYNwDAQy4AQAUuAIAeLwAAjDwA4OsfAEDPNgAgBgwAIHcOAADmLQCA+x8AAA88AICiGQBARjgAAGoYAA==

atoms_y:
YE4aAMDCBADAUjgAQKgXAIAkLgBgBTsA4HQeAKBKCwCgxiAAAAsTAADmLQAAsDYAAGQZACAQNABgQTEAIL8CAIDeDwBAQg8AAGMuAA==

atoms_z:
0KAMAICvAgCQ+REAYJsJAGBVBADQsgkA0MoFAAAbCACwBwwAoOALAAAAAADQygUAoOsFAMDuBQCg+QsAIDgMAIDH/v8AAAAAINf+/w==

atoms_occupancy:
AAk9AEBCDwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AICEHgAACT0AgIQeAA==

atoms_u_iso:
4KsAAOAiAgCgjAAAYG0AAGDqAABgbQAAQBkBAMDaAADgqwAAYOoAAKAJAQBAGQEAQH4FAKAJAQAAfQAA4KsAAEDvBwDARQQAgBoGAA==

qdat:
AAAACAAAAQAAABAAAAEAAAAgAAACAAAKKA4QK0LCAlADAgZAIIQAoCABAIAIAADyUKGZ1oNCSYs2SJUKAgQgAQAEAAAAAHqqObR5Ljre/CBCYCgPIxBAgEAgCAAAFdXMXd+1zdWR2xSEZIhGAgQECpEIQIEDX8x9Jjcb+Z==


formula: Ca2.25 Si3 O11 H5
compound: Bascenov, Urals, Russia
formula_title: <missing>
a: 6.732
b: 7.369
c: 22.680
alpha: 90
beta: 90
gamma: 123.18
cell_volume: 941.668
crystal_density: 2.507
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 The real structure of tobermorite 11A: normal and anomalous forms,
 OD character and polytypic modifications
 Note: MDO2 - synchrotron radiation source

atoms_sites:
["Ca1", "Ca2", "Ca3", "Si1", "Si2", "Si3", "O1", "O2", "O3", "O4", "O5", "O6", "Wat6", "O7", "O8", "O9", "Wat1", "Wat2", "Wat3"]

atoms_x:
IOgQAEBNIgDgkS4A4A4vACB1OACAHi8AwD0vAECCLgBAHwAAALcgAMCKNwBAVAwAoKMRAKDvLgCgxiAAgD4AAKBtGgAg7DkAwD4aAA==

atoms_y:
kPsZAADoAwCA6DcAYGAXAMDGLQBAtzoAYDYeAKBQCgBgKiAAAI4SAOCXLQBgIzYAgJwaAOBzMwDAtDAA4J8CAGCcDQAAoA8AQP8uAA==

atoms_z:
sLYMACC/AgDwAhIAoKEJAJBmBADAvQkAQLAFABD3BwAANQwAYMELAAAAAADgvwUAwLwFABDRBQAAAwwAgEEMAGB5/v8AAAAAQKj+/w==

atoms_occupancy:
AAk9AEBCDwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AICEHgAACT0AgIQeAA==

atoms_u_iso:
AHcBAMBRAgDgpQEAYOQBAMDUAQDgpQEAYGECAOAoAQAA9AEA4CICAEATAgAgPAMAgKMEAOClAQCAMgIAQBMCAABlBAAA4gQAQH4FAA==

qdat:
AAAACAAAAQAAABAAAAEAAAAgAAACAAAKKA4QK0LCAlADAgZAIIQAoCABAIAIAADyUKGZ1oNCSYs2SJUKAgQgAQAEAAAAAHqqObR5Ljre/CBCYCgPIxBAgEAgCAAAFdXMXd+1zdWR2xSEZIhGAgQECpEIQIEDX8x9Jjcb+Z==


formula: Al2.41 Si.59 O4.793
compound: <missing>
formula_title: <missing>
a: 7.5817
b: 7.6813
c: 2.8865
alpha: 90
beta: 90
gamma: 90
cell_volume: 168.102
crystal_density: 3.127
atoms_sites: ["AlM", "AlT", "SiT", "AlT*", "Od", "Oab", "Oc", "Oc*"]
atoms_x: AAAAAEgYCQBIGAkA4AAQAFDLBwCw5BUAgIQeAOCGGwA=
atoms_y: AAAAAJC/FACQvxQA8IoMANBPDQAAyBkAAAAAAKD9AgA=
atoms_z: AAAAAICEHgCAhB4AgIQeAAAAAACAhB4AgIQeAICEHgA=
atoms_occupancy: AAk9AICEHgBgARIAIIMMAAAJPQAACT0AYGAXACCDDAA=
atoms_u_iso: +GYAANBwAADQcAAA2GgAALDbAADoywAAQGQBAEieAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Infrared band assignment and structural refinement of
 Al-Si, Al-Ge, and Ga-Ge mullites
 Sample: Al-Si single-crystal

qdat:
AAAAAAAAAAAAAAAAAAAIAAAAAAAIAAFAAAAAIABAAQASAIAGAIAAAQEQbAQAAaAAAEgkGEIUEEQQAGHRIBrgmCITwEFXUiFwEiCZkQAtwzRpRo8oV9hFv9YECS99BhLOGfRv7DVpZ8Ztnjd2k396vCMUHZm//mYdNoDilf==


formula: Al2.34 Si.66 O4.83
compound: <missing>
formula_title: <missing>
a: 7.5655
b: 7.6883
c: 2.8851
alpha: 90
beta: 90
gamma: 90
cell_volume: 167.814
crystal_density: 3.146
atoms_sites: ["AlM", "AlT", "SiT", "AlT*", "Od", "Oab", "Oc", "Oc*"]
atoms_x: AAAAAAAVCQAAFQkAcDQQAOCzBwBw3hUAgIQeAKBnGwA=
atoms_y: AAAAAADNFAAAzRQA0KAMAOBdDQBwxhkAAAAAAOAcAwA=
atoms_z: AAAAAICEHgCAhB4AgIQeAAAAAACAhB4AgIQeAICEHgA=
atoms_occupancy: AAk9AICEHgBAJBQAQGAKAAAJPQAACT0AQOgdAEBgCgA=
atoms_u_iso: ILIAAAjAAAAIwAAAgO0AAAAdAQAwCwEAMAEBAAgVAQA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Infrared band assignment and structural refinement of
 Al-Si, Al-Ge, and Ga-Ge mullites
 Sample: Al-Si powder data

qdat:
AAAAAAAAAAAAAAAAAAAEAAAAAAASAAFAAAAAIABAAQASAKAGAKAAAQEIZgIAAeAAAEQkHEESCEIQAHJJICrgWCIHwEHLMSCwIhGJmQAroSI1IpaadaxCm70GCT1tRaFFHfl/mTc4x6MtRj8yJfervhMEH46r9nOFPmBWnX==


formula: Al2.36 Ge.64 O4.82
compound: <missing>
formula_title: <missing>
a: 7.6530
b: 7.7779
c: 2.9252
alpha: 90
beta: 90
gamma: 90
cell_volume: 174.120
crystal_density: 3.572
atoms_sites: ["AlM", "AlT", "GeT", "AlT*", "Od", "Oab", "Oc", "Oc*"]
atoms_x: AAAAAMAnCQDAJwkAUHwQAPDaBwBwKRYAgIQeAICWGwA=
atoms_y: AAAAAHCyFABwshQAQG0MAAD9DAAArxkAAAAAAGDeAgA=
atoms_z: AAAAAICEHgCAhB4AgIQeAAAAAACAhB4AgIQeAICEHgA=
atoms_occupancy: AAk9AICEHgAAiBMAgPwKAAAJPQAACT0AgBMcAID8CgA=
atoms_u_iso: KLQAAOjBAADowQAAILIAAPAYAQDwGAEAaFABAPjFAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Infrared band assignment and structural refinement of
 Al-Si, Al-Ge, and Ga-Ge mullites
 Sample: Al-Ge powder data

qdat:
AAAAAAAAAAAAAAAAAAAQAAAAAAAoAAUAAAABAAIACACQBgBgBQAAEBCGYCAANgAACIRDiCSCCEQAHHJEBxQaCILwIMWVEHwQiGVUgBnRkjUmj1ra1Eqd2g4SftqVQow3kq5012O7jdo8/Yie9/K4vODs+/M2HGnSEylP1y==


formula: Ga2.31 Ge.69 O4.84
compound: <missing>
formula_title: <missing>
a: 7.8674
b: 8.0305
c: 3.0148
alpha: 90
beta: 90
gamma: 90
cell_volume: 190.473
crystal_density: 5.032
atoms_sites: ["GaM", "GaT", "GeT", "GaT*", "Od", "Oab", "Oc", "Oc*"]
atoms_x: AAAAAKAkCQCgJAkAQFUQAEDvBwBQPxYAgIQeAKDqGgA=
atoms_y: AAAAAJDOFACQzhQAMPUMALAzDQAQ1hkAAAAAAKD9AgA=
atoms_z: AAAAAICEHgCAhB4AgIQeAAAAAACAhB4AgIQeAICEHgA=
atoms_occupancy: AAk9AICEHgCgDhUA4HUJAAAJPQAACT0AgPUgAMAnCQA=
atoms_u_iso: SKgAACiqAAAoqgAAgO0AAAgVAQCA7QAAiAICAPiMAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Infrared band assignment and structural refinement of
 Al-Si, Al-Ge, and Ga-Ge mullites
 Sample: Ga-Ge powder data

qdat:
AAAAAAAAAAAAAAAAAACAAAAAAAiAAKAAAACAAIAEAIgGAGAKAAAgQJlBAAGoAACEhDkBSEEEgAesUQNNBwSA2CDVUyBoIQmvSgFKJ1DZaXHOt2iL56EkU53UsOSfpJ8ZVTOuy/x26sS75oxxUwbZ97XqbzsSVn395m+Gsx==


formula: (Ca2.97 Ba.03) Mg.11 Zr1.12 Ti.68 Fe.92 Si1.35 Al.81 O12
compound: Anguillara, Mts. Sabatini, Italy
formula_title: <missing>
a: 12.397
b: 12.397
c: 12.397
alpha: 90
beta: 90
gamma: 90
cell_volume: 1905.241
crystal_density: 3.930
atoms_sites: ["Ca", "Ba", "Mg", "Zr", "Ti", "Fe", "Si", "Al", "Fe", "O"]
atoms_x: IKEHACChBwAAAAAAAAAAAAAAAAAAAAAAYOMWAGDjFgBg4xYAoDUCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAsAsDAA==
atoms_z: QEIPAEBCDwAAAAAAAAAAAAAAAAAAAAAAQEIPAEBCDwBAQg8AgOQnAA==
atoms_occupancy: wGw8AECcAABgWwMAAC4iAIDAFAAAcQIAQHcbAMB6EAAAFxEAAAk9AA==
atoms_u_iso: AJYAAACWAACgWgAAoFoAAKBaAACgWgAAAGQAAABkAAAAZAAAEKQAAA==
atoms_aniso_label: ["Ca", "Ba", "Mg", "Zr", "Ti", "Fe", "Si", "Al", "Fe", "O"]
atoms_aniso_u11: 0GsAANBrAACgWgAAoFoAAKBaAACgWgAA0FIAANBSAADQUgAAsP4AAA==
atoms_aniso_u22: QLUAAEC1AACgWgAAoFoAAKBaAACgWgAAYG0AAGBtAABgbQAA8KAAAA==
atoms_aniso_u33: QLUAAEC1AACgWgAAoFoAAKBaAACgWgAAYG0AAGBtAABgbQAA4HkAAA==
atoms_aniso_u12: AAAAAAAAAADQBwAA0AcAANAHAADQBwAAAAAAAAAAAAAAAAAAAM7//w==
atoms_aniso_u13: AAAAAAAAAADQBwAA0AcAANAHAADQBwAAAAAAAAAAAAAAAAAAECcAAA==
atoms_aniso_u23: wCsAAMArAADQBwAA0AcAANAHAADQBwAAAAAAAAAAAAAAAAAAkOj//w==
pub_title:
 Crystal chemistry of kimzeyite from Anguillara, Mts. Sabatini, Italy
 Sample: AD collected with a point detector

qdat:
AAAAAAAAAAAAAAAAAAAACAABAAAAAAACABAAABACAIAgAAIBAAAAgEBAAIECBAgQAAEECCCCCACCAIIQQBCCEIQgCAQiEIBEABEQiIgERAQAREQEAIgAIiBEAQAAQAAAQAAAAAAACQAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Ca2.97 Ba.03) Mg.11 Zr1.12 Ti.68 Fe.92 Si1.35 Al.81 O12
compound: Anguillara, Mts. Sabatini, Italy
formula_title: <missing>
a: 12.397
b: 12.397
c: 12.397
alpha: 90
beta: 90
gamma: 90
cell_volume: 1905.241
crystal_density: 3.930
atoms_sites: ["Ca", "Ba", "Mg", "Zr", "Ti", "Fe", "Si", "Al", "Fe", "O"]
atoms_x: IKEHACChBwAAAAAAAAAAAAAAAAAAAAAAYOMWAGDjFgBg4xYAICkCAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAA0A4DAA==
atoms_z: QEIPAEBCDwAAAAAAAAAAAAAAAAAAAAAAQEIPAEBCDwBAQg8A0N8nAA==
atoms_occupancy: wGw8AECcAABgWwMAAC4iAIDAFAAAcQIAQHcbAMB6EAAAFxEAAAk9AA==
atoms_u_iso: EKQAABCkAABgbQAAYG0AAGBtAABgbQAAYG0AAGBtAABgbQAA4KsAAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal chemistry of kimzeyite from Anguillara, Mts. Sabatini, Italy
 Sample: CD collected with an area detector

qdat:
AAAAAAAAAAAAAAAAAAAACAABAAAAAAACABAAABACAIAgAAIBAAAAgEBAAIECBAgQAAEECCCCCACCAIIQQBCCEIQgCAQiEIBEABEQiIgERAQAREQEAIgAIiBEAQAAQAAAQAAAAAAACQAAAAAAAAAAAAAAAAAAAAAAAAAAAA==


formula: (Y1.534 Er.466) Ti2 Si O9
compound: <missing>
pub_title: The crystal structure of trimounsite-(Y), (Y,REE)2Ti2SiO9: an unusual TiO6-based titanate chain
formula_title: <missing>
a: 12.293
b: 11.124
c: 4.8610
alpha: 90
beta: 95.69
gamma: 90
cell_volume: 661.454
crystal_density: 4.842
atoms_x: QEcjAEBHIwCQxPv/kMT7/zgCFgCwKAkA2OotABBQJwCgwvf/AP8tANiGDwAwuhoAgEsbAHiWDwAQDwQA0O8DAA==
atoms_y: oJk0AKCZNAAgajQAIGo0AGCBKAAIeigAQEc3AACHKACQPSgA8AU3ANCfIQDAeCEAwG4rALBbMACwtSEAIF8rAA==
atoms_z: YB7//2Ae//+oRQMAqEUDANjr9f+oIwwAINfl/5Ay/P8gTgAAYEb6/7BJAQDgh+3/MDkKADALAQDA/hMAYNX3/w==
atoms_occupancy: gKEuAIBnDgBA/y4AwAkOAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: gM8AAIDPAADQzwAA0M8AAPjPAAAozQAAMNkAAAD6AADgDwEAIP0AAGDqAABAAAEAcN8AAADhAABgAwEAsOUAAA==
atoms_aniso_u11: YNEAAGDRAABg0QAAYNEAANDPAABg0QAAgNQAADDZAABgAwEAoPAAAIAGAQDQAQEAEO8AAEDnAAAgFgEA8OsAAA==
atoms_aniso_u22: sMwAALDMAACwzAAAsMwAALDlAADA2gAAwNoAAMAMAQBQDgEAEDoBAJDJAABw+AAAgO0AAJD7AAAg5AAAQAABAA==
atoms_aniso_u33: aM4AAGjOAACY0AAAmNAAAGC4AAAQvQAAwNoAAGADAQAQIQEAAMgAAJD7AADADAEAMMAAAPC5AAAAEwEA4MQAAA==
atoms_aniso_u12: KAAAACgAAADA/v//wP7//9AHAADg/P//AAAAAJAaAAAg6v//gPP//9Du//8Q9f//ECcAADD4///gFQAAwOD//w==
atoms_aniso_u13: WAwAAFgMAACwDgAAsA4AABAOAABQFAAAMBEAAJABAAAwKgAAkAEAAPBVAAAwKgAAgAwAABD1//8QJwAAoA8AAA==
atoms_aniso_u23: 6AMAAOgDAACQBgAAkAYAAHD+//9ABgAA4Pz//7AEAADA+f//ABkAAIDa//9Q4v//gPP//1D7//9AHwAAYAkAAA==
atoms_sites:
["Y1", "Er1", "Y2", "Er2", "Ti1", "Ti2", "Si", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9"]

atoms_aniso_label:
["Y1", "Er1", "Y2", "Er2", "Ti1", "Ti2", "Si", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9"]

qdat:
AAAAAAAAEAAACAAAAQBECAACAHAICEMBAgUEESShIIBNK0pVSgTPVaCRG5XinYlP8S8qd7f8xAerY+/vTNr8WS/Xf/d7u1/3f3u+/Pk/+v3Tn9dvZyvzqez/3Xz1v3lW77f/bo766X59XrnureSa+c4zjvU+1er3qbP081==


formula: Fe5.07 Zn.9 As2.268 Si.246 O15.246 H9.492
compound: Tsumeb, Namibia
formula_title: <missing>
a: 12.773
b: 12.773
c: 5.051
alpha: 90
beta: 90
gamma: 120
cell_volume: 713.664
crystal_density: 3.594
atoms_sites: ["FeM1", "FeM2", "ZnM2", "As1", "As2", "Si2", "O1", "O2", "O3", "O-H4", "O-H5", "H1", "H2"]
atoms_x: iOA3AIjgNwCI4DcAWLgrAKuwKACrsCgAAOokAHAIKAAAbSQAoP0CAKuwKABAnAAAq7AoAA==
atoms_y: yPYiAMj2IgDI9iIAwGA0AFVYFABVWBQAgPkwADAAOQAA0QsAUAMgAFVYFADAox4AVVgUAA==
atoms_z: cDkkAHA5JABwOSQAYB8mAGCgNgAgFjMAwBM2ACCsGgDgICwAQHwvAMAhCgAAnyQAELAXAA==
atoms_occupancy: gAEfAKCRFADAJwkAgIQeAADgLgDAAw8AAAk9AAAJPQAACT0AAAk9AMADDwAACT0AwAMPAA==
atoms_u_iso: MKcAADCnAAAwpwAAUHgAAPBuAABQeAAAECEBAFDDAACAUQEAkMkAAOCSAAAAEnoAABJ6AA==
atoms_aniso_label: ["FeM1", "FeM2", "ZnM2", "As1", "As2", "Si2", "O1", "O2", "O3", "O-H4"]
atoms_aniso_u11: cMYAAHDGAABwxgAAMHUAAKBzAADAdgAAQAABADAkAQDwTwEAgKIAAA==
atoms_aniso_u22: IJkAACCZAAAgmQAAYG0AAKBzAADAdgAAwIkBAMB2AAAwQwAA0LYAAA==
atoms_aniso_u33: 0J0AANCdAADQnQAA0IQAAABkAACgOwEAUKoAAHDGAADgCQIAsP4AAA==
atoms_aniso_u12: MFwAADBcAAAwXAAAYDsAANA5AABgOwAAIIAAAMB2AADQIAAAQFEAAA==
atoms_aniso_u13: 4Pz//+D8///g/P//MPj//wAAAAAAAAAAYFQAALCg//9Qyf//gD4AAA==
atoms_aniso_u23: gAwAAIAMAACADAAA4Pz//wAAAAAAAAAAMCoAANDu//+gkv//QB8AAA==
pub_title:
 Ekatite, (Fe3+,Fe2+,Zn)12(OH)6[AsO3]6[AsO3,HOSiO3]2, a new mineral
 from Tsumeb, Namibia, and its crystal structure

qdat:
AAAAAAAAAEAAAAAAIAAgAABAAgAAoAAAFAQQABAAgMEYCEQIkQYCDCQATCEQkQigImIgIEIsRAqTBG0BREmkVRLDASJZKTCEXk5KchoMWOTUqWMTYMlRLlVphAqtbPBrqnl1E2QRCXUlbqhVaOaNG49GKNM1ZZDFIuTqkF==


formula: Sn Ge S3
compound: Radvanice near Trutnov, Czech Republic
formula_title: SnGeS3
a: 7.2704
b: 10.197
c: 6.8463
alpha: 90
beta: 105.34
gamma: 90
cell_volume: 489.476
crystal_density: 3.902
atoms_sites: ["Sn1", "Ge1", "S1", "S2", "S3"]
atoms_x: CG01AFh2EwCQrQ0AYEkfABDeOQA=
atoms_y: wPkEAMi3DABgVAAA4CsNABAnMgA=
atoms_z: AM8NABhRHgBAOBkAALUxABDwBAA=
atoms_occupancy: 0
atoms_u_iso: IJMBAHD4AACgCQEAUCcBABAhAQA=
atoms_aniso_label: ["Sn1", "Ge1", "S1", "S2", "S3"]
atoms_aniso_u11: QGQBAJAUAQDQAQEAwNoAAHAqAQA=
atoms_aniso_u22: AMIBADDyAAAgywAA8MwBADALAQA=
atoms_aniso_u33: 0H4BAIDtAACwSQEAYNEAAJAtAQA=
atoms_aniso_u12: YCIAAAAAAABABgAA0CAAAHCz//8=
atoms_aniso_u13: 8DwAAGBUAACgQQAAYDsAAEBRAAA=
atoms_aniso_u23: QDgAACADAABQFAAA8L///2AJAAA=
pub_title:
 Natural SnGeS3 from Radvanice near Trutnov (Czech Republic):
 its description, crystal structure refinement and solid solution with PbGeS3

qdat:
AAAAAAAAAAAAAAAgAARAEAAAAIkAABACgISAIBGJAgDCxAgBKohBIWMMLJALLLRe6BOUXqkgmHTO4nHCxnRuST51cfTg8G1/halT3Uf/n+V16y+//Z7devfez9vf4//9vVrX/7P2r5Yv36738/a/d7/6uv/+Z1n7r/7/+R==


formula: Pb9.167 Sb9.833 S23 Cl O.5
compound: Buca della Vena mine, Tuscany, Italy
formula_title: <missing>
a: 49.49
b: 4.1259
c: 21.828
alpha: 90
beta: 99.62
gamma: 90
cell_volume: 4394.399
crystal_density: 5.861
pub_title:
 Lead-antimony sulfosalts from Tuscany (Italy). IV. Crystal structure of pillaite,
 Pb9Sb10S23ClO0.5, an expanded monoclinic derivative of hexagonal Bi(Bi2S3)9I3,
 from the zinkenite group
 Note: changed Pb2(z) to 0.2572 to match reported bond distances

atoms_sites:
["Pb1", "Pb2", "Pb3", "Pb4", "Pb5", "Pb6", "Pb7", "Pb8", "Sb8", "Pb9", "Sb9", "Pb10", "Sb10", "Pb11", "Sb11", "Sb", "Sb1", "Sb2", "Sb3", "Sb4", "Sb5", "Sb6", "Sb7", "S1", "S2", "S3", "S4", "S5", "S6", "S7", "S8", "S9", "S10", "S11", "S12", "S13", "S14", "S15", "S16", "S17", "S18", "S19", "S20", "S21", "S22", "S23", "Cl", "O"]

atoms_x:

atoms_y:

atoms_z:

atoms_occupancy:

atoms_u_iso:

atoms_aniso_label:
["Pb1", "Pb2", "Pb3", "Pb4", "Pb5", "Pb6", "Pb7", "Pb8", "Sb8", "Pb9", "Sb9", "Pb10", "Sb10", "Pb11", "Sb11", "Sb", "Sb1", "Sb2", "Sb3", "Sb4", "Sb5", "Sb6", "Sb7"]

atoms_aniso_u11:
YGcBACBIAQBgZwEAgLUBAGBnAQCgAwIA4KUBAIAsAwCALAMAwMgDAMDIAwDgpQEA4KUBAOAiAgDgIgIAQA0DAMDIAwAgxQEAoAkBAEAZAQDA2gAAIEICAIC1AQA=

atoms_aniso_u22:
oIYBAAB3AQCAtQEAQBMCAMDUAQDA1AEAQBMCAKADAgCgAwIAoAMCAKADAgAAdwEAAHcBAIAyAgCAMgIAoAMCAAD0AQAA6AMA4KUBAKADAgCAJgQAgK8CAABlBAA=

atoms_aniso_u33:
4CICAGDeAgAAdwEA4CICACBIAQDAVwEAIMUBAIC1AQCAtQEAQBMCAEATAgAgPAMAIDwDAKCAAgCggAIAYGcBAMBXAQAgSAEAIL8CAOClAQBgZwEAYOQBACBCAgA=

atoms_aniso_u12:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAIP//8DaAAA=

atoms_aniso_u13:
wOD//2Dw//+APgAA4KsAAOAuAACgkv//AAAAAAB9AAAAfQAAgDgBAIA4AQDgpQEA4KUBAOAuAADgLgAAoJL//wCD//+gkv//QJwAAIA+AABg8P//APoAAGDqAAA=

atoms_aniso_u23:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgET//8BdAAA=

qdat:
AAAAJAAgCCEIBAmBAYSEC0FAIsxdodcJqJpkOAohiUhxCYhHC2D3rX52fFmjhyMCkoGjEGIhDAIBfSnVmSRTRCJgioMUhAgAAAAAAH+/mq81HsckUkoQQAAAAAAAAAA9v+u3JSJomiIAAAAAAAAAAAAAP//221fXUiIAAA==


formula: Pb3 O2 Cl2
compound: <missing>
formula_title: <missing>
a: 11.879
b: 5.808
c: 9.505
alpha: 90
beta: 90
gamma: 90
cell_volume: 655.781
crystal_density: 7.338
atoms_sites: ["Pb1", "Pb2", "Pb3", "O", "Cl1", "Cl2"]
atoms_x: IP4EACAzEQBwLCIAEIsZAJBFFgAwezEA
atoms_y: QEIPAEBCDwBAQg8A4Lo8AEBCDwBAQg8A
atoms_z: sP8EAHB0FgBgkjAAgK4XAIDuBADwKTEA
atoms_occupancy: 0
atoms_u_iso: oAkBAIA4AQDgKAEAAPoAAIC1AQCghgEA
atoms_aniso_label: ["Pb1", "Pb2", "Pb3", "Cl1", "Cl2"]
atoms_aniso_u11: oAkBAGDqAABgZwEAIMUBAIA4AQA=
atoms_aniso_u22: YOoAAEAZAQBAGQEAoAMCACDFAQA=
atoms_aniso_u33: QBkBAOClAQAA+gAAIEgBAOClAQA=
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
atoms_aniso_u13: wOD//yDR//+gDwAAwF0AAACD//8=
atoms_aniso_u23: AAAAAAAAAAAAAAAAAAAAAAAAAAA=
pub_title:
 Crystal chemistry of lead oxide chlorides. I. Crystal structures of
 synthetic mendipite, Pb3O2Cl2, and synthetic damaraite, Pb3O2(OH)Cl

qdat:
AAAAAAAAAAAAAAQAACAABQhCAQAESBAAAFYIgmDCQWIQgtgENLFKlAkzFriyswLK19Wj3gv49XTrs/1Xo0fevzrdX9/b+WX/3Pdef9Ld//57X/+f/9fz/7/x1W/332/uv/Nu3bzf///F/8+/tu+tc+71mb+268v3dkX9vz==


formula: Pb3 O3 Cl H
compound: <missing>
formula_title: <missing>
a: 5.8052
b: 6.9025
c: 15.141
alpha: 90
beta: 90
gamma: 90
cell_volume: 606.706
crystal_density: 7.730
atoms_sites: ["Pb1", "Pb2", "Pb3", "Pb4", "Pb5", "Pb6", "O1", "O2", "O-H3", "O-H4", "Cl1", "Cl2"]
atoms_x: gIQeAICEHgCAhB4AAAAAAAAAAAAAAAAAgGEPAAAjDwAAAAAAgIQeAAAAAACAhB4A
atoms_y: sC4rAOB8DACgzSMAQKQgACD2FgCQfwQAYOIrAIATHADgJisAAIcoAIBK/v8g4/z/
atoms_z: sIUpABA9JgCAzzcAYNMhAMChLwBAExsAIBwAACAHKQBAajIAQNwfALDcJwDAdRUA
atoms_occupancy: 0
atoms_u_iso: 4CgBAEAZAQDAVwEAoAkBAEAZAQBAGQEAoAkBACBIAQDA1AEAYGECAECWAQBAkAIA
atoms_aniso_label: ["Pb1", "Pb2", "Pb3", "Pb4", "Pb5", "Pb6", "O1", "O2", "O-H3", "O-H4", "Cl1", "Cl2"]
atoms_aniso_u11: gDgBAIA4AQDgKAEAQBkBAOAoAQCAOAEAYOoAAOAoAQCAtQEAIL8CACBIAQAAawMA
atoms_aniso_u22: APoAAGDqAACgAwIAoAkBAGBnAQAA+gAAYGcBACBIAQCAMgIAQJYBAKADAgCggAIA
atoms_aniso_u33: IEgBAOAoAQDA2gAAYOoAAMDaAADgKAEAIMsAAGBnAQBAlgEAwM4CAAB3AQDA1AEA
atoms_aniso_u12: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAoA8AAIDB//8AAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u13: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAwOD//6CS//8AAAAAAAAAAAAAAAAAAAAA
atoms_aniso_u23: wOD//0AfAACAwf//oA8AAOAuAABg8P//gD4AAIA+AABAJf//YPb+/6APAADAXQAA
pub_title:
 Crystal chemistry of lead oxide chlorides. I. Crystal structures of
 synthetic mendipite, Pb3O2Cl2, and synthetic damaraite, Pb3O2(OH)Cl

qdat:
AAAAAAAAAAAAABAQCAgAEACEECAKAAIcAoAIpBiSAlAAZUgXA8jMQZWpS50Dzi3e5GmFR5HuynSnSqvWSt37rfNBbT5v1/ffV5Z6mzq1Xj/S7/aa/6qd+v2/i9/cdtf8/fzd76f3u7ff1enz5/z/e9z/65e/3871p/v/6/==


formula: Tl (Al Si3) O8
compound: <missing>
formula_title: TlAlSi3O8
a: 8.882
b: 13.048
c: 7.202
alpha: 90
beta: 116.88
gamma: 90
cell_volume: 744.476
crystal_density: 3.958
atoms_sites: ["Tl", "AlT1", "SiT1", "AlT2", "SiT2", "OA1", "OA2", "OB", "OC", "OD"]
atoms_x: gB0SAJB+AACQfgAA8BUsAPAVLAAAAAAAcE0pAPCHMgCggAIAII8KAA==
atoms_y: AAAAAIDECwCAxAsAMH0HADB9BwBgHgkAAAAAAGDNCQAwThMAQNYHAA==
atoms_z: AJIJAOCPDQDgjw0AsLgUALC4FAAAAAAAkDERAECADQAw4w8AwOAYAA==
atoms_occupancy: AAk9ACDuDwDgGi0AYJYOAKByLgAACT0AAAk9AAAJPQAACT0AAAk9AA==
atoms_u_iso: MKgEADDNAgAwzQIAALwCAAC8AgAQFQMA4BYEACCHAwBwHgMAoGEDAA==
atoms_aniso_label: ["Tl", "AlT1", "SiT1", "AlT2", "SiT2", "OA1", "OA2", "OB", "OC", "OD"]
atoms_aniso_u11: wMgDABB/AgAQfwIAwIMCAMCDAgBwXQUA8KcDAHBpAwBwBQMA8GkFAA==
atoms_aniso_u22: MBkHAMBeBADAXgQAUOMDAFDjAwBAWAMA8DACAPCIBACA9AMAIFUDAA==
atoms_aniso_u33: sPICACCsAQAgrAEAUCECAFAhAgDwBAEAcAwGAJBAAgBg5AEAsDABAA==
atoms_aniso_u12: AAAAAJAaAACQGgAAQB8AAEAfAAAAAAAAAAAAAHAwAAAAzv//YNf//w==
atoms_aniso_u13: YGcBAOAPAQDgDwEAUFkBAFBZAQAg3gEAIN4BADDyAABwrQAA8E8BAA==
atoms_aniso_u23: AAAAAHAXAABwFwAAsB0AALAdAAAAAAAAAAAAAFDJ//+QIP//wJX//w==
pub_title:
 The crystal structure of synthetic TlAlSi3O8: Influence of the
 inert-pair effect of thallium on the feldspar structure

qdat:
AAAAAAAAAAAAAAAEoAAAAABAAAEEAAAgSABApAAAUSIAABIoRBFEBABwLCUBCjwEwYUQC3IEiGiIkIGMK3O0EmLH6YCEFGziUjHSRei9nDYyrkMHRL83TsX1Eoxr80M/p8Nse8ZYkwh0LoONIda/sKaci7PhAerK/ac9sZ==


formula: Mg O
compound: <missing>
formula_title: <missing>
a: 4.2113
b: 4.2113
c: 4.2113
alpha: 90
beta: 90
gamma: 90
cell_volume: 74.688
crystal_density: 3.584
atoms_sites: ["Mg", "O"]
atoms_x: AAAAAICEHgA=
atoms_y: AAAAAICEHgA=
atoms_z: AAAAAICEHgA=
atoms_occupancy: 0
atoms_u_iso: OEUAAEBHAAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-chemical reasons for the immiscibility of periclase and wustite
 under lithospheric P,T conditions
 Sample: Per.synt


formula: (Mg.974 Fe.026) O
compound: <missing>
formula_title: <missing>
a: 4.2154
b: 4.2154
c: 4.2154
alpha: 90
beta: 90
gamma: 90
cell_volume: 74.906
crystal_density: 3.647
atoms_sites: ["Mg", "Fe", "O"]
atoms_x: AAAAAAAAAACAhB4A
atoms_y: AAAAAAAAAACAhB4A
atoms_z: AAAAAAAAAACAhB4A
atoms_occupancy: wHI7AECWAQAACT0A
atoms_u_iso: OEUAADhFAABARwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-chemical reasons for the immiscibility of periclase and wustite
 under lithospheric P,T conditions
 Sample: Per.4041

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAACAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAEAAAgAAAAAAAAAAAAIAAAAAAAAIAAgAAAAAAAAACAAAAAAAQAAAAAAAAAAEAAAAAAgAQAAAAAAAQAAAABABA==


formula: (Mg.958 Fe.042) O
compound: <missing>
formula_title: <missing>
a: 4.2178
b: 4.2178
c: 4.2178
alpha: 90
beta: 90
gamma: 90
cell_volume: 75.034
crystal_density: 3.685
atoms_sites: ["Mg", "Fe", "O"]
atoms_x: AAAAAAAAAACAhB4A
atoms_y: AAAAAAAAAACAhB4A
atoms_z: AAAAAAAAAACAhB4A
atoms_occupancy: wHg6AECQAgAACT0A
atoms_u_iso: WEMAAFhDAABISQAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-chemical reasons for the immiscibility of periclase and wustite
 under lithospheric P,T conditions
 Sample: Per.3363

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAACAAAAAAAAAAAAAAAAAAAAQAAAAAAAAAAAIAAAgAAAAAAAAAAAAIAAAAAAAAQAAgAAAAAAAAACAAAAAAAgAAAAAAAAAAEAAAAABAAgAAAAAAAgAAAABACA==


formula: (Mg.99 Fe.01) O
compound: <missing>
formula_title: <missing>
a: 4.212
b: 4.212
c: 4.212
alpha: 90
beta: 90
gamma: 90
cell_volume: 74.725
crystal_density: 3.611
atoms_sites: ["Mg", "Fe", "O"]
atoms_x: AAAAAAAAAACAhB4A
atoms_y: AAAAAAAAAACAhB4A
atoms_z: AAAAAAAAAACAhB4A
atoms_occupancy: wGw8AECcAAAACT0A
atoms_u_iso: OEUAADhFAABARwAA
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Crystal-chemical reasons for the immiscibility of periclase and wustite
 under lithospheric P,T conditions
 Sample: after heating to 1100 deg C

qdat:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAgAAAAACAAAAAAAAAAAAAAAAAAAAIAAAAAAAAAAAEAAAQAAAAAAAAAAAAEAAAAAAAAIAAQAAAAAAAAABAAAAAAAQAAAAAAAAAACAAAAAAQAQAAAAAAAIAAAAAgAg==


formula: Zr Si O4
compound: <missing>
formula_title: <missing>
a: 6.6039
b: 6.6039
c: 5.9783
alpha: 90
beta: 90
gamma: 90
cell_volume: 260.723
crystal_density: 4.670
atoms_sites: ["Zr", "Si", "O"]
atoms_x: AAAAAAAAAAAAAAAA
atoms_y: wMYtAMDGLQAQBQQA
atoms_z: IKEHAKAlJgAI7AsA
atoms_occupancy: 0
atoms_u_iso: ADwAACA/AACAZgAA
atoms_aniso_label: ["Zr", "Si", "O"]
atoms_aniso_u11: 4DgAANA+AABQkQAA
atoms_aniso_u22: 4DgAANA+AABQRgAA
atoms_aniso_u33: uEIAABBAAACgWgAA
atoms_aniso_u12: AAAAAAAAAAAAAAAA
atoms_aniso_u13: AAAAAAAAAAAAAAAA
atoms_aniso_u23: AAAAAAAAAACA8///
pub_title:
 The dynamic properties of zircon studied by single-crystal X-ray
 diffraction and Raman spectroscopy

qdat:
AAAAAAAAAAAAAAAAAAAAAAACAAAAAAACAAAAAAAEACAABAAAAACAAABAAAABAQAMAAACAAhAAAABBCAAAQARAAAQQiAAAAEQAAhCIAAgCAAFAJAAIBIAGESAAAJCBiBCAgJECAUICBIgxJACAogZIECCgDEogwWQZKIADI==


formula: K2 Na1.026 Ca.356 Mn5.926 Mg.238 Fe.401 (Ti1.896 Nb.104) Si8 O30 F H4
compound: Lovozero massif, Kola Peninsula, Russia
formula_title: <missing>
a: 5.3925
b: 11.9283
c: 11.7256
alpha: 113.044
beta: 94.840
gamma: 103.064
cell_volume: 663.394
crystal_density: 3.249
pub_title:
 Kupletskite polytypes from the Lovozero massif, Kola Peninsula,
 Russia: Kupletskite-1A and kupletskite-Ma2b2c
 Sample: Kupletskite-1A

atoms_sites:
["K1a", "K1b", "Na", "Ca", "Mn1", "Na1", "Mn2", "Mn3", "Mg3", "Mn4", "Fe4", "Ti", "Nb", "Si1", "Si2", "Si3", "Si4", "O1", "O2", "O3", "O-H4", "O-H5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "F16"]

atoms_x:
EBAIACCtBQCAhB4AgIQeAEDhMwBA4TMAiAcRAHDGGQBwxhkAAAAAAAAAAAAw2gQAMNoEAJBpKQAAnDEA0BMXABADHwCgfiwAMA0JAMDiBwDw6REAkI08AEACIgDQFiMAQGsEAMADDwBwXBoAkOoHAGAmEAAQRBAAEOsiAHA8FwAAAAAA

atoms_y:
0CQQAEBaCwAAAAAAAAAAAOCVDADglQwA4BEEACB/FQAgfxUAgIQeAICEHgBwPwUAcD8FABCZEACQTiEASC8pAIDOOACwjBMAELkJAFAaGACwPRwA0EEHAKDIDwDQzwAAUB0kAJCLAgAQWRkAQHAxAHBkOgCgEiUA4I8NACCiCwAAAAAA

atoms_z:
EMw8AMDpPAAAAAAAAAAAAHg4HQB4OB0AsLkdABiJHQAYiR0AgIQeAICEHgB4AwwAeAMMAMAODgDgbw8AyJYPAEBNDgAAVxcAMG4WAMBNJADAShgAcFIkAJAjJACgmBcA8D8MAICiMgCgyjAAoNcyAFBVCgAQXzEAcAQxAIA0CgAAAAAA

atoms_occupancy:
IAQ2AOAEBwCATicAgLoVAKBgMQBgqAsAwHI7AKDFNQBgQwcAwH8kAKB5GACA3DkAgCwDAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
UDoCAFA6AgDA2gAAwNoAAJCXAACQlwAAcK0AAOCrAADgqwAAkJcAAJCXAADQhAAA0IQAAGCGAADQnQAAgKIAAICJAABguAAAsMwAAPC5AADg3QAAYOoAAEC1AABguAAAYBwBAKCGAQDgDwEAAHcBAMBwAQCgIgEAsDABAJB4AQCQTAAA

atoms_aniso_label:
["Na", "Ca", "Mn1", "Na1", "Mn2", "Mn3", "Mg3", "Mn4", "Fe4", "Ti", "Nb", "Si1", "Si2", "Si3", "Si4", "O1", "O2", "O3", "O-H4", "O-H5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "F16"]

atoms_aniso_u11:
ACwBAAAsAQAQiwAAEIsAAPCgAADwoAAA8KAAAKCMAACgjAAA0GsAANBrAAAQiwAA8LkAAPC5AAAwjgAAEL0AAPDSAACAogAAQM4AAODEAACQsAAAQLUAAHDfAADwTwEAQDIBAAAmAgBgywEAQMgBAKDqAQBw+AAA0DkAAA==

atoms_aniso_u22:
oL4AAKC+AAAAlgAAAJYAAJCwAAAArwAAAK8AAICJAACAiQAA4JIAAOCSAAAQcgAA0IQAABCLAADAjwAA8NIAAIDUAADw0gAAIOQAADDyAADAwQAAYOoAAHBcAQBggAEAoDsBAPDMAQBAZAEAYJ8AAFCqAABg5AEAsGgAAA==

atoms_aniso_u33:
sIEAALCBAAAwpwAAMKcAAFDDAADQzwAA0M8AABCkAAAQpAAAUJEAAFCRAABghgAAUJEAAICiAABghgAAEIsAAICiAABwlAAAsOUAAOD2AACQsAAA0IQAABDWAADg9gAAUNwAAIAfAQBQ9QAAgNQAAHARAQDwBAEAQFEAAA==

atoms_aniso_u12:
ECcAABAnAADQIAAA0CAAAOAuAABAOAAAQDgAAJAaAACQGgAA0CAAANAgAAAAGQAAcBcAANAgAADQIAAAsDYAAHAwAABwFwAAQDgAAAAyAADwIwAAoEEAAFDi//8ghv//YLgAAFCLAQCgCQEAABkAABBAAABgWv//cDAAAA==

atoms_aniso_u13:
YAkAAGAJAACQGgAAkBoAAOAuAAAgNQAAIDUAAKAPAACgDwAAwBIAAMASAAAQDgAAMBEAAMASAADAEgAAcDAAACAcAACwBAAAcDAAAMArAAAAGQAAwBIAAEAfAADgYAAAcBcAAECcAACAj///4BUAAABLAAAwxv//sAQAAA==

atoms_aniso_u23:
sDYAALA2AADgRwAA4EcAABBZAACQZQAAkGUAAGA7AABgOwAAEEAAABBAAADgLgAAgD4AAJBMAAAASwAA0DkAALA2AABgOwAA4GAAAKBaAAAQWQAAUEYAAIBwAAAQJwAAwF0AALCzAADwIwAAIE4AAECDAADwuQAAMCoAAA==

qdat:
AAAAAAAAABgAAAAACAABIAAAIiAAADAgQEAwCQAlGAQDHEABUGwdAYvABgBfHgwCcAsvVfYEjwo3JrRWiyFLeOVWT+kvZuUnyzB3r9PnzXH1b/t7dSzVf+m+x7eBe/vb/in/3v9bfSe9329zc/PZH/f+TavnXWn77336bj==


formula: K2 Na.776 Ca.398 Mn6.6 Mg.138 (Ti1.762 Nb.238) Si8 O30 F H4
compound: Lovozero massif, Kola Peninsula, Russia
formula_title: <missing>
a: 5.4022
b: 23.226
c: 21.1782
alpha: 90
beta: 95.246
gamma: 90
cell_volume: 2646.130
crystal_density: 3.294
pub_title:
 Kupletskite polytypes from the Lovozero massif, Kola Peninsula,
 Russia: Kupletskite-1A and kupletskite-Ma2b2c
 Sample: Kupletskite-Ma2b2c

atoms_sites:
["K1", "K2", "Na", "Ca", "Mn1", "Na1", "Mn2", "Mn3", "Mn4", "Mg4", "Ti", "Nb", "Si1", "Si2", "Si3", "Si4", "O1", "O2", "O3", "O-H4", "O-H5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "F16"]

atoms_x:
gHvh/4CEHgAAAAAAAAAAAHBsDwBwbA8A0IktAMCULQBAQg8AQEIPAHCs4/9wrOP/kIsCAPBiAgCQmToAkIsCAEAgBACAniIAABoEAEAF/P/wgRoAELI4AIANBACQzRAAwLzT/wBU8v9QxxAA8P0vAHA9AgDAwzoAMPvy/4B74f8=

atoms_y:
MNAOAPBS/v84hQYAOIUGACj3FwAo9xcAiDQCAJDxCgBAQg8AQEIPAGCKBgBgigYAqMQLAHjdEwAIvwYA6FIBACA+CwDQkgYAIL0TAFAeDwDwYgIAYK0GANDiAQAQ7hUAMP8CANC1FQDAIQoAYPcCAPD1DwAA1QIAwCEKAIB+BgA=

atoms_z:
wL3w/8C98P/AvfD/wL3w/4iaAACImgAA+KP//0CO//8AAAAAAAAAAKC59v+gufb/MMT3/0hq+P9wgwcAAOD3/6By/P+QAPz/YBv9/xAVAwCg5AIAEMoCAFCQ/P9Qzfb/sPX1/6DI9v+Q2fX/EOb1/6CW9v+wSwkA4NT1/8C98P8=

atoms_occupancy:
AAk9AAAJPQBAviQAwEoYAKC5NwBgTwUAwGw8AMD1OgDAnDQAQGwIAKDFNQBgQwcAAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=

atoms_u_iso:
sMACABCYAgAg/QAAIP0AABCkAAAQpAAAcK0AAHCtAABQqgAAUKoAANC2AADQtgAAQJwAAJDJAAAwwAAAIJkAADCnAADQtgAAwKgAAODdAABg6gAAsLMAAPC5AADQsAEAkMMBALDGAQDgvgEAkMMBADBvAQAgkwEAUL0BAMBXAQA=

atoms_aniso_label:
["K1", "K2", "Na", "Ca", "Mn1", "Na1", "Mn2", "Mn3", "Mn4", "Mg4", "Ti", "Nb", "Si1", "Si2", "Si3", "Si4", "O1", "O2", "O3", "O-H4", "O-H5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "O13", "O14", "O15", "F16"]

atoms_aniso_u11:
gHcDALCIAwCgnwEAoJ8BAOCSAADgkgAAwI8AAHCUAABwlAAAcJQAAFB4AABQeAAA0IQAAPAEAQCg8AAAILIAAFCqAADQtgAAYIYAANC2AAAw2QAAkMkAAODEAACQDgIAMOwBALARAgAQ6QEAgM4BAHChAgBg9wIA8LMBAOBaAQA=

atoms_aniso_u22:
cAUDAACKAgDg3QAA4N0AAICJAACAiQAAYIYAAMCPAAAwjgAAMI4AACDLAAAgywAA0J0AADCnAADQnQAAMHUAABC9AADwuQAAwNoAAIDtAAAwwAAAUKoAAHDGAABwCwIAkFkCAIAyAgDAUQIAkCcCADCnAACwswAA4FQCAICcAQA=

atoms_aniso_u33:
UL0BAIC1AQAwdQAAMHUAAGDRAABg0QAA4PYAAGDqAADA2gAAwNoAAJDiAACQ4gAAkLAAAACvAACQsAAAEKQAAAB9AACQsAAAQJwAALD+AADAJQEAUKoAAICiAACg8AAAsBcBAOAPAQBwEQEAMD0BAEAAAQDADAEAIBYBAMAMAQA=

atoms_aniso_u12:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAUPv//xAOAAAgAwAAIAMAADD4//8w+P//QAYAAFD7//8Q9f//kAEAAMD5//+A8///QO3//7AEAAAQ9f//IOr//xD1//8g8P7/ALv+/3BDAQCAOAEAcEMBABD1//+QAQAAUM/+/wAAAAA=

atoms_aniso_u13:
QB8AAHAwAADQBwAA0AcAAJAaAACQGgAAwCsAALA2AABgCQAAYAkAAMASAADAEgAAYAkAADARAABQFAAAMBEAADD4//+QAQAA4BUAAKBBAADwIwAAkBoAAJAaAABABgAAcJQAADAqAACQfgAA4Jj//4AMAAAwKgAA0Ir//yADAAA=

atoms_aniso_u23:
AAAAAAAAAAAAAAAAAAAAAOD8///g/P//UBQAAGAJAADg4///4OP//3Dl//9w5f//MCoAAJABAABgCQAAIAMAAIDz//9w/v//UOL//8DH///Q7v//IOr//2Dw///AEgAAYKX//xBAAADAKwAA0KP//2Dw//8AMgAAQGoAAAAAAAA=

qdat:
AAAAAAAAAgoAAIAAAIiBihAaEApkBpHQgUhFnqB3yyhPh+1dzbW8xiyyWl1c97O9XPMtcYBSmHRoFpI50UWxohtRaCkoYSEwUlxjmYrGG05aGwLCgpgVBW2NcS5UOWVqsSg7KDEAtmWtZY2rIMkZBpFAGACClYjxY1TK1Q==


formula: Ca2 S2 O9 H2
compound: <missing>
pub_title: The monoclinic I2 structure of bassanite, calcium sulphate hemihydrate
formula_title: <missing>
a: 12.0350
b: 6.9294
c: 12.6705
alpha: 90
beta: 90.266
gamma: 90
cell_volume: 1056.649
crystal_density: 2.737
atoms_occupancy: 0
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["Ca1", "Ca2", "Ca3", "Ca4", "S1", "S2", "S3", "O1", "O2", "O3", "O4", "O5", "O6", "O7", "O8", "O9", "O10", "O11", "O12", "Wat1", "Wat2"]

atoms_x:
AAAAAICEHgDAhg4AEIgNAADn///wtg0AoO0NAGDABwAgoQcAQIQEAOCTBACA9gsAIIMMAKB6AwBAigMAAJoQAMCGDgBgeBMAgMwSAAAAAACgKjoA

atoms_y:
gIQeAOCrAABgJQwAIBIKAOB0HgCAAgoAoEoLAODgDADACQ4AAJklAIDXJQCArwIAoBX//8BWFgAA8xYAYOkVACBZEwCg0wkAYEkGAOBzMwCAPgAA

atoms_z:
AAAAAAAAAABQPAoAgJMoAFA3DwBwDDgAIE4ZAAAPPACg3hwA4DkTAADOMQCAQxQAQF40AEDdCgCgEykAoAgWAMAlMwBgfDwA4PcdAAAAAACgixUA

atoms_u_iso:
KLQAACi0AAAotAAAKLQAAHCUAABwlAAAcJQAACCyAAAgsgAAILIAACCyAAAgsgAAILIAACCyAAAgsgAAILIAACCyAAAgsgAAILIAAJDyBACQ8gQA

qdat:
AAAAAAAAIAAAAAAAEMAIAAAAhAAAAAYIAgFBAMCQAIBABgxAQkAYbgRABBwAOhjMAoSHFCQSTQ5Jsb4B6WbiEGG2zHno+bzH011CJQuJji8OJ9QTcTqXG8CzZS/Vi71GciyD2EmZLR1mVJ1XEkWcyxy8q0Wqj/S59pJYCz==


formula: (K.97 Na.03) (Mg2 Fe.33 Li.67) (Si3.4 Al.6) O11.2 F.8 H1.2
compound: <missing>
pub_title: First structure determination of an MDO-2O mica polytype associated with a 1M polytype
formula_title: <missing>
a: 5.2781
b: 9.141
c: 20.124
alpha: 90
beta: 90
gamma: 90
cell_volume: 970.925
crystal_density: 2.857
atoms_x: YKkoAGCpKAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAADgJAoA4CQKAOB1CQDwuRkAwCEKABDHKAAQxygAYPonAA==
atoms_y: AAAAAAAAAAAAAAAAAAAAAAAAAAB4qigAeKooAHiqKABgLAoAYCwKAAAAAAAA8Q4AsCwKAAAAAAAAAAAAAAAAAA==
atoms_z: QEIPAEBCDwAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABgRwgAYEcIAIgnCgBgJwoAWGMDACgqAwAoKgMAAF8FAA==
atoms_occupancy: QDQ7AMDUAQAAgSkAwLYGAEDRDACASCgAwLYGAMAJDgBA4TMAwCcJAAAJPQAACT0AAAk9AACfJAAAahgAAJ8kAA==
atoms_u_iso: YP0BAGD9AQAQpAAAEKQAABCkAACgpQAAoKUAAKClAABghgAAYIYAANAaAQBgHAEAsLMAALDMAACwzAAAwNQBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["K", "Na", "MgM1", "FeM1", "LiM1", "MgM2", "FeM2", "LiM2", "SiT", "AlT", "O1", "O2", "O3", "O-h", "F", "H"]

qdat:
AAAAAAAAAAIAAAAAAAAABABEAQACAAAwAACAAACCAiAgBBQkIAMAyAAEBEEADFCAQEgASMCBAEAECAAJoAiIgYSAICIDMggwBCCBqQgwCsIgQEIACgGiIUCkRbYhgRUG0QwJiAQAgFAuRhBWkEEgCgKiUIEBAECwqiEIkX==


formula: (K.97 Na.03) (Mg2.14 Fe.34 Li.52) (Si3.4 Al.6) O10.8 F1.2 H.8
compound: <missing>
pub_title: First structure determination of an MDO-2O mica polytype associated with a 1M polytype
formula_title: <missing>
a: 5.305
b: 9.199
c: 10.232
alpha: 90
beta: 100.03
gamma: 90
cell_volume: 491.697
crystal_density: 2.846
atoms_x: AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAACgpgQAoKYEALCOAgDwFRMAIOwHACAeCAAgHggAANYGAA==
atoms_y: gIQeAICEHgAAAAAAAAAAAAAAAAAQXhQAEF4UABBeFACgLQoAoC0KAAAAAAAA2A4AYDEKAICEHgCAhB4AgIQeAA==
atoms_z: AAAAAAAAAACAhB4AgIQeAICEHgCAhB4AgIQeAICEHgCY9Q0AmPUNAMA6CgAwOQoA8MUXAAA4GAAAOBgAIF8SAA==
atoms_occupancy: QDQ7AMDUAQAA8isAAFMHAADECQDAVSsAwLYGAID8CgBA4TMAwCcJAAAJPQAACT0AAAk9AABqGAAAnyQAAGoYAA==
atoms_u_iso: 4DsCAOA7AgCgpQAAoKUAAKClAAAwwAAAMMAAADDAAADQhAAA0IQAAGA1AQBAMgEAUKoAABDWAAAQ1gAAwNQBAA==
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
atoms_sites:
["K", "Na", "MgM1", "FeM1", "LiM1", "MgM2", "FeM2", "LiM2", "SiT", "AlT", "O1", "O2", "O3", "O-h", "F", "H"]

qdat:
AAAAAAAAAAIAAAAAAAAABABgAgCAAABQAIAAAACCQFAQAEaIJAkAkIBQCAAFqTOBAgKBo2AsCIE4RYAXxBT6JD5DA8AjWGNQMcMXxmBx1tOSoBuY0HcXk6xNyaM/OfY/udGMGfwbkY4wzonqPrOIF7NlrMxiRGYcYPkdmT==


formula: K.9 Na.05 Al2.11 Mg.32 Fe.18 Ti.03 Si3.4 O12 H2
compound: Cima Pal, Val Savenca, western Alps
formula_title: <missing>
a: 5.220
b: 5.220
c: 29.762
alpha: 90
beta: 90
gamma: 120
cell_volume: 702.318
crystal_density: 2.852
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Coexisting 3T and 2M_1 polytypes of phengite from Cima Pal (Val Savenca, western Alps):
 Chemical and polytypic zoning and structural characterisation
 Sample: 3TY

atoms_sites:
["KI", "NaI", "AlM2", "MgM2", "FeM2", "TiM2", "AlM3", "MgM3", "FeM3", "TiM3", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O6", "H"]

atoms_x:
kNEHAJDRBwCQozAAkKMwAJCjMACQozAAcNMbAHDTGwBw0xsAcNMbAPD9LwDw/S8AEJIcABCSHACgGSgAoMYHAHBrJACA2S0AELgeAFCZBwCAiwgA

atoms_y:
IKMPACCjDwCA1TYAgNU2AIDVNgCA1TYAgOoNAIDqDQCA6g0AgOoNANB6IwDQeiMAAEA4AABAOADQli8AUIkrAPBGDwCgoSIAQHI5AEClCwAAiBMA

atoms_z:
OCwKADgsCgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAiEBQAIhAUACIQFAAiEBQAw5wYAcIkGAPDgBgCAMgIAEDQCAMAfAgDAUQIA

atoms_occupancy:
gO42AEANAwDgFC4AAMQJAEB+BQBg6gAA4BQuAADECQBAfgUAYOoAAEDhMwDAJwkAQOEzAMAnCQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
4IwBAOCMAQDQnQAA0J0AANCdAADQnQAAwKgAAMCoAADAqAAAwKgAAGCGAABghgAA4JIAAOCSAADwBAEAoCIBAIAGAQAQ1gAAENYAACDkAADARQQA

qdat:
AAAAAAAAAAEAAAAAAAAAAQAUQEAQAQAKABAAEAAQaEUBAINkIkBQEIQAQAQAAKRBBAgEAnLCCCAgIBAAMkQnyoYSQICADSIhBBAQA0kRBBbSQhBBAAABqSEQtyTrMpCEA1SIhCAAAAA2TbkaL6SIhAAAzJERAAAAHldUsR==


formula: K.95 Na.01 Al1.9 Mg.34 Fe.27 Ti.03 Si3.5 O12 H2
compound: Cima Pal, Val Savenca, western Alps
formula_title: <missing>
a: 5.228
b: 5.228
c: 29.73
alpha: 90
beta: 90
gamma: 120
cell_volume: 703.715
crystal_density: 2.872
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Coexisting 3T and 2M_1 polytypes of phengite from Cima Pal (Val Savenca, western Alps):
 Chemical and polytypic zoning and structural characterisation
 Sample: 3TG

atoms_sites:
["KI", "NaI", "AlM2", "MgM2", "FeM2", "TiM2", "AlM3", "MgM3", "FeM3", "TiM3", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O6", "H"]

atoms_x:
0L4HANC+BwCwvzAAsL8wALC/MACwvzAA8K0bAPCtGwDwrRsA8K0bAPD9LwDw/S8AgJAcAICQHABQiCcAwLAHAHDoJACg9S0AUHMeAGB1BwDAJwkA

atoms_y:
MH8PADB/DwAg5TYAIOU2ACDlNgAg5TYAwNcNAMDXDQDA1w0AwNcNAJB0IwCQdCMAoDY4AKA2OAAA+S4AYC0sANBDDwCAniIAACE5APCpCwAAiBMA

atoms_z:
OCwKADgsCgAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAiEBQAIhAUACIQFAAiEBQCg5QYA8JUGANDdBgAQNAIAoDUCAAAmAgCAMgIA

atoms_occupancy:
wPs5AECcAACAuSoAQGAKAGA9CABg6gAAgLkqAEBgCgBgPQgAYOoAAOBnNQAgoQcA4Gc1ACChBwAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQAACT0A

atoms_u_iso:
0JcBANCXAQBghgAAYIYAAGCGAABghgAAILIAACCyAAAgsgAAILIAAICJAACAiQAAkH4AAJB+AAAA+gAAkBQBADALAQCw5QAAQM4AAAAsAQAAcQIA

qdat:
AAAAAAAAAAEAAAAAAAAAAQAYQEAgAgAKABAAEAAIyEUCAIJkIkBgIIQAQAQAAaRCCAgIAuTCECBAIBAAZIhPkwwkgQEAFUQhCBAgBpIhCC1EhCCCAAADUkQg7kvWJKEIB0kRCEAAAAB1LbJUP0kRCAADqSIiAAAANT1Joh==


formula: (K.98 Na.02) Al2.17 Mg.24 Fe.21 Ti.02 Si3.38 O12 H2
compound: Cima Pal, Val Savenca, western Alps
formula_title: <missing>
a: 5.2132
b: 9.051
c: 19.937
alpha: 90
beta: 95.76
gamma: 90
cell_volume: 935.971
crystal_density: 2.873
atoms_x: AAAAAAAAAAAIFg8ACBYPAAgWDwAIFg8AkE4cAJBOHABIlxsASJcbAAD0GgAwbA4AoGoOAADuGwCA+RcAcNMbAIAxFwA=
atoms_y: UOEFAFDhBQCYCAUAmAgFAJgIBQCYCAUAKLg4ACi4OABoyQ8AaMkPANCxBQAwXDIAMNgVAJBUOQDYWQ8AEG4iAODBJgA=
atoms_z: QEIPAEBCDwBQAAAAUAAAAFAAAABQAAAAuEQIALhECABYRQgAWEUIAEhOCgAwywkA2FQKACBLAwBISwMA8C8DAABrAwA=
atoms_occupancy: gNA7AIA4AQBgTS8AAFMHAKBoBgBAnAAAIJMzAOB1CQAgkzMA4HUJAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: UHIBAFByAQDAgAAAwIAAAMCAAADAgAAA8G4AAPBuAAAQcgAAEHIAABDvAAAQCAEAEO8AADDAAADAwQAAoPAAAGBhAgA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Coexisting 3T and 2M_1 polytypes of phengite from Cima Pal (Val Savenca, western Alps):
 Chemical and polytypic zoning and structural characterisation
 Sample: 2M1Y

atoms_sites:
["KI", "NaI", "AlM2", "MgM2", "FeM2", "TiM2", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O6", "H"]

qdat:
AAAAAAAAAAEAAAAAAAAAAQAaIEIAgIAKBAAQCAAQZgyDAIMMSwlAJJCEwCEWAPunEUYVEL00jJKiJATQqVWH6/KxSC0SWTnpUzIzF/5csNtvdpSvIpZLZmGplUPczxwbLWqzXIziNIRURd11MlbloaaMmvkmRFRFIERZ00==


formula: K.99 Na.02 Al1.97 Mg.33 Fe.24 Ti.04 Si3.45 O12 H2
compound: Cima Pal, Val Savenca, western Alps
formula_title: <missing>
a: 5.225
b: 9.057
c: 19.956
alpha: 90
beta: 95.73
gamma: 90
cell_volume: 939.656
crystal_density: 2.874
atoms_x: AAAAAAAAAACYDQ8AmA0PAJgNDwCYDQ8ACEocAAhKHADwmRsA8JkbANBGGwBQPQ4AEDcOAPDfGwCgFRgAUNAbAEASFwA=
atoms_y: YNYFAGDWBQBQBQUAUAUFAFAFBQBQBQUAeLM4AHizOAB4yA8AeMgPAGCzBQDwhzIAAK4VAKBJOQCwWQ8A4HUiACBkJgA=
atoms_z: QEIPAEBCDwB4AAAAeAAAAHgAAAB4AAAAWEUIAFhFCAD4RQgA+EUIAHBOCgDY0gkAKFUKAFBNAwDITQMAmDcDAECKAwA=
atoms_occupancy: wGw8AIA4AQDAVSsAIBIKAABTBwCAOAEAkKQ0AHBkCACQpDQAcGQIAAAJPQAACT0AAAk9AAAJPQAACT0AAAk9AAAJPQA=
atoms_u_iso: 4IwBAOCMAQCQfgAAkH4AAJB+AACQfgAAsIEAALCBAADAjwAAwI8AAHD4AAAwCwEAkPsAAEDOAADQzwAAkBQBAMBFBAA=
atoms_aniso_label: "<missing>"
atoms_aniso_u11: 0
atoms_aniso_u22: 0
atoms_aniso_u33: 0
atoms_aniso_u12: 0
atoms_aniso_u13: 0
atoms_aniso_u23: 0
pub_title:
 Coexisting 3T and 2M_1 polytypes of phengite from Cima Pal (Val Savenca, western Alps):
 Chemical and polytypic zoning and structural characterisation
 Sample: 2M1G

atoms_sites:
["KI", "NaI", "AlM2", "MgM2", "FeM2", "TiM2", "SiT1", "AlT1", "SiT2", "AlT2", "O1", "O2", "O3", "O4", "O5", "O6", "H"]

qdat:
AAAAAAAAAAEAAAAAAAAAAQASIEIAgQAKCAAgCAAQbAyFAIMcVRJALSCJgCEWAfOmIoYlIfZZFSVESAmgyecP9uVSYFwkvVLUYpRST/z50K/WnWndRSxTysXLLIeznjx2q1tPOjtIyREpDuirp92Pi6Ys6rKvEkkYgxH5Wx==


formula: K.83 Na.05 Ba.02 O11.72 H1.86 Al1.4 Mg1.84 Fe.69 Mn.01 Ti.13 Si2.8 F.35
compound: Mt. Vulture, Italy
formula_title: <missing>
a: 5.332
b: 9.235
c: 10.220
alpha: 90
beta: 100.06
gamma: 90
cell_volume: 495.506
crystal_density: 2.941
pub_title:
 Trioctahedral micas-1M from Mt. Vulture (Italy): Structural
 disorder and crystal chemistry
 Sample: LC2G

atoms_sites:
["K", "Na", "Ba", "O", "H", "AlM1", "MgM1", "FeM1", "MnM1", "AlM2", "TiM2", "MgM2", "FeM2", "SiT", "AlT", "O1", "O2", "O3", "O-H", "F"]

atoms_x:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAABAdIwAQHSMAkH4yAKBPHwAgfSYAsAYIALAGCAA=

atoms_y:
AAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AgIQeAICEHgCAhB4A0OgyANDoMgDQ6DIA0OgyAEAuCgBALgoAwPANAAAAAACgNwoAAAAAAAAAAAA=

atoms_z:
AAAAAAAAAAAAAAAAAAAAAAAAAACAhB4AgIQeAICEHgCAhB4AgIQeAICEHgCAhB4AgIQeAEDLDQBAyw0AYEoKAOBWCgCg4xcAoGAYAKBgGAA=

atoms_occupancy:
wKgyAEANAwCAOAEAwEUEAEDRDABAYAoAwFwVAIDAFABAnAAAYOoAAKD3AwCgeC0AYK4KAIC5KgCATxIAAAk9AAAJPQAACT0AoFoyAGCuCgA=

atoms_u_iso:
ICkCACApAgAgKQIAICkCACApAgDgqwAA4KsAAOCrAADgqwAAgLsAAIC7AACAuwAAgLsAAMDBAADAwQAA0EwBAFBZAQDAwQAAMMAAADDAAAA=

atoms_aniso_label:
["K", "Na", "Ba", "O", "H", "AlM1", "MgM1", "FeM1", "MnM1", "AlM2", "TiM2", "MgM2", "FeM2", "SiT", "AlT", "O1", "O2", "O3", "O-H", "F"]

atoms_aniso_u11:
4CICAOAiAgDgIgIA4CICAOAiAgDgkgAA4JIAAOCSAADgkgAA0IQAANCEAADQhAAA0IQAADCnAAAwpwAAQBkBAIC1AQDgqwAA4KsAAOCrAAA=

atoms_aniso_u22:
4CICAOAiAgDgIgIA4CICAOAiAgDwhwAA8IcAAPCHAADwhwAAUMMAAFDDAABQwwAAUMMAACCyAAAgsgAA4KUBAOAoAQDgqwAAYOoAAGDqAAA=

atoms_aniso_u33:
gDICAIAyAgCAMgIAgDICAIAyAgBAGQEAQBkBAEAZAQBAGQEAcPgAAHD4AABw+AAAcPgAAAD6AAAA+gAAIEgBAIA4AQBg6gAA4KsAAOCrAAA=

atoms_aniso_u12:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAHD+//9w/v//4LH//wAAAADg/P//AAAAAAAAAAA=

atoms_aniso_u13:
EFkAABBZAAAQWQAAEFkAABBZAABQRgAAUEYAAFBGAABQRgAAkBoAAJAaAACQGgAAkBoAAOAuAADgLgAAIE4AAAAAAABgIgAAoA8AAKAPAAA=

atoms_aniso_u23:
AAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAAJABAACQAQAAwOD//wAAAAAAAAAAAAAAAAAAAAA=

qdat:
AAAAAAAAAAIAAAAAAAAABACgAgCAAABQAQAAAAEFAGAgAJUIUBEAoQBgBAAJ5GEECAUChqBQBgJgJQBHEBUoYLKMByCLIepQ4wZbIoCilsvOoFaLwNWZKzMWxRl4qlQnxsphY/BYyimEbxaCazSQjKWK7JEUSODHE+HuNT==


